This book is devoted to superconductivity, which is one of the most interesting problems in physics. In accordance with

*205*
*115*
*26MB*

*English*
*Pages 308
[306]*
*Year 2021*

- Author / Uploaded
- Sergei Kruchinin

*Table of contents : ContentsPreface1. Theory of Superconductivity 1.1. Introduction 1.2. Spinors 1.2.1. Spinor 1.2.2. Noether theorem and Nambu–Goldstone theorem 1.3. Propagator 1.3.1. Hamiltonian 1.4. Non-interacting 1.5. Interacting 1.5.1. Unrestricted HF 1.5.2. Gap equation for superconductivity 1.6. Illustrative Example, Critical Temperature 1.6.1. Bond alternation 1.6.2. Deformation energy 1.6.3. Polyacene, gap equation, critical temperature 1.6.4. Conclusion 1.7. Linear Response Magnetic Resonance in Normal and Superconducting Species: Spin-Lattice Relaxation Time 1.7.1. Introduction 1.7.2. T1 in NMR 1.7.3. Theory with Green’s function 1.7.4. Non-interacting 1.7.5. Interacting; normal 1.8. Interacting; Superconductor 1.8.1. The extended Nambu spinor 1.8.2. Green’s function 1.8.3. Spin dynamics 1.8.4. Conclusion 1.9. Ginzburg–Landau Theory from BCS Hamiltonian 1.9.1. BCS theory 1.9.2. Hubbard–Stratonovitch transformation 1.9.3. Fourier transform 1.9.4. Nambu spinor 1.9.5. Critical temperature 1.9.6. Temperature dependence of ϕ 1.9.7. Dynamics of the boson field, symmetry breaking 1.9.8. Instability 1.9.9. Supersymmetry 1.9.10. Toward the Ginzburg–Landau equation 1.9.11. Discussion2. Physics of High-Tc Superconductors 2.1. Introduction 2.2. History of the Development of Superconductivity 2.3. Structural Properties of High-Temperature Superconductors 2.3.1. Phase diagram of cuprate superconductors 2.3.1.1. Antiferromagnetism of HTSC 2.4. Mechanisms of Pairing of High-Temperature Superconductors 2.4.1. Specific mechanisms of pairing in superconductivity 2.4.2. Magnetic mechanism of pairing 2.4.3. Exciton mechanisms of pairing 2.4.4. The anharmonic model and superconductivity 2.4.5. Van Hove singularities (vHs) 2.4.6. Plasmon mechanism of pairing 2.4.7. Bipolaronic mechanism of superconductivity 2.5. The Symmetry of Pairing in Cuprate Superconductors 2.5.1. Superconductor’s order parameter 2.5.2. Classification of the superconductor’s order parameter by the representations of symmetry groups 2.6. Experimental Studies of a Symmetry of the Superconducting Order Parameter 2.6.1. Measurements of the Josephson tunnel current 2.6.2. Measurements of the quantization of a flow by the technique of three-crystal unit 2.7. Thermodynamics of the d-Pairing in Cuprate Superconductors 2.7.1. Introduction 2.7.2. Antiferromagnetic spin fluctuations in high-temperature superconductors 2.7.3. Continual model of antiferromagnetic spin fluctuations 2.7.4. Equation for superconducting gap 2.7.5. Thermodynamic potential of antiferromagnetic spin fluctuations 2.7.6. Heat capacity of the d-pairing 2.7.7. Heat capacity jump in superconductors 2.8. Summary3. Iron Superconductors 3.1. Introduction 3.2. Structural Properties of Iron Superconductors 3.3. Compounds of the Type ReFeAsO 3.4. Compounds of the Type AFe2As2 (A = Ba, Sr, Ca) 3.5. Compounds of the Type AFeAs (A = Li) 3.6. Compounds of the Type FeSe and FeTe (iron selenide and iron telluride) 3.6.1. FeSe films 3.7. Superconductivity 3.8. Electronic Structure 3.8.1. Multiorbital and multizone cases 3.9. Minimum Model 3.10. Experimental Study of the Fermi Surface 3.11. Antiferromagnetism 3.12. Phase Diagrams 3.13. Mechanisms and Types of Pairing 3.13.1. Multizone superconductivity 3.13.2. Electron–phonon mechanism 3.13.3. Spin-fluctuation mechanism of pairing 3.13.4. Symmetry of pairing 3.13.5. Multiorbital model 3.14. Properties of a Superconductor with s±-Symmetry of Parameters of Order 3.15. t–J1–J2 Model 3.15.1. Superconductivity with different parameters of order 3.16. Conclusion4. Multiband Superconductivity 4.1. Introduction 4.2. Multiband Hamiltonian 4.2.1. Hamiltonian 4.2.2. Two-particle Green’s function 4.2.3. Traditional superconductivity 4.2.4. Copper oxides 4.2.5. Cooperative mechanism 4.2.6. Room-temperature superconductors 4.3. Two-gap Superconductivity in MgB2 4.3.1. The physical properties of MgB2 4.3.1.1. Mg1−xAlxB2 4.3.2. Theoretical model 4.3.3. Superconductivity in MgB2 4.4. Theoretical Studies of Multiband Effects in Superconductivity by Using the Renormalization Group Approach 4.4.1. Theoretical model 4.4.2. Renormalization group approach 4.4.3. Vertex correction and response function for Cooper pairs 4.4.4. Renormalization equation 4.4.5. Phase diagrams 4.5. Room Superconductors 4.5.1. On the superconductivity of hydrogen sulfide 4.5.2. Formalism for standard superconductors 4.5.2.1. Microscopic theory of superconductivity: BCS theory 4.5.3. Éliashberg theory 4.5.3.1. Theory of superconductivity by Éliashberg–McMillan5. Nanoscale Superconductivity 5.1. Introduction 5.2. Nanosize Two-gap Superconductivity 5.2.1. Hamiltonian for nanosize grains 5.2.2. Path integral approach 5.2.3. Condensation energy 5.2.4. Critical level spacing 5.2.5. Parity gap 5.3. Exact Solution of Two-band Superconductivity in Ultrasmall Grains 5.3.1. Exact solution for two-band superconductivity 5.3.2. Hamiltonian 5.3.3. Exact solution 5.3.4. Preprocessing for numerical calculations 5.3.5. Results and discussion 5.3.6. Pair energy level 5.3.7. Condensation energy 5.3.8. Parity gap 5.4. Kondo Effect Coupled to Superconductivity 5.4.1. Kondo regime coupled to superconductivity 5.4.2. Model 5.4.3. Mean-field approximation 5.4.4. Critical level spacing in the Kondo effect 5.4.5. Kondo effect coupled to the superconductivity 5.4.6. Exact solution for the Kondo regime 5.5. Interaction of Nanoscale Ferromagnetic Granules in London Superconductors 5.5.1. Magnetic field of ferromagnetic inclusions in a London superconductor 5.5.2. Magnetic field of ferromagnetic quantum dots in a superconducting nanocomposite material 5.5.3. Interaction energy of quantum dots in a superconducting nanocomposite material 5.5.4. Spin orientation phase transitions in a nanocomposite material with arrays of ferromagnetic quantum dots 5.6. Spin-orientation Phase Transitions in a Two-dimensional Lattice of Ferromagnetic Granules in a London-type Superconductor 5.7. Energy Spectrum and Wave Function of Electrons in Hybrid Superconducting Nanowires 5.7.1. Methodology 5.7.2. Calculation of the spectrum 5.8. Quantum Computer on Superconducting Qubits 5.8.1. Principle of quantum computers 5.8.2. Superconducting qubits 5.8.3. The Josephson effect 5.8.3.1. Current passing through two series-connected Josephson junctions 5.8.3.2. SQUIDS 5.8.3.3. Flux qubit 5.8.3.4. Charge qubit 5.8.3.5. Phase qubit 5.8.4. Quantum computer 5.8.4.1. D-wave quantum computer 5.8.4.2. Quantum advantage of Google 5.8.5. Topological quantum computers 5.8.5.1. Majorana fermion 5.8.5.2. Kitaev’s superconducting chainSummary and ConclusionsAppendix A A.1. Two-particle Green Function for Multiband SuperconductorsAppendix B B.1. A Solution Method for the Ferromagnetic Granules in the London SuperconductorsBibliographyIndex*

Modern Aspects of Superconductivity Theory of Superconductivity

Second Edition

This page intentionally left blank

Modern Aspects of Superconductivity Theory of Superconductivity Second Edition

Sergei Kruchinin

Bogolyubov Institute for Theoretical Physics, Kyiv, Ukraine

World Scientific NEW JERSEY

•

LONDON

•

SINGAPORE

•

BEIJING

•

SHANGHAI

•

HONG KONG

•

TAIPEI

•

CHENNAI

•

TOKYO

Published by World Scientific Publishing Co. Pte. Ltd. 5 Toh Tuck Link, Singapore 596224 USA office: 27 Warren Street, Suite 401-402, Hackensack, NJ 07601 UK office: 57 Shelton Street, Covent Garden, London WC2H 9HE

British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library.

MODERN ASPECTS OF SUPERCONDUCTIVITY Theory of Superconductivity Second Edition Copyright © 2021 by World Scientific Publishing Co. Pte. Ltd. All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the publisher.

For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher.

ISBN 978-981-123-451-4 (hardcover) ISBN 978-981-123-452-1 (ebook for institutions) ISBN 978-981-123-453-8 (ebook for individuals)

For any available supplementary material, please visit https://www.worldscientific.com/worldscibooks/10.1142/12215#t=suppl Desk Editor: Rhaimie Wahap Typeset by Stallion Press Email: [email protected] Printed in Singapore

Rhaimie - 12215 - Modern Aspects of Superconductivity.indd 1

23/3/2021 11:33:53 am

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

“The single reason for our inability to treat the problems of superconductivity consists in the absence of a suﬃcient imagination.” Richard P. Feynman

v

page v

This page intentionally left blank

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Preface

The study in the ﬁeld of superconductivity theory is one of the most bright, fruitful, and promising trends in the theoretical physics of condensed matter, since superconductivity remains to be one of the most interesting research areas in physics. The goal of the book is to give representation of certain modern aspects of superconductivity. We discuss such important aspects of the theory of superconductivity as the nature of high-Tc superconductivity, twogap superconductivity, room-temperature superconductivity, mesoscopic superconductivity, the pairing state and the mechanism of cuprate high-Tc superconductivity. We will consider also the up-to-date state of the problem of real construction of a quantum computer on the base of superconducting units. In Chapter 1, we consider the ﬁeld-theoretic method of superconductivity and discuss the basic idea of superconductivity and the elaboration of the Ginzburg–Landau and BCS theories in the frame of many-particle quantum ﬁeld theory. In Chapter 2, we consider such topics of high-Tc superconductivity as the structures of high-Tc superconductors, phase diagrams, and the problem of pseudogaps and analyze the mechanisms of superconductivity. We present general arguments as for the pairing symmetry in cuprate superconductors and investigate their thermodynamical properties within the spin-ﬂuctuation mechanism of superconductivity, by using the method of functional integrals. In Chapter 3, we consider the new class of high-temperature superconductors such as Fe-based laminar compounds. We analyze the physical properties and electron models of Fe-based high-temperature superconductors. The particular interest in them is explained be perspectives of their practical application. In the chapter, we give the complete pattern of the formation of their physical properties within theoretical models on the basis of their electron structure.

vii

page vii

March 24, 2021

viii

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Modern Aspects of Superconductivity: Theory of Superconductivity

Chapter 4 concentrates on the two-band and multiband superconductivity. We consider the physical properties of superconductor MgB2 and use our two-band model to explain the two coupled superconductor’s gaps of MgB2 . To study the eﬀect of the increasing Tc in MgB2 , we used the renormalization group approach and phase diagrams. In the ﬁeld of superconductivity, we meet the problem-maximum — it consists in the creation of roomtemperature superconductors. We consider this problem in our book, and give some recommendations on the search for these superconductors. We consider the problem of high-temperature superconductivity at high ´ pressures in hydrides and present the Eliashberg–Migdal theory explaining the room-temperature superconductivity in this case. Chapter 5 deals with the problem of nanoscale superconductivity. We consider the two-band superconductivity in ultrasmall grains, by extending the Richardson exact solution to two-band systems, and develop the theory of interactions between nano-scale ferromagnetic particles and superconductors. The properties of nano-sized two-gap superconductors and the Kondo eﬀect in superconducting ultrasmall grains are investigated as well. At the present time, popular is the topic of the nano-engineering with superconducting states. In this connection, we deal with the physics of magnetic dots on the superconductors and the problem of superconducting wires. We analyze ideas of the quantum information and quantum calculations with the use of superconducting nano-units. We describe the theory of the Josephson eﬀect and its applications in quantum calculations, as well as the idea of qubits. We consider a quantum computer on the basis of superconducting qubits and give a short review of the modern state of the problem of physical realization of quantum computers. We present the idea of a topological quantum computer with qubits in the basis of Majorana fermion quasiparticles. This book deals with a wide scope of theoretical and experimental topics in superconductivity and is written for advanced students and researchers in the ﬁeld of superconductors. Kyiv, November 2020

S. Kruchinin

page viii

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Contents

Preface

vii

1. Theory of Superconductivity 1.1 1.2

1.3 1.4 1.5

1.6

1.7

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . Spinors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.1 Spinor . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.2 Noether theorem and Nambu–Goldstone theorem . . . . . . . . . . . . . . . . . . . . . . . . . Propagator . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.1 Hamiltonian . . . . . . . . . . . . . . . . . . . . . . Non-interacting . . . . . . . . . . . . . . . . . . . . . . . . . Interacting . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.1 Unrestricted HF . . . . . . . . . . . . . . . . . . . 1.5.2 Gap equation for superconductivity . . . . . . . Illustrative Example, Critical Temperature . . . . . . . 1.6.1 Bond alternation . . . . . . . . . . . . . . . . . . . 1.6.2 Deformation energy . . . . . . . . . . . . . . . . . 1.6.3 Polyacene, gap equation, critical temperature 1.6.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . Linear Response Magnetic Resonance in Normal and Superconducting Species: Spin-Lattice Relaxation Time . . . . . . . . . . . . . . . . . . . . . . . . 1.7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . 1.7.2 T1 in NMR . . . . . . . . . . . . . . . . . . . . . . 1.7.3 Theory with Green’s function . . . . . . . . . . 1.7.4 Non-interacting . . . . . . . . . . . . . . . . . . . . 1.7.5 Interacting; normal . . . . . . . . . . . . . . . . .

ix

1 ... ... ...

1 4 6

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

7 11 12 13 16 20 21 22 23 24 25 29

. . . . . .

. . . . . .

. . . . . .

30 30 34 35 37 39

page ix

March 24, 2021

x

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Modern Aspects of Superconductivity: Theory of Superconductivity

1.8

1.9

Interacting; Superconductor . . . . . . . . . . . . . . . 1.8.1 The extended Nambu spinor . . . . . . . . . 1.8.2 Green’s function . . . . . . . . . . . . . . . . . 1.8.3 Spin dynamics . . . . . . . . . . . . . . . . . . 1.8.4 Conclusion . . . . . . . . . . . . . . . . . . . . . Ginzburg–Landau Theory from BCS Hamiltonian 1.9.1 BCS theory . . . . . . . . . . . . . . . . . . . . 1.9.2 Hubbard–Stratonovitch transformation . . 1.9.3 Fourier transform . . . . . . . . . . . . . . . . 1.9.4 Nambu spinor . . . . . . . . . . . . . . . . . . . 1.9.5 Critical temperature . . . . . . . . . . . . . . 1.9.6 Temperature dependence of φ . . . . . . . . 1.9.7 Dynamics of the boson ﬁeld, symmetry breaking . . . . . . . . . . . . . . . . . . . . . . 1.9.8 Instability . . . . . . . . . . . . . . . . . . . . . 1.9.9 Supersymmetry . . . . . . . . . . . . . . . . . . 1.9.10 Toward the Ginzburg–Landau equation . . 1.9.11 Discussion . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

41 41 43 44 45 46 47 49 50 51 54 55

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

56 58 59 62 62

2. Physics of High-Tc Superconductors 2.1 2.2 2.3

2.4

2.5

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . History of the Development of Superconductivity . . . . Structural Properties of High-Temperature Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.1 Phase diagram of cuprate superconductors . . . Mechanisms of Pairing of High-Temperature Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.1 Speciﬁc mechanisms of pairing in superconductivity . . . . . . . . . . . . . . . . . 2.4.2 Magnetic mechanism of pairing . . . . . . . . . . 2.4.3 Exciton mechanisms of pairing . . . . . . . . . . . 2.4.4 The anharmonic model and superconductivity . 2.4.5 Van Hove singularities (vHs) . . . . . . . . . . . . 2.4.6 Plasmon mechanism of pairing . . . . . . . . . . . 2.4.7 Bipolaronic mechanism of superconductivity . . The Symmetry of Pairing in Cuprate Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.1 Superconductor’s order parameter . . . . . . . .

65 .. ..

65 68

.. ..

69 74

..

76

. . . . . . .

. . . . . . .

76 78 79 80 81 82 83

.. ..

84 84

page x

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Contents

2.5.2

2.6

2.7

2.8

Classiﬁcation of the superconductor’s order parameter by the representations of symmetry groups . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Experimental Studies of a Symmetry of the Superconducting Order Parameter . . . . . . . . . . . . . . . 2.6.1 Measurements of the Josephson tunnel current . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.2 Measurements of the quantization of a ﬂow by the technique of three-crystal unit . . . . . . . . . . . . . Thermodynamics of the d-Pairing in Cuprate Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . 2.7.2 Antiferromagnetic spin ﬂuctuations in high-temperature superconductors . . . . . . . . . 2.7.3 Continual model of antiferromagnetic spin ﬂuctuations . . . . . . . . . . . . . . . . . . . . . . . . . 2.7.4 Equation for superconducting gap . . . . . . . . . . . 2.7.5 Thermodynamic potential of antiferromagnetic spin ﬂuctuations . . . . . . . . . . . . . . . . . . . . . . 2.7.6 Heat capacity of the d-pairing . . . . . . . . . . . . . 2.7.7 Heat capacity jump in superconductors . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

xi

3. Iron Superconductors 3.1 3.2 3.3 3.4 3.5 3.6

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . Structural Properties of Iron Superconductors . . . . . . Compounds of the Type ReFeAsO . . . . . . . . . . . . . Compounds of the Type AFe2 As2 (A = Ba, Sr, Ca) . . Compounds of the Type AFeAs (A = Li) . . . . . . . . . Compounds of the Type FeSe and FeTe (iron selenide and iron telluride) . . . . . . . . . . . . . . . . . . . . . . . . 3.6.1 FeSe ﬁlms . . . . . . . . . . . . . . . . . . . . . . . . 3.7 Superconductivity . . . . . . . . . . . . . . . . . . . . . . . . 3.8 Electronic Structure . . . . . . . . . . . . . . . . . . . . . . . 3.8.1 Multiorbital and multizone cases . . . . . . . . . 3.9 Minimum Model . . . . . . . . . . . . . . . . . . . . . . . . . 3.10 Experimental Study of the Fermi Surface . . . . . . . . . 3.11 Antiferromagnetism . . . . . . . . . . . . . . . . . . . . . . . 3.12 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . .

86 88 88 91 93 93 94 97 101 105 108 109 111 113

. . . . .

. . . . .

113 114 114 115 116

. . . . . . . . .

. . . . . . . . .

116 118 119 119 119 122 125 126 127

page xi

March 24, 2021

xii

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Modern Aspects of Superconductivity: Theory of Superconductivity

3.13 Mechanisms and Types of Pairing . . . . . . . . . . . . 3.13.1 Multizone superconductivity . . . . . . . . . . 3.13.2 Electron–phonon mechanism . . . . . . . . . . 3.13.3 Spin-ﬂuctuation mechanism of pairing . . . . 3.13.4 Symmetry of pairing . . . . . . . . . . . . . . . 3.13.5 Multiorbital model . . . . . . . . . . . . . . . . 3.14 Properties of a Superconductor with s± -Symmetry of Parameters of Order . . . . . . . . . . . . . . . . . . . 3.15 t–J1 –J2 Model . . . . . . . . . . . . . . . . . . . . . . . . 3.15.1 Superconductivity with diﬀerent parameters of order . . . . . . . . . . . . . . . . . . . . . . . . 3.16 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

128 128 131 131 133 133

.... ....

134 137

.... ....

138 142

4. Multiband Superconductivity 4.1 4.2

4.3

4.4

4.5

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Multiband Hamiltonian . . . . . . . . . . . . . . . . . . . . . 4.2.1 Hamiltonian . . . . . . . . . . . . . . . . . . . . . . . . 4.2.2 Two-particle Green’s function . . . . . . . . . . . . 4.2.3 Traditional superconductivity . . . . . . . . . . . . 4.2.4 Copper oxides . . . . . . . . . . . . . . . . . . . . . . . 4.2.5 Cooperative mechanism . . . . . . . . . . . . . . . . 4.2.6 Room-temperature superconductors . . . . . . . . Two-gap Superconductivity in MgB2 . . . . . . . . . . . . . 4.3.1 The physical properties of MgB2 . . . . . . . . . . 4.3.2 Theoretical model . . . . . . . . . . . . . . . . . . . . 4.3.3 Superconductivity in MgB2 . . . . . . . . . . . . . . Theoretical Studies of Multiband Eﬀects in Superconductivity by Using the Renormalization Group Approach . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4.1 Theoretical model . . . . . . . . . . . . . . . . . . . . 4.4.2 Renormalization group approach . . . . . . . . . . 4.4.3 Vertex correction and response function for Cooper pairs . . . . . . . . . . . . . . . . . . . . . 4.4.4 Renormalization equation . . . . . . . . . . . . . . . 4.4.5 Phase diagrams . . . . . . . . . . . . . . . . . . . . . . Room Superconductors . . . . . . . . . . . . . . . . . . . . . . 4.5.1 On the superconductivity of hydrogen sulﬁde . . 4.5.2 Formalism for standard superconductors . . . . . ´ 4.5.3 Eliashberg theory . . . . . . . . . . . . . . . . . . . .

145 . . . . . . . . . . . .

145 147 147 149 151 152 153 153 156 156 159 161

. . .

165 166 168

. . . . . . .

168 170 170 172 173 176 178

page xii

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Contents

5. Nanoscale Superconductivity 5.1 5.2

5.3

5.4

5.5

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . Nanosize Two-gap Superconductivity . . . . . . . . . . . 5.2.1 Hamiltonian for nanosize grains . . . . . . . . . 5.2.2 Path integral approach . . . . . . . . . . . . . . . 5.2.3 Condensation energy . . . . . . . . . . . . . . . . 5.2.4 Critical level spacing . . . . . . . . . . . . . . . . 5.2.5 Parity gap . . . . . . . . . . . . . . . . . . . . . . . Exact Solution of Two-band Superconductivity in Ultrasmall Grains . . . . . . . . . . . . . . . . . . . . . 5.3.1 Exact solution for two-band superconductivity . . . . . . . . . . . . . . . . . . 5.3.2 Hamiltonian . . . . . . . . . . . . . . . . . . . . . . 5.3.3 Exact solution . . . . . . . . . . . . . . . . . . . . 5.3.4 Preprocessing for numerical calculations . . . . 5.3.5 Results and discussion . . . . . . . . . . . . . . . 5.3.6 Pair energy level . . . . . . . . . . . . . . . . . . . 5.3.7 Condensation energy . . . . . . . . . . . . . . . . 5.3.8 Parity gap . . . . . . . . . . . . . . . . . . . . . . . Kondo Eﬀect Coupled to Superconductivity . . . . . . 5.4.1 Kondo regime coupled to superconductivity . 5.4.2 Model . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.3 Mean-ﬁeld approximation . . . . . . . . . . . . . 5.4.4 Critical level spacing in the Kondo eﬀect . . . 5.4.5 Kondo eﬀect coupled to the superconductivity . . . . . . . . . . . . . . . . . . 5.4.6 Exact solution for the Kondo regime . . . . . . Interaction of Nanoscale Ferromagnetic Granules in London Superconductors . . . . . . . . . . . . . . . . 5.5.1 Magnetic ﬁeld of ferromagnetic inclusions in a London superconductor . . . . . . . . . . . 5.5.2 Magnetic ﬁeld of ferromagnetic quantum dots in a superconducting nanocomposite material 5.5.3 Interaction energy of quantum dots in a superconducting nanocomposite material . . . 5.5.4 Spin orientation phase transitions in a nanocomposite material with arrays of ferromagnetic quantum dots . . . . . . . . . .

xiii

183 . . . . . . .

. . . . . . .

. . . . . . .

183 186 187 188 190 191 192

...

194

. . . . . . . . . . . . .

. . . . . . . . . . . . .

195 195 197 200 202 203 204 205 207 208 208 210 210

... ...

212 213

...

216

...

218

...

219

...

220

...

221

. . . . . . . . . . . . .

page xiii

March 24, 2021

xiv

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-fm

Modern Aspects of Superconductivity: Theory of Superconductivity

5.6

5.7

5.8

Spin-orientation Phase Transitions in a Two-dimensional Lattice of Ferromagnetic Granules in a London-type Superconductor . . . . . . . . . . . . . . . . . . . . . . . . . . . . Energy Spectrum and Wave Function of Electrons in Hybrid Superconducting Nanowires . . . . . . . . . . . . . 5.7.1 Methodology . . . . . . . . . . . . . . . . . . . . . . . . 5.7.2 Calculation of the spectrum . . . . . . . . . . . . . . . Quantum Computer on Superconducting Qubits . . . . . . 5.8.1 Principle of quantum computers . . . . . . . . . . . . 5.8.2 Superconducting qubits . . . . . . . . . . . . . . . . . 5.8.3 The Josephson eﬀect . . . . . . . . . . . . . . . . . . . 5.8.4 Quantum computer . . . . . . . . . . . . . . . . . . . . 5.8.5 Topological quantum computers . . . . . . . . . . . .

224 230 231 233 239 239 240 241 248 253

Summary and Conclusions

259

Appendix A

261

A.1

Two-particle Green Function for Multiband Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . . .

Appendix B B.1

A Solution Method for the Ferromagnetic Granules in the London Superconductors . . . . . . . . . . . . . . . . .

261 267 267

Bibliography

271

Index

289

page xiv

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

CHAPTER 1

Theory of Superconductivity

1.1. Introduction In the preface of the big folio “superconductivity” edited by Parks [1], one of the editors has told, “During the preparation of this treatise one of the authors commented that it would be “the last nail in the coﬃn [of superconductivity].” Some specialist of superconductivity around me said that we are hardly to ﬁnd articles useful for our future investigation, except for Anderson’s comments at the end of this book. Further we have found that Anderson was pessimistic for the further advance of superconductivity, for example, the high-temperature or room-temperature superconductivity was almost unlikely. However, against his expectation, the discovery of high-temperature superconductivity due to Bednorz and M¨ uller [2] is astonishing. The traditional BCS (Bardeen–Cooper–Schrieﬀer) theory [3] has failed to explain the mechanism of this high-temperature superconductivity. Anderson [5] proposed a new idea called the resonating valence bond (RVB) theory or the t − J model. The term t implies the transfer integral, and J does the electron correlation. We have never heard that his theory successful. Here is a comment of Feynman, found in his book [4], that it takes almost 50 years for the problem of superconductivity to be reduced to that of explaining the gap. Following the theory of Bardeen, Cooper, and Schrieﬀer, we will explain the gap, and the theory is essentially correct, but I believe it needs to be made obviously correct. As it stands now, there are a few seemingly loose ends to be clearly up. The theory of superconductivity seems to be founded on the London postulate [7]. Associated with the gauge transformation, the conserved current is i (1.1) j = − (φ∗ ∇φ − φ∇φ∗ ) − e|φ|2 A. 2

1

page 1

March 24, 2021

2

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

The current due to the ﬁrst term is called the paramagnetic current, while that due to the second, the diamagnetic current. In the superconducting state, the ﬁrst term on the right-hand side changes very slightly, sometimes the wave function is called rigid, so that only the diamagnetic current survives. In this respect, the superconductor is the perfect diamagnetic substance. The current is dominated by j = −k2 A,

(1.2)

where k is a properly chosen positive constant. The Meissner eﬀect is easily derived from the Amp´ere’s equation ∇ × B = j.

(1.3)

∇2 B = k 2 B

(1.4)

Bx = B0 e−kx .

(1.5)

Taking rotation gives

or

It is important to note that |φ|2 in Eq. (1.1) is very large, the classic scale quantity, so that the magnetic ﬁeld in Eq. (1.5) damps very rapidly. This is the Meissner eﬀect. We know similar phenomena, the screening of the Coulomb interaction, or the quark conﬁnement. The boson model of the Cooper pairs is considerably successful. Equation (1.3) yields ∇2 A = k2 A, which is ∂ μ Aμ = −k2 Aμ

(1.6)

in the covariant form, suggesting that a photon is massive, which is a fundamental aspect to superconductivity [8]. The essentially same treatment has been presented by Ginzburg and Landau (GL) [9]. The superconducting state is the macroscopic state, in other words, a thermodynamic phase. They characterize this phase by introducing the order parameter, Ψ. This looks like the Schr¨ odinger function Ψ, and then the primitive quantum theorist confused, saying that, behind the iron curtain, the quantum theory was diﬀerent in feature from that of the western countries.

page 2

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

3

The theory is carried out as the phase transition. The Lagrangian for the superconducting state is postulated as 1 1 e∗ A 2 h2 2 4 (1.7) −i∇ + Fs = F0 + a|Ψ| + b|Ψ| + + 8π , 2 2m∗ c where ∗ indicates quantities in question referred to the superconductor (×2). Note that there are |Ψ|2 and |Ψ|4 terms in the potential parts. These drive the system to the spontaneous symmetry breaking and lead to a phase transition for the suitable choice of constants a and b. This is called now the Higgs mechanism [8]. Certainly the Ginzburg–Landau treatment is a few years ahead the Nambu–Goldstone suggestion. The Ginzburg–Landau theory is called the macroscopic quantum mechanism, and, in this sense, the big Ψ is called sometimes amusingly cat’s Ψ. The very instructive presentation of the macroscopic quantum theory is found in the “Feynman Lectures on Physics, Vol. III, Chapter 21.” Various topics there, for example the Josephson junction, are quite readable. The microscopic theory is prepared by Bardeen, Cooper, and Schrieﬀer [3]. However, as a preliminary discussion, we present the Bogoliubov treatment. The superconductivity is a kind of many-electron problems. The most general Hamiltonian should be 1 + dxdx ψ + (x)ψ(x)v(x, x )ψ + (x )ψ(x ). H = dxψ (x)h(x)ψ(x) + 2 (1.8) Since the algebra of electrons is spinor, the terms other than the above identically vanish. In other words, the 3- or 4-body interactions are useless. First, we specify the spin indices, and next the plane wave representation for the spatial parts. Equation (1.8) is simply written as ∗ ∗ H = k (a+ k + ak ) + vk,−k ak a−k a−k ak .

(1.9)

The simpliﬁcation or the mean-ﬁeld approximation for the two-body part is twofold, say, + Δk,−k akα akα a+ −kβ a−kβ , + Δk,−k a+ kα akβ akα a−kβ + c.c.

(1.10)

The latter looks curious, since such expectation value akα a−kβ vanishes identically. Against this common sense, Bogoliubov put the Hamiltonian ∗ ∗ ∗ H = k (a+ k + ak ) + Δk ak a−k + Δk a−k ak .

(1.11)

page 3

March 24, 2021

4

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

We understand that Bogoliubov presumed the Cooper pair, and provided the eﬀective Hamiltonian for pairs. His theory may be a short-hand treatment of the Bardeen–Cooper–Schrieﬀer (BCS) theory. This Hamiltonian is diagonalized by the so-called Bogoliubov transformation deﬁning the quasiparticle responsible for the superconductivity as ck↑ γk↑ uk −vk = , (1.12) + γ−k↓ c+ vk uk −k↓ with u2k − vk2 = 1.

(1.13)

The spirit of the Bogoliubov transformation is to mix operators ck↑ and c+ −k↓ which are diﬀerent in spin. The quasiparticle yields the new ground state so that the particle pair or the hole pair arises near the chemical potential. The stabilization energy thus obtained is called the gap energy Δk [3, 11]. We now follow the BCS microscopic treatment. The Green’s function has eﬀectively used by employing the Nambu spinor. This makes the uniﬁed treatment of normal and superconducting states possible. However, the temperature Green’s function (Matsubara function) is used from the beginning.

1.2. Spinors We start with the general many-electron Hamiltonian not restricted to the BCS (Bardeen–Cooper–Schrieﬀer) Hamiltonian. The BCS state responsible for the superconducting state is easily recognized from the formal description. The simplest method of the quantum chemistry should be the H¨ uckel theory. This consists of the single energy matrix, (1.14) βrs = dxh(x)ρrs (x), where h(x) is the single-particle quantum mechanical Hamiltonian, and the electron density ρrs (x) is given by the product of the single-particle (atomic) orbitals χr and χs . Note that this is the spinless theory. We then extend the treatment into the spin space, ↑↑ ↑↓ βrs βrs . (1.15) βrs = ↓↑ ↓↓ βrs βrs

page 4

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

5

Any 2 × 2 matrix is expanded in the Pauli spin matrices together with the unit matrix, 0

σ =

1 0 0 1

,

3

σ =

1

0

0 −1

,

1

σ =

0

1

1

0

,

2

σ =

0 −i i

0 (1.16)

However, we employ other combinations: 1 σ = (σ 0 + σ 3 ) = 2

↑

1 σ = (σ 0 − σ 3 ) = 2

↓

1 σ + = (σ 1 + iσ 2 ) = 2 σ− =

1 0 0 0 0 0

,

, 0 1 0 1

1 1 (σ − iσ 2 ) = 2i

, 1 0 0 0 1 0

.

(1.17)

In Eq. (1.24), we then have μ μ σ , βrs = βrs μ = Tr(σ μ βrs ), βrs

(1.18)

in details: ↑ ↑↑ = βrs βrs

↓ ↓↓ βrs = βrs ,

+ ↓↑ = βrs βrs

− ↑↓ βrs = βrs .

(1.19)

As to the Pauli matrices, the ordinary commutators are ⎫ [σ i , σ j ] = 2iijk σ k ⎪ ⎪ ⎪ 3 + ⎪ σ , σ = 2σ + ⎬ 3 − , σ , σ = −2σ − ⎪ ⎪ ⎪ ⎪ ⎭ [σ + , σ − ] = σ 3

(1.20)

page 5

March 24, 2021

6

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

⎫ σ↑ , σ↓ = 0 ⎪ ⎪ ⎪ ↑ + ⎪ + ⎪ ⎪ σ ,σ = σ ⎪ ⎪ ↑ − ⎪ σ , σ = −σ−⎬ ↓ + , ⎪ σ , σ = −σ + ⎪ ⎪ ↓ − ⎪ ⎪ σ , σ = σ− ⎪ ⎪ ⎪ ⎪ ⎭ + − 3 [σ , σ ] = σ

(1.21)

and the anticommutators are

σi , σj

+

= 2iδij

[σ + , σ − ]+ = 1

.

(1.22)

We then express the matrix in Eq. (1.15) as μ μ σ , βrs = βrs μ = Tr(σ μ βrs ), βrs

(1.23)

in details: ↑ ↑↑ = βrs , βrs

↓ ↓↓ βrs = βrs ,

+ ↓↑ = βrs , βrs

− ↑↓ βrs = βrs .

(1.24)

Here, if the quantum mechanical Hamiltonian has the single-particle character without the external ﬁeld causing a rotation in the spin space, the oﬀ-diagonal elements are meaningless. The H¨ uckel theory involves the spin diagonal terms. However, if we taken the electron–electron interaction into account, even in the mean-ﬁeld approximation, the oﬀ-diagonal elements becomes meaningful and responsible for the superconductivity. This is what we investigate here.

1.2.1. Spinor The algebra representing electrons is spinor. The Dirac relativistic (special relativity) function well describes this property. However, the relativity seems not so important for the present problem. We now concentrate on the spinor character of electron. The ﬁeld operator has two components in the spin

page 6

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

7

space. φ(x) =

φ↑ (x)

φ+ ↓ (x)

,

¯ φ(x) = φ (x)σ = +

3

= (φ+ ↑ (x)

(φ+ ↑ (x)

φ↓ (x))

1

0

0

−1

−φ↓ (x)).

(1.25)

This is called the Nambu representation [12]. The negative sign in front of ¯ φ↓ is seen in the Dirac conjugate φ+ → φ. The ﬁeld operators satisfy, of course, the anticommutators [φα (x), φ+ β (s )]+ = δα,β δ(x − x ),

(1.26)

where (α, β) = (↑, ↓), and x = (r, t). Then, for spinors (1.25), the matrix commutator holds: φ (x) ↑ ¯ ) = , (φ+ φ(x), φ(x ↑ (x ) −φ↓ (x )) + (x) φ+ ↓ + )] ), φ (x)] [φ↑ (x), φ+ (x [φ (x + + ↓ ↑ ↑ = + + [φ+ (x), φ ↓ ↑ (x )]+ [φ↓ (x ), φ↓ (x)]+ 0 δ(x − x ) . (1.27) = 0 δ(x − x )

1.2.2. Noether theorem and Nambu–Goldstone theorem We seek for the meaning of the Nambu spinor [13]. Consider a global transformation of ﬁelds with the constant Λ, φα (x) → φα (x)eiΛ , −iΛ . φ+ α (x) → φα (x)e

(1.28)

It is recognized that the Hamiltonian and the equation of motion in coming are invariant under this transformation. We can observe that this transformation is a rotation around the σ 3 -axis with Λ: 3

φ(x) → eiσ Λ φ(x)

(1.29)

page 7

March 24, 2021

8

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

since eiσ

3Λ

= cos(σ 3 Λ) + i sin(σ 3 Λ)

(σ 3 Λ)3 (σ 3 Λ)5 (σ 3 Λ)2 (σ 3 Λ)4 + + ··· + i 1 − + + ··· =1− 2! 4! 3! 5! Λ3 Λ5 Λ2 Λ4 3 + + · · · + iσ 1 − + + ··· =1− 2! 4! 3! 5! = σ 0 cos Λ + iσ 3 sin Λ 0 eiΛ . = 0 e−iΛ

Here, we discuss brieﬂy the Noether theorem and the Nambu–Goldstone theorem. The latter makes a profound investigation possible. If the Lagrangian of the system in question is invariant under some transformation which is just the present case, we have the continuity relation. Notice that the density and the current are, in terms of the Nambu spinor, j 0 = φ+ (x)σ 3 φ(x), + φ (x)∇φ(x) + ∇φ+ (x)φ(x) . j = −i 2m

(1.30)

Then, the continuity relation is ∂t j0 (x) + ∇ · j = 0.

(1.31)

If the system is static, the density must be conserved, ∂t j 0 = 0. Put

(1.32)

G=

dxj 0 (x),

(1.33)

and if it is found that [G, Ψ (x)] = Ψ(x),

(1.34)

and the expectation value of Ψ(x) over the ground state does not vanish, 0|Ψ|0 = 0,

(1.35)

that is to say, if the ground state satisfying relation (1.33) does not vanish, we can expect the appearance of a boson Ψ(x), whose mass is zero. This boson is called a Goldstone boson, and the symmetry breaking takes place

page 8

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

9

in the system. This is what the Goldstone theorem insists. The details are referred to the standard book of the ﬁeld theory [8]. Now we apply this theorem to the superconductivity. The invariant charge is (x)φ (x) = d3 xφ+ (x)σ 3 φ(x). (1.36) Q = d3 xφ+ α α In terms of the Nambu spinor, here σ 3 is crucial. In commutator (2.43), we seek for the spin operators which do not commute with σ 3 and ﬁnd, say, σ ± . We then have the Goldstone commutator as d3 x [φ+ (x )σ 3 φ(x ), φ+ (x)σ ± φ(x)]t=t =

d3 x(±2)0|φ+ (x)σ ± φ(x )|0δ(r − r ).

In details,

+

+

φ (x)σ φ(x) =

(φ+ ↑ (x)

φ↓ (x))

0

φ↑ (x) 1

0

0

+ = φ+ ↑ (x)φ↓ (x)

φ+ ↓ (x)

(1.37)

, (1.38)

φ+ (x)σ − φ(x) = φ↑ (x)φ↓ (x). Notice that here the same symbol φ is used for the ordinary ﬁeld with spin and the Nambu spinor. The aboves are nothing but the Cooper pairs, and we now ﬁnd the Goldstone bosons Ψ∗ , Ψ. In the literature, it is noted that 0|φ+ (x)σ ± φ(x)|0 = ±

Δ± = 0, g

(1.39)

where Δ and g are the gap and the coupling parameter, respectively. We expect the estimate Δ+ ∼ Δ− = Δ to be reasonable. The Cooper pairs are now the Goldstone bosons. A comment about the Goldstone boson or the massless elementary excitation with k = 0 is required. Using Eq. (1.33), we write the the Goldstone commutator (1.34) as (1.40) d3 y[0|j0 (y)|nn|φ (x)|0 − 0|φ (x)|nn|j0 (y)|0]x0 =y0 = 0, where |n is the intermediate state, and x0 = y0 implies that this is the equal time commutator.

page 9

March 24, 2021

10

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

Since j0 (y) = e−ipy j0 (0)eipy ,

(1.41)

it is seen that d3 y[0|J0 (0)|nn|φ (x)|0eipn y −0|φ (x)|nn|J0 (0)|0e−ipn y ]x0 =y0 ,

( p|n = pn |n)

= δ(pn )[0|J0 (0)|nn|φ (0)|0eipn0 y −0|φ (x)|nn|J0 (0)|0e−ipn0 y ]x0 =y0 ] = δ(pn )[0|J0 (0)|nn|φ (0)|0eiMn y0 −0|φ (0)|nn|J0 (0)|0e−iMn y0 ]x0 =y0 ] = 0.

(1.42)

In order to obtain the ﬁrst equality, the spatial integration is carried out. Then considering pμ = (p, M ), we retain the fourth component. In the last equation, when Mn = 0, cancellations will arise for the summation over n. We thus obtain, only for Mn = 0, the ﬁnite result 0|j0 (0)|nn|φ (0)|0 − 0|φ (0)|nn|j0 (0)|0 = Im0|j0 (0)|nn|φ (x)|0,

(1.43)

which is met with requirement (1.34). The excitation with Mn = 0 needs no excitation energy, suggesting the Goldstone boson. We further note that the mass-zero excitation is the imaginary quantity. This suggests the current be the phase current, as is seen in the Josephson eﬀect. Before closing the preliminary discussion, we want to make a few remarks. At the beginning, we have mentioned the London’s postulate that the superconducting state is characterized by a statement that the wave function is rigid, so that the current is entirely the diamagnetic current due to only the vector potential A. “Rigid” is not really rigid, but it is understood that the spatial derivative is vanishing, or the current ﬂows along the entirely ﬂat path which is described as, in a textbook, the path going around the the top of a Mexican hat. Boldly speaking, the electron in the superconducting state is massless. Also we have pointed out that the vector potential A, which leads to the Meissner eﬀect, satisﬁes the covariant

page 10

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

11

relation (1.6) ∂μ Aμ = −k2

(1.44)

so that a photon is massive in the superconductor. In the following chapters, we develop the substantial microscopic explanation of the above assertions.

1.3. Propagator In the previous section, we have found that, as is seen in Eq. (1.41), the superconducting state strongly concerns with the gap function or the anomalous Green’s function. We want to deal with the solid-state substances. However, the inﬁnite crystals described by the single band are already fully investigated in the literature, and the recent investigations are carried on objects with multiband structure [14, 15]. The inﬁnite system with many bands is constructed from the unit cell which is really a chemical molecule. The atoms in this molecule give the band index of the real crystal. In this respect, we investigate ﬁrstly the Green’s function of a unit cell. The Green’s function is now presented in the site representation. Corresponding to spinors (1.24), we deﬁne the spinor in the site representation as ar↑ ¯r = (a+ (1.45) , a ar = r↑ −ar↓ ). a+ r↓ Due to this deﬁnition, it is unnecessary to insert σ 3 in the matrix G, as is seen in the Schrieﬀer’s book [3]. The commutator is [ar↑ , a+ ] [a , a ] + + s↓ r↑ s↑ ¯s ]+ = [ar , a + + [a+ , a r↓ s↑ ]+ [as↓ , ar↓ ]+ δrs 0 (1.46) = δrs 12×2 . = 0 δrs The matrix propagator is deﬁned by ¯s (τ2 ) Grs (τ ) = −ar (τ1 ), a ar↑ (τ1 ), a+ s↑ (τ2 ) =− + ar↓ (τ1 ), a+ s↑ (τ2 )

−ar↑ (τ1 ), as↓ (τ2 )

−a+ r↓ (τ1 ), as↓ (τ2 )

as (τ2 ) + θ(τ2 − τ1 )¯ as (τ2 )ar (τ1 ), (1.47) = −θ(τ1 − τ2 )ar (τ1 )¯

page 11

March 24, 2021

12

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

where τ is the imaginary time, so that the propagator is the temperature Green’s function or the Matsubara function. In what follows, we put τ = τ1 − τ2 ,

(1.48)

and the system depends on (τ1 − τ2 ). If we want to obtain the gap function, we consider + Tr(σ + Grs (τ )) = a+ r↓ (τ1 ), as↑ (τ2 ),

(1.49)

and the standard procedure will be followed.

1.3.1. Hamiltonian Various Hamiltonians can be written by using the charge density matrix, ρr↑s↑ (x) ρr↑s↓ (x) ρrs (x) = ρr↓s↑ (x) ρr↓s↓ (x) = σ μ ρμrs ,

(1.50)

where the basis orbitals are put to be real, so that we not need the conjugation procedure for ﬁeld operators. The H¨ uckel Hamiltonian or the single-particle Hamiltonian has the structure ¯ r σ μ ar , H 0 = hμrs a

(1.51)

where h includes the chemical potential and can be explicitly written as ρr↑s↑ (x) ρr↑s↓ (x) hrs = ρrs h(x) = dxh(x) ρr↓s↑ (x) ρr↓s↓ (x) = σ μ hμrs .

(1.52)

Hereafter, we accept the summation convention that repeated indices imply the summation is carried out to facilitate manipulations. Other two-particle Hamiltonians are given in a similar way. Noting that μν (1.53) vrs;tu = dxdx ρμrs (x)v(x − x )ρνtu (x ), we have [18] 1 ab ar σ a as )vrs;tu (¯ at σ b au ), (a, b =↑, ↓) H dir = (¯ 2 1 aa ar σ a as )vrs;ut (¯ at σ a au ), (a =↑, ↓) H ex = − (¯ 2

page 12

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

1 +− −+ ar σ + as )vrs;tu H super = {(¯ (¯ at σ − au ) + (¯ ar σ − as )vrs;tu (¯ at σ + au )}. 2

13

(1.54)

For the direct interaction, the quantum mechanical Hamiltonian is dir H = dxdx χ∗r↑ (r)χs↑ (r)(x)v(x − x )χ∗↓ (x )χ∗u↓ (x ). For the ﬁeld theoretical Hamiltonian, the wave functions are replaced by the creation–annihilation operators a+ r↑ , ar↑ , and so on. These are written in the spinor notation, for example, as 1 as↑ + a+ 1 0 r↑ as↑ = ar↑ ar↓ a+ 0 s↓ 1 0 ↑ as = a+ = a+ r r σ as . 0 0 Note that H ex is obtained by reversing indices (u ↔ t) in vrs;tu .

1.4. Non-interacting ‘Non-interacting’ implies that the Hamiltonian is bilinear with respective to operators so that the diagonalization is always possible. It should be instructive to begin with the single-particle case, since even if we manipulate the complicated two-particle case, the procedures are almost the same when the mean-ﬁeld approximation is employed. The energy for Hamiltonian (1.52) is ρH 0 ) = hrs ¯ ar as , E 0 = Tr(ˆ

(1.55)

where ρˆ is the statistical operator, ρˆ = eβ(H

0 −Ω)

,

(1.56)

with the normalization factor Ω. We now deﬁne the temperature Green’s function, in which τ is the imaginary time, τ = it, [16, 17], + ρ (θ(τ1 )ar (τ1 )a+ Grs (τ ) = −Trˆ s (τ2 ) − θ(−τ )as (τ2 )ar (τ1 ) = ar (τ1 )a+ s (τ2 ),

(1.57)

where τ = τ1 − τ2 ,

(1.58)

page 13

March 24, 2021

14

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

and it is assumed that the system is only dependent of the relative time τ . Then we can written E 0 in terms of the temperature Green’s function, E 0 = Tr[hrs Gsr (τ = 0− )].

(1.59)

Note that hrs and Gsr are matrices. The equation of motion (1.57) for the non-interacting Hamiltonian (1.51) can be read as ¯r (τ2 )]+ ar (τ2 ) = δ(τ1 − τ2 )[as (τ1 ), a ∂τ1 as (τ1 )¯ ¯s ar hs r (τ1 )]− , a ¯r (τ2 ) +[as (τ1 ), a ¯r (τ2 ) = δ(τ1 − τ2 )δsr + δss hr s (τ1 )ar (τ1 ), a ¯r (τ2 ). = δ(τ1 − τ2 )δsr + {hsr }ar (τ1 ), a

(1.60)

The equation of motion can be solved by the Fourier transformation [16] ar (τ2 ) = as (τ1 )¯

1 iωn τ ¯r ; ωn e as a β n

(1.61)

with ωn = (2n + 1)π/β,

(1.62)

where the odd number indicates that particles are fermions. Then Eq. (1.50) becomes ¯r ; ωn = δsr . (iωn δsr − hsr )ar a

(1.63)

At this step, the matrix structure of the above should be carefully investigated. Let us assume the single-particle Hamiltonian is spin-diagonal, ↑ hsr 0 . (1.64) hsr = 0 h↓sr It is preferable to introduce the ﬂame diagonalizing each element: h↑sr = (s|ii|h|i|iir) ↑ = s|i↑ i↑ i|r↑ . Then we have ¯ r = as a

1 1 ⎛ ↑ (s|ii|r) β n ⎝ iωn −i↑ 0

⎞ 0 (s|ii|r)↓ iωn −i↓

⎠

(1.65)

page 14

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

⎛ (s|ii|r)↑ 1 ⎝ iωn −i↑ = β n 0

=

15

⎞ 0 (s|ii|r)↓ iωn −i↓

⎠

(s|in(i )i|r)↑

0

0

(s|in(i )i|r)↓

,

(1.66)

where n(i↑ ) =

1 1+

ei↑ /kB T

.

(1.67)

Another sophisticated way starts from the decomposed Hamiltonian ¯r σ μ hμrs as . H0 = a

(1.68)

The commutator is evaluated as ¯r σ μ hμr s as ] = δsr σ 0 σ μ hμr s as = σ μ hμss as . [as , a

(1.69)

The equation of motion ¯r ; ωn = σ 0 δsr . (iωn δss − σ μ hμss )as , a

(1.70)

In the matrix notation, ¯; ωn = σ 0 (iωn − σ μ hμ )a, a or ¯; ωn = a, a

σ0 . iωn − σ μ hμ

(1.71)

In the representation where h is diagonal, r|h|s = r|ii|h|ii|s = i r|ii|s,

(1.72)

relation (1.71) becomes ¯; ωn = a, a

(|ii|)(iωn + σ μ μi ) (iωn − σ μ μi )(iωn + σ μ μi )

(|ii|)(iωn + σ μ μi ) . = (iωn )2 − (μi )2

(1.73)

page 15

March 24, 2021

20:13

16

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

Now σ μ μi iωn + σ μ μi iωn = + (iωn )2 − (μi )2 (iωn )2 − (μi )2 (iωn )2 − (μi )2 1 1 1 1 1 σμ = + − + 2 iωn − μi iωn + μi 2 iωn − μi iωn + μi 1 1 1 (summing ωn ) + = 2 iωn + μi iωn + μi →

σμ 1 (n(μi ) + n(−μi )) + (n(μi ) − n(−μi )) . 2 2

(1.74)

We evaluate

σμ σ0 G↑rs = Trσ ↑ < r|i >< i|s > (n(μi ) + n(−μi )) + (n(μi − n(−μi )) 2 2 = r|ii|s]↑ n(↑i ).

(1.75)

We then have 1 r|ii|s 1 ↑ − Grs (0 ) = = r|in(↑i )i|s. β n β n iωn − ↑i

(1.76)

This relation holds for both ↑ and ↑, and we recover result (1.66). By the way, we give the energy expression for Eq. (1.51): E 0 = Tr(hrs Gsr ) ↑ s|in(↑i )i|r hrs 0 = Tr 0 h↓rs 0

0 s|in(↓i )i|r

.

(1.77)

It may be needless to present another illustration: E 0 = Tr(hrs Gsr ) = Tr(σ μ hμrs )(σ ν Gνsr ).

(1.78)

The result is meaningful if σ μ σ ν = σ 0 , which leads to, in the present case, σ μ = σ ν = σ ↑ , or σ μ = σ ν = σ ↓ . Such manipulations will be used in the later investigation.

1.5. Interacting In this chapter, the electron-electron interactions are taken into account, and we will discuss how these interactions lead to the superconducting state. The

page 16

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

17

Hamiltonians given in Eq. (1.54) are 1 ab ar σ a as )vrs;tu H dir = (¯ (¯ at σ b au ), (a, b = ↑, ↓) 2 1 aa ar σ a as )vrs;ut (¯ at σ a au ), (a = ↑, ↓) H ex = − (¯ 2 1 +− ¯ −+ ar σ + as )vrs;tu ar σ − as )vrs;tu (¯ at σ + au )}. (at σ − au ) + (¯ H sup = {(¯ 2 These are written in the mean-ﬁeld approximation. The estimate beyond this approximation is not the case of the present consideration. We have ¯ r σ a ar H 0 = hars a

(a = ↑, ↓)

ab a:dir ar σ a as )vrs;tu ¯ at σ b au = (¯ ar σ a as )Drs H dir = (¯ aa a:ex ar σ a as )vrs;ut ¯ at σ b au = (¯ ar σ a as )Drs H ex = −(¯

(a, b = ↑, ↓) (a = ↑, ↓)

+− −+ ar σ + as )vrs;ut ¯ at σ − au + (¯ ar σ − as )vrs;ut ¯ at σ + au H sup = (¯ −:sup +:sup ¯r σ − as )Drs +a , = (¯ ar σ + as )Drs

(1.79)

where a:dir ab = vrs;tu ¯ at σ b au , Drs a:ex ab = −vrs;ut ¯ at σ b au δab , Drs +:sup +− = vrs;tu ¯ at σ − au , Drs

(1.80)

where · · · implies the ground-state average, which is actually obtained with wave functions in the previous step during the SCF calculations. These Hamiltonians are classiﬁed into two kinds called modes, the normal many-electron problem and that for the superconductivity: H = H norm + H sup ,

(1.81)

where a:dir a:ex ar σ a as )(hars δrs + Drs + Drs ), H norm = (¯ ∓:sup ¯r σ ± as Drs . H sup = a

(1.82)

The main diﬀerence between two is that, in the former, we have the singleparticle Hamiltonian, while in the latter not. Various Drs are complicated, but they are merely the c-numbers in this treatment. The propagator in

page 17

March 24, 2021

18

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

question in Eq. (1.57) is presented here again: + Grs (τ ) = −Trˆ ρ (θ(τ )ar (τ1 )a+ s (τ2 ) − θ(−τ )as (τ2 )ar (τ1 ) = ar (τ1 )a+ s (τ2 ). The equation of motion can be read as ¯r (τ2 )]+ ∂τ1 as (τ1 )¯ ar (τ2 ) = δ(τ1 − τ2 )[as (τ1 ), a ¯s ar Hsa r (τ1 )]− , a ¯r (τ2 ) +[as (τ1 ), a a a ¯r (τ2 ). (1.83) (a; norm, sup) = δ(τ1 − τ2 )δsr + Dsr σ ar (τ1 ), a

Making the Fourier transformation with respect to τ = τ2 − τ2 gives a a (iωn − Drs σ )Gs r = δsr

(1.84)

or, in the matrix form, G(ωn ) =

1 iωn + D a σ a = . iωn − D a σ a (iωn )2 − (D a )2

(1.85)

Note that D a consists of the single-electron part and the two-electron interaction term which involves another mate ρatu combined with the propagator ¯ at σ a au : a a (1.86) D (x) = h (x) + dx v(x − x )ρbtu (x )σ b a¯t at . However, the mean-ﬁeld approximation makes this as if it were the singleelectron interaction. A few comments will be given about the matrix character of G. This is a big matrix with site indices, and each element is a 2 × 2 matrix in the spin space. The index a characterizes the mode of the mean-ﬁeld potential. Every mode is independent of each other and is individually diagonalized. We now introduce a ﬂame, in which these are diagonal, ia |D a |ia = ηia .

(1.87)

Look at the right-hand side of Eq. (1.85) and remember the Einstein convention that repeated indices imply summation, (D a )2 = (η ↑ )2 + (η ↓ )2 + (η + )2 + (η − )2 = (η norm )2 + (η sup )2 ,

(1.88)

page 18

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

19

where the second line is in a simple notation. Then we have |ia (iωn + ia |D a |ia σ a )ia | {iωn − (ηinorm + ηisup )}{iωn + (ηinorm + ηisup )} 1 1 a 1 + ia | = |i 2 iωn − (ηinorm + ηisup ) iωn + (ηinorm + ηisup )

G(ωn ) =

+|ia ×

Diia σ a 2(ηinorm + ηisup ) 1

iωn − (ηinorm + ηisup )

−

1

ia |.

iωn − (ηinorm + ηisup )

Taking the (r, s)-matrix elements and the mode c which is achieved by the operation, Tr σ c Grs = Gc rs

(1.89)

we select the terms on the right-hand side with the mode c satisfying Tr σ c σ a = 1.

(1.90)

Otherwise, the Tr operation leads to the vanishing result. Carrying out the summation over ωn , we get 1 c G (ωn ) β n rs 1 1 1 c a 1 + r |i = β n 2 iωn − (ηinorm + ηisup ) iωn + (ηinorm + ηisup )

Gcrs (0− ) = [2mm]

× ia |sc + ×

1 c a Diia r |i norm β n 2(ηi + ηisup ) 1

iωn − (ηinorm + ηisup )

−

1 iωn + (ηinorm + ηisup )

ia |sc

1 = r c |ia (n(ηinorm + ηisup ) + n(−ηinorm − ηisup ))ia |sc 2 Diia +r c |ia 2(ηinorm + ηisup ) × (n(ηinorm + ηisup ) − n(−ηinorm − ηisup )) ia |sc Diia 1 tanh(ηi /2kB T )ia |sc , = δrs − r c |ia 2 2(ηinorm + ηisup )

(1.91)

page 19

March 24, 2021

20:13

20

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

where n(ηia ) =

1

(1.92)

a

1 + eηi /kBT

and n(η) + n(−η) = 1, n(η) − n(−η) = −tanh

η 2kB T

.

In the estimation of matrix elements, the chemical potential which was disregarded up to now is taken into account. Namely, the Hamiltonian has an additive term −μ¯ ar ar which causes ηia → ηia − μ < 0, while − ηia → −(ηia − μ) > 0. The mean-ﬁeld potentials are carefully treated. In modes with ↑ and ↓, we have the non-vanishing single particle parts, h↑rs δrs and h↓rs δrs which are usually negative. However, for superconducting modes, h± rs = 0, and the chemical potential is lost for the same reason. The latter may be closely related to the fact that the number of particles is not conserved in a superconductor. These circumstances are crucial for the superconducting mode.

1.5.1. Unrestricted HF Let us review the SCF (self-consistent ﬁeld) procedure. We now discuss the ordinary many-electron system. As an example, the propagator with the up spin, Eq. (1.89), is G↑rs (0− ) =

1 ↑ ↑ Diia tanh(ηia /2kB T )ia |s↑ , (1.93) r |s − r ↑ |ia 2 2(ηinorm + ηisup )

where r ↑ |s↑ is the overlap integral between sites r and s and approximately vanishes, and ↑a ↑↑ Gatu − vii;tu G↑tu . Diia = h↑ii + vii;tu

(a :↑, ↓)

(1.94)

Note that tanh(ηia /2kB T ) < 0, since ηia < 0.

(1.95)

page 20

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

Look at the potential of the mode ↑, D ↑ (x) = h↑ (x) + dx v(x − x )ρbtu (x )σ b a¯t at .

21

(1.96)

In this case, there is h↑ (x), whose matrix element should be negative, so that even if the matrix elements of the second terms are positive, the (r, s) matrix element of D ↑ (x) is probably negative. This is usually the cases in atoms, molecules, and solids. In evaluating D ↑ (x), the propagators (wave functions) of all other modes are required. In this respect, Eq. (1.93) is the self-consistent relation between propagators. Usually, the self-consistent relation between wave functions is given in a such a way that, at beginning, the total energy is given by the potentials given in terms of tentatively approximated wave functions, and the new approximate wave functions in the next step are obtained by optimizing the total energy. This procedure is lacking in the present consideration.

1.5.2. Gap equation for superconductivity In the case of superconductivity, since σ + (σ − ) is traceless, the ﬁrst term of Eq. (1.91) vanishes, and also h+ = 0. Now Eq. (1.91) can be read as +− −) ¯ v a a t u ii;tu − + + i+ |s+ tanh(ηi+ /2kB T ). G+ rs (0 ) = − r |i 2(ηinorm + ηisup ) +− − v G tu ii;tu i+ |s+ tanh(ηi+ /2kB T ). (1.97) = − r + |i+ 2(ηinorm + ηisup ) − This complicated equation gives the relation between G+ rs and Grs both referring to the superconductivity and is called the gap equation. A few points should be presented. While selecting the superconducting mode, it is used that 0 1 0 0 1 0 + − = Tr = 1, (1.98) Tr(σ σ ) = Tr 0 0 1 0 0 0

so that +− . Tr(σ + v +a σ a ) = vii;tu

Relation (1.97) yields − r + |i+

+− vii;tu

2(ηinorm + ηisup )

(1.99)

i+ |s+

> 0.

(1.100)

page 21

March 24, 2021

20:13

22

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

As has been mentioned previously, we have no chemical potential in the +− is. Therefore, it superconducting state, so that ηi+ is positive, as same as vii;tu + + + + is required that r |i i |s be negative in order that Eq. (1.100) be hold. This is really possible, as will be mentioned below. Thus, we have nothing to do with the electron–phonon coupling. Let us perform the successive approximations as r |i

+ +

+− + + vii;tu i |s tanh(ηi+ /2kB T )

occ +− + + ≈ r + |i+ vii;tu i |s

(T → 0)

i +− ( 0,

δ/t 1),

(1.105)

and then the Hamiltonian is easily diagonalized as k = ±[t2 (1 + cos k) + δ2 (1 − cos k)]1/2 ,

(1.106)

where + and – correspond to the conduction and valence bands, respectively. We are interested in the features at the zone boundary, k = π, cπ = 2δ,

vπ = −2δ.

(1.107)

Here, the superscripts c and v indicate the conduction and valence bands, respectively. When δ = 0, certainly we have the gap, and if δ = 0, both bands continuously join to a single band called the half-ﬁlled band,

page 23

March 24, 2021

24

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

Next, we turn to the polyacene, whose unit cell is the butadiene molecule. In this case, we obtain four bands 1 ck = [t3 + (t23 + 4|t˜k |2 )1/2 ] = −vk , 2 1 ck = [−t3 + (t23 + 4|t˜k |2 )1/2 ] = −vk , 2

(1.108)

where t˜k = t1 + t2 eik .

(1.109)

The usual pairing property in alternant hydrocarbons is also seen in this case. Employing parameterization (1.105) gives, at k = π, vπ =

1 [t3 + (t23 + 16δ2 )1/2 ] ≈ 4t3 (δ/t1 )2 . 2

(1.110)

When δ = 0 (without bond alternation), we have vk =

1 {t3 − [t23 + 8t2 (1 + cos k)]1/2 }. 2

(1.111)

Consider single-particle states. If δ = 0 and k = π, we have, from Eq. (1.109), t˜ = 0, so that the amplitudes at sites 2 and 5 vanish. Therefore, when δ = 0, we get, at k = π, 1 − a+ |ψkv = (a+ 4k )|0, 2 1k 1 + a+ |ψkc = (a+ 4k )|0. 2 1k

(1.112)

It is seen that |ψkv is antisymmetric about the C2v symmetry axis, and |ψkv is symmetric. Thus, v and c bands are not continuous at k = π.

1.6.2. Deformation energy For these systems, let us study whether the bond alternation is energetically favorable or not. We assume that the energy gain due to the bond alternation mainly contributes to the highest valence band energy, vk . The case of polyacetylene. The energy gain ΔE is

2π

ΔE = 0

dk v ( − vk (0)), 2π k

(1.113)

page 24

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

25

where the second term refers to the case without bond alternation (δ = 0). In Eq. (1.106), we shift the integration origin from 0 to π, then approximating cos k = cos(π + p) ≈ −1 + p2 /2. For small p, we obtain

! dk (tp)2 + 4δ2 − tp 2π 0 2 δ 2t δ , ( ),

(1.154)

(E < ),

we rewrite Eq. (1.151) for ω as ∞ 2 1 1+ T1 ∼ |B|2 N 2 (0) E(E + ω)

2 ×

E(E + ω)kB T (−∂n/∂E)dE , (E 2 − 2 )1/2 [(E + ω)2 − 2 ]1/2

(1.155)

where the coupling constant and the state density are replaced by their suitable averages. This integral is divergent. Therefore, T1 of a superconductor is strongly enhanced just below the critical temperature. This phenomenon was observed and explained by Slichter et al. [25, 26]. This was told one of the brilliant victories of the BCS theory. However, it is found that, in the recent experiments of the high-temperature superconductors or the copperoxide superconductors, the T1 enhancement is lost. This phenomenon is considered deeply connected with the mechanism of the high-temperature superconductivity of these species and attracted the interests of many

page 34

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

35

investigators [28, 30]. However, so long as we know, the theory of magnetic resonance of a superconductor has been done almost all in the scheme mentioned in this introduction. Then it will be preferable to develop the theory of magnetic resonance in accordance with the sophisticated recent theory of superconductivity.

1.7.3. Theory with Green’s function Our idea is as follows: the algebra of electrons is related to their ﬁeld operators. In the same way, we assume the ﬁeld for nuclei. For example, the creation operator for a nucleus a+ KM yields the nuclear motion with K and M which are spatial and spin quantum numbers, respectively. The energy spectrum of the propagator GKM (τ ) = aKM (τ )a+ KM gives the line shape of the magnetic resonance. The nuclear propagator GKM (τ ) sees the electron sea, followed by the electron excitation in the spin space. This gives the additional line width of the nuclear magnetic resonance. The phenomenon looks like the vacuum polarization in quantum electrodynamics. The self-energy part thus arisen in the nuclear energy is the source of the line shape of the nuclear magnetic resonance [24]. The spin-lattice relaxation time of the nuclear spin I z is given by the imaginary part of the magnetic susceptibility χzz which is equal to (χ+− + χ−+ )/2 in the spatially homogeneous system. Here, ± correspond to (I x ± iI y )/2, respectively. The ensemble average of a change, δI + (t), is given by the linear response theory as t + dt Tr{ρG [H ex (t ), I + (t)]− }, (1.156) δI (t) = i −∞

where ρG is the grand canonical statistical operator. However, the chemical potential is not given explicitly, otherwise stated. The rotating magnetic ﬁeld causing the magnetic transition is, assuming a single mode for simplicity, H ex (t) = HR (I + (t)eiωt + I − (t)e−iωt ).

(1.157)

As has been said, the spin-lattice relaxation arises from the interaction between the nuclear spin and the electron spin. In other words, the electron spins play the role of a lattice system. H = γgβB F (R, r)I · S,

(1.158)

where F (R, r) is a function of spatial coordinates of the nucleus R and that of the electron, r. The term γ is the gyromagnetic ratio of the

page 35

March 24, 2021

36

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

nucleus, and g and βB are the g-factor and the Bohr magneton of electron, respectively. Now the second quantization of the aboves are carried out. First of all, the orthonormalized wave function describing the nuclear behavior, |ξK (R)M , is introduced as (HN + HM )|ξK (R)M = (K + M )|ξK (R), M = KM |ξK (R, )M

(1.159)

with KM = K + M, where HN is the spatial part, and HM is the Zeeman part. Then we have I α → ξK (R)M |I α |ξK (R)M a+ KM aK M = M |I α |M a+ KM aK M δKK .

(1.160)

The similar equation is given for electrons (HS + Hm )φk (r)|m = (k + m)|φk (r), m = km |φk (r), m,

(1.161)

where km = k + m, so that H → hγgβB M |I β |M m|S α |m + × ξK (R)φk (r)|F (R, r)|ξK (R)φk (r)(a+ KM aK M )(ckm ck m ).

(1.162) If the nuclear motion is assumed as that of a harmonic oscillator, a+ KM and aKM are the creation and annihilation operators of vibrational excitations. When the nuclei carry a non-integer spins, these are considered to obey the Fermi statistics or satisfy the anticommutation relation [a+ KM , aK M ]+ = δKK δM M .

(1.163)

However, as will be seen in the following, this selection of the statistics is not fatal for the theory. It is needless to say that the operators for electrons satisfy the anticommutation relations.

page 36

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

37

The change of I + in Eq. (1.156) can be written, in the interaction representation, as (we retain the I − term in Eq. (1.157))

t

+

δI (t) = iγHR

−∞

dt e−iωt

×Tr{ρG M − 1|I − |M M |I + |M − 1 + ×[a+ K,M −1 (t )aK,M (t ), aK,M (t)aK,M −1 (t)]− } t dt e−iωt DK,M −1,M (t − t) = −γHR −∞

1 = − γHR e−iωt 2

∞

−∞

dse−iωs

DK,M −1,M (s)

KM

1 = − γHR e−iωt DK,M −1,M (ω). 2

(1.164)

From this result, the magnetic susceptibility of the present system is γ χ+− (ω) = − DK,M −1,M (ω). 2

(1.165)

In the course of derivation, the matrix elements of spin operators are put to be equal to 1, and then the T r operation is carried out. Here, DK,M −1,M (s) is a retarded Green’s function, % & + DK,M −1,M (s) = −iθ(s)Tr ρG [a+ KM −1 (s)aKM (s), aKM aKM −1 ]− , (1.166) and DK,M −1,M (ω) is its Fourier transform. Now our problem is to estimate this retarded function. The retarded Green’s function is easily obtained by the analytical continuation from the Matsubara function (or the temperature Green’s function with imaginary time τ ) which is causal in τ , + DK,M −1,M (τ ) = −Tr{ρG T τ [a+ K,M −1 (τ )aK,M (τ )aK,M aK,M −1 ]},

(1.167)

for which the Feynman diagram analysis is available [16].

1.7.4. Non-interacting Here, we deal with the case without the spin-lattice interaction. It might be trivial; however, it seems instructive for the later investigation. By the use of the simpliﬁed notation, · · · = Tr(ρG · · · ), the Green’s function in this

page 37

March 24, 2021

38

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

case is written as + + 0 DK,M −1,M (τ ) = T τ [aKM −1 (τ )aK,M (τ )aKM aKM −1 ] 0 0 (τ )GKM = GKM −1 (−τ ),

(1.168)

where 0 (τ ) = −T τ [aKM (τ )a+ GKM KM ],

(1.169)

and the corresponding Fourier transform of Eq. (1.168) is 0 DK,M −1,M (ωn ) =

1 0 0 GKM (νn )GKM −1 (νn − ωn ), β ν

(1.170)

1 . iνn − KM

(1.171)

n

where 0 (νn ) = GKM

Therefore, 1 1 1 · β ν iνn − iωn − KM −1 iνn − KM n 1 1 1 = − β ν iνn − iωn − KM −1 iνn − KM

0 DK,M −1,M (ωn ) =

n

×

1 iωn + KM −1 − KM

= [n(KM −1 ) − n(KM )]

1 , iωn − KI

(1.172)

where KI = KM − KM −1 and it is noted that ωn is even, it does not matter in obtaining the particle number. The retarded Green’s function is obtained simply by replacing iωn by ω + iη (η is a positive inﬁnitesimal). Thus, we obtain δI + (t) = e−iωt HR (n (K− ) − n(K+ ))

1 ω − KI + iη

,

(1.173)

page 38

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

39

where the radio frequency arousing the resonance is rewritten by ω 0 . The magnetic susceptibility χ+− thus becomes χ+− (ω) = γ(n(K− ) − n(K+ ))

1 , ω − KI + iη

γ = e−iωt HR ,

(1.174)

whose imaginary part is χ+− (ω) = −πγ(n(K− ) − n(K+ ))δ(ω − KI ).

(1.175)

This gives the sharp δ-function type energy spectrum. We have no line width or the relaxation time, and states are stationary.

1.7.5. Interacting; normal In the interacting system, G 0 in Eq. (1.168) has to be replaced by G including the interaction which, in the present case, is the spin–spin interaction between nuclei and electrons, as has been given in Eq. (1.156), DKM −1,M (ωn ) =

1 GKM (νn )GKM −1 (νn − ωn ), β ν

(1.176)

n

where, for instance, 0 (νn ))−1 − ΣKM (ω)]−1 , GKM (νn ) = [(GKM

(1.177)

where ω is the interaction energy. Our procedure is going on as follows. The two Green’s functions with the self-energy part are evaluated. Combining these gives the retarded Green’s function D to estimate the magnetic susceptibility. The most important (divergent) self-energy part of this self-energy is due to the ring diagram shown in Fig. 1.2. The problem is to examine how the

Fig. 1.2.

Self-energy part G(νn ).

page 39

March 24, 2021

40

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

energy of the nucleus propagator (two-dot-interrupted line) is changed by the ring diagram of the electron (full line). That is to say, G(νn )−1 = G(νn )0 + Σ(ω), Σ(ω) = −|K|2 S(ρn )S(ρn + ω),

(1.178)

where S is the electron propagator, and the minus sign is due to the fermion loop. The self-energy part includes the coupling terms, where |K|2 = M |I + |M − 1m − 1|S − |m|2 × |χK (R)φk (r)|F (R, r)|φk (r)χK (R)|2

(1.179)

and the minus sign is due to a Fermion loop. The ring diagram is calculated as follows: 1 1 · Skm (ρn )Skm−1 (ρn + ω) = iρn − km iρn + ω − km+1 ρn 1 1 = − iρn − km iρn + ω − km+1 ρ n

×

1 ω − km+1 + km

= (n(km ) − n(km+1 ))

1 ω − km+1 + km

. (1.180)

The lattice (electron) gets ω from a nucleus to lift the electron spin from m to m + 1, and, at the other vertex, the inverse process occurs. This looks like the radiation process in the photochemistry. We thus have the self-energy part of GK;M −1,M , ΣK;M −1,M (νn ) = |K|2 (n(km ) − n(km+1 ))

1 , ω − ks

(1.181)

where ks = km+1 − km . Another propagator GK;M has the self-energy part ΣK;M,M −1 (νn ). This is built by replacing ρn + ω by ρn − ω in Fig. 1.2: ΣK;M,M −1(νn ) = |K|2 (n(km ) − n(km−1 ))

1 ω − km−1 + km

1 ω − ks 1 ≈ |K|2 (n(km+1 ) − n(km )) . ω − ks = |K|2 (n(km ) − n(km−1 ))

(1.182)

page 40

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

41

We now turn to the evaluation of the propagator DK;M −1,M (τ ), DK;M −1,M (ωn ) 1 GKM (νn )GKM −1 (νn − ωn ) = β ν n

1 (iνn − KM − ΣKM − )−1 (iνn − iωn − KM −1 − ΣK;M,M −1)−1 = β ν n 1 1 1 = − β ν iνn − iωn − KM −1 − ΣKM −1 iνn − KM − ΣKM n 1 × iωn − KM −1 − ΣKM −1 + KM + ΣKM 1 . (1.183) = (N (KM ) − N (KM −1 )) iωn − KI + ΣKM − ΣKM −1 Here, KI = KM − KM −1 , and the self-energy parts are disregarded in obtaining the particle density. We can observe that the additional terms in the denominator modify the line shape. If we put iωn → ω + iη, we can obtain the retarded Green’s function, whose imaginary part gives the line shape: 1 D(ω) ∼ ω + iη − KI + ΣKM − ΣKM −1 1 − iπδ(ω − KI + ΣKM − ΣKM −1 ) = P ω − −ΣKM −1KI =

i(Im) (Re)2 + (Im)2

(at the resonance point).

(1.184)

The line shape now changed from the δ-function type to the Lorentz type, as expected.

1.8. Interacting; Superconductor 1.8.1. The extended Nambu spinor We then investigate how the line shape obtained above is further modiﬁed in a superconductor. The electron propagators in the previous section are replaced by those in a superconductor. These have been studied already in Sec. 1.3 and are present here in a new fashion adequate for the following

page 41

March 24, 2021

42

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

investigation. As has been done by BCS, let us consider the attractive twobody potential g which is assumed constant for simplicity and further keep in mind the Cooper pair. The Hamiltonian 1 + + + (1.185) Hel = kα ckα ckα + gckα c−kβ c−kβ ckα , 2 where kα is the orbital energy, includes the Zeeman energy in the present case. Now we use the extended Nambu representation of Eq. (1.136), ⎛ ⎞ ckα ⎜ + ⎟ ⎜c−kβ ⎟ + ⎟ c−kβ c−kα c+ (1.186) c+ ck = ⎜ kβ ) k = (ckα ⎜c+ ⎟ , ⎝ −kα ⎠ ckβ with the equal time commutator, [ck , c+ k ]+ = 1δkk .

(1.187)

In these terms, the Hamiltonian is rewritten as 1 3 + + + − Hel = k c+ k Σ ck + 2 g(ck Σ ck )(ck Σ ck ), where k is the diagonal matrix of γ : ⎛ ⎞ kα ⎜ ⎟ ⎜ ⎟ −kβ ⎜ ⎟. k = ⎜ ⎟ −kα ⎝ ⎠ kβ Let us deﬁne 3 σ 0 , Σ3 = 0 −σ 3 with

σ3 =

Σ+ =

σ+

0

0

−σ −

1

0

0

−1

,

σ1 =

0 1 1 0

Σ− =

,

σ2 =

(1.189)

σ−

0

0

−σ +

,

(1.188)

0 i

−i 0

(1.190)

,

1 1 (1.191) σ + = (σ 1 + iσ 2 ), σ − = (σ 1 − iσ 2 ). 2 2 As for the electron–electron interaction, those for the Cooper pairs are only selected: namely Σ+ selects a Cooper pair in the particle state, while Σ− that in the hole state.

page 42

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

43

1.8.2. Green’s function Here, the discussions done in Sec. 1.4 are repeated brieﬂy. The above Hamiltonian is invariant under the scale transformation. Then we have a current conservation; especially the charge conservation in the static state (the Noether’s theorem). If we have any quantity which does not commute with this invariant charge, we can expect a phase transition (the Goldstone theorem). The charge proportional to 3 c = c+ (1.192) c+ kγ kγ k Σ ck k>0

is invariant under the rotation about the Σ3 axis in the space spanned by Σ3 , Σ+ , and Σ− . Observing that [Σ3 , Σ± ] = ±2Σ±

(1.193)

suggests the phase transitions along the Σ± directions. If we deﬁne c¯ = c+ Σ3 as has been done in Sec. 1.43, the discussions parallel to those there will be possible in the following. However, this is not employed in this case. The phase transition cannot be achieved by the perturbational approach, but the eﬀective Hamiltonian giving the phase transition should be included at the beginning. Say, the modiﬁed Hamiltonian 3 + − H 0 = c+ k (k Σ + ρΣ + ηΣ )ck , 1 + + + − + − {(ck Σ ck ) · (c+ H int = g k Σ ck ) − ck (ρΣ + ηΣ )ck }, (1.194) 2 kk

where ρ and η are the so-called gap energies which are assumed independent of k for simplicity. Note that the Hamiltonian H 0 is already symmetrybroken. Here, we adopt a conventional method. In what follows, H int is neglected, that is to say, we start from the Green’s function due to the eﬀective Hamiltonian and then take interaction (1.157) into account. At this stage, we may expect the result that will be obtained in such a manner that the normal and superconducting states contribute additively. The temperature Green’s function with the imaginary time τ is deﬁned as G0kk (τ ) = −Tτ [ck (τ )c+ k ],

(1.195)

page 43

March 24, 2021

44

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

where · · · = Tr{ρG · · · }. The equation of motion of G0kk is + ∂τ G0kk (τ ) = −∂τ [θ(τ )ck (τ )c+ k (0) − θ(−τ )ck (0)ck (τ )] + 0 = δ(τ )[ck (τ ), c+ k (0)]+ + T τ [ck (τ ), H ]− , ck (0)

= δkk + (k Σ3 + ρΣ+ + ηΣ− )G0kk .

(1.196)

In the course of the above derivation, the commutator in Eq. (6.65) was used. We make the Fourier transformation, 1 −iωn τ 0 e Gkk (ωn ), (1.197) G0kk (τ ) = β ω n

where β = kB T and kB is the Boltzmann constant. Then the equation of motion becomes (iωn + k Σ3 + ρΣ+ + ηΣ− )G0kk (ωn ) = δkk .

(1.198)

Namely, G0kk (ωn ) =

1 − ρΣ+ − ηΣ−

iωn − k iωn + k Σ3 + ρΣ+ + ηΣ− = δkk , (iωn )2 − Ek2 Σ3

(1.199)

where Ek2 = 2k + ρη.

(1.200)

1.8.3. Spin dynamics The propagator in Eq. (1.199) is the 4 × 4 matrix. If we ignore ρ and η, this is reduced to the normal propagator. We have already tried this simple case. Now we assume the terms responsible for the superconductivity as a perturbation. Namely (S is the electron propagator), S(νn ) = =

iνn + k Σ3 + ρΣ+ + ηΣ− (iνn )2 − Ek2 iνn + k Σ3 ρΣ+ + ηΣ− + + ··· . (iνn )2 + 2k (iνn )2 + 2k

(1.201)

It is helpful to separate this relation into components and to manipulate each one individually. Noticing σ0 + σ3 = σ↑ + σ↓ ,

page 44

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

45

we have, for example by operating σ ↑ followed by Tr, S ↑ (νn ) =

iνn + k Σ3 + ρΣ+ + ηΣ− (iνn )2 − Ek2

1 ρ+η + + ··· iνn − k↑ (iνn )2 + 2k ρ+η 1 1 1 + − + · · · . (1.202) = iνn − k↑ 2k↑ iνn − k↑ iνn + k↑ =

In order to get the self-energy part of the nuclear propagator, we have to evaluate 1 S(νn )S(νn + ω). (1.203) Σk;M −1,M (ω) = K 2 β ν n

The ﬁrst-order term is already evaluated in Eq. (1.180). Then we have to carry out the complicated manipulation due to the second term of the last line in Eq. (1.202). However, the combinations other than those satisfying the resonance condition ω ∼ ks (see Eq. (1.181)) should give a small eﬀect to be neglected. We then consider that the procedures of the previous section need not be repeated, and we are allowed to multiply the results there by the factor (ρ + η)/2k↑ as the perturbing correction or the superconducting eﬀect.

1.8.4. Conclusion If we review the present investigations from the viewpoints of the line shape problem in the magnetic resonance, three cases are clearly distinguished: In the non-interacting case, the line shape is written in terms of the delta function. In the interacting case of the normal phase, it is presented by the Lorentz-like function, and, in the superconducting phase, it is further multiplied by a coherent factor; whereas the statistical factors referring to the nuclear states never change throughout. For a superconductor, the present theory has almost nothing to give more than the current one has done. However, the theory is not merely to reproduce the experimental result, but to predict the mechanism hidden in observations, in such a way that the manipulations tell step-by-step what are working inside the matter. We might be satisﬁed with a little deeper understanding of the superconductivity. Among various opinions we give, as an example, Scalpino’s one [30]. He pointed out three possibilities that the T1 enhancement is lost in the copper oxide superconductor:

page 45

March 24, 2021

46

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

(1) The d-wave single particle density of states has a logarithmic singularities, rather than the square-root singularity for the s-wave gap. (2) The coherent factor for the quasiparticle scattering vanishes for k ∼ (π, π) for a dx2 −y2 gap. (3) The inelastic scattering acts to suppress the peak just as for an s-wave. The author had an opinion that the theory of superconductivity is already so well furnished that other fundamental ideas beyond the original BCS’s are almost needless, except for a few smart equipments. As the phenomena observed in the copper oxide superconductor are rather qualitative and fairly clear cut, so the explanation of them must be simple. It is expected that a quantum chemical speculation could make this possible. Let us address the author’s opinion. The divergent character of Eq. (1.153) seems a merely mathematical problem. The diﬀerence between Eq. (1.184) and that (will be obtained) for the superconducting case is the coherent factor, (1.202). In the case of a BCS superconductor, it holds that Ek ρ so that the enhancement of the spin-lattice relaxation time T1 is observed due to this factor, which leads to the superconductivity. However, in the case of a high-temperature superconductor, ρ, η ∼ Ek as has been seen in the previous chapter, then we cannot observe the sharp onset of superconductivity. Then we miss the coherent eﬀect. There is presumably a simpler reason why the T1 enhance is not observed. In copper oxide, electrons responsible for superconductivity are probably the d-electrons, then we have the vanishing interaction term if it is the Fermi contact term between a nucleus and an electron, say, F (R, r) ∼ δ(R − r) in Eq. (1.158).

1.9. Ginzburg–Landau Theory from BCS Hamiltonian The macroscopic quantum theory of superconductivity has been given by Ginzburg and Landau (in short, GL) [9]. This looks rather phenomenological, however since a microscopic justiﬁcation has been done by Gorkov and others [17, 31], this obtains a substantial foundation. We also reviewed the GL theory, in the introduction of Sec. 1.4, from the viewpoint of the Landau’s general theory of phase transitions. It is crucial that the Lagrangian of the system is written as the fourth-order function of the order parameter Ψ which is the electron ﬁeld. If the coeﬃcients of the second- and fourth-order terms are suitably chosen, the new ground state shapes a champagne bottle, or the Mexican hat is built. If electrons move on this ﬂat route around the top, the derivative of the orbital vanishes or the kinetic energy vanishes, which implies that the wave function is rigid. We may say that the electron mass is

page 46

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

47

eﬀectively zero. We thus have the current only due to the vector potential, i.e., the diamagnetic current. This causes the Meissner eﬀect. The GL theory is quite helpful for applications, since the microscopic theory by itself is too complicated to manipulate the large-scale problems. If we can solve the GL equation for a real problem under an appropriate boundary condition, various information on this system can be obtained [11]. The macroscopic wave function or GL order parameter Ψ is related to the gap function and understood as the ﬁeld of Cooper pairs. The parameters in the GL equation are also written in the microscopic terms or by the experimental values. In [29], the GL function Ψ is derived directly from the Bardeen–Cooper–Schrieﬀer Hamiltonian, not via the gap function or the anomalous Green’s function related with the gap function. The electron– electron interaction composed of the four fermion operators is transformed by the Hubbard–Stratonovitch transformation to an auxiliary complex boson ﬁeld φ, in which electrons behave as if they were free. Using the path integral method, we can carry out the integration up to the quadratic terms of the electron operators. If we carefully analyze the resulting eﬀective Lagrangian for the boson ﬁeld, it is found that this boson ﬁeld, which is described by a complex function, suggests a phase transition: the condensation arises in particles described by the real part of the boson ﬁeld, while particles in the imaginary (or phase) part turn out to be massless Goldstone bosons. It is then clear that the boson ﬁeld is to be the GL order parameter. In the course of analysis, the concept of supersymmetry is eﬀectively used.

1.9.1. BCS theory We assume the classical ﬁeld of an electron is described by the Grassmann algebra or the anticommuting c-number, namely the creation and annihilation operators a∗k and ak are treated as anticommuting c-numbers. The BCS Hamiltonian is written as H = H0 + Hint , kσ a∗kσ akσ , H0 =

(1.204)

kσ

Hint =

kk

and −gk−k,−kk =

−gk−k,−k k (a∗k↑ a∗−k↓ )(a−k ↓ ak ↑ ),

gk−k,k −k > 0,

dr1 dr2 χ∗k↑ (r1 )χ∗−k↓ (r2 )v(r1 , r2 )χ−k ↓ (r2 )χk ↑ (r1 ), (1.205)

page 47

March 24, 2021

48

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

where v(r1 , r2 ) is the eﬀective coupling giving an attractive character for the electron–electron interaction. Here, the summation convention that repeated indices imply summation is used. This is helpful to facilitate the manipulation. We would consider that the BCS Hamiltonian is an attractive interaction between Cooper pairs rather than an attractive interaction between electrons (Figs. 1.3 and 1.4). In the following, it is assumed that kσ is independent of spin and gk−k,k−k is independent not only of spin but also, ﬁnally, of k and k . Let us investigate the partition function Z = Tre−β(H0 +Hint ) .

(1.206)

This is expressed by the use of the path integral method [32–34]. The spirit of the Feynman path integral is sometimes written as follows: the (imaginary) time interval 0 → β is sliced into numerous pieces, each one being labeled by τp . Since each slice is made arbitrarily small, the quantum eﬀect arising from the commutation relation can be neglected, so that the operators are regarded as c-numbers in each slice. Instead, this c-number function can take any value even in the small time-slice. Connecting these precise values from

Fig. 1.3. In the BCS model, superconductivity arises due to the attractive electron– electron interaction which appears owing to the scattering by phonons.

Fig. 1.4. Excitation of the ground state of a Cooper pair demonstrates the presence of the energy gap Δ which is (very approximately) isotropic in the momentum space.

page 48

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

49

0 → β, we can draw all of the paths in this interval. If we count the eﬀects from all of these paths, the quantum mechanical result of the subject can be obtained. However, this statement seems rather misleading. Feynman’s path integral is the third method of quantization [35]. We begin with the classical treatment, and then if we apply the path integral procedure upon this, the quantum eﬀect is certainly taken into account. This corresponds to the conceptual development from the geometric optics to the physical optics. The Bose system (in quantum mechanical sense) is written by an ordinary c-number, but the Fermi system should be described by a Grassmann number. Thus, we do not worry about the commutation relations of ﬁeld operators and obtain Z = Tr e−β H ' N = lim da∗ (τp )da(τp ) exp [(a˙ ∗ (τp )a(τp ) − H(τp )], ˆ

N →∞

=

= β/N

p

p=1

∗

β

Da (τ )Da(τ ) exp

dτ {a∗kσ (τ )(−∂τ − kσ )akσ (τ )

0

+gk−k,−k k a∗k↑ (τ )a∗−k↓ (τ )a−k ↓ (τ )ak ↑ (τ )},

(1.207)

where ∗

Da (τ )Da(τ ) =

∞ '

da∗kσ (τp )dakσ (τp ).

(1.208)

p=1

1.9.2. Hubbard–Stratonovitch transformation Diﬃculty lies in the quartic term of the electron–electron interaction. Let us deﬁne Bα∗ = a∗k↑ a∗−k↓

and Bα = a−k ↓ ak ↑

(1.209)

to write, in each time slice, gk−k,−k k a∗k↑ a∗−k↓ a−k ↓ ak ↑ = gαα Bα∗ Bα .

(1.210)

This is simpliﬁed by using the identity called the Hubbard–Stratonovitch transformation [36]. We introduce a complex boson ﬁeld φ, since (Bα )∗ = Bα : ∞ ∞ √ √ ∗ ∗ ∗ −πφ∗ φ dφ dφe = dφ∗ dφe−π(φ −i g/πB )(φ+i g/πB) 1= −∞ ∞

=

−∞

−∞

dφ∗ dφe−πφ

∗ φ+i

√

gπ(B ∗ φ−Bφ∗ ) −gB ∗ B

e

,

page 49

March 24, 2021

50

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

namely

∞

−∞

dφ∗ dφe−πφ

∗ φ+i√gπ(B ∗ φ−Bφ∗ )

= egB

∗B

,

(1.211)

where it is deﬁned that dφ∗ dφ = d(Re φ)d(Im φ).a

(1.212)

We cannot apply this identity for the quantum mechanical partition function because of the non-commutativity of the operators involved, but now we have no trouble since, in the present path-integral treatment, operators turn out to be c-numbers. Then Eq. (1.207) becomes Z= Da∗ (τ )Da(τ )dφ∗ (τ )dφ(τ )

β

× exp 0

∗ dτ {−a∗kσ (τ )−1 kσ (τ )akσ (τ ) − πφα (τ )φα (τ )

√ √ + i πgk−k,α a∗k↑ (τ )a∗−k↓ (τ )φα (τ ) − i πgα,−k k a−k ↓ (τ )ak ↑ (τ )φ∗α (τ )} (1.213) with Δ−1 kσ (τ ) = −∂τ − kσ . The essential feature of this expression is as follows: the operator appearing in the exponent in Eq. (1.213) is only quadratic in ak and a∗k , so that the evaluation with respect to the fermion variables is similar to the evaluation for the non-interacting system, in which particles are moving in an eﬀective boson ﬁeld φk . Equation (1.213) shows that, inside the exponent, Z is a weighted average of the second and third terms over the ﬁeld φα .

1.9.3. Fourier transform The Fourier transformation with respect to τ is performed as eiωn τ ak (ωn ), φα (τ ) = eiνn τ φα (νn ), ak (τ ) = ωn

νn

ωn = (2n + 1)π/β,

νn = 2nπ/β.

(1.214)

Note that ωn refers to a fermion, while νn to a boson. a

Really dφR dφI =

1 dφ∗ dφ. 2i

The constants are adsorbed in the normalization factor.

page 50

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

Using the above and the relation β dτ ei(ωn −ωm )τ = βδnm ,

51

(1.215)

0

we have Z=

Da∗ (ωn )Da(ωn )Dφ∗ (νn )Dφ(νn )

× exp

{−βa∗kσ (ωn )kσ (iωn )−1 akσ (ωn ) − βπφ∗α (νn )φα (νn )

ωn ν n

√ + i πgk−k,α a∗k↑ (ωn + νn )a∗−k↓ (ω)φα (νn ) √ − i πgα,−k k ak ↓ (ωn )a−k ↑ (ωn + νn )φ∗α (νn )},

(1.216)

where kσ (iωn ) is Green’s function given as kσ (iωn ) =

1 . iωn − kσ

(1.217)

We can observe in Eq. (1.216): the third line tells that, at the vertex indicated by the coupling gk−k,α , the boson ﬁeld φα sinks, and then the particle pair, a∗k↑ a∗−k↓ arises. The last line displays the reverse phenomenon. Note the energy conservations at vertices.

1.9.4. Nambu spinor At this stage, we would rather use a spinor notation due to Nambu [12] very useful to investigate the superconductivity: ak↑ , a∗k = (a∗k↑ a−k↓ ), ak = a∗−k↓ a−k↓ (1.218) , a∗−k = (a∗−k↓ ak↑ ). a−k = a∗k↑ It is instructive to manipulate the complicated last line in (1.216) in the present language: it has a structure such that φα a∗k↑ a∗−k↓ − φ∗α a−k ↓ ak ↑ ↓ a a 1 0 k↑ −k = φα (a∗k↑ a−k↓ ) (0 1) ∗ (1 0) − φ∗α (a∗−k ↓ ak ↑ ) a−k↓ a∗k ↑ 0 1 = φα a∗k σ + ak + φ∗α a∗−k σ − a−k .

page 51

March 24, 2021

52

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

The positive sign in the second term is due to the Grassmann character of ak↑ and a−k↓ . Also a∗kσ k akσ = a∗ σk3 k ak ,

(1.219)

since k = −k . In the above, the Pauli matrices and related ones are rewritten as 0 1 0 −i 1 0 1 2 3 , σ = , σ = , σ = 1 0 i 0 0 −1 0 1 0 0 1 1 1 1 + 2 − 2 , σ = (σ − iσ ) = . (1.220) σ = (σ + iσ ) = 2 2 0 0 1 0 Equation (1.216) is now written as {−βπφ∗α (ν)φα (ν) Z= Da∗ DaDφ∗ Dφ exp ωn ν n

+ βa∗k (ωn )(iωn − k σ 3 )ak (ωn ) √ + iβ πgα,k −k φα (νn )a∗k (ωn + νn )σ + ak (ωn ) √ + iβ πgα ,k−k φ∗α (νn )a∗−k (ωn )σ − a−k (ωn + νn )}.

(1.221)

We can integrate with respect to fermion variables: note that [32] ∗ dz ∗ dze(z Az) = det A for a fermion, ∗ (1.222) dz ∗ dze(z Az) = (det A)−1 for a boson. Using the upper one, we can immediately obtain ∗ −βπφ∗α (ν)φα (ν) Z = Dφ Dφ exp νn

( ( ( ( √ ( 3 + ∗ − ( β(iωn − k σ ) + iβ πgα,k −k (φα (νn )σ + φα (νn )σ )( , + det ( ( ( ωn

(1.223) where the use was made of a symmetry property, gα,k −k = gα ,k−k , and · · · stands for a matrix. This can be also rewritten as (1.224) Z = Dφ∗ Dφ exp−βW (φ)

page 52

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

53

with the eﬀective action for the boson ﬁeld 1 φ∗α (νn )φα (νn ) − Tr log β (1.225) W (φ) = π β ω νn n √ 3 + ∗ − uα,k (φα (νn )σ + φα (νn )σ ) , × (iωn − k σ ) + i νn

(1.226) where the relation log·det = Tr·log and the simpliﬁed notation uα,k = πgα,k −k = πgα ,k−k

(1.227)

were used. By making use of the steepest descent method, we can obtain a ¯ For example, particular φ, by optimizing W (φ), which will be denoted φ. by diﬀerentiating W (φ) with respect to φ∗δ (νn ), we have √ i uδ,k σ − 1 ∂W (φ) = πφα − Tr √ ∂φ∗δ β ω (iωn − k σ 3 ) + i uα,k (φα (νn )σ + + φ∗α (νn )σ − ) n

= 0.

(1.228)

We thus obtain π φ¯δ (νn ) =

1 β iωn

where Ek2 (ν) = 2k +

)

(uδ,k uα,k ) · φ¯α , (iωn )2 − Ek2

(uα,k uα ,k )φ¯∗α (νn )φ¯α (νn ).

(1.229)

(1.230)

Note that the ﬁeld strength φ∗α (νn )φα (νn ) has the dimension of energy. In obtaining Eq. (1.229), we ﬁrst rationalize the denominator, and then the Tr operation on σ’s is carried out. The numerator remained is the coeﬃcient of Tr σ + σ − = 1. The similar equation is obtained for φ∗ . Equation (1.229) corresponds to the gap equation. Now we employ an approximation in the rest of this study that, as was mentioned at the beginning, uα,k = u (a positive constant). Thus we have, to the ﬁrst approximation, that φ is nearly constant, 1 1 π = . 2 u β ω (iωn ) − Ek2 n

(1.231)

page 53

March 24, 2021

20:13

54

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

Carrying out the frequency sum, we get 1 1 = ±n(x), β ω iωn − x

(1.232)

n

where n(x) is the Fermi or Bose function according to ωn is odd or even, respectively, and we obtain (for fermions) n(Ek ) − n(−Ek ) tanh(βEk /2) π = = . u 2Ek 2Ek

(1.233)

From the above relation combined with Eq. (1.229), we can estimate φ¯ which corresponds to the gap energy.

1.9.5. Critical temperature It is straightforward to obtain the critical temperature, Tc , for the superconductivity from Eq. (1.233) [16]. Here, it is repeated for completeness. In the limit T → Tc , the gap, or φα in the present case, disappears. The summation over k is approximately replaced by the integration: ωD d 2π = tanh , (1.234) uN (0) 2kB Tc 0 where N (0) is the state density at the Fermi surface, and the cut-oﬀ parameter ωD is, in the case of the BCS theory, the Debye frequency of phonons associated with the attractive interaction between electrons. The integration in Eq. (1.241) proceeds as follows:

ωD 0

d tanh = 2kB Tc

βC ωD /2

0

= log ztanh

dz tanh z z β ω /2 z]0 c D

βc ωD − ≈ log 2 = log

(z = βc /2)

−

∞

βc ωD /2

dz log z sech2 z

0

2

dz log z sech z 0

4eγ βc ωD + log . 2 π

βc ωD ≈1 tanh 2 (1.235)

Combined with (1.233), this yields log

2π 4eγ βc ωD = − log , 2 uN (0) π

(1.236)

page 54

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

55

where γ = 0.5772 is the Euler’s constant. This relation will be used in the next section. Simple rearrangements yield Tc ≈ 1.13ωD e−2π/N (0)u .

(1.237)

1.9.6. Temperature dependence of φ For the later investigation, we derive a temperature dependence of φα near the critical temperature [17]. Coming back to (1.231) and restoring the hidden summation with respect to k, we can rewrite this as 2π 1 ωD 1 = . (1.238) d 2 uN (0) β ω 0 (iωn ) − (2 + u|φα |2 ) n

Considering that, |φα |2 1 near the critical temperature, we expand the above as 1 ωD 2π = d uN (0) β ω 0 n u|φα |2 (u|φα |2 ))2 1 + + + ··· . × (iωn )2 − 2 ((iωn )2 − 2 )2 ((iωn )2 − 2 )3 (1.239) For the convergent integrals which are the second and third terms, the integration limit is extended to inﬁnity, and then we obtain (putting = ω tan θ), ωD 1 1 β 1π 1 3π d 2π 2 2 = tanh + u|φα |2 (u|φ + | ) + ··· . α uN (0) 2 β4 ωn3 β 16 ωn5 0 (1.240) The integration of the ﬁrst term on the right-hand side which is similar to (1.235) has β instead of βc . Then, using (1.236), we have, in the lowest approximation, log

1 1π βc = u|φα |2 + ··· . β β4 ωn3

(1.241)

Using ∞ 0

2p − 1 1 = ζ(p) (2n + 1)p 2p

(1.242)

page 55

March 24, 2021

56

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

in (1.241), we have the temperature dependence of φα , * + T 16 2 u|φα | = πkB Tc 1− ζ(3) = 1.202, 7ζ(3) Tc

(1.243)

which is the same as that of the energy gap [16].

1.9.7. Dynamics of the boson field, symmetry breaking The boson ﬁeld φα (νn ) satisfying (1.227) is written as φ¯α , so that φα (νn ) = φ¯α + (φα − φ¯α ) = φ¯α + Φα (νn ).

(1.244)

Now Φα (νn ) is a physical or called ﬂuctuation in solid-state physics. Our aim is to ﬁnd the eﬀective Lagrangian or Hamiltonian for Φα (νn ). In order to ﬁnd the terms proportional to Φα (νn ) in (1.244), we ﬁrst observe that (a) φα (νn )τ + + φ∗α (νn )τ − ≡ φα (νn ) · τ = φ(a) α (νn )τ

= φ¯α (νn ) · τ + Φα (νn ) · τ,

a = 1, 2. (1.245)

Expanding W (φ) in (1.226) in Φα (νn ) and noticing that, upon the Tr operation, the odd terms with respect to τ will vanish, we have W (φ∗ , φ) = π

φ∗α φα −

νn

−

n

1 βω ν

n n

where

√ 1 Tr log β(iωn − τ 3 − i u(φ¯α · τ ) β ω

even n

√ 1 Tr[(ωn )i u(Φα (νn ) · τ )]n , n

√ iωn + k τ 3 + i u(φ¯α · τ ) . k (ωn ) = (iωn )2 − Ek2

(1.246)

(1.247)

Note that now the propagator includes the mean-ﬁeld eﬀect. What we are interested in is the second line of Eq. (1.246). The term with n = 2 is precisely written as −1 ) (a) Tr uk (ωn )(Φ(a) )k+α (ωn + νn )(Φ∗(a (νn )τ (a ) ) α (νn )τ α 2β ω ν n n u|Φα (νn )|2 Pα (νn ), (1.248) = νn

page 56

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

57

where careful manipulations about τ ’s are required. Except for the explicit ones combined with Φ’s, we have τ ’s inside ’s. Let us call the terms with a = a = 1 and a = a = 2 the direct interactions, while the terms with a = 1, a = 2, and a = 2, a = 1 the cross interactions. We then have Pα (νn ) =

−2 iωn (iωn + iνn ) − k k+α + uφ¯∗ · φ¯ , 2 β ω [(iωn )2 − Ek2 ][(iωn + iνn )2 − Ek+α ]

(1.249)

n

where the ﬁrst two terms in the numerator arise from the direct interaction and the third from the cross one. Here the use was made that Tr τ 3 τ + τ 3 τ − = −1. Using (1.231), we can carry out a lengthy but not diﬃcult calculation of Pα (νn ). Note that an even frequency νn has nothing to do with obtaining the Fermi functions. The result is Pα (νn ) = −n(Ek )(1 − n(Ek+α))

, ¯ Ek+α Ek − k+α k + u(φ¯∗ · φ) Ek+α − Ek . × (iν)2 − (Ek+α − Ek )2 Ek+α Ek (1.250)

Here, we again note that, in the square brackets, the ﬁrst two terms are obtained from the direct interaction and the third term from the cross interaction. It might be convenient, for the later investigation, to carry out the frequency sum for Pα (νn ): Ek+α − Ek νn

(iνn )2 − (Ek+α − Ek )2 , 1 1 11 − =β β ν 2 iνn − (Ek+α − Ek ) iνn + (Ek+α − Ek ) n

β [−nB (Ek+α − Ek ) + nB (−Ek+α + Ek )], 2 , β(Ek+α − Ek ) −β coth , = 2 2 =

where nB is the Bose function, and the use of Eq. (1.232) was made for the even frequency νn . Then Eq. (1.250) becomes , β(Eα+γ − Eα ) β Pγ (νn ) = n(Eα )(1 − n(Eα+γ )) coth 2 2 νn , Eα+γ Eα − α+γ α + u(φ¯∗ · φ) . (1.251) × Eα+γ Eα

page 57

March 24, 2021

58

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

We then obtain the eﬀective action for φ up to the second order in Φ as follows: φ∗α (νn )φα (νn ) Wα (φ∗ , φ) = π νn

−

√ 1 Tr log{−β(iωn − k τ 3 − uφ¯α (νn ) · τ )} βω ν n n

Ek+α − Ek 2 − (E 2 (iν) k+α − Ek ) νn , ¯ Ek+α Ek − k+α k + u(φ¯∗ · φ) × . (1.252) Ek+α Ek

−n(Eα )(1 − n(Eα+γ ))

1.9.8. Instability In order to discuss the dynamics of Φα (νn ), we must obtain an expression for the action of Φα (νn ) similar to that for aα (ωn ) given in the exponent of Eq. (1.207). Since we are interested in the energy region much lower than that for the electronic excitation (Eα+γ − Eα ), the denominator of Pα (νn ) in Eq. (1.250) is expanded as , −1 (iνn )2 1 = + ··· . 1+ (iν)2 − (Ek+α − Ek )2 (Ek+α − Ek )2 (Ek+α − Ek )2 (1.253) Substituting this into Pα (νn ) in Eq. (1.250) and taking up the terms of the order of (iν)2 in the above, we have ¯ (Ek+α − Eγ ) + · · · . (iνn )2 + u(φ¯∗ φ) Ek+α Ek 2

(1.254)

The second term is a small and complicated, however positive, quantity. We thus anyway obtain the eﬀective Lagrangian for Φ up to the second order of Φ∗ Φ as LB ∼ Φ∗ (iνn )2 Φ + ηΦ∗ Φ + · · · ,

η > 0.

(1.255)

In the above, iνn is replaced by ∂/∂τ in the future. At this stage, the details of η are immaterial except that this is positive. To put forward the problem, we need the term proportional to Φ∗ Φ∗ ΦΦ. This is obtainable from the term with n = 4 in Eq. (1.246). Without any detailed calculation, we may presume a positive quantity for this, noted by

page 58

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

59

Λ2 . Then the total Lagrangian of the boson ﬁeld becomes LB ∼ Φ∗ (iνn )2 Φ + ηΦ∗ Φ − Λ2 Φ∗ Φ∗ ΦΦ.

(1.256)

This looks like the Lagrangian that Ginzburg and Landau have used for investigating the superconductivity. We thus expect a kind of phase transition. Let us optimize, with respect to Φ∗ , the potential part of Eq. (1.256), V = −ηΦ∗ Φ + Λ2 Φ∗ Φ∗ ΦΦ,

(1.257)

∂V = −ηΦ + 2Λ2 Φ∗ ΦΦ ∂Φ∗ = (−η + 2Λ2 Φ∗ Φ)Φ = 0.

(1.258)

If Φ = 0, nothing happens. While, in the case of Φ = 0, it is possible that Φ∗ Φ =

η ≡a ¯2 . 2Λ2

(1.259)

We now put Φ = (ρ + a ¯)eiθ ,

(1.260)

namely only the radial part is aﬀected. This choice is allowed in the spirit of the unitary gauge. If we insert this into (1.257), it follows that ¯)2 − a ¯2 ]2 − Λ2 a ¯4 = Λ2 [Φ∗ Φ − a ¯2 ]2 − Λ2 a ¯4 . V = Λ2 [(ρ + a

(1.261)

Observing the ﬁnal result, we realize that the potential becomes minimum at |Φ| = a ¯, namely at this position apart from the origin, |Φ| = 0, which corresponds to the Hartree–Fock (HF) state. The mass of the ﬁeld ¯2 for a particle of the ρ Φ is given by the coeﬃcient of Φ∗ Φ, which is 4Λ2 a ﬁeld, while the term involving θ is completely lost. That is, the particle in the θ ﬁeld is massless, which is called the Goldstone boson. This is due to the occurrence of the inﬁnite degeneracies along the direction perpendicular to the ρ coordinate.

1.9.9. Supersymmetry The total Lagrangian of the system is Ltot = Le + LB + Lint ,

(1.262)

page 59

March 24, 2021

60

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

where Le = a∗i (iωn − i τ 3 )ai , ˙ ∗Φ ˙ − Λ2 [Φ∗ Φ − a ¯2 ]2 , LB = −Φ √ Lint = −i u(Φa∗ τ + a + Φ∗ a∗ τ − a).

(1.263)

In the above, the second line is obtained from Eqs. (1.256) and (1.261), and then the third line from Eq. (1.245) supplied by necessary terms, and a compact notation is used, and the immaterial constant terms are omitted. The L in the above is, strictly speaking, the Lagrangian density, and the action which we are interested in is the space–time integral of the Lagrangian density, so that the partial integration with respect to τ (after replacing iνn → ∂τ ) gives the ﬁrst term with the minus sign. If we deﬁne the momentum conjugate to Φ, ∂Ltot ˙ ∗ Π∗ = ∂Ltot = −Φ, ˙ = −Φ ˙ ˙∗ ∂Φ ∂Φ the total Hamiltonian for the boson ﬁeld is obtained as Π=

(1.264)

˙ + ΠΦ ˙∗−L Htot = Π∗ Φ √ ¯2 ]2 . (1.265) = Π∗ Π + i u(a∗ Φτ + a + a∗ Φ∗ τ − a) + Λ2 [Φ∗ Φ − a The momenta, Π∗ and Π conjugate to Φ∗ and Φ respectively, have properties ∂ ∂ f (Φ∗ , Φ), [Π∗ , f (Φ∗ , Φ)]− = f (Φ∗ , Φ), (1.266) ∂Φ ∂Φ∗ since we are now dealing with the classical operators in the framework of the path integral formalism. Let us turn to a supersymmetric treatment [37–39]. The fermionic composite charge operators are deﬁned as √ ¯2 )a∗ τ − , Q∗ = Π∗ a∗ − i u(Φ∗ Φ − a √ ¯2 )τ + a. (1.267) Q = Πa + i u(Φ∗ Φ − a [Π, f (Φ∗ , Φ)]− =

First of all, we have to manipulate the commutator √ √ ¯2 )a∗ τ − , Πa+i u(Φ∗ Φ− a ¯2 )τ + a]+ . (1.268) [Q∗ , Q]+ = [Π∗ a∗ −i u(Φ∗ Φ− a Straightforward calculations give [Π∗ a∗ , Πa]+ = [Π∗ a∗ , a]+ Π − a[Π, Π∗ a∗ ]+ = Π∗ [a∗ , a]+ Π − a[Π, Π∗ ]+ a∗ = Π∗ Π.

page 60

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

61

Here, for the Grassmann numbers, the use was made of the relation [a∗ , a]+ =

∂ ∂a ∂ ∂ ∂ a−a = +a −a = 1. ∂a ∂a ∂a ∂a ∂a

Further, √ ¯2 )τ + a]+ [Π∗ a∗ , i u(Φ∗ Φ − a √ √ = [Π∗ a∗ , i u(Φ∗ Φ − a ¯2 )]− τ + a − i u(Φ∗ Φ − a ¯2 )[τ + a, Π∗ a∗ ]+ √ √ = [Π∗ , i u(Φ∗ Φ − a ¯2 )]− a∗ τ + a − i u(Φ∗ Φ − a ¯2 )τ − Π∗ [a, a∗ ]+ √ = i uΦa∗ τ + a and √ ¯2 )a∗ τ − , Πa]+ [i u(Φ∗ Φ − a √ √ = [Πa, i u(Φ∗ Φ − a ¯2 )]− a∗ τ − − i u(Φ∗ Φ − a ¯2 )[a∗ τ − , Πa]+ √ √ = [Π, i u(Φ∗ Φ − a ¯2 )]− aa∗ τ − − i u(Φ∗ Φ − a ¯2 )τ − Π[a∗ , a]+ √ = i uΦ∗ aa∗ τ − √ = −i uΦ∗ a∗ τ − a. The ﬁnal term must be symmetrized: 1 ∗ + − {[a τ , τ a]+ + [a∗ τ − , τ + a]+ } 2 [b, b∗ ]+ 1 1 = {[(0, a∗ ), (0, a)]+ + [(b, 0), (b∗ , 0)]+ } = 2 2 0

[a∗ τ + , τ − a]+ →

(1.269) 0 [a∗ , a]+

(1.270)

1 (1.271) = 1. 2 In the second line, b and b∗ which are used in the literature are deﬁned. We thus obtain the fundamental relation in the supersymmetric quantum mechanics, H = [Q, Q∗ ]+ ,

(1.272)

if we endow, to the constant Λ2 in (1.264), a speciﬁed value, Λ2 = 2u,

(1.273)

which is reasonable [39]. However, as was mentioned before, this had to be obtained analytically from the term with n = 4 in Eq. (1.252). If it is assumed that the present system is the case of supersymmetry, we can avoid this tedious calculation.

page 61

March 24, 2021

62

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

The nilpotency of the charge operators, Q2 = 0,

(Q∗ )2 = 0,

(1.274)

is clearly preserved from a2 = 0 and (a∗ )2 = 0. We have thus completed a supersymmetric analysis.

1.9.10. Toward the Ginzburg–Landau equation Now we can think about the Ginzburg–Landau equation. Since the GL equation concerns only with the static part of the condensed boson ﬁeld, we keep the ﬁrst and third terms in Eq. (1.265). The ﬁrst term is the kinetic part, while the last term is the potential part, HGL = Π∗ Π − ηΦ∗ Φ + Λ2 (Φ∗ Φ)2 ,

(1.275)

with ¯ η = u(φ¯∗ φ)

(Ek+α − Eγ )2 . Ek+α Ek

As usual, the coeﬃcients of Φ∗ Φ and (Φ∗ Φ)2 in the Ginzburg–Landau equation are a and b, respectively. It is crucial that a is negative, which is given by −η in the present consideration. The temperature dependence of ¯ as in Eq. (1.265). This is exactly the same as that η is found through u(φ¯∗ φ) obtained by Gorkov [31].

1.9.11. Discussion Somebody seemed to be puzzled by a curious looking of the Ginzburg– Landau equation when it was published: the superconductivity being a macroscopic, thermodynamically stable phase, why it is predicted by a Schr¨ odinger-like wave function, to which the microscopic phenomena are subjected. Several years later on, the microscopic theory was established by BCS, and soon Abrikosov has successfully correlated these two treatments. He has made clear that the GL function is deeply concerned with the gap function characteristic of the superconductivity and is a wave function describing the condensed Cooper pairs. The superconducting state is certainly a stable thermodynamical state, and a phase transition from the normal state to the superconducting state is interpreted as a long-distance correlation between the Cooper pairs. Yang [40] developed a uniﬁed treatment of the phase transition in terms of the density matrix. According to his treatment, the onset of the superconductivity is understood in such a way that the oﬀ-diagonal

page 62

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Theory of Superconductivity

63

long-range order (ODLRO) of the second-order density matrix has nonvanishing value. This concept is clearly related to the London’s rigid function, the quasiboson condensation being widely seen as a powerful model of superconductivity and the variational wave function tired by BCS [3]. Recently, Dunne et al. [41] applied the concept of ODLRO to argue the high-temperature superconductivity in copper oxide, where the attractive interaction between electrons is assumed to be originated from Friedel oscillations in the screened potential. However, the previous presentation of Abrikosov looks as a detour, a complicated tedious procedure; the condensed pair is characterized by an anomalous temperature Green’s function which is diﬃcult to manipulate for beginners. Therefore, the direct way to reach the GL theory from the BCS Hamiltonian should be preferable. What we have done in the present investigation is the following: the auxiliary boson ﬁeld driven by the Hubbard–Stratonovitch transformation to eliminate the quartic term of electron operators is just the GL function. Conclusively, we should like to state, from the so far treatments, the conditions which is necessary for occurrence of superconductivity. (1) The wave function which means the ground-state average of operators of a Cooper pair must be complex or two-dimensional. If one of these two degrees of freedom gets a new stable structure, the other degree of freedom, whose direction is perpendicular to the former, oﬀers the inﬁnite degeneracy. In the Nambu theory, the ﬁrst refers to the σ 1 direction, and the second to σ 2 in the ﬁctitious spin space. (2) The electron–electron interaction should be attractive, otherwise the negative coeﬃcient of Φ∗ Φ in Eq. (1.275) cannot be obtained. In the present consideration, we have observed that this condition is established in the eﬀective electron–electron interaction of the system involving the multiband structure. However, we will discuss a little more about the normal state under the usual condition. In the normal species, the coupling constant between electrons is intrinsically positive. However, if we are interested in the exchange interaction, the so-called Fock term with negative coupling, this is met by condition (2). This is a short range, while the direct coupling is so strong as to overwhelm the exchange interaction. Let us turn to the behavior of the quartic electron operators. It is unexpected that these are grouped into the pair operators of particle–particle and hole–hole, which do not conserve the particle number. Thus, it is natural

page 63

March 24, 2021

64

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch01

Modern Aspects of Superconductivity: Theory of Superconductivity

to group them into a couple of particle–hole pairs. This choice makes the auxiliary boson function to be real. The Hamiltonian which satisﬁes the above two conditions, looking like the BCS Hamiltonian, is the one with the dipole–dipole interaction. The simplest case is that of the intermolecular interaction due to the induced dipole–dipole interaction with a coupling constant −d: Hd = −d a∗r b∗r bs as ,

(1.276)

where, for example, a∗r and b∗r are the creation operators for a particle and a hole, respectively. If the electron–electron interaction is screened enough, this may be another possibility for the superconductivity of a molecular complex.

page 64

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

CHAPTER 2

Physics of High-Tc Superconductors

2.1. Introduction In 1986, K.A. M¨ uller and J.G. Bednorz discovered the phenomenon of superconductivity in Cu-oxide compounds of lanthanum and barium at the temperature Tc = 35 K [2], which was marked by the Nobel’s prize in 1987. This discovery gave the additional push to the intensiﬁcation of the scientiﬁc activity in the ﬁeld of superconductivity. For the last 35 years, the superconducting transition temperature has been increased to 140 K. Moreover, one may expect the discovery of new superconductors with higher critical temperatures. Recently, the high critical temperatures of new Mg-containing superconductors (MgBr2 ) (Tc = 39 K) and superconducting oxypnictides LnO(1−x) Fx FeAs (Tc = 50 K) were registered. The main purpose of solid-state physics is the development and the fabrication of substances which possess the superconductivity at room temperature. At present, there proceeds the great-scale search for such high-temperature superconductors. Especially promising is the method of production of superconducting materials with the help of the laser spraying of layers. After the discovery of HTSC, the following problems become urgent: (1) Conceptual-theoretic one: the problem of the clariﬁcation of mechanisms of high-temperature superconductivity. (2) Engineering and technical ones: the the problem of the practical applications of HTSC. (3) Research one: the problem of the search for materials with higher Tc . The great interest in the phenomenon of superconductivity is caused by the basic possibility to use it in the future for the electric power transfer without losses and for the construction of quantum high-power generators. This phenomenon would be applied in superconductive electronics and computer technique (superconducting elements of memory). At the present time, a new 65

page 65

March 24, 2021

66

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

trend in technology, namely the construction of quantum computers on the basis of high-temperature superconductors with d-pairing, is developed. High-temperature superconductors have unique physical properties both in the normal state and the superconducting one. To comprehend the physics of these complex compounds is one of the main tasks of the theory of superconductivity, whose solution will allow one to explain the mechanism ensuring the high-temperature superconductivity. The disappearance of resistance on the cooling of superconductors down to a certain critical temperature is one of the most characteristic eﬀects in superconductors. But, in order to understand the reason for the rising of superconductivity, it is necessary to study the other eﬀects which accompany this phenomenon. Consider brieﬂy the main properties of high-temperature superconductors (HTSC): (1) New HTSC have a great anisotropy across the axis c and possess a multilayer structure. The main block deﬁning the metallic and superconductive properties is planes with CuO2 which form the square lattices of Cu ions. (2) HTSC are superconductors of the second kind (l/κ 1, where l is the coherence length, and κ is the penetration depth of a magnetic ﬁeld). (3) High-temperature superconductors have high critical temperatures Tc . (4) They have antiferromagnetic ordering of spins of Cu in the CuO2 planes and powerful spin ﬂuctuations with a wide spectrum of excitations. At the present time, there exists no theoretical approach which would explain the totality of thermodynamical, magnetic, and superconductive properties of high-temperature superconductors from the single viewpoint. The electron–phonon mechanism of pairing, being principal in standard superconductors, gives a considerable contribution to the establishment of the superconducting state in high-temperature superconductors. But, in order to attain the proper description, it is necessary to consider the other mechanisms inherent to high-temperature superconductors. One of such mechanisms is the spin-ﬂuctuation one proposed by D. Pines (USA). The reason for the pairing of electrons can be the scattering of electrons on spin ﬂuctuations. This model of pairing is one of the most actual models of high-temperature superconductivity. The thermodynamics of superconductors at low temperatures is determined by the excitation of two quasiparticles. In the traditional superconductors with pairing of the BCS type, the energy gap is isotropic (s-pairing),

page 66

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

67

and the temperature dependence of the heat capacity has exponential form ∼ exp−Δ/kB T , where Δ is the superconductor’s gap. In superconductors with anisotropic pairing, the temperature dependence of the heat capacity has power character, namely, T n . The appearance of such temperature dependences is related to that the superconductor’s gap has zeros on the Fermi surface. The development of the thermodynamics of this model is the actual problem of high-temperature superconductors. In Sec. 2.2, we consider the history of the development of studies of the phenomenon of superconductivity. The structure of high-temperature superconductors and their physical properties are analyzed. We make survey of the mechanisms of superconductivity and discuss the problem on the symmetry of the order parameter. We draw conclusion that, on the whole, the most probable is the “synergetic” mechanism of pairing which includes, as components, the electron–phonon and spin-ﬂuctuation interactions in cuprate planes. Only if the interaction of all the degrees of freedom (lattice, electronic, and spin ones) is taken into account, a number of contradictory properties observed in the superconducting and normal phases can be explained. Moreover, one needs also to consider a complicated structure of hightemperature superconductors. It will be emphasized that new experiments should be executed in order to explain the available experimental data. In this section, we also consider the thermodynamics of the spinﬂuctuation mechanism of pairing, present the method of functional integration for the calculation of thermodynamical properties on the basis of the Pines spin-ﬂuctuation Hamiltonian, and deduce the Schwinger– Dyson equations for Green’s functions and equations for the thermodynamic potential. Based on the Schwinger–Dyson equation, we obtain equations for the superconductor gap, which are used in numerical calculations of the thermodynamics of high-temperature superconductors. We present analytic formulas for the thermodynamic potential and its jump. The numerical calculations of the temperature dependence of the electron heat capacity indicate that the temperature dependence of the heat capacity is proportional to the square of the temperature. We emphasize that such temperature dependence is related to the d-pairing. It is shown that the measurement of the temperature dependence of the heat capacity can be a supplementing test for the establishment of a type of the symmetry of pairing in high-temperature superconductors. The jump of the heat capacity of cuprate superconductors near the critical temperature is evaluated as well.

page 67

March 24, 2021

68

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

2.2. History of the Development of Superconductivity The phenomenon of superconductivity was discovered by the physicist H. Kamerlingh-Onnes at the Leiden Laboratory (the Netherlands) in 1911, in the same year when Rutherford discovered an atom. H. KamerlinghOnnes registered the disappearance of resistance of Hg at the temperature T = 4.5 K. This state was called superconducting. Being cooled down to a temperature less than the above-mentioned critical temperature, many conductors can be transferred in the superconducting state, in which the electric resistance is absent. The disappearance of resistance is the most dramatic eﬀect in superconductors. But, in order to comprehend the reason for the origin of superconductivity, we need to study the other eﬀects accompanying this phenomenon. The dissipationless current states in superconductors were a puzzle for a long period. The phenomenon of superconductivity is a bright example of the manifestation of quantum eﬀects on the macroscopic scale. At present, the superconductivity occupies the place of the most enigmatic phenomenon in condensed-state physics, namely in the physics of metals. The main purpose of solid-state physics consists in the creation of superconductors which have the superconductive property at room temperature. At the present time, the researchers continue the wide-scale search for such high-temperature superconductors by testing the variety of various substances. A number of phenomenological models were proposed to clarify the phenomenon of superconductivity, namely the models advanced by London and Ginzburg–Landau [9, 42]. The essence of these theories which have played the important role in the development of ideas of superconductivity was presented in Chapter 1. The success of the Ginzburg–Landau theory was related to the circumstance that it is placed in the mainstream of the general theory of phase transitions. Among the ﬁrst microscopic theories devoted to the consideration of the electron–phonon interaction, the work by H. Fr¨ ohlich [43] is of the greatest importance. The following stage in the development of superconductivity started from the universal theory of BCS published in 1957 [148] which strongly promoted the subsequent study of superconductivity [44]. The authors of this theory were awarded by the Nobel’s prize. The BCS theory gave the possibility to elucidate a lot of experiments on superconductivity of metals and alloys. However, while developing the theory, some grounded assumptions and approximations were accepted.

page 68

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

69

Therefore, the BCS theory was needed in a substantiation with the help of more strict arguments. This was made by Academician N.N. Bogoliubov in [44]. He developed a microscopic theory of the phenomena of superconductivity and superﬂuidity. By using the Fr¨ohlich eﬀective Hamiltonian, N.N. Bogoliubov calculated the spectrum of excitations of a superconductor within the method of canonical transformations proposed by him in 1947. In 1962, B.D. Josephson advanced the theory of tunnel eﬀects in superconductors (the Josephson eﬀect) which was marked by the Nobel’s prize in 1973 [45]. This discovery strongly intensiﬁed the experimental studies of superconductivity and was applied to electronics and computer technologies. In 1986, K.A. M¨ uller and J.G. Bednorz discovered high-temperature superconductors [2], which initiated the huge “boom” manifested in the publication of plenty of works. The principal thought of K.A. M¨ uller was the following: by selecting the suitable chemical composition, one can enhance the electron–phonon interaction and, thus, increase the critical temperature Tc . K.A. M¨ uller and J.G. Bednorz found a new class of high-temperature superconductors, the so-called cuprate superconductors. High-temperature superconductors are studied already 35 years by making signiﬁcant eﬀorts, but the while pattern is not else clear completely. This is related to a complicated structure of cuprates, diﬃculties in the production of perfect single crystals, and a hard control over the degree of doping. The comprehension of HTSC will be attained if our knowledge about HTSC will approach some critical level which will be suﬃcient for the understanding of a great amount of experimental data from the single viewpoint. In Fig. 2.1, we present the plot of the critical temperatures of superconductivity over years [46–48].

2.3. Structural Properties of High-Temperature Superconductors The properties of new high-temperature superconductors diﬀer essentially from the properties of traditional superconductors which are described by the BCS theory. Let us brieﬂy consider the main properties of high-temperature superconductors. As known, the atomic structure deﬁnes the character of chemical bonds in solids and a number of relevant physical properties. Even small changes of the structure lead frequently to signiﬁcant changes of their electron properties; for example, at the phase transitions metal-dielectric. Therefore, the study of a crystal structure with long-range atomic order and

page 69

March 24, 2021

70

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 2.1.

The evolution of critical temperatures since the discovery of superconductivity.

its dependence on the temperature, pressure, and composition is of great importance for high-temperature superconductors. These investigations are signiﬁcant for the comprehension of mechanisms of high-temperature superconductivity. At the present time, we have several families of HTSC: thermodynamically stable Cu oxides containing lanthanum, yttrium, bismuth, thallium, and mercury [47]. We note that the structure of all Cu-oxide superconductors has a block character. The main block deﬁning metallic and superconductive properties of a compound is the plane with CuO2 which form the square lattices of Cu ions coupled with one another through oxygen ions. Depending on the composition, the elementary cell of a high-temperature compound can have one, two, and more cuprate layers. In this case, the critical temperature of the superconducting transition increases with the number of cuprate layers. In Fig. 2.2, we present an elementary cell of the orthorhombic structure of yttrium ceramics YBa2 Cu3 O7−δ , δ ≈ 0.1–0.3. The maximum Tc ≈ 90 K.

page 70

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

71

Fig. 2.2. Elementary cell of yttrium ceramics YBa2 CuO7 : 1-yttrium, 2-barium, 3 -oxygen, 4-copper.

The size of the cell is characterized by the following parameters: a = 3.81 ˚ A, b = 3.89 ˚ A, c = 11.7 ˚ A. Thus, the high-temperature superconductors are characterized by both large volumes of elementary cells and a clearly manifested anisotropy of layers. Of signiﬁcant interest is the discovery of the compounds Bi2 CaSr2 Cu2 O8 (Bi/2–1–2–2) and Tl2 CaBa2 Cu2 O8 (Tl/2–1–2–2) with the temperature of the superconducting transition Tc > 100 K. These compounds can have diﬀerent numbers of cuprate layers and are described by the general formula A2 Can Y2 Cun O2n4 , where A = Bi(T l), Y = Sr(Ba). Their temperature Tc depends on the number of cuprate layers and take values of 10, 85, and 110 K for the compounds with Bi and 85, 105, and 125 K for the compounds with Tl for n = 1, 2, 3, respectively. We mention also the compounds with Tl with the single layer Tl–O with the general formula TlCan−1 Ba2 Cun O2n+3 (Tl/1 . . .), where the number of cuprate layers reaches n = 5. Below, we present the structures of the family of Tl-based superconductors in Figs. 2.3 and 2.4.

page 71

March 24, 2021

72

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 2.3. Schematic distribution of ions in the unit cell of superconductors Tl1 Ba2 CaN−1 CuN O2N+4 or, in the brief notation, Tl(1: 2: N-1: N) at N = 1, 2, . . . , 5.

Fig. 2.4. Schematic distribution of ions in the unit cell of superconductors Tl1 Ba2 CaN−1 CuN O2N+4 or, in the brief notation, Tl(1: 2: N − 1 : N ) at N = 1, 2, . . . , 5.

page 72

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors Tl-based systems Tl1 Ba2 CaN−1 CuN O2N+3 .

Table 2.1. N a (˚ A) Tc (K)

73

1

2

3

4

5

6

— 13–15

3.8500 78–91

3.8493 116–120

3.8153 122

3.8469 106

— 102

(a)

(b)

Fig. 2.5. Structure of energy bands near the Fermi energy for, (a) high-temperature superconductor Bi2 Sr2 CaCu2 O8 and, (b) low-temperature superconductor Bi2 Sr2 CaCuO6 .

In Table 2.1, we show the dependences of Tc and the interplane distance (˚ A) on the number of layers in the unit cell N . The explanation of the dependence of the critical temperature on the number of cuprate layers is an urgent problem [49, 50]. All high-temperature superconductors have a complicated multiband structure [139] shown in Fig. 2.5. We note the importance of the structure of zones near the Fermi level. For example, the structures of the bands of two superconductors (hightemperature Bi2 Sr2 CaCu2 O8 and low-temperature Bi2 Sr2 CaCuO6 ) are signiﬁcantly diﬀerent at point K. The energy interval from the band bottom to the Fermi surface is equal to 0.7 eV at point K for the high-temperature

page 73

March 24, 2021

74

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

superconductor and 0.1 eV for the low-temperature one. The explanation of the inﬂuence of the multiband structure on Tc is given in Chapter 3 of this book. It is worth noting that all copper-oxide superconductors have block character of their structure. The main block deﬁning the metallic and superconductive properties of a compound of a plane with CuO2 which contains the square lattice of Cu ions coupled with one another through oxygen ions. Depending on the composition, the elementary cell of a hightemperature compound can have one, two, three, and more cuprate layers. Moreover, the critical temperature of the superconducting transition has a nonmonotonous dependence on the number of cuprate layers [49].

2.3.1. Phase diagram of cuprate superconductors All electron properties of high-temperature superconductors depend strongly on the doping. High-temperature superconductors without doping are dielectrics and antiferromagnetics. As the concentration x increases, these materials become metals. Superconductivity arises at large x, behind the limits of the magnetically ordered phase. The experiments showed that the charge carriers have the hole character for all classes of high-temperature superconductors. It becomes clear recently that the high-temperature superconductivity is related to peculiarities of the behavior of these compounds in the normal phase. As seen from the phase diagram (Fig. 2.6), the superconducting states arise near the antiferromagnetic phase. In yttrium-containing systems, the antiferromagnetic and superconducting regions adjoin one another. The experiments on the inelastic magnetic scattering of neutrons indicate the existence of strong magnetic ﬂuctuations in the doped region, even beyond the limits of the antiferromagnetic phase. This points out the important role of antiferromagnetic ﬂuctuations in the compounds with hightemperature superconductivity. In high-temperature superconductors, the gap is present in the absence of the phase coherence, i.e., in nonsuperconducting specimens. This gap is called a pseudogap. A pseudogap is shown in Fig. 2.6. It appears at temperatures less than some characteristic temperature T ∗ which depends on the doping. Its nature is not completely explained else. The study of a pseudogap in the electron spectrum of high-temperature superconductors was carried out in many works [51]. Metals become superconductors, if their free electrons are bound in Cooper’s pairs. Moreover, the pairs are formed in such a way that their wave functions have the same phase. The phase coherence is responsible for

page 74

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

75

Fig. 2.6. Phase diagram of cuprate superconductors in the temperature-doping variables, TN — the N´eel temperature, Tc — the critical temperature of the superconducting transition, T ∗ — the characteristic temperature of a pseudogap, T 0 — upper crossover temperature.

the change of the resistance on the cooling below the critical temperature Tc . The presence of coupled pairs in a superconductor causes the appearance of a gap in the spectrum of excitations. In the standard superconductors, the phase coherence of pairs appears simultaneously with the appearance of pairs. From one viewpoint, a pseudogap is related to the appearance of coupled pairs, which is not related to the phase coherence. Another viewpoint consists in the following. The pseudogap arises in HTSC in connection with the formation of magnetic states which compete with superconducting states. The eﬀorts of experimenters aimed at the solution of this dilemma are complicated by a strong anisotropy of the superconductor gap. Some physicists believe that the most probable situation is related to the creation of the superconducting state with paired electrons at a certain doping which coexists with antiferromagnetism. It is possible that just it is the “new state of matter” which has been widely discussed for the last years in connection with HTSC.

2.3.1.1. Antiferromagnetism of HTSC An interesting peculiarity of copper-oxide compounds which has universal character consists in the presence of the antiferromagnetic ordering of spins of Cu in the CuO2 planes. The suﬃciently strong indirect exchange interaction of spins of Cu induces the 3D long-range antiferromagnetic order with the relatively high N´eel temperatures TN = 300–500 K [52]. Though the longrange order disappears in the metallic (and superconducting) phase, strong

page 75

March 24, 2021

76

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

ﬂuctuations with a wide spectrum of excitations are conserved. This allows one to advance a number of hypotheses on the possibility of electron pairing in copper-oxide compounds through the magnetic degrees of freedom. Therefore, the study of the antiferromagnetic properties of hightemperature superconductors is of importance for the veriﬁcation of the hypotheses on the magnetic mechanism of superconductivity. The interaction of spins of Cu in a plane has 2D character, and their small values, S = 1/2, lead to signiﬁcant quantum ﬂuctuations. The ﬁrst indications to the existence of antiferromagnetism in the copperoxide compounds were obtained on the basis of macroscopic measurements of susceptibility. The detailed investigation of both the magnetic structure and spin correlations in the metallic phase became possible only with the help of the neutron scattering.

2.4. Mechanisms of Pairing of High-Temperature Superconductors To explain the high-temperature superconductivity, a lot of models and mechanisms of this unique phenomenon were proposed. The key question is the nature of the mechanism of pairing of carriers. There are available many diﬀerent models of superconductivity, among which we mention the following ones: the magnon model, exciton model, model of resonant valence bonds, bipolaronic model, bisoliton model, anharmonic model, model of local pairs, plasmon model, etc. We give some classiﬁcation of mechanisms of pairing for high-temperature superconductors which is shown in Fig. 2.7, according to [53]. This classiﬁcation demonstrates the diverse physical pattern of hightemperature superconductors. Together with the ordinary BCS mechanism based on the electron– phonon interaction, there exist many other mechanisms, as was mentioned above. All these models used the conception of pairing with the subsequent formation of the Bose-condensate at temperatures Tc irrespective of the nature of the resulting attraction.

2.4.1. Specific mechanisms of pairing in superconductivity Consider the models most popular at the present time. Along with the ordinary BCS mechanism based on the electron–phonon interaction, we turn to the magnetic, exciton, plasmon, and bipolaronic mechanisms of pairing. All these models applied the conception of pairing with the subsequent

page 76

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

Fig. 2.7.

77

Classification of mechanisms of pairing in HTSC.

formation of a Bose-condensate (at certain temperatures Tc ) regardless of the reasons for the attraction. The BCS theory presents the formula for the critical temperature Tc in the case of the weak electron–phonon interaction: Tc = 1.14Θ exp(−1/N0 V ),

(2.1)

where Θ = ΩD /kB , ΩD is the Debye energy, N0 is the density of states of the Fermi level, and V is the attractive pairing potential acting between electrons. The maximum value of the critical temperature given by the BCS theory is 40 K. Therefore, there arises the question about the other mechanisms of pairing. The interaction of electrons is repulsive, i.e., one needs to seek a

page 77

March 24, 2021

78

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

“transfer system” in metals which is distinct from the phonon system. The general scheme of the interaction of electrons via a transfer system X can be schematically presented as e1 + X → e11 + X ∗ , (2.2) e2 + X ∗ → e12 + X, where ei corresponds to an electron with momentum pi , X is the ground state, and X ∗ is the excited state of the transfer system. As a result of this reaction, the system returns to the initial state, and the electrons make exchange by momenta. It can be shown that such an interaction leads to the attraction, and the critical temperature is given by the formula Tc ∼ ΔE exp(−1/λ), where ΔE is the diﬀerence of energies of the states X and X ∗ , and λ depends on the interaction of electrons with the system X [54].

2.4.2. Magnetic mechanism of pairing The magnetic mechanism of pairing in high-temperature superconductors was studied by many researchers. These studies used the assumption that the pairing is realized due the exchange by spin excitations — magnons, i.e., the transfer system is the system of spins in a magnetic metal. Magnon is a quasiparticle which is the quantum synonym of a spin wave of excitation in a magnetically ordered system. A great attention was attracted by the pioneer work by A.I. Akhiezer and I.Ya. Pomeranchuk (see [55, 56]). They considered the interaction between conduction electrons caused by both the exchange by acoustic phonons and an additional interaction related to the exchange by spin waves (magnons). It was shown that superconductivity and ferromagnetism can coexist in the same spatial regions. At suﬃciently low concentrations of the ferromagnetic component, an increase of its concentration leads to an increase of Tc in the case of the triplet pairing. Within the phonon mechanism, the pairing occurs in a singlet state, then an increase of the concentration of the ferromagnetic component induces a decrease of Tc . It is known that ferromagnetism competes with superconductivity. The diﬀerent situation is characteristic of antiferromagnetism. High-temperature superconductors are antiferromagnetic dielectrics. As was mentioned above, high-temperature superconductors reveal strong magnetic ﬂuctuations in the region of doping which can be responsible for the pairing. In this chapter, we will consider the spin-ﬂuctuation model of pairing.

page 78

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

79

After the discovery of HTSC, a lot of relevant works dealt with namely the problem of the evolution of a system of Cu ions under the transition from the dielectric antiferromagnetic state to the metallic one. It is worth also noting the model of resonance valence bonds (RVB) which was advanced by Nobel’s Prize winner P. Anderson in 1987 [5] who made attempt to explain the Cooper pairing in HTSC by the participation of magnetic excitations. The Anderson model is based on the conception of magnetic ordering which was named the model of resonance valence bonds. The RVB mechanism ensures the joining of carriers in pairs with compensated spin, the so-called spinons. At the doping of HTSC compounds, there arise holes which can form the complexes with spinons—holons. Superconductivity is explained by the pairing of holons, i.e., by the creation of spinless bosons with double charge. That is, the pairing of carriers in the RVB model is realized due to the exchange by magnons. At low temperatures, the paired holons form a superconducting condensate. The RVB model has played a positive role, by attracting the attention of researchers to the study of antiferromagnetism in HTSC though spinons and holons have not been experimentally identiﬁed.

2.4.3. Exciton mechanisms of pairing According to the general principle concerning the “transfer system” in superconductors, the electron–phonon interaction should not be obligatorily realized. Some other interaction ensuring the pairing of electrons can be suitable. In principle, the mechanism of superconductivity can be switched on by bound electrons which interact with conduction electrons. The ﬁrst exciton model, in which the pairing is realized due to electron excitations, was proposed by W.A. Little [57] for organic superconductors and V.L. Ginzburg and D.A. Kirzhnitz [42] for layered systems. In the construction of this model, it was necessary to assume the existence of two groups of electrons: one of them is related to the conduction band, where the superconducting pairing occurs due to the exchange by excitons which are excitations in the second group of almost localized electrons. In view of the many-band character of the electron spectrum, layered structure, and other peculiarities of the electron subsystem in high-temperature superconductors, such a distribution of electron states is quite possible. This underlies the development of a lot of exciton models. The searches for superconductivity in organic materials were stimulated to a signiﬁcant degree by the idea of W.A. Little about a possibility of high-temperature superconductivity due to the excitonic mechanism of the Cooper pairing of electrons in long conducting polymeric

page 79

March 24, 2021

80

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

chains containing lateral molecular branches-polarizers. Since the mass M of such excitonic excitations is small, it would be expected to observe a high value of the temperature Tc ∼ M −1/2 . But this model was not practically realized, since high-energy intramolecular excitonic excitations cannot ensure the binding of electrons in pairs. At the present time, a number of quasi-one-dimensional organic superconductors with metallic conductance have been synthesized. They pass to the superconducting state at T = 10 K. Crystals of similar organic superconductors consist of, as a rule, planar molecules packed in zigzag-like stacks which form chains. The good overlapping of electron wave functions of neighboring molecules in a stack ensures the metallic conductance along a chain. The overlapping of electron wave functions of neighboring chains is small, which leads to the quasi-one-dimensional character of the electron spectrum and to a strong anisotropy of electronic properties of a crystal. Up to now, no experimental proofs of a manifestation of the excitonic mechanism is such systems are available. As the example of a laminar system, we mention a quasi-two-dimensional structure of the “sandwich” type (dielectric–metal–dielectric). In such structures, the Cooper pairing of electrons in a metal ﬁlm occurs due to the attraction caused by their interaction with excitons in the dielectric plates.

2.4.4. The anharmonic model and superconductivity It is known that the appearance of superconductivity is often preceded by structural transformations in a crystal. They are usually explained within the anharmonic model. In the opinion of some researchers [47], such structural transformations foregoing the start of superconductivity decrease signiﬁcantly the frequencies of phonons and, due to this, increase the parameter of electron–phonon interaction. The softening of the phonon spectrum is caused by the great amplitudes of displacements of ions in the two-well potential which models the structural transformations. In some works [52], the eﬀect of a structural transformation on superconductivity in the limiting case of a weak pairing interaction and the isotropic gap was studied. The properties of high-temperature superconductivity were studied also within the model, where the superconductivity is enhanced due to the singularity of the density of electron states which appears at structural or antiferromagnetic phase transitions. The weak point of the models relating the superconductivity to structural phase transitions owes to a signiﬁcant temperature interval between the known structural transitions and the temperature Tc . The works, where non-phonon pairing mechanisms

page 80

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

81

are introduced, include the studies [52] which use the Hubbard Hamiltonian in systems, where only the interaction of repulsive type is present. It is considered that the eﬀect of pairing is caused by the kinematic interaction at a non-complete occupation of Hubbard subbands. Unfortunately, no clear comprehension of the nature of the arising attraction is attained in this case. It is possible that the bound state of quasiparticles is virtual, i.e., it decays. The search for new mechanisms of superconductivity caused by a strong correlation of electrons in cuprate superconductors with quasi-twodimensional electron structure is reduced to the search for new non-standard ground states. We brieﬂy mention the polaron mechanism of pairing which is related to the Jahn–Teller eﬀect well-known in the quantum chemistry of complex compounds. The essence of the Jahn–Teller eﬀect consists in that a nonlinear system in the presence of the electron degeneration deforms spontaneously its structure so that this degeneration disappears or decreases. The Jahn–Teller eﬀect leads to the rearrangement of the atomic orbitals of copper under conditions of the octahedral oxygen surrounding. A displacement of oxygen ions inside of an elementary cell which is caused by the appearance of a quasiparticle induces the displacement of equilibrium positions in the neighboring cells. In such a way, there arises the strong electron–phonon interaction of a quasiparticle with a local deformation.

2.4.5. Van Hove singularities (vHs) A van Hove singularity (vHs) in the density of states (DOS) N (E) has been proposed as a Tc -enhancement mechanism for intermetallic superconductors two decades ago. All cuprate superconductors possess two-dimensional elements of their structures. In the construction of the microscopic theory of high-temperature superconductivity, it is important to clarify the speciﬁc features of the dispersion E(k) and the behavior of the density of states N (E). For a two-dimensional problem (n = 2, 2D), the density of states is independent of the energy, N (E) = constant, and the band is dispersionless. The photoemission experiments indicate the existence of an almost ﬂat band near the Fermi surface for cuprate superconductors. The presence of a ﬂat band and an isoenergetic surface in the form of the elongated saddle leads to the existence of van Hove singularities in the density of states near the Fermi surface. In this model in the calculations of Tc by the BCS formula, N (E) is replaced by N (EF ). The formula for Tc looks like Tc = 1.14Θ exp(−1/λ), where λ = V N (E).

(2.3)

page 81

March 24, 2021

82

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

If the function N (E) has the corresponding singularity at E = EF , it will be related to the van Hove singularity. In the two-dimensional case, the presence of a logarithmic singularity of the density of states on the Brillouin zone boundary is possible: D , N (E) ∼ ln (2.4) E − EF where D is the characteristic energy cutoﬀ. Then Tc has the form: √ Tc ∼ D exp(−1/ λ).

(2.5)

We note that, in connection with the quasi-two-dimensionality of lattices of HTSC, the hypothesis of anyonic superconductivity is of a certain interest (Fig. 2.7). Anyons are quasiparticles with intermediate statistics (between the Bose- and Fermi-statistics) which can exist just in two-dimensional structures. The term “anyon” was introduced by F. Wilczek in the framework of the conception of supersymmetry.

2.4.6. Plasmon mechanism of pairing Many works are devoted to attempts to explain the high-temperature superconductivity on the basis of the idea of the pairing as a result of the exchange by quanta of longitudinal plasma waves — plasmons. Longitudinal plasma waves are formed in solids in the region of frequencies, at which the dielectric permeability of the medium becomes zero. The characteristic frequency of plasma waves in 3D crystals is deﬁned by the formula ω ˜ p = 4πe2 N/m,

(2.6)

where N is the concentration of electrons, and e and m are their charge and mass, respectively. At the electron density N ∼ (1–3) × 1022 cm−3 , the plasma frequency ω ˜ p ∼ 1015 –1016 . We might assume that the exchange by plasmons, rather than by phonons, would induce an increase of the preexponential factor in the formula deduced in the BCS theory, 1 , (2.7) Tc = Θ exp λ − μ∗ by two-three orders, if Θ = ˜ ωp /kB . However, such an increase does not cause a signiﬁcant growth of Tc , because the plasmons at the frequency ω ˜ p which is close to the frequency of electrons, EF /, cannot cause the superconducting pairing and their role is important only for the dielectric properties of crystals [46].

page 82

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

83

2.4.7. Bipolaronic mechanism of superconductivity One of the attempts to explain the phenomenon of high-temperature superconductivity was named the bipolaronic theory. Bipolarons are Boseparticles like the ordinary Cooper’s pairs. In the theory of bipolarons, the superconductivity is caused by the superﬂuidity of the Bose-condensate of bipolarons. The ideas of polarons and bipolarons were used by A.S. Aleksandrov and J. Ranninger [58] to clarify the high-temperature superconductivity. The idea of a polaron is based on the assumption about the autolocalization of an electron in the ion crystal due to its interaction with longitudinal optical vibrations under the local polarization which is caused by the electron itself. The electron is conﬁned in the local polarization-induced potential well and conserves it by the own ﬁeld. The idea of the autolocalization of electrons in ion crystals was intensively developed by S.I. Pekar [59]. The eﬃciency of the interaction of an electron with mass m and charge e with long-wave longitudinal optical vibrations with frequency Ω in the medium is characterized by the dimensionless parameter e2 m/2Ω2 (2.8) ε˜ introduced by H. Fr¨ ohlich. Here, ε˜ is the dielectric permeability of the inertial polarization. The interaction is assumed to be small if g < 1. Due to a high frequency Ω, the deformation ﬁeld is a faster subsystem. Therefore, it has time to follow the movement of an electron. This ﬁeld accompanies the movement of the electron in the form of a weak cloud of phonons. The energy of interaction of the ﬁeld and the electron is proportional to the ﬁrst degree of g. In the BCS theory, the pairing of conduction electrons is realized due to the interaction with acoustic phonons and is characterized by the dimensionless constant of interaction g=

λ = V N (EF ),

(2.9)

where N (EF ) is the density of energy states of electrons on the Fermi surface, and the quantity V is inversely proportional to the coeﬃcient of elasticity of a crystal. In the bipolaronic model [60], we have the parameter λ∗ = (2λ2 Ωz − Vc )/D,

(2.10)

where λ is deﬁned by relation (2.9), z is the number of the nearest neighbors, D is the width of the conduction band of free quasiparticles.

page 83

March 24, 2021

84

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

A bipolaron, like a Cooper’s pair, has charge 2e, and its eﬀective mass is determined by the formula m ˜ ≈m

exp(λ2 ). D

(2.11)

The eﬀective mass m ˜ can be very high and can excess the mass of a free quasiparticle in the conduction band by several orders. To calculate the superconducting transition temperature Tc which corresponds to the Bose-condensation, the authors applied the formula for the ideal Bose-gas ˜ kB Tc = 3.312 N 2/3 /m.

(2.12)

At m ˜ = 100 and N = 1021 cm−3 , the last formula yields Tc ∼ 28 K. Analogously to the bipolaronic model, the bisoliton mechanism of hightemperature superconductivity was proposed in [47, 49].

2.5. The Symmetry of Pairing in Cuprate Superconductors Of great importance for high-temperature superconductors is the pairing symmetry or the symmetry of the order parameter. This question was considered at many conferences and seminars over the world. Several NATOseminars and conferences on this trend which hold in Ukraine in the town of Yalta were organized by one of the authors of this book [61–64]. The development of the microscopic theory of superconductivity was followed by the interest in the question about the nontrivial superconductivity corresponding to the Cooper’s pairing with nonzero orbital moment. The system, in which the nontrivial pairing was ﬁrst discovered, is He3 . To explain this phenomenon, it was necessary to introduce a supplementing mechanism of pairing due to spin ﬂuctuations.

2.5.1. Superconductor’s order parameter Most physical properties depend on the properties of the symmetry of a superconductor’s order parameter which is deﬁned by the formula Δαβ (k) = aαk aβ−kα .

(2.13)

The problem of pairing symmetry is the problem of the pairing of charged fermions into states with the ﬁnal orbital moment. As usual, both the standard pairing called the s-pairing and the nonstandard d-pairing are considered. They diﬀer by the orbital moment

page 84

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

85

of the pair: in the ﬁrst and second cases, the moments are L = 0 and L = 2, respectively. We note also that the continuous symmetry group in crystals is broken, and it is necessary to speak not about the orbital moment, but about the irreducible representations, by which the order parameter is classiﬁed. We will consider this question in the following subsection. Usually, the standard pairing frequently called the s-pairing and the nonstandard pairing are distinguished. At the nonstandard pairing, the symmetry of the order parameter is lower than the symmetry of a crystal. For a two-dimensional tetragonal crystal (square lattices), the possible symmetries of the superconductor’s order parameter were enumerated by M. Sigrist and T.M. Rice [65] on the basis of the theory of group representations. The basis functions of relevant irreducible representations deﬁne the possible dependence of the order parameter on the wave vector. It is worth noting that the anisotropic pairing with the orbital moment L = 2, i.e., dx2 −y2 , has the following functional form in the k space: Δ(k) = Δo [cos(kx a) − cos(ky a)],

(2.14)

where Δo is the maximum value of the gap, and a is the lattice constant. The gap is strongly anisotropic along direction (110) in the k space. In this case, the order parameter sign is changed in the directions along kx and ky . Together with the d-symmetry, it is worth to consider also the ssymmetry, for which we can choose two collections of basis functions: Δ(k) = Δo .

(2.15)

The anisotropic s-pairing is considered as well. This form of the pairing is analyzed in works by P.W. Anderson [5] with co-workers who have studied the mechanism of pairing on the basis of the tunneling of electrons between layers. In these states, the order parameter sign is invariable, and its amplitude is varied along direction (110): [anisotropic s]Δ(k) = Δo [cos(kx a) − cos(ky a)]4 + Δ1 ,

(2.16)

where Δ1 corresponds to the minimum along direction (110). It follows from the symmetry-based reasoning that the mixed states with various symmetries can be realized. We mention the states which are mostly in use. The “extended” s-coupled states were considered in works by D.J. Scalapino [67]. A possible functional form of these states is as follows: [extended s-wave] Δ(k) = Δo {(1 + γ 2 )[cos(kx a) − cos(ky a)]2 − γ 2 }. (2.17)

page 85

March 24, 2021

86

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

They have eight parts with alternating signs and eight nodes which are split by ±γπ/2 along direction (110). G. Kotliar with co-workers used mixed s + id states [67]: [s + id] Δ(k) = Δo [ε + i(1 − ε)[cos(kx a) − cos(ky a)]].

(2.18)

R.B. Laughlin [66] analyzed the mixed states dx2 +y2 + idxy on the basis of the anyonic mechanism of pairing: [d + id]Δ(k) = Δo [(1 − ε)[cos(kx a) − cos(Ky a)] + iε[2 sin(kx a) sin(ky a)]],

(2.19)

where ε is the share of s or dxy states mixed with the dx2 +y2 states, and εΔo is the minimum value of the energy gap. These mixed states are of interest because they are not invariant with respect to the inversion in the time. The value and phase of the superconductor’s order parameter, as functions of the direction in cuprate planes CuO2 are given in Fig. 2.8 for various kinds of the pairing symmetry.

2.5.2. Classification of the superconductor’s order parameter by the representations of symmetry groups It should be noted that there is no classiﬁcation of states by the orbital moment for crystals. The general theory of nonstandard pairing has been developed on the basis of the analysis of point symmetry groups. J. Annett was one of the ﬁrst who classiﬁed superconducting states by the irreducible representations of groups for high-temperature superconductors [68]. As for superconductors with heavy fermions, the group analysis was carried out in [69]. Of importance is the question whether the symmetry of the order parameter in HTSC is lower than the symmetry of the crystal lattice. The order parameter can be represented as a linear combination ηΓi fΓi (k), (2.20) Δk = where ηΓi is the irreducible representation of groups, by which the order parameter is transformed, fΓi (k) is basis functions of the irreducible representation, A1g corresponds to the anisotropic s-symmetry, and B1g corresponds to the d-pairing.

page 86

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

87

Fig. 2.8. Kinds of pairing symmetries which are considered for high-temperature superconductors.

An analogous decomposition of the superconducting order parameter was performed for a superconductor with heavy fermions U P t3 . The symmetric states of the system can be presented by the indication of all possible subgroups of the full group, relative to which the order parameter

page 87

March 24, 2021

88

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

is invariant [70]. The full symmetry group of a crystal includes a point symmetry group G, operations of inversion of the time R, and the group of calibration transformations U (1). That is, we have the following partition into subgroups: G × R × U (1).

(2.21)

The La- and Y-based superconductors which have the tetragonal symmetry of crystal lattices, i.e., G = D4h = D4 × I [62], are most studied. In the Y-based compounds, one observes small orthorhombic distortions of a crystal lattice. Group D4h includes the operations of rotations Cn , around the z-axis by angles of πn/2 and rotations Un by angles of π: x cos(πn/2) + y cos(πn/2),

(2.22)

where n = 0, 1, 2, 3 have ﬁve reducible representations: four one-dimensional (A1g , A2g , B1g , B2g ) and one two-dimensional (E).

2.6. Experimental Studies of a Symmetry of the Superconducting Order Parameter At the present time, the results of three groups of experiments, in which the symmetry of the order parameter is revealed, are available. The ﬁrst group joins diﬀerent low-temperature characteristics of superconductors such as the Knight shift, the rate of relaxation in NMR, the temperature dependence of the heat capacity, the penetration depth, etc. If the superconductor’s order parameter has zeros on diﬀerent areas of the Fermi surface (as in the case of the dx2 −y2 -symmetry), the mentioned quantities will have the power temperature dependence, rather than the exponential one. The second group of experiments is based on the direct measurement of the phase of the order parameter with the help of interference phenomena on Josephson junctions in a magnetic ﬁeld. The third group deals with the direct measurements of a value of the gap by means of spectroscopic experiments. Here, the most interesting results are presented by photoemission spectroscopy with angle resolution, and Raman and neutron spectroscopies.

2.6.1. Measurements of the Josephson tunnel current The most deﬁnite information about a symmetry of the superconducting order parameter can be obtained from the studies of the phase of the order

page 88

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

89

parameter, in which the critical current in Josephson junctions positioned in a magnetic ﬁeld is measured. The critical current for a rectangular Josephson junction oscillates with the ﬁeld by the Fraunhofer diﬀraction law: Ic (Φ) = J0 A

sin(πΦ/Φ0 ) , πΦ/Φ0

(2.23)

where Φ is the magnetic ﬂux through the junction, Φ0 is the quantum ﬂux, J0 is the density of the critical current in the zero ﬁeld, and A is the junction area. A diﬀraction pattern is shown in Fig. 2.9(a). Let us consider the superconductor Y BCO which possesses the tetragonal symmetry. Let its axis be oriented normally to the plane of the ﬁgure, and let its edges be perpendicular to the axes A and B of the base plane. In the tunnel junction with corner geometry, another superconductor is applied to both edges which are perpendicular to A and B and, moreover, are joined with each other (Figs. 2.9(b) and 2.9(c)). This experiment can be compared with that involving a two-junction SQUID, in which there occurs a superposition of tunnel currents produced by electrons with wave vectors kx and ky , so that the resulting diﬀraction pattern depends on the symmetry of the order parameter of a superconductor under study. At the s-symmetry, the order parameter on both edges of the corner junction is the same, and the resulting diﬀraction pattern will be such as that in the case of the standard junction. But, in the case of the d-symmetry, the order parameter on the corner junction edges has diﬀerent signs, and this fact changes basically the diﬀraction pattern. The total current is illustrated in Fig. 2.10(a). In the zero ﬁeld, the critical current turns out to be zero due to the mutual compensation of its two components. In the symmetric contact, the dependence on the ﬁeld is determined by the formula [71] Ic (Φ) = J0 A

sin2 (πΦ/2Φ0 ) , πΦ/2Φ0

(2.24)

corresponding to the pattern in Fig. 2.10(b). Thus, by the diﬀerence of a diﬀraction pattern from both the standard one and that corresponding to the corner Josephson junction, we can judge about a symmetry of the order parameter. In work [71], a similar experiment was carried out on the tunnel junction YBCO–Au–Pb. The results presented in Fig. 2.10 testify to the d-symmetry of the order parameter in superconducting YBCO.

page 89

March 24, 2021

90

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity (a)

(b)

(c)

Fig. 2.9. Critical current in a Josephson junction versus the applied magnetic field: (a) standard tunnel contact, (b) corner tunnel junction for a superconductor with the s-symmetry of the order parameter, (c) corner tunnel junction for a superconductor with the d-symmetry of the order parameter [71].

page 90

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

91

(a)

(b)

Fig. 2.10. Critical current as a function of the magnetic field in a Josephson junction YBCO–Au–Pb in two0 geometries: (a) standard and (b) corner ones [71].

All the above-mentioned experiments with Josephson junctions were performed with a single crystal YBa2 Cu3 O6 .

2.6.2. Measurements of the quantization of a flow by the technique of three-crystal unit Another type of experiments on the determination of a symmetry of the order parameter is based on the measurement of a ﬂow quantum in a superconducting ring fabricated from three superconducting single crystals of yttrium with diﬀerent orientations.

page 91

March 24, 2021

92

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

The idea of such an experiment is based on the theoretical result obtained by M. Sigrist and T.M. Rice [65]: for superconductors with the d-symmetry, the tunnel current between two superconducting crystals separated by a thin boundary depends on the orientation of the order parameter with respect to the interface. The current between the superconductors with numbers ij is given by the formula Isij = (Aij cos 2θi cos 2θj ) sin ΔΦij .

(2.25)

Here, Aij is the constant which characterizes the junction of ij, θi , θj are the angles of the crystallographic axes with the boundary plane, and Φij is the diﬀerence of phases of the order parameters on both sides of the boundary. It was shown that a spontaneous magnetization, which corresponds to the ﬂow equal to a half of Φ0 , appears in a superconducting ring with a single Josephson junction with the phase diﬀerence π. If the ring has odd number of π-junctions, the result is the same. The direct measurement of a halfquantum of the ﬂow through such a ring would testify to the d-symmetry of the order parameter. The direct measurement of a half-quantum of the ﬂow was realized in work [72]. The scheme of the experiment is shown in Fig. 2.11.

Fig. 2.11. Scheme of the experiment on the measurement of a half-integer number of quanta of the flow captured by a superconducting ring with three Josephson junctions with the d-symmetry of the order parameter [34].

page 92

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

93

2.7. Thermodynamics of the d-Pairing in Cuprate Superconductors 2.7.1. Introduction The basic question of the theory of superconductivity concerns the mechanism ensuring the pairing of electrons. In the BCS theory, it is the electron– phonon interaction. Some recent theoretical models postulate the mechanism of antiferromagnetic spin ﬂuctuations [73–79], so that the electron scattering on them can be the reason for the pairing of electrons. Spin ﬂuctuations play an important role in superconductors with heavy fermions [76, 77]. The authors of works [68, 69] performed the calculations of a value of the superconductor gap, the critical temperature, the temperature dependence of the resistance, and many other quantities, but the thermodynamics was not considered. For this reason, it is of interest to calculate the thermodynamics of antiferromagnetic spin ﬂuctuations, namely the temperature dependence of the heat capacity, its jump near Tc , and the parameter R = ΔC/(γTc ) equal to 1.42 by the BCS theory. The purpose of this section is the calculation of the thermodynamics of antiferromagnetic spin ﬂuctuations, namely the electron heat capacity and the jump of the heat capacity. The thermodynamics of superconductors at low temperatures is determined by the excitation of two quasiparticles. In the traditional superconductors with pairing of the BCS-type, the energy gap is isotropic (s-pairing), and the temperature dependence of the heat capacity has the exponential form ∼ exp−Δ/kB T , where Δ is the superconductor’s gap. In the superconductors with the anisotropic pairing, the temperature dependence of the heat capacity has a power character, namely, T n . The appearance of such temperature dependences is related to the fact that the superconductor’s gap has zeros on the Fermi surface. As was noted above, the anisotropic pairing with the orbital moment L = 2, i.e., with the dx2 −y2 -symmetry, has the following functional form in the k space: Δ(k) = Δo [cos(kx a) − cos(ky a)],

(2.26)

where Δo is the maximum value of the gap, and a is the lattice constant. The gap is strongly anisotropic in direction (110) in the k space, and the sign of the order parameter is changed along the directions kx and ky . The main results of this section are published in works [82–85].

page 93

March 24, 2021

94

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

2.7.2. Antiferromagnetic spin fluctuations in high-temperature superconductors For the ﬁrst time, the idea of the possibility for the electron pairing through spin ﬂuctuations was advanced by A.I. Akhiezer and I.Ya. Pomeranchuk [85]. They showed that the indirect interaction of electrons through spin waves in a ferromagnetic metal has the character of attraction in the triplet state and, hence, can lead to the triplet pairing. Consider some experiments and facts on antiferromagnetic spin ﬂuctuations. The basis for the hypothesis on the spin-ﬂuctuation mechanism of pairing consists in the fact that the stoichiometric compounds La2 CuO4 and YBa2 Cu3 O6 are antiferromagnetic dielectrics. The doping of superconductors leads to the appearance of the metallic state and superconductivity. The closeness of high-temperature superconductors to the antiferromagnetic transition with the wave vector Q = (π/a, π/a) deﬁnes the important role of spin ﬂuctuations, the interaction with which forms the quasiparticle spectrum of electrons and can simultaneously cause the Cooper’s pairing. High-temperature superconductors are referred to the class of strongly correlated systems which are theoretically studied in the frame of the Hubbard model. This model describes the hops of electrons in the lattice with the matrix element t for the nearest neighbors with regard for the Coulomb repulsion U , when the electrons are positioned at the same site. The model is set by the Hamiltonian † Ciσ Cjσ + U ni↑ ni↓ , (2.27) H = −t i,j,σ

i,

† (Cjσ ) is the operator of creation (annihilation) of an electron at where Ciσ † Cjσ is the number of electrons at the site i with spin σ, and ni↑ = Ciσ the site. In the given region of the parameters t, U , and n (the electron concentration), the appearance of magnetically ordered phases is possible. Near the boundary of the existence of such a phase from the side of the paramagnetic region, strong ﬂuctuations of the magnetic order parameter, paramagnons, must be manifested. In the two-dimensional system of CuO layers in cuprate superconductors, the electron spectrum is presented by the formula

ε (t) = −2t cos kx a + cos ky a),

(2.28)

and the chemical potential μ is determined by the given electron concentration n. On the half-ﬁlling (n = 1), this spectrum has the nesting at the wave vector q = Q, which induces a sharp peak in the spin susceptibility near this

page 94

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

95

point. This means an instability of the system relative to the formation of the antiferromagnetic state with the wave vector Q and the intensiﬁcation of spin ﬂuctuations near the point of the magnetic phase transition. Near the half-ﬁlling, when the system is really antiferromagnetically unstable, the numerical calculations indicate that the superconducting order parameter has d-symmetry, i.e., the gap depends on the wave vector by relation (2.26). Gap (2.26) is an alternating function of the wave vector (Fig. 2.12) and has zero values on the diagonals. Figure 2.12 shows that the wave function of a Cooper’s pair is equal to zero just on the diagonals of the square. Therefore, the repulsive interaction on these diagonals does not act on the pair, and a Cooper’s pair with the d-symmetry survives even at large values of U . The superconductors with the d-pairing should have a number of particular properties which can be observed in experiments. Many of these peculiarities are related to the zeros of the order parameter. The quasiparticle spectrum at low temperatures must give the power contribution to the thermodynamic properties, such as the heat capacity, parameters of NMR, and the penetration depth of a magnetic ﬁeld, rather than the exponential one as in ordinary isotropic superconductors. The observation of such power contributions will indicate the presence of a nontrivial order parameter with zeros on the Fermi surface. The totality of experimental data for various high-temperature superconductors indicates the certain realization of the anisotropic order parameter in them and, with a high probability, with the d-symmetry. The last circumstances present the important argument in favor of the spin-ﬂuctuation mechanisms of hightemperature superconductors. One of them is intensely developed by Pines and his co-workers [73,75] who used a phenomenological form of the magnetic

Fig. 2.12.

Distribution of signs of the gap function in the limits of the Brillouin first band.

page 95

March 24, 2021

96

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

susceptibility with the parameters determined from the experiments on cuprates. Let us consider this model in more details. We introduce a Hamiltonian which involves antiferromagnetic spin ﬂuctuations, as it was made in works by Pines [73, 74]: H = Ho + Hint ,

(2.29)

where H0 is Hamiltonian of free electrons. The interaction is described by the Hamiltonian 1 g(q)s(q)S(−q), (2.30) Hint = Ω q where Ω is the cell volume, g(q) is the interaction constant; s(q) =

1 + Ψk+q σαβ Ψkβ 2

(2.31)

α,β,k

is operator of spin density; σαβ is Pauli matrix; Ψ+ k+q,α is operator of creation of an electron with the momentum k + q and the spin projection α; Ψkβ is operator of creation of a hole with the momentum k and the spin projection β; S(−q) is operator of spin ﬂuctuations, whose properties are set by the correlator χ(q, ω) [73, 74], χij (n, m) is the spin susceptibility which is modeled by χ(q, ω) =

χQ , 1 + ξ 2 (q − Q)2 − iω/ωSF qx > 0,

qy > 0,

(2.32)

where χQ is the static spin susceptibility with the wave vector Q = (π/a, π/a), ξ is the temperature-dependent antiferromagnetic correlation length, and ωSF is the characteristic frequency of spin ﬂuctuations of the paramagnon energy. All parameters are taken from experiments, including the data from NMR studies [73]. In this case, the interaction constant is a free parameter of the theory. It can be determined, by calculating some quantity with the help of the Hamiltonian and by comparing the result with experiments. We now deﬁne the quantities χQ and ωSF as χQ = χ0 (ξ/a)2 β 1/2 , ωSF = Γ/(π(ξ/a)2 β 1/2 ),

(2.33) (2.34)

page 96

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

97

where χ0 is the experimentally measured long-wave limit of the spin susceptibility, β = π 2 , and Γ is the energy constant. The NMR data for the compounds yield ξ(Tc ) = 2.3a, ωSF = 8 meV, Γ = 0.4 meV. It is foreseen that the phenomenological Hamiltonian will give a selfconsistent description of the spin dynamics of the system in the sense that the spin susceptibility calculated with its help (through the characteristics of a quasiparticle spectrum which themselves depend on the susceptibility) will agree with values determined by formula (2.32).

2.7.3. Continual model of antiferromagnetic spin fluctuations The authors of works [82–85] proposed a continual model for the spinﬂuctuation mechanism of pairing which allows one to eﬃciently solve the problem of thermodynamics for this mechanism. Let us consider this model in more details. We now calculate the thermodynamics which is set by the Pines spin-ﬂuctuation Hamiltonian. We write the Hamiltonian in the lattice representation (2.35) H = H0 + Hint , 1 ψα+ (n)ψα (n + p) + Si (n)χ−1 H = −t ij (n, m)Sj (m) 2 n,p n,m σ i ψα+ (n) ψβ (n)Si (n), (2.36) +g 2 αβ n H0 = −t

ψα+ (n)ψα (n + p) +

n,p

Hint = g

n

ψα+ (n)

σ i

2

αβ

1 Si (n)χ−1 ij (n, m)Sj (m), (2.37) 2 n,m

ψβ (n)Si (n),

(2.38)

where the sum is taken over all the sites of the inﬁnite lattice (the lattice constant is equal to a), ρ is the unit vector joining the neighboring sites, Si is

the spin operator, N = n ψα+ (n)ψα (n) is the operator of the number of particles, t is the half-width of the conduction band [73,74], and χij (n, m) — the spin correlation function. It is necessary to calculate the grand partition function exp{−βΩ(μ, β, g)} ≡ Tr exp{−β(H − μN )}, β = 1/kT,

(2.39)

page 97

March 24, 2021

20:13

98

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

where μ is the chemical potential, g is the coupling constant, and Ω(μ, β, q) is the thermodynamic potential. It is convenient to use the formalism of continual integration for a system of Fermi-particles. The method of functional integration, i.e., the integration in the space of functions, was proposed by N. Wiener in 1925, but the physicist-theorists paid no attention to this method. Continual integrals were introduced in physics by R. Feynman [4] in the 1940s and were used for the reformulation of quantum mechanics. The continual integration is one of the most powerful methods of the contemporary theoretical physics which allows one to simplify, accelerate, and clarify the process of analytic calculations. The application of the method of continual integration to a system with inﬁnite number of degrees of freedom allows one to develop, in such a way, the diagram theory of perturbations. The grand partition function can be written in the form of a continual integral [87]: exp −βΩ = N

dSi (n)dψα+ (n, τ )dψα (n, τ ) exp

−

β

dτ L(τ ) ,

0

n

(2.40) where L(τ ) =

ψα+ (n, τ )

n

+g

n

+

∂ − μ ψα (n, τ ) − t ψα+ (n, τ )ψα (n + p, τ ) ∂τ n,p

ψα+ (n, τ )

σ i

2

α,β

ψβ (n, τ )Si (n, τ )

1 Si (n, τ )χ−1 ij (n, m, τ )Sj (m, τ ), 2 n,m

(2.41)

where L(τ ) is the Lagrangian of the system, and N is the normalizing factor, N −1 =

n

dSi (n)dψα+ (n, τ )dψα (n, τ ) exp

β

−

dτ L(τ, μ = g = 0) .

0

(2.42) We will use the matrix formalism to construct the theory of perturbations for the Green functions. It is convenient to introduce a four-component

page 98

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

99

bispinor (Majorana) ψ , Ψ= −σ2 ψ ∗ ψ1 ψ= , ψ2

(2.43)

where σ1 is Pauli spin matrices. The Majorana spinor is a Weyl spinor written in the four-component form. Now, we can write L in the form 1− 0 ∂ 0 0 ˆ ˆ − Γ Γ5 μ δ − t(τ − δ)Γ Γ5 Ψ(n, τ ) Γ L= 2 n,p ∂τ × ψ(n + p, τ ) + +

g− Ψ(n, τ )Γi Γ5 Ψ(n, τ )S i (n, τ ) 4 n

1 Si (n, τ )χ−1 ij (n, m, τ )Sj (m, τ ), 2 n,m

where

0

Γ =

0 I

I 0

0 σi

(2.45)

,

−σi Γ = 0 1 0 I= , 0 1 i

(2.44)

,

(2.46)

¯ ≡ Ψ+ Γ0 , δ = δn,n+p , and Γi are where Γi are the Dirac gamma matrices, Ψ given in the chiral representation. ¯ Ψ = CΨ ¯ T , where C is There exists the connection between Ψ and Ψ: the matrix of charge conjugation, C = Γ0 Γ2 , C T = −C. In terms of Ψ, the partition function takes the form β −βΩ =N ndSi (n, τ )dΨ(n, τ )e− 0 dτ L(τ ) . (2.47) e We now use the method of bilocal operators [88] to calculate the grand partition fuction. In this way, we obtain the Schwinger–Dyson equation and the equation of free energy. The details of calculations can be found in [82–85].

page 99

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

100

In order to calculate Ω, we introduce a source of the bilocal operator [88] −βΩ(J)

e

β dSdΨe −

=N

dτ 0

⎤ β 1 Ψ(n, τ )J(m, n, τ, τ )Ψ(m, τ )⎦. × ⎣L(τ ) + n, m 2 ⎡

(2.48)

0

The full Green fermion function is determined by the formula βΩ(J) ¯ dS dΨΨ(n, τ )Ψ(m, τ ) exp{. . .} Gnm (J) = e ¯ = 0|T Ψ(n, τ )Ψ(m, τ )|0 .

(2.49)

Let us write the Schwinger–Dyson equation for the Green function G, by using the method of bilocal operator [85]: δF = 0, δG F (G) = βΩ(J = 0).

(2.50) (2.51)

First, we consider the case of a free system. By integrating over the fermion ﬁelds in the functional integral, we obtain 1 1 −1 0 F0 = βΩ(J) = − Tr Ln(G−1 0 − Γ Γ5 μ + J) + Tr Ln G0 , 2 2 −1 0 ∂ 0 − t(1 − δ)Γ Γ5 . G0 = Γ ∂τ

(2.52) (2.53)

For the interacting system, the free energy takes the form (2.54) F = F0 + Fint .

We represent Fint as a series in g: Fint = n=1 (g2 )Fn . In the lowest order in g, we get the relation F1 = −

g2 i Tr Γ G T rΓj G − 2GΓi GΓj χij , 32

where the Green function for fermions and spins is as follows: ¯ τ ) = G(x, τ ; y, τ ), Ψ(x, τ )Ψ(y, Si (x, τ )Sj (y, τ ) = χij (x, τ ; y, τ ).

(2.55)

(2.56)

page 100

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

Fig. 2.13.

Fig. 2.14.

101

Graphical form of Eq. (2.57).

Graphical form of the right-hand side of Eq. (2.58).

Taking the condition δF/δG = 0 into account, we obtain the Schwinger– Dyson equation 0 G−1 = G−1 0 − Γ Γ5 μ +

g2 i {Γ T rΓj Gχij − 2Γi GΓj χij }, 12

(2.57)

where Γ0 and Γi are Dirac matrices (Fig. 2.13). Here, the continuous line corresponds to the Green function for fermions G, and the wavy line does to the Green function for spins χi,j (= δij χ). The equation for free energy F1 = −

g2 i Tr Γ G TrΓj G − 2GΓi GΓj χij , 32

(2.58)

where G and χij are, respectively, the Green fermion and spin functions, corresponds to the contribution of two vacuum diagrams (Fig. 2.14).

2.7.4. Equation for superconducting gap From Eq. (2.57), it is easy to deduce the equation for a gap which can be found in [74]. By executing the Fourier transformation G(x, τ ) =

∞

π/a

n=−∞ −π/a

d2 k G(k, ωn )eiωn τ −ikx (2π)2

⎧ (2n + 1) π ⎪ ⎪ ⎨ ωn = β × 2nπ ⎪ ⎪ ⎩ ωn = β

for fermions, for bosons,

page 101

March 24, 2021

102

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

we rewrite Eq. Eq. (2.57) in the momentum space as π/a 2 ∞ g2 d p −1 G−1 (k, iωn ) = G (k, iω ) + n 0 4β m=−∞ −π/a (2π)2 × Γi Γ5 T rΓi Γ5 G (p, iωm ) − 2Γi Γ5 G (p, iωm ) Γi Γ5 × χ (k − p, iωn − iωm ) ,

(2.59)

where we set χij = δij χ, ! G−1 0 (k, iωn )

=

0

{iωn − (ε(k) − μ)}I

{iωn + ε(k) − μ}I

0

≡ Γ0 iωn − Γ0 Γ5 (ε(k) − μ),

"

(2.60)

ε(k) = −2t[cos kx a + cos ky a].

(2.61)

According to the standard relation of the diagram technique, we denote the free energy by Σ(k, iωn ). Then we have −1 G−1 (k, iωn ) = G 0 (k, iωn ) − Σ(k, iωn ),

(2.62)

and Eq. (2.57) is the equation for Σ. We write the solution for Σ in the form Σ = Γ0 A + Γ0 Γ5 B + Δ + Γ0 Γ5 Γi Δ i

(2.63)

(A, B, Δ, and Δi are functions of k and iωn ). By determining the matrix which is inverse to (2.62), we get G(k, iωn ) =

Γ0 (ωn − A) − Γ0 Γ5 (ε(k) − μ + B) + Δ + Γ0 Γ5 . (ωn − A)2 − (ε(k) − μ + B)2 − Δ2 − Δ2i

(2.64)

Substituting (2.64) and (2.63) in (2.63), we obtain the system of equations for the functions A, B, Δ, and Δi : A(k, iωn ) =

B(k, iωn ) =

3g2 d2 p iωn − A(p, iωm ) 4β m D(iωm , p) (2π)2 × χ(k − p, iωn − iωm ), 3g2 d2 p ε(p) − μ + B(p, iωm ) 4β

m

(2π)2

(2.65)

D(iωm , p)

× χ(k − p, iωn − iωm ),

(2.66)

page 102

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

103

3g2 d2 p Δ(p, iωm ) Δ(k, iωn ) = 4β m (2π)2 D(iωm , p) × χ(k − p, iωn − iωm ), g2 d2 p Δi (p, iωm ) Δi (k, iωn ) = − 4β m (2π)2 D(iωm , p) × χ(k − p, iωn − iωm ),

(2.67)

(2.68)

where D(iωm , p) = (ωn − A)2 − (ε(k) − μ + B)2 .

(2.69)

Equations (2.67) and (2.68) correspond, respectively, to the singlet and triplet pairings. Moreover, the singlet channel is characterized by the repulsion, whereas the triplet one by the attraction. Therefore, it is necessary to take the trivial solution, Δ = 0, of Eq. (2.67). In the following calculations, we will neglect the contributions from the functions A and B, which leads only to the renormalization of the wave function and the chemical potential, and will study only Eq. (2.67). By neglecting Δ2 in the denominator, we get the linearized equations for Δ0 which determine the critical temperature Tc . For the correlation function χ(q, iωn ), we will use the dispersion relations 1 ∞ dω Im χ(q, ω ) χ(q, iωn ) = − π −∞ iωn − ω ∞ ∞ 1 dω Im χ(q, ω ) dω Im χ(q, −ω ) =− + . (2.70) π 0 iωn − ω iωn + ω 0 In order to sum over m in (2.70), we consider the contour C = C1 + C2 (Fig. 2.15). is valid: The following formula for ωn = (2n+1)π β ∞

β F (iωn ) = − 2πi n=−∞

C

β F (ω)dω =− exp βω + 1 2πi

or ∞ n=−∞

F (iωn ) = −

β 1 2πi 2

C

F (ω)th C

F (ω)dω , exp −βω + 1

(2.71)

βω dω. 2

(2.72)

Taking into account that Im χ(q, −ω) = −Im χ(q, ω), Eq. (2.70) can be reduced to 1 ∞ 1 1 dω Im χ(q, ω ) − . (2.73) χ(q, iωn ) = − π 0 iωn − ω iωn + ω

page 103

March 24, 2021

104

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 2.15.

Integration contour C = C1 + C2 .

With the help of formula (2.72), we can rewrite (2.67) in the form Δ(k, iωn ) =

∞ d2 p g2 dωF (p, ω) dω Im χ(k − p, ω ) 2 8π (2πi) (2π) C 0 1 βω 1 (2.74) − th , × iωn − ω − ω iωn − ω + ω 2

where F (p, ω) =

ω2

Δ(k, iωn) . − (ε(p) − μ)2

After some calculations and transformations, we get the general formula for the superconducting parameter [83–85]: g2 Re(k, ω) = 8

π/a −π/a

d2 p (2π)2

th β(ε(p)−μ) 2 2(ε(p) − μ)

× [Re χ(k − p, ω − (ε(p) − μ)) + Re χ(k − p, ω + (ε(p) − μ))] ∞ βν dν cth Im χ(k − p, ν) × ReΔ(p, ν) − 2 π 2 0

page 104

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

105

#

(ω − ν)2 − (ε(p) − μ)2 − δ2 × ((ω − ν)2 − (ε(p) − μ)2 − δ2 )2 + 4 (ω − ν)2 δ2 × ReΔ(p, ω − ν) (ω + ν)2 − (ε(p) − μ)2 − δ2 + ((ω + ν)2 − (ε(p) − μ)2 − δ2 )2 + 4 (ω − ν)2 δ2 $% × ReΔ(p, ω + ν) Re F (p, ω + iδ) = Re Δ(p, ω)

,

(2.75)

ω 2 − (ε(p) − μ)2 − δ2 [ω 2 − (ε(p) − μ)2 − δ2 ]2 + ω 2 δ2

.

(2.76)

If the superconducting gap depends weakly on the frequency, then Δ(k, ω) Δ(k, 0). In this case, we set ω = 0 in Eq. (2.75). Considering the relation Re χ(q, ω) = Re χ(q, −ω) and making the simple transformations, we obtain the equation similar to that in [74]: g2 Δ(k) = 8

π/a −π/a

∞

+2 0

×

d2 p (2π)2

) th β(ε(p)−μ) 2 Re χ(k − p, ε(p) − μ) (ε(p) − μ)

βν dν cth Im χ(k − p, ν) π 2

(ε(p) − μ)2 − ν 2 + δ2 [(ε(p) − μ)2 − ν 2 + δ2 ]2 + 4ν 2 δ2

Δ(p).

(2.77)

It is important that our method of calculations yields a more general equation for the superconducting gap than that obtained by D. Pines. Our equation coincides with the Pines equations after some simpliﬁcation, which is the test for our calculations.

2.7.5. Thermodynamic potential of antiferromagnetic spin fluctuations For the free energy, we have the equation 1 o −1 F (G) = βΩ = − Tr[ln Go G−1 + (G−1 o + Γ Γ5 μ)G ] 2 g2 − Tr{Γi GT rΓj Gχij − 2GΓi GΓj χij }, 32

(2.78)

page 105

March 24, 2021

106

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

where G satisﬁes Eq. (2.57). We now multiply Eq. (2.58) by G and take the trace, Tr. This allow us to obtain g2 i Tr Γ GT rΓj Gχij − 2GΓi GΓj χij 8 o = −Tr{(G−1 o + Γ Γ5 μ)G − 1}.

(2.79)

Using (2.57), we can rewrite relation (2.79) for the functional of free energy calculated with the use of solutions of the Schwinger–Dyson equation in the form 1 −1 1 1 −1 o . (2.80) βΩ = − Tr ln Go Γ + (Go + Γ Γ5 μ)G − 2 2 2 By implementing the Fourier transformation, we get ∞ π/a d2 k 1 V Tr ln Go (k, iwn )G−1 (k, iwn ) Ω= 2β n=−∞ −π/a (2π)2 1 1 −1 o , + (Go (k, iwn ) + Γ Γ5 μ)G(k, iwn ) − 2 2

(2.81)

where V is the two-dimensional volume (the area of the cuprate plane), and Tr stands for the trace of a matrix. For the free energy functional Ω(Δ), we have the formula # ∞ d2 k V Tr ln Go (k, iωn )−1 (k, iωn ) Ω=− 2β n=−∞ (2 ∗ π)2 $ 1 1 −1 o , + (Go (k, iωn ) + r r5 μ)G(k, iωn ) − 2 2

(2.82)

o o where G−1 o (k, iωn ) = r iωn − r r5 ε(k), and G(k, iωn ) is given by formula (2.57). We note that the functional Ω(Δ, μ) is normalized so that Ω(Δ = 0, μ = 0) = 0. By calculating the trace of the r-matrix, we obtain the expression

∞ d2 k ωn2 + (ε − μ)2 + Δ2 V ln Ω(Δ, μ) = − β n=−∞ (2 ∗ π)2 ωn2 + ε2 Δ2 − 2 . ωn + (ε − μ)2 + Δ2

(2.83)

page 106

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

107

By using the formula ∞

ω 2 + b2 ln 2n = ωn + a2 n=−∞

#

√ β β a2 + x dx √ th 2 2 a2 + x 0 $ √ ch βb β b2 + x β 2 th , − √ = 2 ln βa 2 2 b2 + x ch

∞

(2.84)

2

we get the equation for the thermodynamic potential: β d2 k 2 ch 2 (ε − μ)2 + δ2 Ω(Δ) = V − ln (2π)2 β ch βε 2 % β (ε − μ)2 + Δ2 Δ2 . + th 2 2 (ε − μ)2 + Δ2

(2.85)

By making some transformations and calculating the traces of Γ matrices, we arrive at the equation d2 k 4 dw V Δ (k, w) Ω(Δ) − Ω(0) = 2 C 2πi (2π)2 i ×

1 1 . 2 + 1 [w − (ε(k − μ)2 ]2

eBw

(2.86)

By expanding the contour C and calculating the contribution to the integral at poles w = ±(ε(k) − μ), we get d2 k Δ4i (k) V Ω(Δ) − Ω(0) = 8 (2π)2 [ε(k) − μ]2

β β(ε(k) − μ) 1 − th2 × 2 2 (ε(k) − μ) 1 th , (2.87) − (ε(k) − μ) 2 where ε(k) describes the spectrum of two-dimensional electrons, the free energy F is connected with the thermodynamic potential Ω by the relation F = βΩ; Ω(Δ) and Ω(0) are the thermodynamic potentials at T < Tc and T > Tc , respectively; and V is the two-dimensional volume (the area of a cuprate layer). It is easy to verify that, despite the presence of the factors (ε(k) − μ) in the denominator in formula (2.87), no singularity on the Fermi surface ε(k) − μ is present.

page 107

March 24, 2021

108

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

Equations (2.85) and (2.87) (at T ∼ Tc ) can be a basis for calculations of various thermodynamic quantities, including a jump of the heat capacity. A similar method of calculations was developed by St. Weinberg [89].

2.7.6.

Heat capacity of the d-pairing

Equation (2.85) yields the following formula for the thermodynamic potential Ω(Δ) [83]: β 2 ch 2 ( (ε(k) − μ)2 + Δ(k)2 ) d2 k − ln Ω(Δ) = V (2π)2 β ch βε 2 % (ε(k) − μ)2 + Δ(k)2 Δ(k)2 . (2.88) + th 2 2 (ε(k) − μ)2 + Δ(k)2 Here, V is the two-dimensional volume (the area of a cuprate layer), Δ(k) is the superconductor gap, k is the momentum of an electron, and ε(k) = −2t[cos(kx a) + cos(ky a)] gives the spectrum of two-dimensional electrons. The heat capacity is calculated by the formula ∂2Ω . (2.89) ∂T 2 The results of calculations of the heat capacity C are given in work [45]. We have carried out the computer-based calculations of the heat capacity of the compound YBa2 Cu3 O6.63 . The equation for the superconductor gap Δ was obtained in Sec. 2.7.5. The task of solving the integral equation was reduced to that of an algebraic equation which was solved by the method of iterations. The equation for the superconductor gap depends on the spin correlation function. For it, the necessary data were taken from works [73, 74]. In calculations, we used the following values of parameters of the correlator: ωSF (TC ) ≈ 7.7 meV, χS (Q) = 44 eV, ξ/a ≈ 2.5, t = 2 eV, μ = 0.25, Tc = 95 K. We chose such a value of the constant g which satisﬁes the relation 2Δ/kTc = 3.4 like that in works [70, 71]. The results of numerical calculations are presented in Fig. 2.15, where we can see the temperature dependence of the electron heat capacity: 1 — the curve which is an approximation of the results of computer-based calculations (crosses); 2 — the curve which describes the exponential BCS dependence. These results are in good agreement with experiments made by the group of A. Kapitulnik [90] at low temperatures. The calculations showed a square dependence of the heat capacity on the temperature in the temperature range from zero to the superconducting C = −T

page 108

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

109

temperature. It was shown [45, 46, 83, 84] that the dependence has the form C = AT 2 ,

(2.90)

where A = 0.126 J/K3 mole.

2.7.7. Heat capacity jump in superconductors In what follows, we present the results of calculations of a jump of the heat capacity near the critical temperature, ΔC = −T

∂ 2 ΔΩ , ∂T 2

β=

1 , T

(2.91)

and evaluate the parameter R = ΔC/γTc . Omitting the awkward and quite complicated details, we will give the ﬁnal results. We obtained R = 1.6. This value of the parameter is larger than that in the BCS theory, where R = 1.43. It is worth noting that the heat capacity jump is very sensitive to the doping. Figure 2.16 shows the results of recent calculations of one of the authors [85] for R as a function of the doping. It is seen that this parameter depends strongly on the doping. By using these

Fig. 2.16. Temperature dependence of the electron heat capacity, where 1 — the curve which is an approximation of the results of computer-based calculations (crosses); 2 — the curve which describes the exponential BCS dependence, points give the experimental data [90].

page 109

March 24, 2021

110

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

results of calculations, it is possible to evaluate the condensation energy for high-temperature superconductors which is proportional to R2 (see [86]). The calculations imply that the heat capacity depends on the temperature as T 2 . Analogous results were obtained for the physics of heavy fermions [95]. It was shown in this work that d-symmetry leads to a linear dependence of C/T on the temperature, whereas the s-symmetry is related to the exponential dependence of this quantity on the temperature. The linear dependence of C/T on the temperature was observed in the experimental works [91–94] for YBaCuO superconductors, The experimental results are presented in Fig. 2.17. As was mentioned above, the problem of the determination of the symmetry of a gap in cuprate superconductors is urgent at the present time. Many experiments have conﬁrmed the d-symmetry of the pairing [71, 72]. In particular, we mention new experiments [72], in which the researchers have studied the quantization of magnetic ﬂows in a ring which includes three Josephson junctions. These works supporting the existence of d-pairing in high-temperature superconductors were marked by the Barkley prize. It was also shown that the sign of the order parameter in YBa2 Cu3 O7−δ depends on the direction. This dependence corresponds to the dx2 −y2 -symmetry. The temperature dependence of the electron heat capacity obtained in our calculations [83, 84] is related to the d-pairing. These thermodynamic

Fig. 2.17. Parameter R(Tc ) characterizing the heat capacity jump as a function of the doping for Y0.8 Ca0.2 Ba2 Cu3 O7−x . The solid curve presents the results of theoretical calculations, the points mark the experimental data [93].

page 110

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Physics of High-Tc Superconductors

111

calculations can be a supplementing test in the determination of the pairing symmetry in high-temperature superconductors. It should be noted that the thermodynamic calculations clarifying the behavior of high-temperature superconductors have been also performed in [96–99] in the frame of the other mechanisms of pairing.

2.8. Summary The high-temperature superconductivity is a dynamical ﬁeld of solid-state physics which is intensively developed by theorists and experimenters. By summarizing the physical properties and the mechanisms of superconductivity in new high-temperature superconductors, we should like to separate the main properties and the theoretical problems arising in the studies of high-temperature superconductors. In order to comprehend the nature of the superconducting state, it is necessary to construct a consistent microscopic theory which would be able to describe superconductive and normal properties of high-temperature superconductors. It is seen from the above-presented survey that many mechanisms of pairing in high-temperature superconductors, which pretend to the explanation of this phenomenon, have been advanced. On the whole, the most probable seems to be the “synergetic” mechanism of pairing, whose constituents are the electron–phonon interaction, spin-ﬂuctuation, and other types of interaction in cuprate planes. We believe that the known challenging properties, which are contradictory to a certain extent, of many chemical compounds in the superconducting and normal phases can be explained only by considering the interaction of all the degrees of freedom such as lattice-, electron-, and spin-related ones. In this case, it is also necessary to take the complicated structure of hightemperature superconductors into account. The further development of the theory will require not only the execution of bulky numerical calculations, but also the solution of a number of fundamental problems concerning the strong electron correlations. It seems to us that one of the key problems in the ﬁeld of superconductivity is the mechanism and the symmetry of pairing. Above, we have shown that some thermodynamical problems of hightemperature superconductivity, in particular the problem of antiferromagnetic spin ﬂuctuations, can be eﬃciently solved within the method of continual integrals. We would like to conclude by the following remarks: (1) The thermodynamic theory of antiferromagnetic spin ﬂuctuations in high-temperature superconductors is constructed. The method of

page 111

March 24, 2021

112

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch02

Modern Aspects of Superconductivity: Theory of Superconductivity

functional integration is applied to the calculations of the superconductor gap and the thermodynamic potential. The Schwinger–Dyson equation and the equation for the free energy are deduced. (2) From the Schwinger–Dyson equation, the equations for the superconductor gap, which are used in the numerical calculations within the thermodynamics of high-temperature superconductors, are constructed. The analytic formulas for the thermodynamic potential and its jump are obtained. (3) The numerical calculations of the temperature dependence of the electron heat capacity are carried out, and it is shown that the electron heat capacity is proportional to the square of the temperature. It is emphasized that such a temperature dependence is related to the d-pairing. It is shown that the measurement of the temperature dependence of the heat capacity can be a supplementing test in the determination of the type of a pairing symmetry in high-temperature superconductors. The jump of the heat capacity of cuprate superconductors near the critical temperature is evaluated as well.

page 112

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

CHAPTER 3

Iron Superconductors

3.1. Introduction At the beginning of 2008, the huge interest was induced by the discovery of a new class of high-temperature superconductors, namely, layered compounds on the basis of iron. It gave hope for the progress in the synthesis of new high-temperature superconductors up to room-temperature superconductors [100]. At present, the nature of the high-temperature superconductivity (HTS) is not yet completely understood. The main problem of the solid-state physics is the production of superconductors that ensure the superconductivity at room temperatures. Now, the large-scale search for such high-temperature superconductors is continued. This discovery broke the “monopoly” of cuprates in the physics of hightemperature superconductors and inspired new hopes for the close success in the synthesis of new superconductors and for a more profound theoretical comprehension of the mechanisms of HTS. The “iron age” was short, and the term “HTS” is now equally related to cuprate and iron superconductors. Three decades ago, the researchers moved by touch. But, at the time of the discovery of iron superconductors, they have accumulated a signiﬁcant experience of studies of complex compounds and have had the newest experimental methods and the algorithms of calculations of the electronic structure. Moreover, more powerful computational facilities appear, and, what is the principal point, the physical ideas developed in the studies of cuprates can be applied to the new ﬁeld of studies. The progress in experimental and theoretical studies in this ﬁeld is quite impressive. The goal of the present chapter is to give a short introduction into the physics of new superconductors on the basis of layered compounds of iron. We will analyze the physical properties and electronic models of the new class of high-temperature superconductors in layered compounds on the basis of iron. Despite the diﬀerent chemical compositions and the diﬀerence in the crystal 113

page 113

March 24, 2021

114

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

structures, they have similar physical properties determined by electron carriers in FeAs layers. The exceptional interest in them is explained by perspectives of the practical application, though the critical temperature of iron compounds did not exceed the liquid nitrogen temperature. Now, the record among the monocrystals belongs to SmFeAsO1−x Fx with Tc = 57.5 K. A high optimism was also induced by the discovery of the superconductivity at Tc = 100 K in one-layer ﬁlms of FeSe [101, 102].

3.2. Structural Properties of Iron Superconductors At the present time, three classes of compounds containing FeAs planes are under study: LaOFeAs, AFe2 As2 , LiFeAs and the analogous compound FeSe, in which the superconductivity was observed at high Tc . The physical properties of these compounds are similar in many aspects and are determined by a one-type crystal structure including the common element such as FeAs layers. We now consider the physical properties of these compounds. Among the iron compounds possessing the superconductivity, we also separate the following two classes: pnictides and chalcogenides. Pnictides are compounds containing elements of the V group of the periodic table such as nitrogen, phosphorus, and arsenic. The basic element of those compounds is a square lattice of iron. Pnictides can be one-layer such as 1111 (LaFeAsO, LaFePO, Sr2 VO3 FeAs) and 111 (LiFeAs, LiFeP) and two-layer of type 122 with two layers of FeAs (BaFe2 As2 , KFe2 As2 ). Chalcogenides include compounds of type 11 (Fe1−d Se, Fe1+y Te1−x Sex ﬁlms of FeSe) and type 122 (KFe2 Se2 ). The structure and physical properties of compounds of iron are considered in many reviews [103–105] in details.

3.3. Compounds of the Type ReFeAsO The crystal structure of compound ReFeAsO is shown in Fig. 3.1 [106]. Such substances have a tetragonal structure at room temperature with the space group P4/nmm. The crystal structure is formed by alternating layers of FeAs manifesting the antiferromagnetism that are separated by layers of ReO. The FeAs layer is really represented by three closely placed atomic planes that form a square lattice of Fe atoms. From top and from bottom, we see the square lattices of As atoms that are located relative to the Fe-plane so that Fe atom is surrounded by a tetrahedron of As atoms. In other words, the FeAs layer is formed by FeAs4 -complexes. The distance between FeAs and LaO layers is equal to 1.8 ˚ A. The results of calculations of the electron spectrum can be found in [107]. It is worth to note that the speciﬁc features of the electron spectrum are

page 114

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

Fig. 3.1.

115

Crystalline structure of ReFeAsO.

connected with the quasitwo-dimensional character of the superconductivity in the FeAs planes. As an example, we mention compound SmFeAsO1−x Fx whose the highest temperature Tc = 57.5 K is attained at x = 0.1.

3.4. Compounds of the Type AFe2 As2 (A = Ba, Sr, Ca) In a wake of compounds of the type ReFeAsO which are input ones for the creation of superconductors with high Tc , compounds BaFe2 As2 [108] and SrFe2 As2 [109] were synthesized. After the doping, they became superconductors. The discovery of the superconductivity on compound Ba(1 − x)Kx Fe2 As2 caused a new splash of studies of the systems on the basis of FeAs4 . In Fig. 3.2, we present the crystal structure of BaFe2 As2 . It is a tetragonal structure with the space group I4/mm and is composed from AsFe planes separated by Ba planes. Compound LaFeAsO has one Fe plane in the elementary cell, wheres BaFe2 As2 has two such planes. By the data in [111], the parameters of the crystal lattice in the last compound are: a = 3.9090 ˚ A, c = 13.2121 ˚ A. Thus, the cell size in the basis plane is close to that in compound ReFeAsO, whereas the size in the direction along the c-axis is signiﬁcantly larger.

page 115

March 24, 2021

116

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 3.2.

Crystalline structure of AFe2 As2 .

3.5. Compounds of the Type AFeAs (A = Li) After compounds ReFeAsO and AFe2 As2 , a new compound from the FeAs-group, LiFeAs, was synthesized. In it, the superconductivity with a suﬃciently high Tc = 18 K was measured [110]. The detailed structural and physical studies of the compound [110] showed that LiFeAs belongs to the class of compounds containing the layers of LiFeAs such as in ReFeAsO and AFe2 As2 . The FeAs planes are separated by planes with Li. (Fig. 3.3). Contrary to all available undoped FeAs-compounds, LiFeAs reveals no magnetic instability, and the superconductivity in it exists in the absence of any doping. Its charge carriers are electrons. The important information about properties of LiFeAs compounds is given by the results of measurements of Tc under pressure [111]. It is of interest that the superconductivity in these compounds decreases under the applied pressure. It is worth to note that the lattice parameter and the volume of an elementary cell in LiFeAs are comparatively less than in other iron superconductors.

3.6. Compounds of the Type FeSe and FeTe (iron selenide and iron telluride) A new family of superconductors on the basis of iron was found in FeSe and FeTe compounds whose Tc increases at the doping and under pressure [112].

page 116

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

Fig. 3.3.

117

Crystal structure of LiFeAs [110].

Among all superconductors on the basis of iron, the highest attention is attracted to FeSe due to the simplicity of the crystal structure and remarkable physical properties (Fig. 3.4). The group of scientists from the Oak Ridge National Laboratory carried out the theoretical study of properties of a new group of superconductors FeX, by using the widely spread method of solid state physics, namely, the density functional theory, and showed that those substances have the same structural, magnetic, and electron–phonon eﬀects as iron oxypnictides that were opened earlier. It was also shown that FeSe is a representative of the whole superconducting family FeX (X = Se, Te, S). The simplicity of the crystal lattice and the nontoxicity of compounds FeX favor the study and prediction of the superconductivity characteristics of substances containing iron. The crystal structure of iron selenide has many common features with the earlier considered compounds with FeAs layers. Compound FeSe also consists of FeSe-planes positioned one above another. Moreover, nothing is placed between those planes. The atoms of Fe form a square lattice, and each Fe atom is located in the tetrahedral environment of Se atoms (or Te). These compounds are not superconductors at the atmospheric pressure. The superconductivity arises at the doping or under pressure. Compound FeSe1−x for x = 0.12 reveals the superconductivity with Tc = 8 K. In compounds FeSe at the pressure P = 1.48 GPa, the superconductivity was observed at Tc = 28 K.

page 117

March 24, 2021

118

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 3.4.

Crystalline structure of FeSe.

The detailed studies of the structural and superconductivity properties of FeSe at pressures up to 26 GPa were executed in work [113]. At P = 12 GPa, the phase transition from the tetragonal to orthorhombic phase was found. The highest value Tc = 34 K was obtained in the orthorhombic phase at the pressure P = 22 GPa.

3.6.1. FeSe ﬁlms FeSe ﬁlms deserve a separate consideration. Recently, a number of hightemperature superconductors on the basis of FeSe monolayers were discovered. First of all, we mention the systems of the following type: a monoatomic FeSe layer on a substrate of the type SrTiO3 (FeSe/STO). At the present time, the record value of the superconductivity temperature among one-layer FeSe ﬁlms equals Tc = 100 K [101, 102]. Apparently, the question about the superconductivity in ﬁlms was ﬁrst considered by Gor’kov [114, 115] who advanced the idea of a possible mechanism of enhancement in the superconductivity transition temperature Tc in the system FeSe/STO due to the interaction with high-energy phonons in SrTiO3 [103]. If the experimental sample is made in the form of a thin ﬁlm, like famous graphene, then the transition temperature becomes as high as 100 K. This is of great importance, since we can go beyond the boiling temperature of liquid nitrogen, which looks tremendously, by opening the amusing perspectives. It should be added that the just ﬁlm technologies have high potentialities for the applications.

page 118

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

119

3.7. Superconductivity Soon after the discovery of the superconductivity in LaO1−x Fx FeAs, it was reported that the external pressure applied to compounds with x = 0.11 increases Tc maximally to 43 K at a pressure of 4 GPa. It was assumed that the compression of the lattice is responsible for the observed eﬀect. Indeed, in compound ReFeAsO, the atoms of the rare-earth element have a less radius than that of La atom, and Tc is signiﬁcantly higher than 55 K. In many works, an increase in Tc caused by the replacement of La by other rare-earth elements is frequently called the “chemical pressure eﬀect” [103] characteristic of high-temperature superconductors [104]. The replacement of various rare-earth ions in a number of compounds ReFeAsO, as distinct from cuprate superconductors ReBaCuO, leads to a rather large dispersion of values of Tc . In order to explain this phenomenon, two scenarios can be proposed. First, the eﬀect can be caused by the disorder arising at the replacement of rare-earth elements and the realization of an anomalous pairing in FeAs (e.g., anisotropic pairing, d-pairing). Second, we may consider the magnetic mechanism of pairing in iron superconductors. The spins of rare-earth ions strongly interact with the Fe spins and can signiﬁcantly aﬀect the spectrum of spin ﬂuctuations in FeAS planes, which increases Tc by the magnetic mechanism. In addition to thee doping, the physical properties of iron superconductors are changed signiﬁcantly under pressure. The pressure applied to FeAs compound induces the bulk structural and magnetic phase transition. In this case, we observe the tendency to the appearance of the superconductivity. In work [116], the dependence of the superconductivity transition temperature on the height of an anion for typical superconductors on the basis of iron was determined. It is shown in Fig. 3.5. The large symbols denote the initial temperature. This dependence is used in one of the key strategies aimed at the comprehension of the mechanism of superconductivity in substances on the basis of iron and the search for new superconductors on the basis of iron with higher Tc .

3.8. Electronic Structure 3.8.1. Multiorbital and multizone cases In the explanation of the physical properties of superconductors, the signiﬁcant role is played by ﬁrst-principles calculations of the electronic structure. It is worth to note that one of the basic properties of high-temperature superconductors is the presence of many orbitals and many zones [117]. The superconductors on the basis of iron are represented by quasitwo-dimensional

page 119

March 24, 2021

120

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 3.5. Dependence of Tc on the height of an anion for typical superconductors on the basis of Fe. Large symbols denote the initial temperature. The temperatures with zero resistance at the ambient pressure are shown by small blue circles. Filled symbols indicate the data at a certain pressure. Open symbols correspond to SrFe2 As2 and BaFe2 As2 at the optimum pressure. Open squares denote the data on NdFeAsO0.85 at a high pressure. The data on FeSe at a high pressure are given by uncolored circles. The ﬁlled circle indicates the data on FeTe0.8 S0.2 .

substances in which the conducting plane is the square lattice of Fe atoms. At once after the discovery of iron superconductors, the detailed calculations of the zone structure of those superconductors were carried out, ﬁrst of all, within the general method of local density approximation (LDA). In [107], the ab initio calculations of the zone structure were executed for a number of oxypnictides of the type ReFeAsO. In Fig. 3.6, we present the electron spectra of LaFeAsO and PrFeAsO along the basic directions in the Brillouin zone. It is seen that the diﬀerence in spectra related to the replacement of a rare-earth ion is quite insigniﬁcant. In a rather interval of energies near the Fermi level that is of importance from the viewpoint of the formation of the superconducting state, the spectra are practically identical. The forms of the partial densities of states (Fig. 3.7) imply that the density of states near the Fermi level is practically completely determined by the d-state of Fe (at a rather insigniﬁcant contribution of the p-state of As). E may say that all phenomena related to the superconductivity are realized on the square Fe lattice of compounds FeAs.

page 120

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

121

Fig. 3.6. Electron spectra of LaFeAsO and PrFeAsO along the directions with high symmetry in the Brillouin zone obtained by LDA.

Fig. 3.7. Comparison of the total density of states of electrons and the partial densities of states of LaFeAsO and PrFeAsO.

page 121

March 24, 2021

122

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 3.8.

The Fermi surface of compound LaFeAsO.

The results of the ﬁrst calculations within the density functional theory showed that 3d6 states of Fe2 are dominant. In this case, all ﬁve orbitals dx2 −y2 , dxy , dxy , dxz , dyz lie on the Fermi surface or near it. Such situation leads to the existence of many orbitals and many zones in the low-energy electronic structure. The structure of dispersion curves crossing the Fermi level determines the Fermi surface that is a multisheet one for compounds of the type LaFeAsO. The Fermi level crosses two hole zones outgoing from point Γ and two electron zones starting from point M. It is worth to mention the planar character of the curves in direction ΓZ, which indicates a weak dependence of hole quasiparticles on the momentum kF. Therefore, the Fermi surface in a vicinity of point Γ has hole character. The same is true for sheets of the Fermi surface in a vicinity of point M (Fig. 3.8). Thus, two hole cylindrical sheets with the axis along direction ΓZ and two electron sheets along axis MA are formed on the Fermi surface of compound LaFeAsO.

3.9. Minimum Model The relative simplicity of the spectrum of FeAs superconductors near the Fermi surface forces one to think about the construction of an analytic model of a spectrum that would describe the properties of electrons near the Fermi surface. The above-presented results of zone calculations imply that the highest contribution to the electron density of states near the Fermi level is given by 3d-states of Fe atoms. Among ﬁve d-orbitals, we separate two degenerate orbitals dxz and dyz . The overlapping of orbitals determines the values of matrix elements of the hops between them for the nearest and next-nearest neighbors. If we consider only these two orbitals, we get the two-orbital model of FeAs compounds. It is called the minimum model

page 122

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

characterized by the Hamiltonian + ψkσ T (k)ψkσ , H0 =

123

(3.1)

kσ

+ + = (c+ where ψkσ xkσ , cykσ ) is the two-component spinor composed of the + operators of creation c+ xkσ and cykσ of electrons, respectively, on the orbitals dxz and dyz , and T (k) is a two-row matrix composed of matrix elements of the transitions shown in the following equation: εxy (k) εx (k) − μ . (3.2) T (k) = εy (k) − μ εxy (k)

Here, εx (k) = −2t1 cos kx − 2t2 cos ky − 4t3 cos kx cos ky , εy (k) = −2t2 cos kx − 2t1 cos ky − 4t3 cos kx cos ky ,

(3.3)

εxy (k) = −4t4 sin kx sin ky . Hamiltonian (3.1) that is a quadratic form of Fermi operators is diagonalized with the help of the canonical transformation of the operators cskσ (s = x, y) to the γskσ : asν (k)γνks . (3.4) cskσ = ν=±

Here, ⎞⎤1/2 ⎡ ⎛ ε− (k) 1 ⎠⎦ = ay+ , ax− (k) = ⎣ ⎝1 + 2 ε2− (k) + ε2+ (k) ⎞⎤1/2 ⎡ ⎛ ε− (k) 1 ⎠⎦ = −ay+ . ax+ (k) = ⎣ ⎝1 − 2 ε2− (k) + ε2+ (k)

(3.5)

With regard for the chemical potential, the Hamiltonian of the model takes the form + Eν (k)γνkσ γνkσ , (3.6) H0 = kσ ν=±

where the zone energies E± (k) = ε+ (k) ± and ε± (k) =

1 2

[εx (k) ± εy (k)].

ε2− (k) + ε2xy (k) − μ,

(3.7)

page 123

March 24, 2021

124

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

We now introduce the one-electron Matsubara Green function ˆ σ (k, τ ) = −Tˆτ ψkσ (τ )ψ + (τ ), G kσ

(3.8)

After some calculations, it takes the following form: ˆ σ (k, iωn ) = G =

1 (iωn − E+ (k)) (iωn − E− (k)) −εxy (k) iωn − εx (k) − μ −εxy (k)

iωn − εy (k) − μ

.

(3.9)

The poles E+ (k) and E− (k) of the Green function determine the spectrum of quasiparticles on the model. There are two branches whose the mutual position and the shape of dispersion curves depend on the values of matrix elements t1 , t2 , t3 , t4 . They should be chosen from the condition that the formulas give the spectrum consistent with the results of numerical calculations for FeAs compounds. Spectrum (3.7) is shown in Figs. 3.9(a) and 3.9(b) in the extended and reduced Brillouin zones. The Fermi surface is approached by (a)

(c)

(b)

(d)

Fig. 3.9. (a) and (b) The zone structure of the two-orbital model with parameters t1 = −1, t2 = 1.3, t3 = t4 = −0.85 and the chemical potential μ = 1.45. (c) and (d) The Fermi surface in the two-orbital model for the extended (a) and reduced (b) Brillouin zones. (Here α1,2 are hole Fermi surfaces determined by the condition (E − (kF ) = 0 and β1,2 are electronic Fermi surfaces determined by E + (kF ) = 0.

page 124

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

125

two branches of hole quasiparticles in a vicinity of point Γ and two branches of electron ones in a vicinity of point M. The Fermi surface is shown in Figs. 3.9(c) and 3.9(d) in the extended and reduced Brillouin zones. The model under study gives two hole pockets in a vicinity of point Γ and two electron ones in a vicinity of point M. Therefore, it can be called the minimum model of FeAs compounds. We dealt only with the kinetic part of the energy of the system. To describe various orderings of the model phases, it is necessary supplement the Hamiltonian by terms describing the interaction, ﬁrst of all, the Coulomb repulsion of electrons on one node or the exchange interaction on diﬀerent nodes. The ﬁrst-principles calculation of the electron structure plays a crucial role in the explanation of physical properties of superconductors. The presence of many zones is one of the principal properties of high-temperature superconductors [117]. It was shown in [104] that the information about the electron spectrum and the density of states near the Fermi surface is of a high importance for the formation of a superconducting state.

3.10. Experimental Study of the Fermi Surface There are available two methods of experimental determination of the Fermi surface in metals: one method is based on the de Haas–van Alphen (dHvA) eﬀect, and the second one is referred to photoelectron spectroscopy with angular resolution (ARPES). In the ﬁrst case by the measured osciillations of the magnetization in a magnetic ﬁeld, we can get the information about the cross-section areas of the Fermi surface. This method is of high accuracy, but does not attach the measured area to the k-space of the Brillouin zone. The ARPES method has a less accuracy, but allows one to directly restore the Fermi surface in the k-space. Both methods have own advantages and shortcomings, supplement each other, and are signiﬁcant for the construction of the pattern of superconducting pairing. LDA calculations of compounds ReOFeAs show the structure of the Fermi surface: it consists of two cylindrical hole pockets centered at the nodes of the Brillouin zone. In addition, the three-dimensional hole pocket centered at point M is observed near point Γ. The experimental veriﬁcation of these conclusions was performed with the help of ARPES [118–120]. For example, the ARPES spectra were measured in [121] on a monocrystal NdO1−x Fx FeAs. They show the presence of pockets of the Fermi surface near points Γ and M of the Brillouin zone in agreement with numerical ﬁrst-principles calculations (Fig. 3.6). In parallel, the Fermi surface was studied with the help of the measurement of the dHvA eﬀect in which the quantum oscillations of the magnetization in a

page 125

March 24, 2021

126

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

magnetic ﬁeld are determined. It was shown that the iron superconductors are characterized by cylindrical hole surfaces centered at point Γ and two electron ones centered at point M. The detailed comparison of the results of LDA calculations with ARPES spectra shows a good agreement of theory and experiment, which is conﬁrmed by the studies of the dHvA eﬀect.

3.11. Antiferromagnetism The possibility of the antiferromagnetic ordering in the studied systems was noticed before the implementation of neutronographic studies. Compounds ReOFeAs are antiferromagnetics. The ﬁrst indications of the possibility of the magnetic ordering in LaOFeAs were given by the measurements of the temperature dependences of the electric resistance and the magnetic susceptibility that demonstrated some anomalies at the temperature T = 150 K. At this temperature, the structural transition from the tetragonal into orthorhombic phase was found. The complete neutronographic studies reﬁned the situation [121]. It turned out that the magnetic phase transition arises somewhat lower at TN = 137 K. The main result of studies of LaOFeAs is the magnetic structure that is realized on Fe atoms. This magnetic structure is the antiferromagnetic alternation of ferromagnetic chains in the basis plane and in the perpendicular direction. This structure is in agreement with theoretical predictions following from the calculation of the zone structure of a compound [122, 123]. In this case, the compound itself is a metal. The magnetic ordering in FeAs compounds is diﬀerent from that in cuprates. The cuprate superconductors demonstrate the ordering in the basic layers, where the magnetic moments of Cu are antiparallel to moments on the nearest neighbors of the Cu sublattice. The cuprate superconductors are Mott dielectrics. The doping of cuprates causes the fracture of the longrange magnetic order and the appearance of the superconducting state. An analogous situation holds in FeAs compounds. The neutronographic studies of the doped superconductor LaOFeAs showed the absence of longrange magnetic order. Thus, the superconductivity arises, like in cuprates, near the magnetic phase transition, which indicates the signiﬁcant role of antiferromagnetic ﬂuctuations at the electron pairing. At low temperatures, the spin density wave (SDW) arises in iron superconductors. SDW is some ordering that aﬀects the electron spectrum, density of states, and dispersion curves. A signiﬁcant task is the calculation of the electron spectrum at a doping. The electron doping should increase the electron pockets of the Fermi surface, whereas the hole doping causes an increase in hole pockets. In this case, we need to calculate the compounds with a given level of doping.

page 126

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

127

3.12. Phase Diagrams Analogously to superconducting cuprates, the properties of superconductors on the basis of iron are sharply changed at the doping. The parent compounds FeAs are, as a rule, metals (as distinct from cuprates that are dielectrics), but, like cuprates, are ordered antiferromagnetically. Such order is called frequently the spin density waves (SDWs). The superconductivity arises at any electron doping, which causes the appearance of SDWs. Generally, the phase diagram is analogous to that of cuprates. At the doping of compounds in which the magnetic structure SDW is realized, the temperature TN of the magnetic ordering gradually decreases, and the superconducting state appears in the system. It is of interest to establish the boundaries of all three phases — magnetic, structural, and superconducting ones. The local methods such as M¨ ossbauer spectroscopy give information about the long-range magnetic order, but are not sensitive to structural distortions. The X-ray diﬀraction analysis enables one to study the crystal structure, but is not sensitive to the magnetic order. Only the neutron spectroscopy gives possibility to study both aspects simultaneously. The ﬁve-orbital model from work [105] well reproduces the results of calculations of the Fermi surface consisting of four pockets: two hole pockets near the point (0, 0) and two electron ones at the points (0, p) and (p, 0) (Fig. 3.11). Such geometry in the k-space leads to the possibility of the appearance of a spin density wave due to the nesting between the hole and electron Fermi surfaces on the wave vector Q = (p; 0) or Q = (0; p). In Fig. 3.10, we show schematically the phase diagram and Fermi stufaces for various levels of doping. Depending on the topology and the mutual

(a)

Fig. 3.10. doping.

(b)

Schematic phase diagrams of cuprates and pnictides at the hole or electron

page 127

March 24, 2021

128

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

(a)

(b)

Fig. 3.11. Schemes of two-dimensional cross-sections of the Fermi surfaces for cuprates and pnictides: (a) for weakly doped cuprates, the Fermi surface has one sheet, and the ﬁlled states (that are closer to point Γ) occupy about a half of the Brillouin zone; (b) for pnictides, the Fermi surface consists of several sheets: two pockets centered at Γ, electron pockets centered at (0, π) and (π, 0), and a hole pocket centered at M = (π, π).

exchange of hole and electron pockets, we can observe the appearance of the competition between gaps of the s- and d-types. The phase diagram of iron superconductors diﬀers rather noticeably by the concentration of a doping element from the phase diagram of cuprates (Fig. 3.10). In Fig. 3.11, we present the schemes of two-dimensional crosssections of the Fermi for cuprates and pnictides [124]. We recall that the HTS cuprates are antiferromagnetic dielectrics (Mott strongly correlated ones), and the new Fe superconductors are antiferromagnetic metals. The superconductivity in systems on the basis of iron can be induced not only by the doping, but also under pressure.

3.13. Mechanisms and Types of Pairing The discovery of the high-temperature superconductivity in layered compounds on the basis of iron was followed by the publication of tens of theoretical works with various propositions on the microscopic mechanisms of Cooper pairing in such systems. We dwell only on several most signiﬁcant mechanisms of pairing. The calculations of the electron–phonon coupling in those compounds showed that the standard electron–phonon mechanism of pairing cannot ensure so high Tc in those compounds.

3.13.1. Multizone superconductivity The main speciﬁc feature of new superconductors is their multizone character. The electron structure in a suﬃciently narrow vicinity of the Fermi level

page 128

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

(a)

129

(b)

Fig. 3.12. Schematic view of the electron spectrum: (a) Fermi surfaces; (b) iron superconductor in the scheme of extended zones. Around point Γ, there are two hole surfaces, and the electron surfaces are at points X.

is formed practically only by d-states of Fe. The Fermi surface consists of several hole and electron cylinders. On each cylinder, the energy gap can be formed. Such situation is not new and will be considered in Chapter 4 “Multizone model of superconductivity”. The schematic views of the electron spectrum and Fermi surface are shown in Fig. 3.12 [111]. The electron doping decreases the sizes of hole channels, and the hole doping decreases the sizes of electron ones. In work [125], the symmetry analysis of possible types of the superconductivity parameters of order is presented, and the BCS solutions are constructed. The electron spectrum of the system is given in Fig. 3.12. The BCS pairing interaction in the problem under study can be represented by the matrix ⎛ ⎞ u u t t ⎜ ⎟ ⎜u u t t ⎟ ⎜ ⎟, V =⎜ (3.10) ⎟ t t λ μ ⎝ ⎠ t t μ λ where λ = V eX,eX = V eY,eY sets the interaction on one electron pocket at the point X, μ = V eX,eY connects the electrons from diﬀerent pockets at the points (π, 0) and (0, π), u = V h1,h1 = V h2,h2 = V h1,h2 characterizes the BCS interaction in two hole pockets surrounding point Γ, and t = V h,eX = V h,eY connects the electrons at points X and Γ.

page 129

March 24, 2021

130

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

The critical temperature of the superconductivity transition is determined by the solution of the system of linearized equations for a gap 2γ ω ¯ , (3.11) V¯ i,j Δj ln Δi = πTc j

where ω ¯ is the ordinary frequency of a cutting of the logarithmic divergence in the Cooper channel, 1 (3.12) V¯ i,j ≡ − V i,j νj , 2 and νj is the density of states on the j-th pocket of the Fermi surface. Introducing the eﬀective coupling constant g and writing Tc as 2 2γ ω ¯ exp − , (3.13) Tc = π g we ﬁnd the solutions of three types: (1) a solution corresponding to the dx2 −y2 -symmetry, when the gaps on diﬀerent pockets at points X diﬀer by sign, and the gaps on hole pockets are equal to zero: Δ1 = Δ2 = 0,

Δ3 = −Δ4 = Δ,

g = (μ − λ)ν3 ;

(3.14) (3.15)

the possibility of a solution of such type follows from the total symmetry analysis [125]; (2) two solutions corresponding to the so-called pairing of the s± -type for which the gaps at points X have the same sign, and the gaps on the Fermi surfaces surrounding point Γ can have another sign. In this case, 2g+, − = −u(ν1 + ν2 ) − (λ + μ)ν3 ± (u(ν1 + ν2 ) − (λ + μ)ν3 )2 + 8t2 ν3 (ν1 + ν2 ),

(3.16)

and Δ1 = Δ2 = κΔ,

Δ3 = Δ4 = Δ,

(3.17)

where κ−1 = −(g+, − + u(ν1 + ν2 ))/(tν3 ). For the ﬁrst time, the possibility of a pairing of the s± -type in compounds on the basis of FeAs was indicated in [126]. This solution is in the qualitative correspondence with the data of ARPES. At a diﬀerence of the BCS constants on hole cylinders, it is easy to get diﬀerent values of the gaps and to attain the agreement of the theoretical results and experimental data.

page 130

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

131

This case will be considered in the section on the symmetry of a pairing in this chapter in more details.

3.13.2. Electron–phonon mechanism As the mechanism of pairing, we consider the electron–phonon one. In connection with the discovery of the direct and inverse isotopic eﬀects, the superconductivity transition temperature was calculated in work [127] in the model with s± -symmetry of the parameter of order by means of the solution ´ of the Eliashberg equations for a superconductor with hole and electron pockets on the Fermi surface. The coarse solution of the equations in the spirit of the BCS approximation led to the following formulas for Tc and the isotopic parameter α: + 1 + λ+ + λ AF ph , (3.18) Tc = 1.14ωph exp Λ − λ− ph ⎡ 2 ⎤ + + λ 1 + λ+ Λ AF ph ⎦, (3.19) α = 1/2 ⎣1 − + 1 + λAF Λ − λ− ph where Λ=

λ− AF

1−

λ− AF 1+λ+ AF

ln

ωAF ωph

.

Here, ωAF and ωph are the limiting frequencies of spin ﬂuctuations and ± phonons, and the quantities λ± AF and λph represent linear combinations of the corresponding quantities related to the pairing inside one pocket and between diﬀerent pockets: inter intra λ± AF = λAF ± λAF ,

inter intra λ± ph = λph ± λph .

(3.20)

Soon after the discovery of the superconductivity in pnictides, some estimates of the pairing owing to the electron–phonon interaction were executed. The coupling constant turned out to be lower than that for aluminium, which allows one to conclude that the electron–phonon interaction is not dominant.

3.13.3. Spin-ﬂuctuation mechanism of pairing Such situation led to the search for new mechanisms of pairing. Let us focus on the more promising mechanism of pairing, namely, the spin-ﬂuctuation one. We mention the following causes to separate it as a perspective one:

page 131

March 24, 2021

132

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

(1) this theory is based on the model of strongly delocalized electrons, which serves a good starting point in the description of iron; (2) to describe the various observable properties of pnictides and chalcogenides, we should not introduce some additional parameters into the theory but need to consider the speciﬁc features of the interaction of a zone structure and the interaction in various classes of Fe compounds. At the present time, popular are the models of pairing based on the deﬁning role of spin ﬂuctuations. At many aspects, they are analogous to those in the physics of HTS-cuprates which were considered in Chapter 2. The detailed analysis of possible electron mechanisms of pairing in the framework of a Hubbard generalized Hamiltonian was carried out in [128, 129]. It is worth to note that most works devoted to the mechanism of pairing and based on the exchange of spin ﬂuctuations contain yet no direct calculations of Tc and comparison with experiments. The spin ﬂuctuations are connected with the jittering of spins in the electron subsystem. Such excitations distort the lattice, which forces the spins to jitter more consistently and to form chains (stripes) along some of the directions in a crystal. This induces, in turn, the nematicity that should be understand as a self-organized electron state violating the rotational symmetry of the lattice. Such general jittering of spins, the lattice, and distribution of electrons leads to the creation of Cooper pairs in the space. Such pairs can move through the crystal lattice, as if not noticing its presence. The spin ﬂuctuations tend to the self-organization in order to form strings (in the solid-state physics, they are called stripes). In the plane with Fe atoms, the chains of spins are formed and are self-organized. These chains cause, in turn, the so-called the nematic transition. The nematic state is referred to the physics of liquid crystals. But, in this case, it is related to the loss of the rotational symmetry of the electron ﬂuid, which is caused by the appearance of the chains of spins in iron superconductors. For the further lowering in the temperature, it was shown that a strong interaction is formed in those stripes and increases at the transition to the superconducting state. So, we may conclude that the spin ﬂuctuations have played the key role in the formation of the superconductivity, in particular, in iron selenides. Thousands of physicists deal with the superconductivity. They can be partitioned into diﬀerent camps. Some physicists assert that the key mechanism is a phonon one, whereas others say about the exchange by virtual magnons, i.e., by spin oscillations. As was mentioned in Chapter 2, the synergetic mechanism of pairing accounting for all degrees of freedom on

page 132

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

133

the same footing is of importance as well. We emphasize that the smallest changes in the chemical composition can cause a change in the ratios of diﬀerent mechanisms.

3.13.4. Symmetry of pairing We note that there exists a consensus in the comprehension of the crystal, magnetic, and electron structures of FeAs systems. But the problems of the symmetry of the superconductivity parameters of order and the mechanism of electron pairing are far from their solution. The diﬀerent experimental methods lead to contradictory results. This is true for the question about the number of superconductivity gaps for the given compound. There are available two groups of experimental methods. In the ﬁrst one, the value of the superconductivity parameters of order is determined, whereas the second group gives its phase that is related to the presence or absence of zeros in the superconductivity parameter of order. The ﬁrst group includes the thermodynamic methods based on measurements of the electron heat capacity, London depth of penetration of the ﬁeld, and NMR. Close to such thermodynamic methods are the tunnel measurements, including the Andreev reﬂection. The second type of methods is based on measurements of the phase of the superconductivity parameters of order in Josephson’s contacts in a magnetic ﬁeld. Such experiments allowed one to uniquely determine the symmetry of a pairing in cuprates as dx2 −y2 . As for the FeAs systems, few experiments of such type are known. Most experiments on various classes of FeAs compounds were performed by thermodynamic and tunnel methods. Unfortunately, the obtained data are frequently contradictory, and their interpretation is ambiguous. The experiments showed that the pairing is a siglet one. Three versions of the symmetry of the superconductivity gap are considered: the ordinary pairing (mainly with several gaps), s± -type, and d-type. The totals of the studied executed till now are such that it is impossible to make an unambiguous conclusion about the symmetry of the superconductivity parameters of order in FeAs compounds. The various electron models of FeAs compounds lead to the s± superconducting state as the most energetically optimum under conditions where the hole and electron pockets exist.

3.13.5. Multiorbital model Consider the results of calculations in a two-zone model of FeAs systems. The mean-ﬁeld approximation in the spirit of the BCS theory leads to the

page 133

March 24, 2021

134

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity (a)

(b)

Fig. 3.13. Symmetry of the superconductivity parameters of order of the s± -type (a) and dx2 −y 2 (b).

possibility to realize the superconducting states in the system with diﬀerent symmetries of parameters of order. One of the possibilities is the realization of the so-called s± -symmetry of parameters of order. It is characterized by the appearance of the isotropic superconductivity gap (delta) on the hole and electron sheets of the Fermi surfaces with opposite signs on sheets. Considering such parameter of order as a function of the momentum in the Brillouin zone, it is seen that it changes its sign at the transition from one sheet onto the second one (Fig. 3.13). Since the sizes of the hole sheet and electron sheet are small, the line of zeros of the parameter of order with s± symmetry passes outside the Fermi surface, and those zeros do not lead to speciﬁc dependences of some properties of a superconductor as, for example, in the case of dx2 −y2 -symmetry of parameters of order. For the ﬁrst time, the assumption about the superconductivity with the ± s -symmetry of parameters of order for FeAs systems was advanced in [130, 131]. The idea of the s± -symmetry was introduced prior to the discovery of iron superconductors in theoretical descriptions of the superconductivity in other compounds described by the multiorbital models [132]. It was shown that, in such superconductors, the temperature dependence of the spinlattice relaxation can have a quasipower character (not the exponential one, as in the BCS theory). In works [130, 131], the authors started from a more realistic idea of the electron structure of iron superconductors, rather from the minimum two-orbital model.

3.14. Properties of a Superconductor with s± -Symmetry of Parameters of Order In the BCS model, let us consider the appearance of the the superconducting state with s± -symmetry in the case where the Fermi surface has hole and electron pockets.

page 134

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

135

Consider the Hamiltonian H=

kaσ

+

εak c+ kaσ ckaσ

kk q

Va,a c+ c+ c q c q , k+ q a↑ −k+ q a↓ −k + a ↓ k + a ↑ 2

aa

2

2

2

(3.21)

where the index a = (h, e) enumerates the hole and electron pockets, Va,a is the eﬀective interaction electrons by means of spin ﬂuctuations (its speciﬁc form is completely insigniﬁcant; therefore, we omit a dependence on the wave vector). In the mean-ﬁeld approximation, Hamiltonian (3.21) takes the form HMF =

kaσ

εak c+ kaσ ckaσ +

ka

+ [Δa c+ ka↑ c−ka↓ + h.c.].

(3.22)

Here, the parameters Δh and Δe are given by the following formulas:

Δh = Vhh

c−kh↓ ckh↑ + Vhe

k

Δe = Vee

c−ke↓ cke↑ ,

(3.23)

c−kh↓ ckh↑ .

(3.24)

k

c−ke↓ cke↑ + Veh

k

k

Choosing the Hamiltonian in the form (3.22), we account for the pairing of electrons located in the limits of one pocket. Consider the simple situation where the interaction of pairs inside of one pocket can be neglected, i.e., we set Vhh = Vhe = 0. Then Eqs. (3.23) and (3.24) are reduced to two equations of the form: Δh = Vhe

k

Δe = Vhe

k

Δe ε2k

2

th

1 2T

th

1 2T

+ |Δe | Δh

2

ε2k + |Δh |

ε2k + |Δe |2 ,

ε2k + |Δh |2 .

(3.25)

(3.26)

It is known that the eﬀective interaction of electrons by means of spin ﬂuctuations in singlet Cooper pairs has the character of repulsion, i.e., Veh = Vhe > 0. In this case, Eqs. (3.25) and (3.26) have a solution, if Δh and Δe are opposite by sign. Let us write the linearized equations for the

page 135

March 24, 2021

136

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

parameters of order Δh and Δe in the form:

|Δh | = Vhe Ne (0) |Δe | ln |Δe | = Vhe Nh (0) |Δh | ln

2γω0 πTc 2γω0 πTc

,

(3.27) .

They yield the formula for the superconductivity transition temperature: 2γω0 exp −1/Vh Nh (0)Ne (0) . (3.28) Tc = π Here, ω0 is the cutting energy for the pairing interaction, and γ = 1.78. Formula (3.28) is a generalization of the BCS formula to the case of a two-component parameter of order [163]. It was derived in work [163] under the condition that the pairing interaction Vhe < 0, i.e., it has character of attraction. In this case, both parameters of order have the same sign. The above-presented simple calculation shows that, in the case of repulsion (Vhe < 0), the signs of the parameters of order on diﬀerent sheets of the Fermi surface are opposite. In other words, we have the superconducting state with the s± -symmetry of the parameters of order. The anisotropy of the superconductivity gap for the doped superconductor FeTe0.6 Se0.4 (Tc = 14.5 K) was studied by the ARPES method [133]. The single gap on the hole sheet of the Fermi surface was found near point Γ. The studies executed by the ARPES method for superconductors FeAs showed some anisotropy (Fig. 3.14). The measured anisotropy of the

Fig. 3.14. Superconductivity gap on the hole sheet of the Fermi surface centered at point Γ by data of the ARPES method.

page 136

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

137

superconductivity gap indicates deﬁnitely that the binary interaction is not the traditional phonon one. The results indicate the importance of electron interactions of the nearest neighbors of iron in the framework of the s± -wave superconductivity.

3.15. t–J1 –J2 Model In order to simplify the theoretical study based on the analytic methods, it is expedient to use the minimum model of FeAs compounds. The minimum electron model of FeAs systems follows from the crystal structure of FeAs layers. Atoms of Fe form a square plane lattice. From top and from bottom of such plane, the planes containing the square lattices are positioned. Thus, each Fe atom is surrounded by a tetrahedron of As atoms (Fig. 3.15(a)). In FeAs systems, the eﬀective exchange interaction arises not only between the nearest neighboring atoms. We now present the explanation to Fig. 3.15. Here, t2g orbitals dxz , dyz , and dxz are four-lobe structures located in the planes xz, yz, and xz, respectively. The four lobes at a deﬁnite node of the lattice is composed of two degenerate orbitals (dxz and dyz ). The signs “+” and “−” indicate the sign of the wave function for a separate lobe of the orbital. The dotted lines coming from two lobes of the orbitals of the nearest neighbors indicate the corresponding matrix element of hops. Its value depends on the signs of the wave function. For the FeAs systems, the eﬀective exchange interaction arises not only between the nearest-neighboring atoms of Fe, but also between the nextnearest ones due to the complex structure of hoppings (Fig. 3.7). We should (a)

(b)

Fig. 3.15. Crystal and electron structures of a FeAs layer. (a) Location of atoms of Fe and As in the planes positioned above the Fe plane and under it. (b) Location of dxz , dyz orbitals of Fe atoms and the matrix elements of electron hops between the nearest neighbors.

page 137

March 24, 2021

138

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

include two types of interaction in the Hamiltonian of the two-orbital model H0 [133–135]: H1 describes the exchange by electrons on diﬀerent nodes, and H2 corresponds to the Hund exchange in a single node. Below, we give both expressions: Jnab [Sai Sbi+δn − nai nbi+δn ], (3.29) H1 = n

iab

H2 =

JSai Sa¯i .

(3.30)

ia

Here, Sai is the electron spin operator on the node i and orbital a. It can be represented in terms of the pair of Fermi-operators c+ iaσ and ciaσ of creation and annihilation of an electron in this state by means of the well-known formula: c+ (3.31) Sai = iaσ σσσ caiσ , σσ

where σ is the vector composed of Pauli matrices. We recall that the index a = 1, 2 enumerates the orbitals dxy and dyz introduced into the model. The number of particles nai in the state ai can be presented in terms of Fermi operators: c+ (3.32) nai = aiσ caiσ . σ

Eventually, the Hund exchange H2 is determined by electrons on the opposite orbitals. The Hamiltonian H = H0 + H1 + H2 describes the so-called t–J1 –J2 model that includes the antiferromagnetic exchange on the nearest and nextnearest neighbors, as well as the motion of electrons along the lattice. In what follows in the mean-ﬁeld approximation, we will study a possibility of the appearance of the superconducting state within this model with various symmetries of the parameters of order.

3.15.1. Superconductivity with diﬀerent parameters of order Let us simplify the model in order to get the analytic solutions: we will consider that the exchange interaction exists only between electrons on the same orbital. Then the reduced Hamiltonian of the exchange interaction takes the form [136] + Vkk c+ (3.33) Hred = kα↑ c−kα↓ c−k α↓ ck α↑ , kk

α

page 138

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

139

where Vkk = −2J1 [(cos kx + cos ky )(cos kx + cos ky ) + (cos kx − cos ky )(cos kx − cos ky )] − 8J2 (cos kx cos ky cos kx cos ky + sin kx sin ky sin kx sin ky ). (3.34) We note also that the Hund term in Hred is omitted, and only the interaction of Cooper pairs with opposite momenta and spins are retained in the exchange term. Thus, the reduced Hamiltonian corresponds to the BCS approximation. In Hamiltonian (3.33), we separate the mean values for the operators of a Cooper pair: Δα (k ) = cα−k ↓ cαk ↑ .

(3.35)

We now pass to the mean-ﬁeld approximation. In the Nambu representation with four-component ﬁeld operators + Ψk = (c1k↑ , c+ 1−k↓ , c2k↑ , c2−k↓ ),

(3.36)

we can write the total Hamiltonian of the model that includes the kinetic term H0 and the reduced interaction operator Hred taken in the mean-ﬁeld approximation as H=

Ψ+ (k)A(k)Ψ(k),

(3.37)

k

where A(k) is the 4 × 4 matrix: ⎛

ξx (k) − μ

⎜ ⎜ Δ∗ (k) 1 ⎜ A(k) = ⎜ ⎜ εxy (k) ⎝ 0

Δ1 (k) −εx (k) + μ 0 −εxy (k)

εxy (k)

0

⎞

⎟ −εxy (k) ⎟ ⎟ ⎟. εy (k) − μ Δ2 (k) ⎟ ⎠ ∗ Δ2 (k) −εy (k) + μ 0

(3.38)

Here, Δa (k), a = 1, 2, presents the pairing amplitude composed of the binary mean quantities for electrons referred to the hole or electron sheet of the Fermi surface. The amplitude consists of ﬁve terms corresponding to diﬀerent

page 139

March 24, 2021

140

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

symmetries of the operators: Δα (k) = s0a + sx2 +y2 a (k) + sx2 y2 a (k) + dx2 −y2 a (k) + dxya (k),

(3.39)

where sx2 +y2 a (k) = Δ0x2 +y2 a (cos kx + cos ky ), sx2 y2 a (k) = Δ0x2 y2 a cos kx cos ky , dx2 −y2 a (k) = Δ0x2 −y2 a (cos kx − cos ky ),

(3.40)

dxya (k) = Δ0xya sin kx sin ky , and s0a is independent of the momentum k. Thus, the pairing amplitude consists of three contributions with s-symmetry and two contributions with d-symmetry. The amplitures of the corresponding parameters of order are as follows: Δ0x2 +y2 a = − Δ0x2 y2 a

2J1 (cos kx ± cos ky )Δa (k ), N k

8J2 =− cos kx cos ky Δa (k ), N

(3.41)

k

Δ0xya = −

8J2 sin kx sin ky Δa (k ). N k

To calculate the quantity Δa (k), we need to construct the equations of motion for the electron Green function in the superconducting state: G(k, τ ) = −Tˆτ Ψk (τ )Ψ+ k (0).

(3.42)

Matrix (3.37) can be diagonalized with the help of the unitary transformation U + (k)A(k) U (k). The four eigenvalues are given by the formulas: (3.43) E1 (k) = −E2 (k), E3 (k) = −E4 (k), 1 E1,3 (k) = √ ξx2 + ξy2 + ε2xy + Δ21 + Δ22 2 1/2 ± (ξx2 − ξy2 + Δ21 − Δ22 )2 + 4ε2xy [(ξx + ξy )2 + (Δ1 − Δ2 )2 ] , (3.44)

page 140

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

141

where ξx = εx − μ, ξy = εy − μ. Thus, we get the equations of self-consistency for the pairing amplitudes and for the occupation numbers. We have ∗ Vkk U2m (k )U1m (k )F (Em (k )), 0Δ1 (k) = k m

Δ2 (k) =

k m

where n1 =

k m

n2 =

∗ Vkk U4m (k )U3m (k )F (Em (k )),

(3.45)

∗ U1m (k)U1m (k )F (Em (k )), ∗ U3m (k)U3m (k )F (Em (k )),

k m

and f (E) is the Fermi function. In Eq. (3.45), we sum the vectors over the index m = 1, 2, 3, 4 that enumerates components of superspinor (3.36). The equation for the superconductivity transition temperature can be obtained by the linearization of the equations for the amplitudes Δ1 (k) and Δ2 (k). For Δ2 (k), we get Vkk W3 (k ) − W1 (k ) , (3.46) Δ2 (k) = k

where Wi =

˜ 2 )Δ2 + ε2xy Δ1 ˜i ((εx − μ)2 − E E i , th ˜i 4ε2xy + (εx − εy )2 2T 2 |εx + εy − 2μ| E

(3.47)

˜i = Ei (Δ1 = Δ2 = 0). and E On the phase diagram (Fig. 3.16), we present the numerical solutions of the equations in the framework of the two-orbital model. In the upper left corner, where J2 > J2c 1.2, the pure phase with s-symmetry sx2 y2 is realized. In the right lower corner, where J1 > J1c 1.05, we observe the mixed phase with dx2 −y2 and sx2 +y2 . The remaining large part (J1 , J2 ) of the area is occupied by another mixed phase dx2 −y2 + sx2 y2 . In this case, the signs of the parameter of order with dx2 −y2 -symmetry are diﬀerent for two orbitals. For example, if Δ1 = a cos kx cos ky +b(cos kx −cos ky ), then Δ2 = a cos kx cos ky −b(cos kx −cos ky ). No solution corresponding to the dxy -symmetry of the parameter of order was found. In Fig. 3.17, we show the result of the intraorbital and interorbital pairings for the case J1 = J2 with the chemical potential μ = 1.8.

page 141

March 24, 2021

142

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 3.16. Phase diagram on the plane J1 –J2 for superconductivity states with diﬀerent parameters of order in the two-orbital model with the electron doping δ = 0.18 [134].

Fig. 3.17. The intraorbital pairing order parameter with sx2 y 2 and dx2 −y 2 and the interorbital pairing order parameter with dxy as functions of J = J1 = J2 , when the chemical potential is μ = 1.8 [136].

3.16. Conclusion We now indicate the common features of superconductors on the basis of iron and copper oxides: (1) Both classes of superconductors are quasitwo-dimensional (layered) systems from the viewpoint of their electron properties, which leads to the strong anisotropy. (2) In both classes, the region of coexistence of the superconductivity on the phase diagram is adjacent to the region of antiferromagnetism.

page 142

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch03

Iron Superconductors

143

(3) In both classes, the Cooper pairing is a singlet one. (4) The main properties of the superconducting state are typical of superconductors of the II kind. What are the diﬀerences between the superconductors on the basis of iron and copper oxides? (1) HTS cuprates are antiferromagnetic dielectrics (Mott strongly correlated ones), whereas new superconductors are antiferromagnetic metals. (2) Cuprates in the superconducting state are one-zone metals with one Fermi surface (hole or electron), whereas new superconductors are multizone metals with several Fermi surfaces of the electron and hole types. (3) In cuprates, the anisotropic Cooper pairing of the d-type is realized. In new superconductors, the isotropic pairing of the s± -type is observed. (4) The microscopic mechanisms of pairing in both classes of superconductors are diﬀerent: the unambiguously electron mechanism (spin ﬂuctuations) in cuprates, whereas the electron–phonon interaction (isotope-eﬀect) can turn out to be quite signiﬁcant in iron superconductors. It is clear that there are more diﬀerences between cuprates and iron superconductors, than similarities. We can conclude that HTS is the unique property of cuprates, i.e., strongly correlated systems close to the dielectric state. Iron superconductors are simpler and more understandable. Their normal state is not so mysterious, as that of cuprates, though the presence of many zones introduces a certain complexity. We may say that the phenomenon of HTS is much more spread, than it was considered two decades ago, so the community of researchers of the superconductivity can optimistically look at the future.

page 143

This page intentionally left blank

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

CHAPTER 4

Multiband Superconductivity

4.1. Introduction In this chapter, we present the theory of superconductivity with regard for a complicated multiband structure of superconductors. Calculations of the band structure of cuprate superconductors indicate that several energy bands intersect one another on the Fermi surface in these compounds [137], and the Fermi surface passes through high-symmetry points which correspond to the Lifshitz electronic topological transition. In addition, the discovery of two-gap superconductivity in two-band superconductors MgB2 allows one to consider the possibility to use a multiband theory of superconductivity. In Section 4.2, we analyze the problems of multiband superconductivity and superconductivity at room temperature. In Section 4.3, we study the physical properties of superconductors MgB2 and problems of twogap superconductivity, as well as the phase diagram for superconductors MgB2 on the basis of the renormalization group approach. In the ﬁeld of superconductivity, we meet the problem-maximum—it consists in the creation of room-temperature superconductors. We consider this problem in our book and give some recommendations on the search for these superconductors. In Section 4.5, we analyze the problem of high-temperature superconductivity at high pressures in hydrites. The results of this chapter were obtained by the author and published in works [137–147]. The theory of superconductivity arising from the electron–phonon interaction mechanism by Bardeen, Cooper, and Schrieﬀer (BCS) [148] has been well established, and it is now the standard theory for superconductivity [2,3,6,16,17,148]. In Chapter 2, we have considered non-BCS mechanisms via spin ﬂuctuations, charge ﬂuctuations (plasmons), and electron excitations (excitons) which have attracted a great interest, for example, in relation to the possibility of high-Tc superconductivity. These mechanisms have a common characteristic that the electron–electron (e–e) interaction is an origin of the superconductivity. After the discovery of the high-Tc copper 145

page 145

March 24, 2021

146

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

oxides [2], Anderson [6] has indeed emphasized an important role of the e–e interaction. For the past decade, many non-BCS theories [150–155] have been proposed, but they do not converge as a uniﬁed and well-accepted theory yet. On the other hand, a lot of experimental studies on copper oxides have revealed the following characteristics: (1) these species are antiferromagnets before doping, in accord with the importance of the e–e interaction, (2) the high-Tc superconductivity appears in the intermediate region of the metal-insulator transition and disappears in the metallic or overdoped region [156–158]. Accumulated experimental results on the species and related materials suggest a guiding principle that the doping in magnetic systems, more generally charge-transfer (CT) insulators, may provide several exotic phases which are (a) (b) (c) (d) (e) (f)

ferromagnetic metal or insulator, spin glass, paramagnetic metals, antiferromagnetic metals, ferrimagnetic metal or insulator, charge- or spin-mediated superconductor.

Relative stabilities of these phases should be dependent on several factors. This indicates, in turn, that the theoretical description of such phases and phase transitions in a systematic fashion is quite hard. Recently, the importance of multiband eﬀects in high-Tc superconductivity has been pointed out [3, 17, 144, 148]. In the framework of the two-particle Green’s function techniques [139,142], it is shown that a class of new so-called coupled states arises in electron–phonon system. The model numerical calculations have shown that the superconducting (SC) gap depends on the number of bands crossing the Fermi level, and the temperature dependence of the SC gap for high-Tc superconductors is more complicated than that predicted in the BCS approach. We have also investigated anomalous phases in a two-band model by using the Green’s function techniques [14, 159]. The expressions for the transition temperature for several phases have been derived, and the approach has been applied to the superconductivity in molecular crystals by charge injection and ﬁeld-induced superconductivity. In this chapter, we investigate the superconductivity, by using the twoband model and the two-particle Green’s function technique. In the framework of the two-band model, the coupled states in the electron system and the conditions when the coupled states can appear are investigated. We apply

page 146

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

147

the model to the electron–phonon mechanism within the traditional BSC method, the electron–electron interaction mechanism for high-Tc superconductivity, and the cooperative mechanism in relation to the multiband superconductivity.

4.2. Multiband Hamiltonian In this section, we brieﬂy summarize the two-band model for superconductivity, introduce a two-particle Green’s function, and investigate the spectral properties of the model.

4.2.1. Hamiltonian We start from the Hamiltonian for two-bands i and j : H = H0 + Hint , where H0 =

+ [[εi − μ] a+ ikσ aikσ + [εj − μ] ajkσ ajkσ ],

(4.1)

(4.2)

k,σ

Hint =

1 4

δ(p1 +p2 ,p3 +p4 ) αβγδ

+ + [Γiiii αβγδ aip1 α aip2 β aip3 γ aip4 δ + (i → j)

+ + + Γiijj αβγδ aip1 α aip2 β ajp3 γ ajp4 δ + (i → j) + + + Γijij αβγδ aip1 α ajp2 β aip3 γ ajp4 δ + (i → j)],

(4.3)

Γ is the bare vertex part: Γijkl αβγδ = ip1 α jp2 β | kp3 γ lp4 δ δαδ δβγ − ip1 α jp2 β | lp4 δ kp3 γ δαγ δβδ , (4.4) with

ip1 αjp2 β | kp3 γlp4 =

dr1 dr2 φ∗ip1 α (r1 )φ∗jp2 β (r2 )

× V (r1 , r2 )φkp3 γ (r2 )φlp4 δ (r1 ),

(4.5)

and a + ipσ (a ipσ ) is the creation (annihilation) operator corresponding to the excitation of electrons (or holes) in the i th band with spin σ and momentum p, μ is the chemical potential, and φ∗ipα is a single-particle wave function. Here, we suppose that the vertex function in Eq. (4.3) consists of the eﬀective interactions between the carriers caused by the linear vibronic coupling in several bands and the screened Coulombic interband interaction

page 147

March 24, 2021

148

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

of carriers. When we use the two-band Hamiltonian (4.1) and deﬁne the order parameters for the singlet exciton, triplet exciton, and singlet Cooper pair, the mean-ﬁeld Hamiltonian is easily derived [159–163, 166, 167]. Here, we focus on four-electron scattering processes: g1 = ii|ii = jj|jj,

(4.6)

g2 = ii|jj = jj|ii,

(4.7)

g3 = ij|ij = ji|ji,

(4.8)

g4 = ij|ji = ji|ij.

(4.9)

Here g 1 and g 2 represent the intraband two-particle normal and umklapp scatterings, respectively, g 3 means the interband two-particle umklapp process, and g 4 indicates the interband two-particle interaction on diﬀerent bands (see Fig. 4.1). Note that Γ’s are given by jjjj Γiiii αβγδ = Γαβγδ = g1 (δαδ δβγ − δαγ δβδ ), jjii Γiijj αβγδ = Γαβγδ = g2 (δαδ δβγ − δαγ δβδ ),

(4.10)

jiji Γijij αβγδ = Γαβγδ = g3 δαδ δβγ − g4 δαγ δβδ ,

where an antisymmetrized vertex function Γ is considered to be a constant independent of the momenta. The spectrum is elucidated by the Green’s function method. Using Green’s functions, which characterize the CDW (charge-density-wave), SDW (spin-density-wave), and SSC (singlet superconducting) phases, we obtain a self-consistent equation, according to the traditional procedure [14, 137, 159, 160]. Then, we can obtain expressions for the transition temperature for some cases.

Fig. 4.1. Electron–electron interactions. Dependence of g on the direction in the momentum space is ignored in this model gx (k) ≈ gx (x = i, j). We assume that g x is constant.

page 148

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

149

In the framework of the one-band model, the electronic phases are characterized by −g2 − 2g3 + g4 > 0, g2 + g4 > 0, −g1 > 0,

for CDW

for SDW for SSC.

In the framework of the two-band model, we have already derived expressions of the transition temperature for CDW, SDW, and SSC. In the previous paper [14, 159], we have investigated the dependence of Tc on the hole or electron concentration for the superconductivity of copper oxides by using the two-band model and have obtained a phase diagram of Bi2 Sr2 Ca1−x Yx Cu2 O8 (Bi-2212) by means of the above expressions for the transition temperature. The dependence of Tc on Δp can be reproduced in agreement with the experiment [161]. Recently, we have also obtained phase diagrams of copper oxides, anthracene, oligothiophene, and C60 crystals by using the analytic solutions [159].

4.2.2. Two-particle Green’s function In this subsection, we introduce a two-particle Green’s function [137–139] to investigate the physical properties of superconductivity in the twoband model. In statistical mechanics, Green’s functions are a convenient generalization of the notion of correlation functions. Like the latter, the former are closely related to the calculations of observables and give the well-known advantages in the construction and the solution of equations. First, let us deﬁne one-particle Green’s functions: , (4.11) Gνσ k, t − t = −iT aνkσ (t) a+ νkσ t where σ and ν mean labels for a spin and a band, respectively. The equation for a Green’s function derived by using the two-band model (4.1) is written as i

∂ −iT aνkσ (t) a+ νkσ t ∂t

∂aνkσ (t) + aνkσ t , = δ t − t + −iT i ∂t

(4.12)

where i

∂aνkσ (t) = [aνkσ , H] . ∂t

(4.13)

page 149

March 24, 2021

150

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

The equation for Green’s function (4.12) is rewritten after inserting Eq. (4.13) as i

∂ −iT aνkσ (t) a+ t νkσ ∂t = δ t − t + [εν − μ] −iT aνkσ (t) a+ νkσ t 1 g1 (δσδ δβγ − δσγ δβδ ) + 2 βγδ δ(k+p2 ,p3 +p4 )

× Gγδβσ 2νννν p3 , p4 , p2 , k; t, t 1 g2 (δσδ δβγ − δσγ δβδ ) + 2 ν

βγδ δ(k+p2 ,p3 +p4 )

× Gγδβσ 2ν ν νν p3 , p4 , p2 , k; t, t 1 (g3 δσδ δβγ − g4 δσγ δβδ ) + 2 ν

βγδ δ(k+p2 ,p3 +p4 )

× Gγδβσ 2νν ν ν p3 , p4 , p2 , k; t, t ,

(4.14)

where Gγδβσ 2νννν p3 , p4 , p2 , k; t, t

+ = −iT [aνp3 γ (t) aνp4 δ (t) a+ νp2 β (t − 0) aνkσ t ], Gγδβσ 2ν ν νν p3 , p4 , p2 , k; t, t + = −iT [aν p3 γ (t) aν p4 δ (t) a+ νp2 β (t − 0) aνkσ t ], Gγδβσ 2νν ν ν p3 , p4 , p2 , k; t, t + = −iT [aνp3 γ (t) aν p4 δ (t) a+ ν p2 β (t − 0) aνkσ t ].

(4.15)

(4.16)

(4.17)

Here ν indicates a band diﬀerent from ν. To calculate the density of electron states, we have to focus on the case where t → t − 0. The two-particle Green’s functions in Eq. (4.14) is rewritten as G 2 (p3 , p4 , p2 , k; t-t’ ) (t → t − 0 ). In this study, we investigate only the spectral properties of two-particle Green’s functions for the superconductivity. Therefore, we focus on the following two-particle Green’s function: Gγδβσ 2νννν p3 , p4 , p2 , k; t, t + (4.18) = −iT [aνp3 γ (t) aνp4 δ (t) a+ νp2 β t aνkσ t ].

page 150

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

151

For simplicity, we consider only three cases: (4.1) g1 = 0 and others = 0, (4.2) g2 = 0 and others = 0, and (4.3) g1 = 0, g2 = 0 and others = 0.

4.2.3. Traditional superconductivity In general, in the framework of the BCS theory, the Hamiltonian is described by a single-band model. In the eﬀective electron–electron interaction (4.1), we consider that g1 = 0 and others = 0 and focus only on the single-band model. According to the approach [156] used for phonon systems which is based on the method of Bogoliubov–Tyablikov [192], we can derive the equation for a two-particle electron Green’s function. The spectral features of the electron system in the mentioned region of energy are described by the Fourier transform of this function. For the simplest case of a one-electron zone crossing the Fermi energy level, it can be given as f (k, k , ω) σ,σ φ (σ, σ ) γδβσ , (4.19) G2νννν p3 , p4 , p2 , k; t − t = 1 − g1 q K (ω, k, k , q) where 2 − nνk+q − nνk −q , K ω, k, k , q = 2ω − ενk+q − ενk −q

(4.20)

n k indicates the ﬁlling number of electrons, and g 1 is the eﬀective Fourier transform of the electron–electron interaction. If the e–e interaction constant renormalized by the electron–phonon interaction becomes negative, coupled states will appear in the electron system. In the previous papers [137–139], we have presented analysis of the spectral properties of the two-particle Green’s function. According to the same procedure [17, 139], we obtain the equation for coupled states in the electron system: Δ (4.21) 1 − g1 N (εf ) − ln 1 − = 0, a where N (εf ) = nνk =

√

2πm∗ν

m∗ν ε 2 − nνk+q − nνk −q |ε=εf ,

1 ν , exp εk − εf /T + 1

(4.22) (4.23)

a = 2(ω − εf − Δν − E), E = k2 /2m, ε = q 2 /2m, and m∗ ν = mν /m. m∗ ν means the reduced eﬀective mass of electron in the crystal energy zone.

page 151

March 24, 2021

20:13

152

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

m is mass of free electron. If g1 < 0, we can ﬁnd solutions of Eq. (4.21) for superconductivity.

4.2.4. Copper oxides In copper oxides, the eﬀective electron–electron interaction g 2 is eﬃciently important to realize the high-Tc superconductivity [161, 164]. Therefore, we consider that g2 = 0 and others = 0. The two-particle Green’s function of Eq. (4.18) is rewritten as f (k, k , ω) σ,σ φ (σ, σ ) γδβσ , (4.24) G2νννν p3 , p4 , p2 , k; t − t = 1 − g22 q,q K2 (ω, k, k , q, q ) where

ν ν ν ν 2 − n − n − n 2 − n k+q k+q−q k −q+q k −q . K2 ω, k, k , q, q = 2ω − ενk+q−q − ενk −q+q 2ω − ενk+q − ενk −q (4.25)

According to similar procedure in previous papers [137, 139], we study the situation near the extremum (minimum or maximum) of the electron zone. Then we suppose k = k = k0 + k , and ενk0 = εν corresponds to the extremum of the zone. We expand the energy in the momentum k ± q in a series up to terms of the second order and suppose that the energy extremum is located near the Fermi-level energy. Then, the sum in the denominator of Eq. (4.24) is approximately reduced to the following expression: ν ν 2Δ 2Δ K2 ω, k, k , q, q ≈ N εf N εf ln 1 − 1− . aν aν q,q

(4.26) Therefore, we obtain the equation for coupled states in the electron system: ν ν 2Δ 2Δ 2 1− = 0. (4.27) 1 − g2 N εf N εf ln 1 − aν aν From Eq. (4.27), we ﬁnd the possibility of the existence of a solution for the coupled states, if g2 = 0. Thus, the eﬀective electron–electron interaction g 2 with positive value contributes to the superconductivity.

page 152

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

153

4.2.5. Cooperative mechanism Here, we consider that g1 = 0, g2 = 0, and others = 0. In a similar way, the two-particle Green’s function of Eq. (4.18) is approximately derived as Gγδβσ 2νννν p3 , p4 , p2 , k; t − t f (k, k , ω) σ,σ φ (σ, σ ) , = [1 − (g1 + g2 ) q K (ω, k, k , q)][1 − (g1 − g2 ) q K (ω, k, k , q)] (4.28) where K(ω, k, k , q) is given by Eq. (4.20). The summation in the denominator of Eq. (4.28) is performed in a similar way, and the equation for coupled states in the electron system is approximately derived as Δ Δ 1 − (g1 + g2 ) N (εf ) ln 1 − 1 − (g1 − g2 ) N (εf ) ln 1 − = 0. a a (4.29) When g1 + g2 < 0 or g1 − g2 < 0, we can ﬁnd solutions of this equation.

4.2.6. Room-temperature superconductors In the previous section, we have approximately calculated two-particle Green’s functions for three cases, which are the traditional superconductivity, copper oxides, and cooperative mechanism in the framework of the twoband model. From these Green’s functions, we have derived the equation for coupled states for each case. In the case of a single-band model, which indicates the traditional superconductivity such as the BCS theory, it is necessary that the eﬀective electron–electron interaction be negative (g1 < 0) to realize the superconductivity. The maximal transition temperature for the superconductivity predicted by the theory is about 40 K. On the other hand, we can expect in a two-band model for negative g1 that the transition temperature becomes higher than that derived within the single-band model, because of the tunneling of Cooper pairs between two bands. The tunneling of Cooper pairs causes the stabilization of the order parameter of the superconductivity [163, 164, 173]. In the framework of the two-band model, we consider that the Fermi energy level crosses with two bands. The results derived from the two-particle Green’s function in the previous section suggest that the superconductivity appears for g2 < 0 or g2 > 0. Note that

page 153

March 24, 2021

154

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 4.2.

Schematic diagram for superconductivity. MB means multiband eﬀects.

g2 contributes to SDW. From the results derived from calculations involving g1 and g2 (cooperative mechanism), we expect a higher Tc than that of copper oxides. On the basis of the results obtained in this section, we present a schematic diagram for superconductivity shown in Fig. 4.2. The mechanism of high-Tc superconductivity of materials such as copper oxides might be around the cooperative mechanism in Fig. 4.2. In what follows, we calculate a twoparticle Green’s function in the two-band model and derive an equation for coupled states. In the framework of the two-band model, the results predict that superconductivity appears even if the electron–electron interaction is positive. We can expect that the transition temperature is higher (300 K) than that for copper oxides by the cooperative mechanism (Fig. 4.3). Let us discuss the problem of superconductors operating at room temperature (RTSC). It is obvious that the main task in the ﬁeld of superconductivity is the fabrication of materials with superconducting properties at room temperature. The study of HTSC is only a stage on the way to the main purpose, namely to the development of room-temperature superconductors. At the present time, the highest known Tc = 135 K (at the atmospheric pressure). Now there occurs the wide-scale search for such superconductors. Since none of the known physical laws allows one to exclude the possibility for RTSC to exist, the future discovery of RTSC seems to be doubtless. New materials are created by means of physical and chemical modiﬁcations of the known compounds, including the application

page 154

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

155

Fig. 4.3. The structure of MgB2 containing graphite-tape B layers separated by hexagonal close-packed layers of Mg.

of methods named “nanotechnological”. The creation of new materials with preassigned physical properties is one of the actual problems of modern science. At present, various approaches are developed in order to avoid the labor-consuming sorting of diﬀerent chemical compounds and conditions of synthesis, i.e., to optimize the solution of this problem. One of the most eﬃcient and promising is the method of structural design. In work [165], the structural design was used in solving the problems related to the search for new HTSC on the basis of complex copper oxides. We now present the recommendations concerning the search for new HTSC with higher critical temperatures which were advanced by the Nobel’s Prize winner K.A. M¨ uller [166]. He divided the well-known HTSC into three classes: (1) layered cuprates; (2) MgB2 ; (3) doped fullerenes of the type K3 C60 . K.A. M¨ uller emphasizes that the discovery of cuprate superconductors was promoted by the conception of Jahn–Teller polarons. Two singlet polarons form a bipolaron. Bipolarons are able, in turn, to form metallic clusters (stripes). K.A. M¨ uller indicated the following factors which Should be taken into account in the search for new HTSC: (1) superconductivity is favored by a layered (quasi-two-dimensional) crystalline structure;

page 155

March 24, 2021

156

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

(2) oxygen ions are proposed as anions; (3) ﬂuorine, chlorine, and nitrogen can be considered as well. It is worth noting that the recent discovery of FeAs superconductors eliminated the monopoly of cuprates in the physics of HTSC. It is possible that new superconductors should be sought in the other rows and columns of the Periodic Table. It is necessary to concentrate eﬀorts on the purposeful search and the creation of new HTSC.

4.3. Two-gap Superconductivity in MgB2 4.3.1. The physical properties of MgB 2 Recently, the superconductivity of MgB2 with Tc = 39 K, which is the highest temperature among two-component systems, was discovered [168]. A great interest in the study of magnesium diboride is related to the fact that MgB2 has occupied the “intermediate” place between low- and high-temperature superconductors by the value of Tc . Therefore, the modern literature names MgB2 a “medium Tc -superconductor” (MTSC). It is necessary to mention the cheapness of this superconductor as for the applications. We recall that wires made of cuprate superconductors include 70% of silver which is expensive. An important peculiarity of MgB2 is its quasi-two-dimensional structure of the AlB2 type. Interestingly, AlB2 is not superconducting. Note that magnesium diboride is another example of the crucial role played by the lattice structure regarding superconductivity [167]. MgB2 is an “old” material which has been known since the early 1950s, but it was only recently discovered to be superconducting. MgB2 has a hexagonal structure [162], see Fig. 4.4 [24]. The results of calculations of the temperature dependence of the speciﬁc heat of MgB2 given in Fig. 4.5 follow the corresponding experimental data. The band structure of MgB2 has been calculated in several works since the discovery of superconductivity [172]. The electronic properties of MgB2 are plotted in Fig. 4.2. The band structure of magnesium diboride is similar to that of graphite and is formed by the σ and π zones. The important problem for the superconductivity in magnesium diboride is the mechanism of superconductivity. It can be the conventional electron– phonon mechanism or a more exotic mechanism of superconductivity. The presence of an isotope eﬀect is a strong indicator of the phonon mediation of superconductivity. The large isotope eﬀect αB = 0.26 [169] shows that phonons associated with B vibrations play a signiﬁcant role in the magnesium diboride superconductivity, whereas the magnesium isotope eﬀect is very

page 156

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

Fig. 4.4.

157

Band structure of MgB2 .

Fig. 4.5. The MgB2 speciﬁc heat vs. temperature. Solid line — theory. Points represent the experimental data.

small: αM = 0.02 [169]. The total isotope eﬀect is αB + αM = 0.3, which supports the electron–phonon mechanism of superconductivity. Magnesium diboride is the II-type superconductor [167]. The discovery of the superconductivity of MgB2 has aroused a great interest in the multigap

page 157

March 24, 2021

158

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

superconductivity [169]. Magnesium diboride has two superconducting gaps, 4 meV and 7.5 meV, due to the π and σ electron bands. The two-gap structure was established in a number of experiments [162]. The plot of the speciﬁc heat of MgB2 vs. temperature (Fig. 4.5) demonstrates a good agreement between the theoretical and experimental data. Both gaps have s-symmetry and are resulted from the highly anisotropic layer structure of MgB2 . Although the multigap superconductivity was discussed theoretically [163, 164, 173] as early as 1958, it has been observed experimentally [170] in the 1980s. MgB2 is the ﬁrst material, in which the eﬀects of the multigap superconductivity are so dominant, and its implications so thoroughly explored. The Nature has let us have a glimpse of a few her multigap mysteries and has challenged us. Recent band calculations [171,172] of MgB2 with the McMillan formula for the transition temperature have supported the e–p interaction mechanism for the superconductivity. In this case, the possibility of two-band superconductivity has also been discussed in relation to two-gap functions experimentally and theoretically. Very recently, the two-band or multiband superconductivity has been theoretically investigated in relation to the superconductivity arising from Coulomb repulsive interactions. The two-band model was ﬁrst introduced by Kondo [173]. We have also investigated anomalous phases in the twoband model by using the Green’s function techniques [137–140, 142, 143]. Recently, we have pointed out the importance of multiband eﬀects in high-Tc superconductivity [137–139]. The expressions for the transition temperature for several phases have been derived, and the approach has been applied to the superconductivity in molecular crystals by charge injection and the ﬁeldinduced superconductivity [14]. In the previous paper [137–140,142,143], we have investigated the superconductivity by using the two-band model and the two-particle Green’s function techniques. We have applied the model to the electron–phonon mechanism for the traditional BCS method, electron– electron interaction mechanism for high-Tc superconductivity [2], and cooperative mechanism. In the framework of the two-particle Green’s function techniques [142], it has been shown that the temperature dependence of the superconductivity gap for high-Tc superconductors is more complicated than that predicted in the BCS approach. In paper [172], phase diagrams for the two-band model superconductivity have been investigated, by using the renormalization group approach. Below, we will discuss the possibility of the cooperative mechanism of two-band superconductivity in relation to the high-Tc superconductivity and study the eﬀect of the increasing of Tc in MgB2 due to the enhanced interband pairing scattering. In this section, we will investigate our two-band model for the explanation the multigap

page 158

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

159

superconductivity of MgB2 . We apply the model to the electron–phonon mechanism for the traditional BCS method, electron–electron interaction mechanism for high-Tc superconductivity, and cooperative mechanism in relation to multiband superconductivity.

4.3.1.1. Mg1−x Alx B2 Critical temperature and other superconducting properties of two-band superconductors depend on the doping level and on the interband and intraband scattering and can be modiﬁed by chemical substitutions. The inﬂuence of doping on the transition temperature in Mg1−x Alx B2 is illustrated in Fig. 4.6. It is seen that the doping destroys the superconductivity in MgB2 . This can be understood as a result of the competition of two eﬀects: the ﬁrst one is a coupling eﬀect related to the changes of the carrier concentration, and the second one depends on the introduction of new scattering centers leading to a modiﬁcation of the interband and intraband scattering.

4.3.2. Theoretical model In this section, we will use the two-band model for superconductivity. We start from the Hamiltonian for two-bands i and j: H = H0 + Hint ,

(4.30)

where H0 =

[[ i (k) − μ] a†ikσ aikσ + [ j (k) − μ] a†jkσ ajkσ ],

(4.31)

k,σ

Fig. 4.6. The inﬂuence of doping on Tc in Mg1−x Alx B2 . Solid line — theory. Points represent the experimental data.

page 159

March 24, 2021

20:13

160

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

Hint =

1 4

δ(p1 +p2 ,p3 +p4 ) α,β,γ,δ

† † [Γiiii αβγδ aip1 α aip2 β aip3 γ aip4 δ + (i ↔ j)

† † + Γiijj αβγδ aip1 α aip2 β ajp3 γ ajp4 δ + (i ↔ j) † † + Γijij αβγδ aip1 α ajp2 β aip3 γ ajp4 δ + (i ↔ j)],

(4.32)

Γ is the bare vertex part: Γijkl αβγδ = ip1 αjp2 β|kp3 γlp4 δδαδ δβγ − ip1 αjp2 β|lp4 δkp3 γδαγ δβδ (4.33) with ip1 αjp2 β|kp3 βlp4 α = dr1 dr2 φ∗ip1 α (r1 )φ∗jp2 β (r2 )V (r1 , r2 )φkp3 β (r2 )φlp4 α (r1 ),

(4.34)

where aipσ+ (aipσ ) is the creation (annihilation) operator corresponding to the excitation of electrons (or holes) in the ith band with spin σ and momentum p, μ is the chemical potential, and φ is a single-particle wave function. Here, we suppose that the vertex function in Eq. (4.32) involves the eﬀective interactions between the carriers caused by the linear vibronic coupling in several bands and the screened Coulombic interband interaction of carriers. When we use the two-band Hamiltonian (4.1) and deﬁne the order parameters for a singlet exciton, triplet exciton, and singlet Cooper pair, the mean-ﬁeld Hamiltonian is easily derived [137–140, 142, 143]. Here, we focus on three electron scattering processes contributing to the singlet superconducting phase in Hamiltonian (4.1): gi1 = ii|ii,

gj1 = jj|jj,

(4.35)

g2 = ii|jj = jj|ii,

(4.36)

g3 = ij|ij = ji|ji,

(4.37)

g4 = ij|ji = ji|ij,

(4.38)

gi1 and gj1 represent the ith and jth intraband two-particle normal scattering processes, respectively, and g2 indicates the intraband two-particle umklapp scattering (see Fig. 4.7). For simplicity, we consider three cases in [171]: (1) g1 = 0 and others = 0, (2) g2 = 0 and others = 0, and (3) gi1 = 0 and gj1 = 0, and others = 0, using the two-particle Green’s function techniques (see Fig. 4.7). It was shown that, possibly, the two-gap superconductivity arises in case (3). The superconductivity arising from the electron–phonon mechanism

page 160

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

161

Fig. 4.7. Electron–electron interactions. Solid and dashed lines indicate π- and σ-bands, respectively; gi1 , gj1 , g2 , g3 , and g4 contribute to superconductivity.

(g1 < 0 and g1 < g2 ) such as for MgB2 is in the two-gap region. On the other hand, the superconductivity of copper oxides (g1 > g2 ) is outside the twogap region. These results predict that we may observe two-gap functions for MgB2 and only a single-gap function for copper oxides.

4.3.3. Superconductivity in M gB 2 We used case (3) for gi1 and gj1 , g2 = 0 and others = 0 to describe the superconductivity in MgB2 . We have a reduced Hamiltonian H = H0 + Hint ,

(4.39)

where H0 =

[[ i − μ] a†ikσ aikσ + [ j − μ] a†jkσ ajkσ ], k,σ

Hint =

g1i a†ik a†i−k ai−k aik + + g2 a†ik a†i−k aj−k ajk .

(4.40)

i→j (4.41)

page 161

March 24, 2021

162

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

We now deﬁne the order parameters which are helpful to construct the meanﬁeld Hamiltonian: † † aip↑ ai−p↓ , (4.42) Δi = p

Δj =

a†jp↑ a†j−p↓ .

(4.43)

p

The relation between two superconducting gaps of the system is as follows: Δj = where

μ−Ec

fi = μ

μ−Ej

fj = μ−Ec

1 − gi1 ρi fi Δi , g2 ρj fj

2 1/2 ξ + Δ2i , 1/2 tanh 2T ξ 2 + Δ2i 1/2 2 + Δ2 ξ j dξ 1/2 tanh 2T ξ 2 + Δ2j

(4.44)

dξ

(4.45)

with the coupled gap equation (1 − gi1 ρi fi ) (1 − gj1 ρj fj ) = g22 fi fj .

(4.46)

We have tried to estimate the coupling constant of the pair electron scattering process between π- and σ-bands of MgB2 . We have calculated the parameters by using a rough numerical approximation. We focus on one π-band and σ-band of MgB2 and consider electrons near Fermi surfaces. We ﬁnd that the parameter g1 = −0.4 eV, by using the transfer integral between the π- and σ-bands. We estimate the coupling parameter g2 of the pair electron scattering process by the expression 1,2 Vk1,k2 , (4.47) g2 = k1,k2 1,2 = Vk1,k2

u∗1,r (k1)u∗1,s (k1)vrs u2,t (k2)u2,u (k2),

(4.48)

r,s,t,u

where labels 1 and 2 mean the π- and σ-bands, respectively, ui,r (ξ) is the LCAO coeﬃcient for the ith band, and ξ is the moment [159, 160]. The indices k1 and k2 are summed over each Fermi surface. However, it is diﬃcult to perform the sum exactly. In this case, we used a few points near the Fermi surface. The coupling constant of the pair electron scattering between the π-band and σ-band g2 = 0.025 eV. From numerical calculations

page 162

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

Fig. 4.8.

163

Temperature dependence of two superconducting gaps.

of Eqs. (4.44)–(4.46), we can also obtain the temperature dependence of the two-gap parameters (see Fig. 4.8). We have used the density of states of the π- and σ-bands (ρi = 0.2 eV −1 , ρj = 0.14 eV −1 ), chemical potential μ = −2.0, the top energy of σ-band Ej = −1.0, and the ﬁtting parameters (gi1 = −0.4 eV, gj1 = −0.6 eV, g2 = 0.02 eV). These calculations have qualitative agreement with experiments [162, 174, 175]. The expression for the transition temperature of superconductivity is derived in a simple approximation: Tc+ = 1.13(ζ − Ej ) · exp(−1/g+ ρ),

(4.49)

where g+ =

1 (B + B 2 − 4A) 24

(4.50)

and A = g1i g1j − g22 ,

(4.51)

B = g1i + g1j ,

(4.52)

ζ = −μ.

(4.53)

page 163

March 24, 2021

164

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 4.9.

Schematic diagram of the mechanism of pairing for two gaps.

From the expressions for Tc+ , we can see the eﬀect of increase of Tc+ due to the enhanced interband pairing scattering (g2 ). Figure 4.9 shows a schematic diagram of the mechanism of pairing for two gaps. The scenario is as follows. Electrons from the π- and σ-bands make up the subsystems. For g2 , we have two independent subsystems with the diﬀerent transition temperatures of superconductivity Tcπ and Tcσ and two independent superconducting gaps. In our model, we have two coupled superconducting gaps with relation (16) and one transition temperature of superconductivity Tc+ , which is in agreement with experiments. In this model, we have two channels of superconductivity: conventional channel (intraband g1 ) and unconventional channel (interband g2 ). Two gaps appear simultaneously in diﬀerent bands which are like BCS gaps. The gap in the π-band is bigger as compared with that for the σ-band, because the density of state is 0.25 eV in the π-band and 0.14 eV in the σ-band. The current of Cooper pairs ﬂows from the π-band into the σ-band, because the density of Cooper pairs in the π-band is much higher. The tunneling of Cooper pairs also stabilizes the order parameter in the σ-band. In this way, we can predict the physical properties of the multigap superconductivity, if we have the superconductors with a multiband structure, as shown in Fig. 4.9. Thus, we have presented our two-band model with the intraband twoparticle scattering and interband pairing scattering processes to describe two-gap superconductivity in MgB2 . We deﬁned the parameters of our model and made numerical calculations of the temperature dependence of two gaps in a qualitative agreement with experiments. We have proposed a twochannel scenario of superconductivity : the ﬁrst one is the conventional channel (intraband g1 ) which is connected with the BCS mechanism in diﬀerent bands and the unconventional channel (interband g2 ) which describes the tunneling of Cooper pairs between two bands. The tunneling of Cooper pairs also stabilizes the order parameters of superconductivity and increases the critical temperature of superconductivity.

page 164

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

165

4.4. Theoretical Studies of Multiband Eﬀects in Superconductivity by Using the Renormalization Group Approach We present the renormalization equations by using the two-band model and construct phase diagrams for the two-band superconductivity. In the framework of the two-band model, the given results predict that superconductivity appears, even if the electron–electron interaction is positive. We discuss the possibility of a cooperative mechanism in the two-band superconductivity in relation to high-Tc superconductivity. The recent discovery of superconductivity of MgB2 [168] has also attracted a great interest in the elucidation of its mechanism from both experimental and theoretical viewpoints. A crucial role of the electron–phonon (e–p) interaction has been pointed out for the superconductivity of MgB2 . Recent band calculations of the transition temperature for MgB2 [171, 172] with the McMillan formula [176] have supported the e–p interaction mechanism for the superconductivity. In this case, the possibility of the two-band superconductivity in relation to two-gap functions has also been considered experimentally and theoretically. Very recently, the two-band or multiband superconductivity has been theoretically investigated in relation to the superconductivity arising from Coulomb repulsive interactions [177, 231]. The two-band model was ﬁrst introduced by Kondo [173]. Recently, we have pointed out the importance of multiband eﬀects in high-Tc superconductivity [182]. We have also investigated anomalous phases in the two-band model by using the Green’s function techniques [180]. The expressions of the transition temperature for several phases have been derived, and the approach has been applied to the superconductivity in several crystals by charge injection and the ﬁeld-induced superconductivity [180, 183]. In the previous section, we have investigated superconductivity by using the two-band model and the two-particle Green’s function techniques [142, 192]. We have applied the model to the electron–phonon mechanism for the traditional BSC method, electron–electron interaction mechanism for high-Tc superconductivity, and cooperative mechanism. In the framework of the two-particle Green’s function techniques [142], it has been shown that, in the electron–phonon system, a class of new so-called coupled states arises. In this section, we investigate two- or multiband eﬀects in superconductivity by using the twoband model within the renormalization group approach. Renormalization equations for the two-band superconductivity are derived from the response function and the vertex correction of the model. Phase diagrams numerically obtained from the renormalization equations are presented. We also discuss

page 165

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

166

the superconductivity arising from the e–e repulsive interaction in relation to the two-band superconductivity.

4.4.1. Theoretical model In this section, we brieﬂy summarize the two-band model for the superconductivity and introduce the renormalization group approach [186, 188]. We consider a Hamiltonian for two bands i and j written as H = H0 + Hint ,

(4.54)

where H0 =

Hint =

[[ i (k) − μ] a† aikσ + [ j (k) − μ] a† aj kσ ], ik σ j kσ k,σ 1 4

δ(p1 +p2 ,p3 +p4 ) α,β,γ,δ

(4.55)

† † [Γiiii αβγδ aip α aip β aip3 γ aip4 δ + (i ↔ j) 1

2

† † + Γiijj αβγδ aip1 α aip2 β aj p3 γ aj p4 δ + (i ↔ j) † † + Γijij αβγδ aip1 α aj p2 β aip3 γ aj p4 δ + (i ↔ j)],

(4.56)

Γ is the bare vertex part: Γijkl αβγδ = ip1 αjp2 β|kp3 γlp4 δδαδ δβγ − ip1 αjp2 β|lp4 δkp3 γδαγ δβδ , (4.57) with ip1 αjp2 β|kp3 βlp4 α = dr1 dr2 φ∗ip1 α (r1 )φ∗j p2 β (r2 )V (r1 , r2 )φkp3 β (r2 )φlp4 α (r1 ),

(4.58)

where a†ipσ (aipσ ) is the creation (annihilation) operator corresponding to the excitation of electrons (or holes) in the ith band with spin σ and momentum p, μ is the chemical potential, and φ∗iαp is a single-particle wave 1 function. Here, we suppose that the vertex function in Eq. (4.56) involves the eﬀective interactions between carriers caused by the linear vibronic coupling in several bands and the screened Coulombic interband interaction of carriers.

page 166

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity i

j

i

j =gj1

=gi1 i

i

j

j

i

j

j

i

=g2 i

j

167

=g2 j

i

Fig. 4.10. Electron–electron interactions. Dependence of g on the direction in the momentum space is ignored in this model (gx (k) ≈ gx (x = i, j)). We assume that gx is constant.

We focus on three electron scattering processes contributing to the singlet superconducting phase in Hamiltonian (4.56), as shown in Fig. 4.10, gi1 = ii|ii,

(4.59)

gj1 = jj|jj,

(4.60)

g2 = ii|jj = jj|ii,

(4.61)

gi1 and gj1 represent the ith and jth intraband two-particle normal scattering processes, respectively, and g2 indicates the intraband two-particle umklapp scattering. Note that Γ’s are given by Γiiii αβγδ = gi1 (δαδ δβγ − δαγ δβδ ), Γjjjj αβγδ = gj1 (δαδ δβγ − δαγ δβδ ),

(4.62)

jjii Γiijj αβγδ = Γαβγδ = g2 (δαδ δβγ − δαγ δβδ ),

where we assume that an antisymmetrized vertex function Γ is a constant independent of the momenta. The spectrum is elucidated by the Green’s function method. Using Green’s functions which characterize the CDW, SDW, and SSC phases, we obtain a self-consistent equation according to the traditional procedure [159, 180, 182, 188–191]. Then we can obtain expressions for the transition temperature in some cases. Electronic phases of a one-dimensional system have been investigated by using a similar approximation in the framework of the one-band model [188–191]. In the framework of the meanﬁeld approximation within the two-band model, we have already derived expressions for the transition temperature for CDW, SDW, and SSC.

page 167

March 24, 2021

168

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

In paper [180, 182], we have investigated the dependence of Tc on the hole or electron concentration for the superconductivity of copper oxides by using the two-band model and have obtained a phase diagram of Bi2 Sr2 Ca1−x Yx Cu2 O8 (Bi-2212) by means of the above expressions for the transition temperature.

4.4.2. Renormalization group approach The Dyson equation is invariant under a multiple renormalization of Green’s function and coupling parameters g. From this invariance for a scaling procedure, we obtain diﬀerential equations for the coupling parameters and the external vertex of a Cooper pair: ∂ ∂ g˜i (y, u, g) = g˜i (ξ, u/y, g˜(t, u, g))|ξ=1 , ∂y ∂ξ

(4.63)

∂ ∂ ln Λ(y, u, g) = ln Λ(ξ, u/y, g˜(t, u, g))|ξ=1 , ∂y ∂ξ

(4.64)

y y

where y and u are parameters with the dimension of energy, g means the set of original couplings, and Λ is the external vertex.

4.4.3. Vertex correction and response function for Cooper pairs To solve Eqs. (4.63) and (4.64), we estimate the right-hand side of Eq. (4.63) by using the perturbation theory. We consider the lowest order correction to the vertex for a Cooper pair as shown in Fig. 4.11. From these diagrams, we obtain 2 −g22 −gi1 gi1 Li g˜i1 = + , (4.65) 2 2 −gj1 −g2 g˜j1 gj1 Lj g2 −gi1 g2 −g2 gj1 Li g˜2 = + , (4.66) g˜2 g2 −gj1 g2 −g2 gi1 Lj where T Gi (q, ω )Gi (k − q, ω − ω ), N q,ω T Gj (q, ω )Gj (k − q, ω − ω ), Lj = Πj (k, ω) = N q ,ω Li = Πi (k, ω) =

(4.67)

page 168

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity (a)

(b)

(c)

(d)

(e)

(f)

(g)

(h)

169

Fig. 4.11. Diagrams of the ﬁrst-order vertex correction: (a) and (b) contribute to g˜i1 , (c) and (d) are diagrams for g˜j1 , (e)–(h) for g˜2 .

where G and T are the temperature Green’s function and temperature, respectively. For the special case ω = 0, k = 0, the above functions Li and Lj become ui /y ui /y + tanh ln ξ − 2A, (4.68) Li = − tanh 2ξ 2ξ uj /y uj /y + tanh ln ξ − 2A, (4.69) Lj = − tanh 2ξ 2ξ where

A=

dx ln x sech2 x,

(4.70)

ui (uj ) and ui (uj ) are dimensionless functions expressed by the chemical potential, cut-oﬀ energy, the top energy of jth band, and the density of state for the ith (jth) band. Next, we consider a ﬁrst-order response function for a singlet Cooper pair as shown in Fig. 4.12. Then the ﬁrst-order vertex function Λ for the

page 169

March 24, 2021

170

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity (a)

(b)

(c)

(d)

Fig. 4.12. Diagrams of the ﬁrst-order response function: (a) and (b) contribute to Λi , (c) and (d) show diagrams for Λj .

ith and jth bands can be written as 2 Λi + Λj −g1 = + −g1 Λi − Λj 0

−g2 g2

Li + Lj . Li − Lj

(4.71)

4.4.4. Renormalization equation For simplicity, hereafter we assume gi1 = gj1 . From Eqs. (4.63), (4.65), and (4.66), we obtain the diﬀerential equations written as ∂ g˜1 = − g˜12 + g˜22 , ∂x ∂ g˜2 = −2˜ g1 g˜2 . ∂x

(4.72) (4.73)

In similar way, using Eqs. (4.64) and (4.71), we obtain the diﬀerential equations written as ∂ ln Λ+ = −˜ g1 − g˜2 , ∂x ∂ ln Λ− = −˜ g1 + g˜2 , ∂x

(4.74) (4.75)

where Λ+ = Λi + Λj and Λ− = Λi − Λj .

4.4.5. Phase diagrams In the previous section, we have derived the basic equations (4.72)–(4.75) to ﬁnd the low-temperature phases. For the special case of g2 = 0, we obtain

page 170

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

171

an analytic solution g˜1 =

1 , x + g1−1

(4.76)

g˜2 = 0, Λi = Λj =

(4.77) 1 . g1 x + 1

(4.78)

4

2

2

2

4

g

g

2

From these solutions, we ﬁnd that the superconducting phase appears only when the intraband interaction g1 is negative. In the case of the traditional superconductivity described by the BCS theory, it is necessary that the eﬀective electron–electron interaction be negative (g1 < 0) to realize the superconductivity. The present result agrees with that of the traditional theory for superconductivity expressed by the one-band model. For the case of g2 = 0, the phase diagrams numerically obtained from the above renormalization equations are shown in Fig. 4.13. Figure 4.13(a) shows the phase diagram for the sum of contributions to the superconductitivity from the ith and jth bands. Thus, this phase implies that the signs of the superconducting state for the ith and jth bands are the same. From this diagram, we ﬁnd the superconductivity only for −g1 − g2 > 0 with negative g2 . On the other hand, the phase diagram for the diﬀerence between the superconducting states for the ith and jth bands is shown in Fig. 4.12(b). In this case, this phase means that the sign of the superconductivity for the ith band is diﬀerent from that of the jth band. We can ﬁnd that the superconductivity appears only for −g1 + g2 > 0 with positive g2 from Fig. 4.13(b). Thus, the present results suggest that the two-band

0

0

-2

-2

-4

-4

(a)

Fig. 4.13.

(b)

Phase diagrams for superconductivity: (a) Λi + Λj , (b) Λi − Λj .

page 171

March 24, 2021

172

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

superconductivity appears, when the intraband umklapp repulsive scattering g2 is larger than the normal repulsive scattering g1 . In the region of g2 > g1 with g2 < 0 and g2 < −g1 with g2 > 0 (two-gap region), we can expect that two-gap functions are observed. In the former region, those superconducting gaps may be expressed by |Λ+ | > |Λ− |, and the latter may be |Λ+ | < |Λ− |. On the other hand, we expect only a single-gap function in the other region. These results agree with the previous solutions [140] derived by using the two-particle Green’s function techniques. The superconductivity arising from the electron–phonon mechanism (g1 < 0 and |g2 | < |g1 |) such as that in MgB2 is in the two-gap region. On the other hand, the superconductivity such as in copper oxides (|g2 | > |g1 |) is outside the two-gap region. These results predict that we may observe two-gap functions for MgB2 and only a single-gap function for copper oxides. In the two-band model for negative g1 with transferring or tunneling of Cooper pairs between two bands, we can expect that the transition temperature becomes higher than that derived from the single-band model. The tunneling of Cooper pairs causes the stabilization of the order parameter of superconductivity [163, 173]. We can also expect higher Tc of the superconductivity than that for copper oxides in two regions (g1 < 0, g2 < 0 and g1 < 0, g2 > 0) by the cooperative mechanism. Phase diagrams for CDW, SDW, and singlet superconductivity derived from a more general Hamiltonian will be presented elsewhere. Thus, we have derived the renormalization equations and present the phase diagrams for the two-band superconductivity. In the framework of the two-band model, the present results predict that superconductivity appears, even if the electron–electron interaction is positive. We can expect that the transition temperature becomes higher than that of copper oxides by the cooperative mechanism.

4.5. Room Superconductors Superconductivity sets up a new temperature record. The physicists dealing with the condensed matter made huge eﬀorts in the ﬁelds of theory, computer modeling, and experiment in the search for new superconductors at room temperature. Their work has led to the discovery of many types of high-temperature materials, including a family of compounds on the basis of copper and iron, fullerides, and magnesium diboride. In all those cases, the materials were studied in laboratories before the theorists try to describe them.

page 172

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

173

The list of physical news in 2019 [193] was rightly headed by the communications of two independently groups working at George Washington University (USA) [194] and Max-Planck Institut f¨ ur Chemie (Germany) [195] on the observation of the superconductivity in lanthanium hydride LaH10 at about 260 K. This value is well perceived already on the Celsius scale to be −13◦ C, which corresponds to the ordinary winter temperature on the northern latitudes. However, the conditions under which the superconductivity was registered (pressure of several millions of atm.) are hardly called normal. The required value (180 GPa) was attained with the use of a cell with diamond anvils. This history is distinct from the previous breakthroughs in the superconductivity in that the discovery was not completely unpredictable: the direction of searches was set as early as in 1968 by N. Ashcroft who pointed out that, according to the BCS (Bardeen, Cooper, and Schrieﬀer) theory, metallic hydrogen and the compounds with its high content should possess the property of a high-temperature superconductor. The targeted seeking of the superconductivity among rare-earth hydrides started in 2017 [196] and has recently reached the success. The scheme of the experiment and the crystalline structure of LaH10 are shown in Figs. 4.14 and 4.15, respectively.

4.5.1. On the superconductivity of hydrogen sulfide The recent discovery of the superconductivity with Tc = 203 K in the compound H3 S, being an ordinary superconductor, has returned the interest

Fig. 4.14. Scheme of the experiment,where the diamond anvils, spacer, and pistons creating a high pressure are seen.

page 173

March 24, 2021

174

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 4.15.

Crystalline structure of LaH10 .

in the BCS predictions about a possible superconductivity at room temperature. The mictoscopic BCS theory of superconductivity implies that, at a favorable combination of parameters of a material, the superconductivity at room temperature is possible. The absence of the upper theoretical limit for the critical temperature of the superconductivity transition follows from the Allen–Dynes formula √ Tc = 0.182ωln λ,

(4.79)

where ωln is the mean frequency of phonons, and λ is the constant of the electron–phonon interaction. This formula is applicable only for λ > 5, but it allows one to conclude that Tc = 300 K, if the material has simultaneously the high Debye frequency and the large constant of the electron–phonon interaction. The critical temperature depends linearly on the averaged phonon frequencies. Therefore, promising are the materials with light that possess high frequencies in the phonon spectrum. It is natural to consider pure hydrogen which can be a high-temperature superconductor. Hydrogen has high phonon frequencies (TD = 2000 K) and a large constant of the electron–phonon interaction (λ = 1 − 2). V.L. Ginzburg in [199] referred the possibility to create metallic hydrogen to the most signiﬁcant problems. However, metallic hydrogen remains unattainable experimentally till now, because its metallization requires too high pressures. Nevertheless, many theoretical and experimental works are referred to this trend.

page 174

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

175

Since the high frequencies in the phonon spectrum favor the attainment of a critical temperature, it is obvious that hydrides are perspective materials with high content of hydrogen as the lightest element. N. Ashcroft [201] proposed to make experiments with such substances as CH4 , SiH4 , GeH4 , etc. instead of hydrogen. They can be transformed into a metal at less attainable pressures and can become high-temperature superconductors by the same reason as hydrogen due to a high Debye temperature and a strong electron– phonon interaction. As one more promising material, we mention graphane (hydrogenated graphene) [140]. The superconductivity transition temperature is predicted for it to be 90 K and, for a multilayer system, can increase up to 160 K. So far, the majority of predictions for hydrides were focused in twoelement (binary) compounds [197]. It is worth to note that the hightemperature superconductivity can be realized by means of the use of three-element (triple) hydrides such as, for example, Li2 MgH16 [208]. Now, we have heard about a new record. Researchers from University of Rochester and University of Nevada, Las Vegas (USA) attained the superconductivity at room temperature (287.7 K) and a pressure of 267 GPa [200]. To stay in such room is not comfortable (a temperature of about 15◦ C), and the pressure is fantastic. But anyway, the progress is on hand. At once, this result aroused a storm of comments and the intense discussions in the scientiﬁc and near-scientiﬁc publications. The authors of work [200] placed some mixture of carbon, hydrogen, and sulfur in a microscopic cavity (really, methane, hydrogen sulﬁde, and molecular hydrogen were mixed) compressed by diamond anvils. On the basis of the comments of experts, we may expect that the triple carbon–hydrogen– sulfur system will be very promising in the search for new superconductors. The superconductivity was registered starting from a pressure of about 140 GPa and Tc of about 150 K. Then Tc increases comparatively slowly with the pressure. But, starting from approximately 190 GPa, the sharp increase in Tc was observed. The presence of the superconductivity was conﬁrmed also by measurements of the magnetic susceptibility: the system demonstrated the well-manifested Meissner eﬀect. It is natural that Tc decreased, as the magnetic ﬁeld increased. The estimates of the upper critical ﬁeld at the zero temperature made by the Ginzburg–Landau theory gave its value equal to about 62 T. In the theory of hydrides as a signiﬁcant success, we indicate the prediction of their crystalline structure from the ﬁrst principles. As soon as the crystalline structure of a material becomes known, the phonon and electron spectra can be calculated. Then we can evaluate the critical ´ temperature with the help of the Migdal–Eliashberg theory [201, 202].

page 175

March 24, 2021

176

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

As a result of many experimental and theoretical works, the hightemperature superconductivity with Tc = 203 K in sulfur hydride was reliably established [203]. Probably, the discovery of the high-temperature superconductivity in H2 S will restore the interest in superconductors described by the BCS theory, and new superconductors will be found. In this connection, we will consider the BCS theory, as well as the ´ Eliashberg theory describing the superconductivity in the case of strong coupling.

4.5.2. Formalism for standard superconductors 4.5.2.1.

Microscopic theory of superconductivity: BCS theory

The theory by Bardeen, Cooper and Schrieﬀer [202] was the ﬁrst theory of superconductivity. It was able to explain the microscopic nature of the superconductivity state and is one of the most successful theories in the condensed matter physics. Though its predictable ability is limited relative to the modern ab initio methods, the BCS theory is else a signiﬁcant theoretical and computational base aimed at the characterization and the understanding of superconducting materials till now. The BCS theory was constructed with the use of a model Hamiltonian based on the assumption that, in the superconductivity state, all electrons near the Fermi surface are correlated, by forming the pairs. In each pair, the momenta and spins of two electrons are equal and opposite to each other. It is worth to note that a more substantiated theory of superconductivity in the case of weak electron–phonon coupling was advanced by a Soviet physicist theorist N. N. Bogolyubov [44] in the framework of a generalization of the method of canonical transformations. The BCS theory includes the following electron Hamiltonian: H = H0 + Hint , εk c†kσ ckσ , H0 =

(4.80) (4.81)

kσ

Hint = −

kk

Vkk (c†−k ↓ c†k ↑ ) (ck↑ c−k↓ ),

(4.82)

where ckσ and c†kσ are the operators of annihilation and creation of a Bloch wave with the wave vector k and spin σ, respectively, and Vkk are matrix elements of the basic superconductivity interaction. By assuming that the

page 176

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

177

electron–phonon coupling is independent of the momentum, we can write (4.83) Vk,k = −V θ (ωD − |εk |) θ ωD − εk , where ωD is the Debye frequency. BCS found the exact solution of the problem within this model with the help of the ansatz for the multiparticle wave function. Using the method of Green’s functions developed by L.P. Gor’kov [203–205], we present the solution for Green’s function: (4.84) G(k, τ ) = − Tτ ckσ (τ )c†kσ (0) , where the imaginary time dependence of the operators is deﬁned and means the time-ordered product X (τ ) = exp (Hτ ) X exp (−Hτ ) and Tτ is the time of the ordered process and the expectation of a physical quantity A is calculated as A =

Tr (exp(−βH)A) , Tr (exp(−βH))

(4.85)

The Green’s function G satisﬁes the equation of motion d − εk G(k, τ ) = δ(τ ) − Vkk Tτ c†−k↓ (τ )ck ↑ (τ )c−k ↓ (τ )c†k↑ (0). − dτ k

(4.86) In the mean-ﬁeld approximation, the solution takes the form Tτ c†−k↓ (τ ) ck ↑ (τ )c−k ↓ (τ )c†k↑ (0) → F (k, 0)F ∗ (k, τ )

(4.87)

and the anomalous Green’s function is deﬁned as F (k, τ ) = − Tτ ck ↑ (τ )c−k ↓ (0) . This yields G(k, iωn ) =

−iωn − εk , ωn2 + Ek2

F (k, iωn ) =

Δ∗k , ωn2 + Ek2

where ωn = (2n + 1) πkB T is the Matsubara frequency, Ek2 ≡ ε2k + |Δk |2 and Δk is deﬁned as follows: Vk,k F (k , 0). (4.88) Δk ≡ k

page 177

March 24, 2021

178

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

This quantity determines the superconductivity gap and satisﬁes the BCS self-consistent equation: Δk =

∞ Vkk Δk Ek 1 Vkk Δk . = tanh 2 + E2 β 2E 2k T ω B n k k n=−∞ k

(4.89)

k

If we assume that the gap function is isotropic: Δk = Δ = 0, then we can ﬁnd the following limits: (1) In the approximation T → 0 and V N (EF ) 1, −1 , Δ ∼ 2ωD exp V N (EF )

(4.90)

where N (EF ) is the density of states in the Fermi level. (2) For T ∼ Tc , as Δ → 0, we get the critical temperature of the superconductivity transition: −1 . (4.91) Tc = 1.13ωD exp V N (EF ) Comparing (4.90) and (4.91), we arrive at the universal relation of the BCS theory that connects. The energy gap width at the zero temperature and the temperature Tc of the superconductivity transition is given by 4 2Δ ∼ 3.54. ∼ Tc 1.13

(4.92)

This relation is reliably corroborated experimentally for many superconducting elements.

´ 4.5.3. Eliashberg theory 4.5.3.1.

´ Theory of superconductivity by Eliashberg–McMillan

´ The Eliashberg theory of superconductivity is the most perfect approach to the microscopic description of properties of traditional superconductors with the electron–phonon mechanism of pairing. Recently, this theory has been successfully applied to the description of the record superconductivity in compounds of hydrogen at a high pressure. ´ The Eliashberg theory represents a multiparticle approach to the superconductivity that involves the Coulomb interaction and phonon propagators. The BCS model Hamiltonian of pairing is replaced by a Hamiltonian accounting for the interaction of electrons and phonons.

page 178

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

179

´ The Eliashberg equations are a system of coupled nonlinear integral equations constructed in the basis of the method of Green;s functions applied to the theory of superconductivity. The calculations were carried out by the theory of perturbations in which the dimensionless parameter of expansion is the ratio [206] η = λωD /EF 1,

(4.93)

where λ is the dimensionless parameter of the electron–phonon coupling, ωD is the maximum frequency of phonons, and EF is the Fermi energy. In calculations, the state derived in the theory of superconductivity and corresponding to the energy spectrum εk = ε2 (k) + Δ2 was taken as the zero approximation, rather than the state of noninteracting electrons. Thus, the principal eﬀect of pairing was considered already in the zero approximation. Then Green’s function for such new zero approximation was deﬁned and determined as the solution of the equations of perturbation theory in the parameter (ν). In the theory, the frequency dependence of the matrix element was taken into account with the introduction of both a function of the density of phonon states (ω − ωq ), F (ω) = q

where ωq is the spectral distribution of phonon frequencies and a function α2 (ω) characterizing the intensity of the electron–phonon interaction. The spectral and tunnel measurements of properties of superconductors gave possibility to directly determine the product α2 (ω)F (ω). In 1971, F. Allen showed that, with regard for the expressions ωD dω α2 (ω)F (ω) λ=2 ω 0 and

2 ω2 = λ

ωD 0

ω 2 α(ω)F (ω)

dω , ω

it is possible to determine the dimensionless 2 constant λ of the electron– phonon interaction and the mean value ω of the squared frequency of the phonon spectrum.

page 179

March 24, 2021

180

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Modern Aspects of Superconductivity: Theory of Superconductivity

In order to analyze the dependence of this dimensionless parameter in properties of a metal, McMillan proposed the simple formula λ = N0 q 2 /a2 /M ω 2 ,

(4.94)

where N0 is the energy density of states of electrons on the Fermi surface, q/a is the matrix element of the electron–phonon interaction, ω 2 is the mean square of the frequency of phonons, and M is the ion mass. He derived also the socalled McMillan relation for Tc that includes a small number of simple parameters: Tc =

1.04(1 + λ) ωD exp − . 1.45 λ − μ∗c (1 + 0.62λ)

(4.95)

In 1972 Dynes [207] introduced the prefactor ωD /1.20 instead of ωD /1.45. Later in 1975 Allen and Dynes [210] made a careful analysis of the dependence of Tc on the properties of a material λ and μ∗c and rewrote the relation in a somewhat diﬀerent form ωlog 1.04(1 + λ) exp − , (4.96) Tc = 1.2 λ − μ∗c (1 + 0.62λ) where ωlog

α2 Γ(ω) 2 log(ω) dω . = exp λ ω

(4.97)

This change corrected the contribution of phonons with low energies to the superconductivity pairing. So, the McMillan relation in the Allen–Dynes form (4.99) is widely used in the calculations of the superconductivity critical temperature from the ﬁrst principles. One of the aspects making this relation so suitable, despite its formal simplicity, consists in that such parameterization of μ∗c with its typical value of 0.11 eliminates noticeably the dependence of the results on a material. It is worth noting that this universal character of μ∗c holds only for the McMillan formula. ´ The McMillan approach starts to deviate from the Eliashberg one at a very strong coupling (λ > 15), where the former underestimates the true critical temperature. This distinction was overcame by Allen and Dynes [210] by introduction of the additional parameter 1/2 2 2 ωα F (ω) dω ω2 = λ

(4.98)

page 180

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch04

Multiband Superconductivity

181

and the prefactor 3/2 1/3 (ω2 /ωlog − 1)λ2 λ 1+ 2 f = 1+ 2.46(1 + 3.8μ∗c ) λ + 3.31(1 + 6.3μ∗c )(ω2 /ωlog ) (4.99) on the right-hand side of relation (4.96) that becomes ωlog 1.04(1 + λ) Tc = f exp − . 1.2 λ − μ∗c (1 + 0.62λ)

(4.100)

´ The BCS Eliashberg and NcMillan theories deal with isotropic media. This decreases signiﬁcantly the region of their applicability to nonmetallic superconductors. In subsequent studies, the theorists should ﬁnd the mean allowing one to conserve the high-temperature superconductivity at lower pressures and, what is better, at the ambient one. To answer this challenge, the predictable power of computational tools must be made more reliable and exact, in particular, in the consideration of extreme conditions.

page 181

This page intentionally left blank

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

CHAPTER 5

Nanoscale Superconductivity

5.1. Introduction Recent advances in nanoscience have demonstrated that fundamentally new physical phenomena are found, when systems are reduced in size to dimensions which become comparable to the fundamental microscopic lengths of the investigated material. Superconductivity is a macroscopic quantum phenomena, and it is therefore especially interesting to see how this quantum state is inﬂuenced when the samples are reduced to nanometer sizes. Recent developments in nanotechnologies and measurement techniques nowadays allow the experimental investigation of the magnetic and thermodynamic superconducting properties of mesoscopic samples in this regime. In this book, we develop some theoretical models to describe such nanoscale superconducting systems and explore possible new experimental phenomena which we can predict based upon these theoretical models. In bulk samples, the standard Bardeen–Cooper–Schrieﬀer (BCS) theory gives a good description of the phenomenon of superconductivity [148]. However, it was noticed by Anderson in 1959 that, as the size of a superconductor becomes smaller, and the quantum energy level spacing of the electrons in the sample approaches the superconducting gap, then the BCS theory will fail [6]. The exact solution to the reduced BCS Hamiltonian for ﬁnitesize systems was developed by Richardson in the context of nuclear physics a long time ago [211]. This shows that, while the grand canonical BCS wave function gives a very accurate solution of the BCS Hamiltonian in the limit where the number of electrons is very large N 1, for small values of N , one has to use exact analytical methods to obtain reliable results. The recent experimental advances in fabricating and measuring superconductivity in ultrasmall mesoscopic and nanoscale grains has renewed a theoretical interest in the Richardson solution [212–215]. Reference [10] shows the measurement for the smallest size of a superconductor in the world which is 5 A, Fig. 5.1. Such systems are interesting for nanoelectronics 183

page 183

March 24, 2021

184

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.1.

The smallest superconductor in the world.

and quantum computing. In this book, we propose to develop theoretical models for nanoscale superconducting systems and to apply these models to a variety of systems of current experimental interest. The Richardson solution depends on the electron energy level spacings near to the Fermi level, and so these diﬀerent geometric shapes will lead to diﬀerent size dependences of the thermodynamic and electronic properties. Experiments have recently demonstrated superconductivity in one-dimensional nanowires of lead [216] and carbon [217]. Our theoretical predictions will include the even-odd parity eﬀects in tunneling spectra, which have already been observed on the nanometer scale in Al grains, Fig. 5.2, [212], but which could also be observed in nanotube superconductors. In Figs. 5.2 and 5.3, we can see the ensemble of small metallic grains which can be in the normal or superconducting state. For such systems, the important parameters are the l-granular size, electron coherence length, and the penetration depth [167]. In grains, there appears the quantum size eﬀect (discretization of the electron energy spectrum). In Fig. 5.3, we show the size eﬀect in grains. We note that the level spacing depends on many parameters such as the electron coherence length and the penetration depth. Carbon nanotubes were ﬁrst observed in 1991 by Iijima in Japan, Fig. 5.4. In this chapter, we investigate properties of nanosize two-gap superconductivity by using a two-sublevel model in the framework of the mean-ﬁeld approximation. A model corresponding to a nanosize two-gap superconductivity is presented, and the partition function of the nanosize system is

page 184

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

Fig. 5.2.

Illustration of superconductor grains.

Fig. 5.3.

Size eﬀect in superconductor grains.

Fig. 5.4.

185

Carbon nanotube revealing superconductivity.

analytically derived by using the path integral approach. A deﬁnition of the critical level spacing of the two-gap superconductivity is also presented, and we discuss the condensation energy and the parity gap of two-gap superconductivity in relation to the size dependence of those properties with two bulk gaps and the eﬀective pair scattering process between two sublevels. We present the theory of interactions between two nanoscale ferromagnetic particles embedded into a superconductor and spin orientation phase transitions in such a system. We investigate the energy spectrum and wave function of electrons in hybrid superconducting nanowires. We also consider the ideas of quantum computing and quantum information in mesoscopic circuits. The theory of the Josephson eﬀect is presented, and its

page 185

March 24, 2021

186

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

applications in quantum computing are analyzed. The results of this chapter were obtained by the author and published in works [218–226].

5.2. Nanosize Two-gap Superconductivity Multiband superconductivity has been theoretically investigated in relation to MgB2 superconductivity in Chapter 4. Recent experiments [228, 232] by Black et al. have also generated a high interest in the size dependence of the superconductivity. Properties of ultrasmall superconducting grains have been theoretically investigated by many groups [229, 230, 233–237]. In such ultrasmall grains, the old but fundamental theoretical question was noticed by Anderson [6]. The standard BCS theory gives a good description of the phenomenon of superconductivity in large samples. However, as the size of a superconductor becomes small, the BCS theory fails. In ultrasmall Al grains, the bulk gap has been discussed in relation to physical properties in ultrasmall grains such as the parity gap [237], condensation energy [235], electron correlation [230], etc. with the size dependence of the level spacing [229] of samples. In the recent years, great eﬀorts have been devoted to the fabrication of MgB2 nanostructures that could play a crucial role in the ﬁeld of applied superconductivity, nanotubes, nanowires and nanoparticles. As for MgB2 , nanoparticles of approximately 40–100 nm in size are available (Fig. 5.5). In this section, we investigate the properties of nanosize two-gap superconductivity by using a two-sublevel model in the framework of the mean-ﬁeld approximation. A model corresponding to a nanosize two-gap

Fig. 5.5.

TEM micrograph of 20–100 nm nanoparticles of MgB2 .

page 186

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

187

superconductivity is presented, and the partition function of the nanosize system is analytically derived by using the path integral approach. A deﬁnition of the critical level spacing of the two-gap superconductivity is also presented, and we discuss the condensation energy and the parity gap of two-gap superconductivity in relation to the size dependence of those properties with two bulk gaps and the eﬀective pair scattering process between two sublevels. In nanosize grains of a superconductor, the quantum level spacing approaches the superconducting gap. In the case of a two-gap superconductor, we can consider a model with two sublevels corresponding to two independent bands. In this section, we present a model for nanosize two-gap superconductivity and an expression for the partition function of the system.

5.2.1. Hamiltonian for nanosize grains We consider a pairing Hamiltonian with two sublevels corresponding to two bands 1 and 2 written as H = H0 + Hint ,

(5.1)

where H0 =

[ε1j − μ]a†jσ ajσ +

j,σ

Hint = −g1

k,σ

a†j↑ a†j↓ aj ↓ aj ↑ − g2

j,j ∈I

+ g12

[ε2k − μ]b†kσ bkσ ,

j∈I,k∈J

(5.2)

b†k↑ b†k↓ bk ↓ bk ↑

k,k ∈J

a†j↑ a†j↓ bk↓ bk↑ + g12

b†k↑ b†k↓ aj↓ aj↑ .

(5.3)

j∈I,k∈J

Here, a†jσ (ajσ ) and b†jσ (bj,σ ) are the creation (annihilation) operator in sublevels 1 and 2 with spin σ and the energies ε1j and ε2j , respectively, the operators for each sublevel satisfy the anticommutation relations, and the operators between sublevels are independent, μ is the chemical potential, the second term in Eq. (5.1) is the interaction Hamiltonian, g1 and g2 are the eﬀective interaction constant for sublevels 1 and 2, and g12 is an eﬀective interaction constant which corresponds to the pair scattering process between two bands. The sums of j and k in Eq. (5.3) are over the set I of N1I states corresponding to the half-ﬁlled band 1 with ﬁxed width 2ω1D and the set J of N2J states for band 2, respectively. In this study, we assume that the Debye energies for two sublevels are the same: ω1D = ω2D = ωD . Within this assumption, N1I and N2J are relatively

page 187

March 24, 2021

188

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

estimated by the density of state (DOS) for two bands as N1I /N2J = ρ1 /ρ2 , where ρ1 and ρ2 are DOS for two bands. The interaction constants g1 and g2 can be written as d1 λ1 and d2 λ2 , respectively. d1 = 2ωD /N1I and d2 = 2ωD /N2J mean the mean energy level spacing, and λ1 and λ2 are the dimensionless parameters √ for two sublevels. We take the intersublevel interaction constant g12 = d1 d2 λ12 . In summary, we obtain a relation of ρ1 /ρ2 = N1I /N2J = d2 /d1 .

5.2.2. Path integral approach It is convenient to introduce a path integral approach for the treatment of ﬂuctuations of the order parameters. This approach gives an exact expression for the grand partition function of a superconductor H − μN Z(μ, T ) = Tr exp − , (5.4) T where T is the temperature, and N is the number operator in the grain. The idea of the path integral approach is to replace the description of a system under study in terms of electronic operators by an equivalent description in terms of the superconducting order parameter. By the path integral approach, we obtain an expression for the grand partition function for the Hamiltonian (5.1): (5.5) Z(μ, T ) = DΔ1 DΔ∗1 DΔ2 DΔ∗2 e−S[Δ1,Δ2 ] . Here, the action S[Δ1 , Δ2 ] is deﬁned as ξ1j ξ2k −1 −1 − Tr ln G1j − Tr ln G2k − S[Δ1 , Δ2 ] = − T T j

k

1/T

dτ

+ 0

1 g2 |Δ1 (τ )|2 + g1 |Δ2 (τ )|2 2 g1 g2 − g12

+ g12 (Δ1 (τ )Δ2 (τ )∗ + Δ1 (τ )∗ Δ2 (τ ))] .

(5.6)

Δ1 and Δ2 are bulk gaps for sublevels 1 and 2, respectively, ξ1j = ε1j − μ and ξ2k = ε2k − μ, and the inverse Green’s functions d −1 z + ∗ − − ξ1j σ − Δ1 (τ )σ − Δ1 (τ )σ δ(τ − τ ), (5.7) G1j (τ, τ ) = − dτ and G−1 2k (τ, τ )

d z + ∗ − − ξ2k σ − Δ2 (τ )σ − Δ2 (τ )σ δ(τ − τ ), = − dτ

(5.8)

page 188

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

189

−1 where σ ± = σ x ± iσ y , and σ x,y,z are the Pauli matrices. G−1 1 and G2 satisfy antiperiodic boundary conditions. In the case of a stronger interaction, Δ1 d1 and Δ2 d2 , we consider the mean-ﬁeld approximation for the order parameters in the path integral approach. Substituting the time-independent order parameters into the action (5.6), we have (ξ1j − 1j ) + (ξ2k − 2k ) Ω(μ) = j

+

k

1 g2 Δ21 + g1 Δ22 + g12 (Δ∗1 Δ2 + Δ1 Δ∗2 ) , 2 g1 g2 − g12

(5.9)

2 + Δ2 )1/2 , and

2 2 1/2 . In Eq. (5.9), the values where 1j = (ξ1j 2k = (ξ2k + Δ2 ) 1 of Δ1 and Δ2 must be chosen in such a way which minimizes Ω. From the minimization of Ω, we obtain a coupled gap equation at zero temperature for the two-gap system: ⎛ 1 1 ⎞ −g12 g1 ⎜ 2 1j 2 2k ⎟ Δ1 ⎜ ⎟ Δ1 j k =⎜ . (5.10) 1 1 ⎟ ⎝ −g ⎠ Δ2 Δ2 g2 12 2 1j 2 2k j

k

From the coupled gap equation, Eq. (5.10), we formally obtain an expression for the bulk gap for two-gap superconductivity at zero temperature: 1 −1 ˜ , (5.11) Δ1 = ω sinh η1 and ˜ 2 = ω sinh−1 Δ

1 η2

,

(5.12)

where λ2 + α± [η1 , η2 ] λ12 1 = , η1 λ1 λ2 − λ212

(5.13)

λ1 + α−1 1 ± [η1 , η2 ] λ12 = , η2 λ1 λ2 − λ212

(5.14)

and

α± [η1 , η2 ] = ±

sinh sinh

1 η1

. 1 η2

(5.15)

page 189

March 24, 2021

190

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

For the two-band superconductivity, we can consider two cases for the phase ˜ 2 ), and sgn(Δ ˜ 1 ) = −sgn(Δ ˜ 2 ). For the same ˜ 1 ) = sgn(Δ of the gaps: sgn(Δ phase, α+ is used in Eqs. (5.13) and (5.14), and we use α− for the opposite ˜ 2 in the limit of strong intersublevel coupling λ12 , ˜ 1 = −Δ phase. Note that Δ that is, the opposite phase. For λ12 = 0, we ﬁnd the same results for two bulk gaps derived from the conventional BCS theory for two independent sublevels.

5.2.3. Condensation energy In this section, we discuss properties such as condensation energy, critical level spacing, and parity gap of nanosize two-gap superconductivity by using the partition function derived in the previous section. In nanosize superconductivity, the condensation energy can be deﬁned as C G (0) − E G (λ) − nλd, where E G is the ground-state energy of EN,b (λ) = EN,b N,b N,b the N -electron system in the interaction band, b is the number of electrons on single occupied levels, and λ and n are the dimensionless coupling parameter and the number of pair occupied level, respectively. In the case of a nanosize two-band system, the condensation energy can be written as C G G (λ1 , λ2 , λ12 ) = EN (0, 0, 0) − EN (λ1 , λ2 , λ12 ) EN 1 ,b1 ;N2 ,b2 1 ,b1 ;N2 ,b2 1 ,b1 ;N2 ,b2

−n1 λ1 d1 − n2 λ2 d2 ,

(5.16)

G (λ1 , λ2 , λ12 ) means the ground-state energy of (N1 + N2 )where EN 1 ,b1 ;N2 ,b2 electron system. From Eqs. (5.4) and (5.9), the condensation energy of the two-sublevel system can be expressed by the condensation energy of independent single-level systems: C C C (λ1 , λ2 , λ12 ) = EN (λ1 ) + EN (λ2 ) − EN 1 ,b1 ;N2 ,b2 1 ,b1 2 ,b2

×

λ212 λ1 λ2 − λ212

Δ21 Δ22 2 (Δ∗1 Δ2 + Δ1 Δ∗2 ) √ + + d1 λ1 d2 λ2 d1 d2 λ12

, (5.17)

C C (λ1 ) and EN (λ2 ) correspond to the condensation energy for where EN 1 ,b1 2 ,b2 the single band case. In the same phases of Δ1 and Δ2 , the condensation energy (5.17) decreases, that is, there appears the instability by the coupling constant λ12 . On the other hand, in the opposite phases, the condensation energy becomes larger, because Δ∗1 Δ2 + Δ1 Δ∗2 < 0. We can expect that the condensation energy for two-gap superconductivity leads to a higher stability, than that of two independent systems, due to the intersublevel coupling λ12 and the opposite phases.

page 190

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

191

5.2.4. Critical level spacing To discuss the critical level spacing for a two-gap system, we start from the coupled gap equation (5.10). For the case of the critical level spacing of the two-gap system, we have 1 = λ1

j

1 1 1 1 + λ2 − (λ1 λ2 − λ212 ) , 2|ξ˜1j | 2|ξ˜2k | 2|ξ˜1j | k 2|ξ˜2k | j k (5.18)

where ξ˜i = ξi /di for sublevel i = 1, 2. For the odd or even cases, Eq. (5.18) can be approximately solved by using the digamma function: For the odd case, the critical level spacing becomes 1 d2 o γ (5.19) d1c = ωD e exp − , do2c = do1c , λ d1 and, for the even case, 1 d2 = 4ωD e exp − , de2c = de1c . λ d1

de1c

γ

(5.20)

Here, we use 1 1 2 2 = λ1 + λ2 − ax + (λ1 − λ2 − ax) + 4λ12 λ 2x

(5.21)

x = λ1 λ2 − λ212 ,

(5.22)

with

a = log

d1 . d2

(5.23)

From these expressions, we ﬁnd some relations:

and do1/2c

de1c = 4do1c , de2c = 4do2c

(5.24)

1 eγ 1 ˜ exp Δ1/2 . ≈ − 2 η1/2 λ

(5.25)

In the case of |λ1 − λ2 | λ12 , Eq. (5.25) can be approximately rewritten as λ2 − λ1 + 2αλ12 ˜ eγ o exp (5.26) Δ1/2 . d1/2c ≈ 2 λ1 λ2 − λ212

page 191

March 24, 2021

192

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

On the other hand, in the limit of |λ1 − λ2 | λ12 , we have (1 + α) λ12 ˜ eγ o d1/2c ≈ exp Δ1/2 . 2 λ1 λ2 − λ212

(5.27)

For the case of λ12 = 0, Eq. (5.25) can be rewritten as do1/2c ≈ ˜ 1/2 . Therefore, when the coupling constants λ1 exp[γ]/2 exp[1/λ1 − 1/λ2 ]Δ and λ2 take the same value, we have a relation similar to that for a single˜ 1/2 . These results suggest the critical level spacing level system: do1/2c ≈ 0.89Δ strongly depend upon λ12 and the diﬀerence between the eﬀective interaction constants for sublevels. The relation in Eq. (5.24) is the same relation in the conventional nanosize BCS theory.

5.2.5. Parity gap In this subsection, we consider a parity gap in the case of two-gap superconductivity in ultrasmall grains. In the case of two sublevel spacings, the chemical potential lies halfway between the highest occupied and the lowest unoccupied levels of a smaller level spacing in the half-ﬁlled case, as shown in Fig. 5.6(a). We assume that d1 < d2 and that the numbers of occupied levels corresponding to each sublevel are n1 and n2 , respectively. Then, the total number of electron becomes N = 2n1 + 2n2 . When we consider N = 2n1 + 2n2 + 1, the chemical potential lies on the level ε1n1 +1 , as shown in Fig. 5.6(b). Figure 5.6(c) shows the position of the chemical potential in the case of N = 2n1 + 2n2 + 2. The parity gap of nanosize two-gap superconductivity is written as 1 G G G − (E2n + E2(n ). Δ1p = E2n 1 +1+2n2 ,1 1 +2n2 ,0 1 +1)+2n2 ,0 2

(5.28)

G = Ω From Eq. (5.9) and for the ground-state energy EN,b μN + μN N , we obtain d1 ρ1 1 −1 . (5.29) Δp = Δ1 − 4 ρ2

From Figs. 5.6(c)–5.6(e), we can deﬁne another parity gap: 1 G G G − (E2(n + E2(n ). Δ2p = E2(n 1 +1)+2n2 +1,1 1 +1)+2n2 ,0 1 +1)+2(n2 +1),0 2 From the latter deﬁnition of Eq. (5.30), we have d2 3ρ2 2 −1 . Δp = Δ2 − 4 ρ1

(5.30)

(5.31)

page 192

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity (a)

(b)

(d)

(e)

193

(c)

Fig. 5.6. Position of the chemical potential relative the electronic energy levels in a twogap superconducting grain. Solid and dotted lines mean two sublevels. (a) Half-ﬁlled system with 2n1 + 2n2 electrons. (b) 2n1 + 1 + 2n2 -electron system. (c) 2(n1 + 1) + 2n2 -electron system. (d) 2(n1 + 1) + 2n2 + 1-electron system. (e) 2(n1 + 1) + 2(n2 + 1)-electron system.

The present results suggest two kinds of the dependence of the parity gap on the level spacing. The parity gap does not depend upon the eﬀective interaction λ12 . The structure around the Fermi level plays an important role of the contribution to the size dependence of the parity gap. We have investigated the properties of nanosize two-gap superconductivity by using a two-sublevel model in the framework of the mean-ﬁeld approximation. From the discussion of the condensation energy in nanosize two-gap superconductivity, the phases of the gaps are very important to stabilize the superconductivity. In the same phases, the two-gap superconductivity is instable by the coupling constant λ12 . On the other hand, in the opposite phases, the superconductivity becomes stable. We can expect that, due to the condensation energy, the two-gap superconductivity becomes more stable than that for two independent systems due to the intersublevel coupling λ12 and the opposite phases. We have also discussed the critical level spacing for two-gap superconductivity in ultrasmall grains. These results suggest that the critical

page 193

March 24, 2021

194

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

level spacing strongly depends upon λ12 and the diﬀerence between the eﬀective interaction constants for sublevels. Moreover, the relation between the critical level spacing and the bulk gaps is modiﬁed as compared with the result obtained for ultrasmall superconducting Al grains. For the parity gap in two-gap superconductivity, the present results suggest two kinds of the dependence of the parity gap on the level spacing and that the structure around the Fermi level plays an important role by contributing to the size dependence on the parity gap. The parity gap does not depend upon the eﬀective interaction λ12 . In the case of a cluster system, we have to apply a more accurate approach beyond the mean-ﬁeld approximation presented in this study by investigating the physical properties, and we have also to consider the contribution of the surface of samples to the level structure around the Fermi level. We will present these problems in the next section. On the basis of the presented results, we might expect the possibility of a new multigap superconductivity arising in the nanosize region with a higher critical transition temperature. In summary, a model corresponding to a nanosize two-gap superconductivity has been presented, and an expression for the partition function of the nanosize system has been analytically derived by using the path integral approach. A deﬁnition of the critical level spacing of the two-gap superconductivity has been also presented, and we discuss the condensation energy and the parity gap of the two-gap superconductivity in relation to the size dependence of those properties with two bulk gaps, as well as the eﬀective pair scattering process between two sublevels.

5.3. Exact Solution of Two-band Superconductivity in Ultrasmall Grains Many groups have theoretically investigated the physical properties such as critical level spacing, condensation energy, parity gap, etc. in ultrasmall grains with the conventional superconductivity [229, 230, 233–237]. The question concerning such nanosize superconducting grains has been discussed by Anderson [6]. The standard BCS theory becomes false, when the level spacing approaches the superconducting gap. To investigate the properties in such nanosize systems, it is necessary to take a more accurate treatment. Braun and von Delft [233, 234, 241] have reintroduced the exact solution to the reduced BCS Hamiltonian developed by Richardson [238–240]. It is noteworthy that the Richardson’s solution is applicable at distributions of single-electron energy levels. V.N. Gladilin et al. [235] have investigated the

page 194

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

195

pairing characteristics such as the condensation energy, spectroscopic gap, parity gap, etc., by using the Richardson’s exact solution for the reduced BCS Hamiltonian. The recent discovery of superconductivity of MgB2 [168] with Tc = 39 K has also been much attracted a great interest aimed at the elucidation of its mechanism from both experimental and theoretical viewpoints. Since this discovery, the possibility of two-band superconductivity has also been discussed in relation to two-gap functions experimentally and theoretically. In this section, we investigate the two-band superconductivity in ultrasmall grains. The Richardson’s exact solution is extended to two-band systems, and a new coupled equation is derived according to the procedure of Richardson’s works. The parity gap and the condensation energy of an ultrasmall two-band superconducting grain are numerically given by solving the coupled equation. We discuss these properties of ultrasmall grains in relation to the correlation, interband interaction, and size dependence.

5.3.1. Exact solution for two-band superconductivity In this section, we derive an exact solution of the two-band superconductivity for a reduced BCS Hamiltonian.

5.3.2. Hamiltonian We consider a Hamiltonian for two bands 1 and 2 written as H = H1 + H2 + Hint , where H1 =

ε1j a†jσ ajσ − g1

jσ

H2 =

jσ

Hint = g12

(5.32)

a†j↑ a†j↓ ak↓ ak↑ ,

(5.33)

b†j↑ b†j↓ bk↓ bk↑ ,

(5.34)

jk

ε2j b†jσ bjσ − g2 jk

jk

a†j↑ a†j↓ bk↓ bk↑ + g12

b†j↑ b†j↓ ak↓ ak↑ .

(5.35)

jk

The ﬁrst and second terms of Eq. (5.32) correspond to the reduced BCS Hamiltonian for bands 1 and 2, respectively. The third term means a coupling between them and corresponds to the pair scattering process between these two bands (see Fig. 5.7). a†jσ (ajσ ) and b†jσ (bjσ ) are the creation (annihilation) operator in bands 1 and 2 with spin σ and the single-particle levels ε1j and ε2j , respectively. The sums of j and k are taken over a set

page 195

March 24, 2021

196

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.7. Two-band system. The dotted line means the chemical potential; εnj is the single-particle energy for band n and level j; −g1 and −g2 are the intraband pair interaction coupling constants; g12 are the interband pair interaction coupling constant.

of N1 states for band 1 with ﬁxed width 2ω1D and a set of N2 states for band 2 with ﬁxed width 2ω2D , respectively. In this study, we assume that the Debye energies for two bands coincide with each other, i.e., ω1D = ω2D = ωD .

(5.36)

Within this assumption, N1 and N2 are relatively estimated by the density of state (DOS) for two bands as ρ1 N1 = , N2 ρ2

(5.37)

where ρ1 and ρ2 are DOS for two bands, respectively. The interaction constants g1 and g2 can be written as g1 = d1 λ1 ,

g2 = d2 λ2 ,

(5.38)

where d1 and d2 mean the mean single-particle level spacing, d1 =

2ωD , N1 − 1

d2 =

2ωD , N2 − 1

(5.39)

page 196

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

197

and λ1 and λ2 are the dimensionality interaction parameters for two bands. We deﬁne the interband interaction constant as g12 =

d1 d2 λ12 .

(5.40)

In summary, we obtain the relation d2 N1 − 1 ρ1 = . ≈ ρ2 N2 − 1 d1

(5.41)

The system we are considering consists of two half-ﬁlled bands, each of which has equally spaced Nn single-particle levels and Mn (= Nn /2) doubly occupied pair levels (n = 1, 2). We take the single-particle level spacing as our energy unity. Thus, the single-particle spectrum is given by εnj = dn j − ωD ,

j = 1, 2, . . . , Nn

(n = 1, 2).

(5.42)

Richardson has obtained his solution within the single-band model for an arbitrary set of single-particle levels. For simplicity, we assume that there are no singly occupied single-particle levels. As can be seen from Eqs. (5.33)– (5.35), these levels are decoupled from the rest of the system. They are said to be blocked and contribute with their single-particle energies to the total energy. The above simpliﬁcation implies that every single-particle level j is either empty (i.e. |vac), or occupied by a pair of electrons (i.e. a†j↑ a†j↓ |vac

and b†j↑ b†j↓ |vac). These are called as the unblocked level.

5.3.3. Exact solution In order to extend Richardson’s solution to a two-band system, we deﬁne two kinds of hard-core boson operators as cj = aj↓ aj↑ , dj = bj↓ bj↑ ,

c†j = a†j↑ a†j↓ , d†j = b†j↑ b†j↓ ,

(5.43) (5.44)

which satisfy the commutation relations, c†2 j = 0,

[cj , c†k ] = δjk (1 − 2c†j cj ),

d†2 j = 0,

[dj , d†k ] = δjk (1 − 2d†j dj ),

[c†j cj , c†k ] = δjk c†j , [d†j dj , d†k ] = δjk d†j ,

(5.45) (5.46)

which reﬂects the Pauli principle for the fermions they constructed from.

page 197

March 24, 2021

198

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Hamiltonian equation (5.32) for the unblocked levels can be then written as HU = 2

N1

ε1j c†j cj − g1

N1

j

+2

c†j ck

jk N2

ε2j d†j dj − g2

j

+ g12

N2

d†j dk

jk

N1 N2 j

c†j dk + g12

N2 N1 j

k

d†j ck .

(5.47)

k

We ﬁnd the eigenstates |M1 ; M2 of this Hamiltonian with M1 + M2 pairs in the form HU |M1 ; M2 U = E(M1 ; M2 )|M1 ; M2 U M M2 1 = E1J + E2K |M1 ; M2 U , J=1

(5.48)

K=1

where E(M1 ; M2 ) is the eigenvalue and M1

|M1 ; M2 U =

J=1

M2

CJ†

† DK |vac,

(5.49)

K=1

and CJ† =

N1

c†j

j

2ε1j − E1J

,

DJ† =

N2

d†j

j

2ε2j − E2J

.

(5.50)

Now, we deﬁne C0† and D0† as C0†

=

N1

c†j ,

j

D0†

=

N2

d†j .

(5.51)

j

Then we can rewrite Eq. (5.47) as HU = 2

N1

ε1j c†j cj − g1 C0† C0

j

+2

N2

ε2j d†j dj − g2 D0† D0

j

+ g12 C0† D0 + g12 D0† C0 .

(5.52)

page 198

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

199

The commutation relations for new operators are given as c†j

[c†j cj , CJ† ] = [C0 , CJ† ]

2ε1j − E1J

N1 1 − c†j cj

=

2ε1j − E1J

j

HU , CJ†

[d†j dj , DJ† ] =

,

E1J CJ†

=

+ C0†

[D0 , DJ† ]

,

+

g1 C0†

=

,

N2 1 − d†j dj

2ε2j − E2J

(5.53)

,

(5.54)

N1 1 − c†j cj

N1 1 − c†j cj j

2ε2j − E2J

j

2ε1j − E1J

j

+ g12 D0†

d†j

2ε1j − E1J

,

(5.55)

and

N2 N2 1 − d†j dj 1 − d†j dj + g12 C0† . HU , DJ† = E2J DJ† + D0† + g1 D0† 2ε2j − E2J 2ε2j − E2J j

j

(5.56) Using the above-presented commutation relations, we ﬁnd HU |M1 ; M2 U M M2 1 = E1J + E2K |M1 ; M2 U J=1 M1 †

+ C0

⎝1 −

J=1 M1 †

+ D0

M2 K=1

+ D0†

N1

⎛ N1 ⎝

J=1

+ C0†

K=1

⎛

M2 K=1

⎛ ⎝

j N2

⎛

j

⎝1 −

j

g1 + 2ε1j − E1J

M1 J =J

⎞ 2g1 ⎠ |M1 (J); M2 U E1J − E1J

⎞ M1 g12 2g12 ⎠ |M1 (J); M2 U − − E1J 2ε1j − E1J E 1J J =J

g12 − 2ε2j − E2K N2 j

2ε2j

M2 K =K

⎞ 2g12 ⎠ |M1 ; M2 (K)U E2K − E2K

⎞ M2 g2 2g2 ⎠ |M1 ; M2 (K)U , + − E2K E2K − E2K K =K

(5.57)

page 199

March 24, 2021

200

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

where |M1 (L); M2 U =

L−1

M1

CJ†

CJ†

J=1

J =L+1

M1

L−1

M2

† DK |vac,

(5.58)

† DK |vac.

(5.59)

K=1

and |M1 ; M2 (L)U =

CJ†

J=1

M2

† DK

K=1

K =L+1

Comparing Eq. (5.57) with Eq. (5.48), we obtain, for arbitrary J and K, (C0† D0† )

1 + g1 A1J

−g12 A2K

−g12 A1J

1 + g2 A2K

|M1 (J); M2 U

|M1 ; M2 (K)U

= 0,

(5.60)

where AnL = −

Nn j

2εnj

Mn 1 2 + . − EnL EnL − EnL

(5.61)

L =L

A nontrivial solution of Eq. (5.60) is derived from the determinantal equation 2 A1J A2K = 0. FJK = (1 + g1 A1J ) (1 + g2 A2K ) − g12

(5.62)

This constitutes a set of M1 + M2 coupled equations for M1 + M2 parameters E1J and E2K (J = 1, 2, . . . , M1 ; K = 1, 2, . . . , M2 ), which may be thought of as self-consistently determined pair energies. Equation (5.62) is the exact eigenvalue equation for a two-band superconducting system and can be regarded as a generalization of the Richardson’s original eigenvalue equation.

5.3.4. Preprocessing for numerical calculations To remove the divergences from the second term of AnL in Eq. (5.61), we make changes of the energy variables: En2λ = ξnλ + iηnλ , En2λ−1 = ξnλ − iηnλ , λ = 1, 2, . . . , Mn /2,

(5.63)

page 200

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

201

where we assume that the number of pairs is even. Since the complex pair energies appear in complex conjugate pairs, the total energy is kept in real. A further transformation is necessary in order to remove the divergences from the ﬁrst term of AnL . We deﬁne new variables xnλ and ynλ as ξnλ = εn2λ + εn2λ−1 + dn xnλ

(xnλ ≤ 0) ,

(5.64)

2 ηnλ = − Δε2n2λ − d2n x2nλ ynλ

(ynλ ≥ 0) ,

(5.65)

and

where Δεn2λ = εn2λ − εn2λ−1 .

(5.66)

Considering the sign of ynλ , we can express ηnλ as ηnλ = |ηnλ |e−iφnλ , 0 for Δε2n2λ − d2n x2nλ ≤ 0, φnλ = π/2 for Δε2n2λ − d2n x2nλ > 0.

(5.67)

Then we can rewrite FJK , by using the new variables, and deﬁne the result as Fαβ . We extract the real and imaginary parts of Fαβ as + = Fαβ

− Fαβ

1 ∗ Fαβ + Fαβ 2

2 R1α R2β = 1 + g1 R1α + g2 R2β + g1 g2 − g12 2 − g1 g2 − g12 I1α I2β cos (φ1α + φ2β ) 2 R2β I1α sin φ1α − g1 + g1 g2 − g12 2 − g2 + g1 g2 − g12 R1α I2β sin φ2β , 1 ∗ Fαβ − Fαβ = 2i 2 I1α I2β sin (φ1α + φ2β ) = − g1 g2 − g12 2 R2β I1α cos φ1α + g1 + g1 g2 − g12 2 + g2 + g1 g2 − g12 R1α I2β cos φ2β ,

(5.68)

(5.69)

page 201

March 24, 2021

202

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

where Rnλ = −

2dn xnλ (1 + ynλ ) 2

(1 − ynλ ) Δε2n2λ − (1 + ynλ )2 d2n x2nλ

+4

− Inλ =

Mn

2 2 + η2 ) ξnμλ (ξnμλ + ηnμ nλ

μ=λ

2 2 + η 2 )2 − 4η 2 η 2 (ξnμλ + ηnμ nμ nλ nλ

Nn

2εnλ − ξnλ , 2 (2εnλ − ξnλ )2 + ηnλ j=2λ−1,2λ

(5.70)

2 1 − ynλ

(1 − ynλ )2 Δε2n2λ − (1 + ynλ )2 d2n x2nλ − 4ynλ

Mn

2 2 + η2 ξnμλ − ηnμ nλ

2 2 + η 2 )2 − 4η 2 η 2 (ξnμλ + ηnμ nμ nλ nλ ⎫ ! " 2 " Nn ⎬ " Δεn2λ − d2n x2nλ " 1 " " × " " 2 ⎭ ynλ (2εnλ − ξnλ )2 + ηnλ

μ=λ

+ ynλ

n=2λ−1,2λ

(5.71) and ξnμλ = ξnμ − ξnλ .

(5.72)

Therefore, for an arbitrary combination of α and β, we must solve the following equations: + = 0, Fαβ − =0 Fαβ

(5.73) (α = 1, 2, . . . , M1 /2; β = 1, 2, . . . , M2 /2).

5.3.5. Results and discussion We now apply the exact solution for a two-band system to discuss the properties of the two-band superconductivity in ultrasmall grains. The single-particle level patterns of the (2M1 + m) + 2M2 electron system (m = 0, 1, and 2) under consideration are represented in Figs. 5.8(a), 5.8(b), and 5.8(c), respectively. The dotted lines mean the chemical potential, and d1 and d2 (d1 < d2 ) are the mean level spacings. As seen these ﬁgures, the additional electrons ﬁrst occupy band 1 and then band 2.

page 202

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

(a)

(b)

203

(c)

Fig. 5.8. Single-particle levels near the Fermi level in a the case of two-band superconductivity. The dotted lines mean the chemical potential. The left and right bands are band 1 and 2, respectively. d1 and d2 are the mean level spacings. (a) 2M1 + 2M2 electron system, where Mn is a number of pair levels, (b) (2M1 + 1) + 2M2 electron system, (c) (2M1 + 2) + 2M2 electron system.

Numerical calculations are carried out under the condition that N1 :N2 = 3:2, ωD = 50, and λ1 = λ2 = λ.

5.3.6. Pair energy level By minimizing the sum of squares of Eqs. (5.68) and (5.69)

M1 /2 M2 /2

F =

+2 −2 (Fαβ + Fαβ )

(5.74)

α=1 β=1

for various interaction parameters, we obtain a behavior of pair energy levels EnJ of two bands as shown in Fig. 5.9, in which the solid and broken lines correspond to the pair energy levels of band 1 and band 2, respectively. Parameters used in this calculation are N1 = 12, N2 = 8, M1 = 6, M2 = 4, 0 ≤ λ ≤ 1.0, and 0 ≤ λ12 ≤ 0.2. As seen in the ﬁgures, band 2 condenses into degenerate levels, but the band 1 does not. In general, we can expect that the single-particle levels in a band, whose mean level spacing d is larger than that of the other band, degenerate faster. The behavior of the condensing band is qualitatively the same as that in the case of calculations for the single band [234]. The coexistence of the normal band and the condensed one may be reﬂected in the opposite phase of the gaps of these bands [218].

page 203

March 24, 2021

204

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.9. Typical behavior of pair energy levels of two bands for the ground state. Parameters used in calculation are N1 = 12, N2 = 8, M1 = 6, M2 = 4, ωD = 50, 0 ≤ λ1 = λ2 ≤ 1.5, and 0 ≤ λ12 ≤ 0.3. Solid and broken lines correspond to the pair energy levels of band 1 and band 2, respectively.

5.3.7. Condensation energy The condensation energy of band n for the (2M1 + m)+ 2M2 electron system can be deﬁned as m gn EnC (2M1 + m, 2M2 ) = En (2M1 + m, 2M2 ) + Mn + 2 −En0 (2M1 + m, 2M2 ),

(5.75)

where En (2M1 + m, 2M2 ) and En0 (2M1 + m, 2M2 ) are the ground-state energies and the sum of the single-particle energies, respectively. We calculate the condensation energies and show them in Figs. 5.10(a) and 5.10(b). The parameters used in this calculation are λ = 0.5, and λ12 = 0.01 for (a), λ 12 = 0.1 for (b). Values are normalized by the bulk −1 λ . The solid and broken lines correspond to gap, Δ = ωD sinh λ2 −λ212 the condensation energy for bands 1 and 2, respectively. Lines plotted by squares, by triangles, and by circles are for the 2M1 + 2M2 electron system, (2M1 + 1) + 2M2 electron system, and (2M1 + 2) + 2M2 electron system, respectively. As seen in the ﬁgures, we can understand that band 2 condenses, but band 1 does not because of the sign of values. This diﬀerence of signs may also be reﬂected in the opposite phases of the gaps of these bands. The behavior of the results for the condensed band (band 2) is qualitatively the same as in the case of the single-band calculations. The condensation energy of band 2 for the (2M1 + 2) + 2M2 electron system is, however, diﬀerent from

page 204

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

(a)

205

(b)

Fig. 5.10. Condensation energy. Parameters used in calculation are ωD = 50, and λ1 = 2 λ2 = 0.5. Values are normalized by the bulk gap, Δ1 = ωD sinh−1 ( λ λλ−λ 2 ) or Δ2 = 1

2

12

1 ωD sinh−1 ( λ λλ−λ 2 ). The solid and broken lines correspond to the condensation energy 1 2 12 for bands 1 and 2, respectively. Lines plotted by squares, by triangles, and by circles are for the 2M1 + 2M2 electron system, for (2M1 + 1) + 2M2 electron system and for (2M1 + 2) + 2M2 electron system, respectively. (a) The condensation energy for the interband coupling parameter λ12 = 0.01. (b) The condensation energy for λ12 = 0.1.

the others. We can also see that the condensation energy is aﬀected by the interband interaction λ12 . This is mentioned in our previous work [218].

5.3.8. Parity gap The parity gap of band n is deﬁned as Δpn = En (2M1 + 1, 2M2 ) 1 − {En (2M1 , 2M2 ) + En (2M1 + 2, 2M2 )} 2

(5.76)

which was introduced by Matveev and Larkin and characterizes the diﬀerence of even–odd ground-state energies [237]. We have also calculated the parity gaps shown in Fig. 5.11. The solid and broken lines correspond to the parity gap for bands 1 and 2, respectively. Lines plotted by triangles and by squares are for the interband coupling parameter λ12 = 0.01 and for λ12 = 0.1, respectively. Other parameters used in this calculation are the same as for the calculation of the condensation energy. Values are normalized by the bulk gap. For the condensed band, we obtain qualitatively the same result as that in the case of the single-band calculations, i.e., there is a minimal point and a tendency toward 1 for d → 0. The mean level spacing giving the minimal point is, however, much less than that for the case of calculations

page 205

March 24, 2021

206

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.11. Parity gap. Parameters used in calculation are ωD = 50, and λ1 = λ2 = 0.5. The solid and broken lines correspond to the parity gap for bands 1 and 2, respectively. Lines plotted by triangles and by squares are for the interband coupling parameter λ12 = 0.01 and for λ12 = 0.1, respectively. Values are normalized by the bulk gap.

for the single-band. The parity gap is almost independent of the interband interaction λ12 . This is also mentioned in our previous work [218]. We have extended the Richardson’s exact solution to the two-band system, and have derived a new coupled equation. To investigate the properties of the two-band superconductivity, we have solved the equation numerically and have determined the behavior of pair energy levels, the condensation energy, and the parity gap. The band, whose mean level spacing is larger than that of the other band, degenerates and condenses faster. The behavior of the condensing band is qualitatively the same as that for the case of calculations for the single band. The co-existence of the normal band and the condensed one may be reﬂected in the opposite phases of the gaps of these bands. This phase character appears in every of the results of numerical calculations. Therefore, the phase of a gap is important to stabilize the two-band superconductivity. We have also calculated the condensation energy and the parity gap for two-band superconductivity. The results suggest that the interband interaction λ12 aﬀects the condensation energy, but not the parity gap. In summary, the expression of Richardson’s exact solution for two-band superconductivity has been presented, by solving numerically a new coupled equation. Then, the behaviors of pair energy levels, the condensation energy, and the parity gap have been determined. The results for the condensed band

page 206

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

207

is almost qualitatively the same as those for the single-band calculation, and the co-existence of the normal band and the condensed one may be originated from the opposite phases of the gaps of these bands.

5.4. Kondo Eﬀect Coupled to Superconductivity The Kondo eﬀect has attracted a great interest, while considering the properties of semiconductor quantum dots. The Kondo eﬀect can be understood as the magnetic exchange interaction between a localized impurity spin and free conduction electrons [242]. To minimize the exchange energy, the conduction electrons tend to screen the spin of the magnetic impurity, and the ensemble forms a spin singlet. In a quantum dot, some exotic properties of the Kondo eﬀect have been observed [243, 244]. Recently, Sasaki et al. has found a signiﬁcant Kondo eﬀect in quantum dots with an even number of electrons [245]. The spacing of discrete levels in such quantum dots is comparable with the strength of the electron-electron Coulomb interaction. The Kondo eﬀect in multilevel quantum dots has been investigated theoretically by several groups [246–248]. They have shown that the contribution from many levels enhances the Kondo eﬀect in normal metals. There are some investigations on the Kondo eﬀect in quantum dots revealing ferromagnetism [249], noncollinear magnetism [250], superconductivity [251] and so on [252, 253]. Properties of ultrasmall superconducting grains have been also theoretically investigated by many groups [228–230, 232–237, 254]. Black et al. have revealed the presence of a parity-dependent spectroscopic gap in the tunneling spectra of nanosize Al grains [228, 232]. For such ultrasmall superconducting grains, the bulk gap has been discussed in relation to physical properties such as the parity gap [237], condensation energy [233], and electron correlation [234] with the size dependence of the level spacing of samples [235]. In the previous works [218], we have also discussed physical properties such as condensation energy, parity gap, and electron correlation of two-gap superconductivity in relation to the size dependence and the eﬀective pair scattering process. The possibility of new two-gap superconductivity has been also discussed by many groups [15, 138, 163, 173, 177, 179, 181, 184, 255, 256]. In a standard s-wave superconductor, the electrons form pairs with antialigned spins and are in a singlet state as well. When the superconductivity and the Kondo eﬀect present simultaneously, the Kondo eﬀect and the superconductivity are usually expected to be competing physical phenomena. The local magnetic moments from the impurities tend to

page 207

March 24, 2021

208

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

align the spins of the electron pairs in the superconductor, which often results in a strongly reduced transition temperature. Buitelaar et al. have experimentally investigated the Kondo eﬀect in a carbon nanotube quantum dot coupled to superconducting Au/Al leads [251]. They have found that the superconductivity of the leads does not destroy the Kondo correlations in the quantum dot at the Kondo temperature. A more subtle interplay has been proposed for exotic and not well-understood materials such as heavy-fermion superconductors, in which both eﬀects might actually coexist [257]. In this paper, we investigate the Kondo eﬀect and the superconductivity in ultrasmall grains by using a model which consists of the sd and reduced BCS Hamiltonians with the introduction of a pseudofermion. The meanﬁeld approximation for the model is introduced, and we calculate physical properties of the critical level spacing and the condensation energy. These physical properties are discussed in relation to the coexistence of both the superconductivity and the Kondo regime. Finally, we derive the exact equation for the Kondo regime in a nanosystem and discuss the condensation energy from the viewpoint of the correlation energy.

5.4.1. Kondo regime coupled to superconductivity In nanosize superconducting grains, the quantum level spacing approaches the superconducting gap. It is necessary to treat the discretized energy levels of a small-sized system. For ultrasmall superconducting grains, we can consider the pairing-force Hamiltonian to describe the electronic structure of the system [240] and can determine the critical level spacing in the case where the superconducting gap function vanishes at a quantum level spacing [235]. In this section, we present a model for a system in the Kondo regime coupled to the superconductivity and discuss the physical properties such as critical level spacing and condensation energy by using the meanﬁeld approximation in relation to the gap function, spin singlet-order as the Kondo eﬀect, coexistence, and so on.

5.4.2. Model We consider a model coupled to the superconductivity for quantum dots to investigate the Kondo eﬀect in normal metals, which can be expressed by the eﬀective low-energy Hamiltonian obtained by the Schrieﬀer–Wolﬀ transformation [258]: H = H0 + H1 + H2 ,

(5.77)

page 208

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

where H0 =

εk a†kσ akσ +

Eσ d†σ dσ ,

(5.78)

σ

k,σ

H1 = J

209

[S+ a†k ↓ ak↑ + S− a†k ↑ ak↓ + Sz (a†k ↑ ak↑ − a†k ↓ ak↓ )],

(5.79)

k,k

H2 = −g

a†k↑ a†k↓ ak ↓ ak ↑ .

(5.80)

k,k

a†kσ (akσ ) and d†σ (dσ ) are the creation (annihilation) operator corresponding to conduction electrons and the eﬀective magnetic particle as an impurity, respectively. In this study, we assume the magnetic particle is a fermion with S = 1/2 for simplicity. E means an extraction energy given by E↑,↓ = −E0 ± Ez included the Zeeman eﬀect. The second term in Eq. (5.77) means the interaction between conduction electrons and the spin in a quantum dot. S is the spin operator as S+ = d†↑ d↓ , S− = d†↓ d↑ , and Sz = (d†↑ d↑ − d†↓ d↓ )/2. The third term corresponds to the interaction between conduction electrons included in the pairing force Hamiltonian. Here, we introduce a pseudofermion for the magnetic particle operator [259] as d†↑ = f↓ , d↑ = f↓† , d†↓ = −f↑ , d↓ = −f↑†.

(5.81)

For this transformation, we have the condition f↑† f↑ + f↓† f↓ = 1,

(5.82)

and we have |σ = fσ† |0. The spin operator S can be presented as S+ = f↑† f↓ ,

S− = f↓† f↑ , and Sz = (f↑† f↑ − f↓† f↓ )/2. The Hamiltonian can be rewritten as ε˜k c†kσ ckσ + Efσ† fσ , (5.83) H0 = k,σ

H1 = J

σ

fσ† fσ c†k σ ckσ ,

(5.84)

k,k ,σ,σ

H2 = −g

c†k↑ c†k↓ ck ↓ ck ↑ ,

(5.85)

k,k

# # † ˜k = where ckσ = i Uik aiσ with ε i,j Uki [εi δij − J/2]Ujk . For the sake of simplicity, we only focus on Ez = 0 without an external magnetic ﬁeld: E = E0 .

page 209

March 24, 2021

210

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

5.4.3. Mean-ﬁeld approximation In this section, we introduce the mean-ﬁeld approximation for the present Hamiltonian (5.77). Eto et al. have presented the mean-ﬁeld approximation for the Kondo eﬀect in quantum dots [260]. In the mean-ﬁeld approximation, we can introduce the spin-singlet-order parameter 1 †

fσ ckσ . (5.86) Ξ= √ 2 k,σ This order parameter describes the spin couplings between the dot states and conduction electrons. The superconducting gap function can be expressed as

ck↓ ck↑ . (5.87) Δ= k

Using these order parameters in Eqs. (5.84) and (5.85), we obtain the meanﬁeld Hamiltonian √ ˜ σ† fσ + 2J ε˜k c†kσ ckσ + [Ξfσ c†kσ + Ξ∗ ckσ fσ† ] Ef HMF = k,σ

−g

σ

k,σ

[Δ∗ ck↓ ck↑ + Δc†k↑ c†k↓ ].

(5.88)

k

Constraint (5.82) is taken into account by the second term with a Lagrange multiplier λ. In this study, we assume a constant density of states with the energy region of the Debye energy, and the coupling constants can be expressed as J = dJ˜ and g = dλ.

5.4.4. Critical level spacing in the Kondo eﬀect By minimizing the expectation value of HMF in Eq. (5.88), the order parameters can be determined self-consistently. First, we show the Kondo eﬀect without the pairing force part (g = 0) in the framework of the mean-ﬁeld approximation. Next, the Kondo eﬀect in the presence of the superconductivity is discussed in relation to the critical level spacing and the condensation energy. Finally, we derive the exact equation for the Kondo eﬀect in ultrasmall grains coupled to normal metals and discuss properties such as the condensation energy in relation to Richardson’s exact equation for the superconductivity. For ultrasmall superconducting grains, the critical level spacing dBCS c γ exp(−1/λ) for even number of electrons, can be expressed as dBCS = 4ω e D c where ωD means the Debye energy. This result suggests that the gap function

page 210

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

(a)

211

(b)

Fig. 5.12. Gap function and spin singlet-order: (a) the gap function. The gap function vanishes in the region of λ values less than λc . (b) Spin singlet-order parameter. In the case of J˜ < J˜c , the singlet-order vanishes. The system consists of eight energy levels and eight electrons with the level spacing d = 1.0 and ωD = 1.0.

of a nanosize system with the level spacing d vanishes, when the coupling parameter λc is less than the value (ln 4ωD /d + γ)−1 . The bulk gap function Δc with λc can be expressed as Δc = ωD sh−1 (1/λc ). Figure 5.12(a) shows the gap function of a nanosize system in the framework of the standard BCS theory. We can ﬁnd the region where the gap function vanishes, when the coupling becomes less than λc . This means the level spacing is larger than the gap function in this region. Here, we drive the critical level spacing for only the Kondo regime (λ = 0). The equation determining the singlet-order parameter can be expressed as Ξ=

k

Ξ (ξk − x) , (ξk − x)2 + Ξ2

(5.89)

˜ ± (˜ ˜ 2 + 4Ξ2 ]]/2, and μ is the chemical εk + E εk − E) where ξk = ε˜k −μ, x = [˜ potential. For the case of the critical level spacing, the solution shows that the spin singlet-order parameter vanishes. From Eq. (5.89), we can ﬁnd the for the Kondo regime critical level spacing dKondo c 1 Kondo γ . (5.90) = 4ωD e exp − √ dc 2 2J˜ √ When the coupling parameter J˜ is smaller than J˜c = [2 2(ln(4ωD /d)+γ)]−1 , the spin singlet-order parameter vanishes.

page 211

March 24, 2021

212

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Figure 5.12(b) presents the spin singlet-order parameter given by Eq. (5.86) in the case g = 0. In the region of J˜ < J˜c , the order parameter vanishes. This result suggests the critical level spacing in the Kondo eﬀect.

5.4.5. Kondo eﬀect coupled to the superconductivity Here, we consider a simple system which consists of 8 energy levels and eight electrons and investigate the critical level spacing and the condensation energy of the coupled system between the superconductivity and the Kondo regime in the framework of the mean-ﬁeld approximation of Eq. (5.88). Figure 5.13(a) shows the spin singlet-order parameter and the gap function for several cases. We can ﬁnd the critical level spacings for the gap function and for the spin singlet-order parameter. When λ < λc and J˜ > J˜c , we can ﬁnd only the spin singlet-order parameters. In the region of λ/λc from ˜ J˜c = 0.189, we can ﬁnd the coexistence of both the gap 1.4 to 1.7 with J/ function and the spin singlet-order parameter. For λ/λc larger than 1.7, only the gap function still exists, and the spin singlet-order parameter vanishes. At ˜ J˜c = 0.284, we can ﬁnd the coexistence in the region λ/λc = 1.7–2.3. These J/ results suggest that strong local magnetic moments from the impurities make the transition temperature for superconductivity to be reduced. However, the weak couplings λ of the superconductivity do not destroy the spin singlet-order parameter at all. These results are in good agreement with the experimental results [251]. We can ﬁnd that there is the coexistence region for both the superconductivity and the Kondo regime.

(a)

(b)

Fig. 5.13. Physical properties in a coupled system: (a) Gap function and spin singletorder parameter. (b) Condensation energy. J˜/J˜c = 0, 0.94741, 1.8948, and 2.8422. Other parameters are the same.

page 212

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

213

Figure 5.13(b) shows the condensation energy for several λ and J˜ values. We have found that the condensation energy of the coupled system between the superconductivity and the Kondo regime becomes lower than that for the pure superconductivity. In the coexistence region, the highest value of the condensation energy appears in all cases.

5.4.6. Exact solution for the Kondo regime The standard BCS theory gives a good description of the phenomenon of superconductivity in large samples. However, when the size of a superconductor becomes small, the BCS theory fails. To investigate the physical properties such as the condensation energy, parity gap, etc., it is necessary to make a more accurate treatment. For the superconductivity in ultrasmall grains, the exact solution to the reduced BCS Hamiltonian presented by Richardson [240] has been applied to investigate the above-mentioned physical properties [236]. By using the wave function describing all pair electron excitations, we can derive the exact solution for the pairing force (reduced) Hamiltonian 2−

N k=1

n λ 2λ + = 0, ε˜k − Ei El − Ei

(5.91)

l=1,l=i

where N and n are the number of orbitals and the number of the occupied orbitals, respectively, and Ei corresponds to the exact orbital. Figure 5.14 shows the condensation energy and the pairing energy level for the nanosize superconductivity. Note that the physical properties obtained in the meanﬁeld approximation give a good description for the high density of states (d → ∞). We have found the diﬀerent behavior of the condensation energy from that obtained in the mean-ﬁeld approximation, as shown in Fig. 5.14(a). Figure 5.14(b) presents the qualitative behavior of the pairing energy level in the ground state. At λ about 1.6, above two energy levels in Fig. 5.14(b) are completely paired. The pairing behavior has been already reported by many groups [182, 240]. Let us derive the exact equation for the Kondo regime in ultrasmall grains. We can consider the Hamiltonian H = H0 + H1 in Eq. (5.77). We introduce a creation operator describing all excited states at the spin singlet coupling between a conduction electron and a pseudofermion: Bj† =

c† fσ kσ , ε˜k − Ej k,σ

(5.92)

page 213

March 24, 2021

214

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

(a)

(b)

Fig. 5.14. Exact solution for the superconductivity: (a) Condensation energy of the exact solution and that obtained in the mean-ﬁeld approximation (b) Pairing energy level with energy level obtained in the mean-ﬁeld approximation: Eight energy levels, eight electrons, d = 1.0, ωD = 4.0.

where Ej means the exact eigenenergies in the Kondo regime. The exact eigenstate |Ψn for the Kondo regime can be written as |Ψn = Πnν=1 Bν† |0. Other electrons, which are not related to the spin singlet-order, contribute # Esingle = nk=1 ε˜k to the eigenenergy. The ground-state energy EGS can be # written as EGS = nk=1 [Ek + ε˜k ]. By operating the Hamiltonian to the exact eigenstate, we obtain the condition 1+

N k=1

J˜ = 0. ε˜k − Ej

(5.93)

This equation gives the exact solution for the Kondo regime. Note that the creation operator (5.92) might be a true boson one as compared with the case of the reduced BCS model. Figure 5.15 shows the condensation energy of the exact solution in the Kondo regime with that obtained in the mean-ﬁeld approximation. We can ﬁnd the diﬀerent behavior of the condensation energy from that obtained in the mean-ﬁeld approximation. However, the behavior is similar to that in the case of the superconductivity in nanosize systems. We have investigated properties of the Kondo regime coupled to the superconductivity in ultrasmall grains by using the mean-ﬁeld approximation. In the framework of the mean-ﬁeld approximation, we have found the critical level spacing for the Kondo regime. The result suggests that the

page 214

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

215

Fig. 5.15. Condensation energy for the Kondo regime: all parameters used in the system are as follows: Eight energy levels, eight electrons, d = 1.0, and ωD = 4.0.

Kondo eﬀect vanishes, when the level spacing becomes larger than the critical level spacing. We have calculated physical properties of the critical level spacing and the condensation energy of the coupled system by using the meanﬁeld approximation. From the results, we have found that strong local magnetic moments from the impurities make the transition temperature for superconductivity to be reduced. However, weak couplings λ of the superconductivity do not destroy the spin singlet-order parameter at all. These results are in good agreement with the experimental results [251]. We have found that there is the coexistence region for both the superconductivity and the Kondo regime. Finally, we have derived the exact equation for the Kondo regime in a nanosystem, which was not an easy task, and have discussed the condensation energy from the viewpoint of energy levels. The further study of the properties in the Kondo regime with the use of the exact equation will be presented elsewhere. In summary, we have investigated the Kondo eﬀect and the superconductivity in ultrasmall grains by using a model which involves the sd and reduced BCS Hamiltonians with the introduction of a pseudofermion. The mean-ﬁeld approximation for the model have been introduced, and we have calculated physical properties of the critical level spacing and the condensation energy. These physical properties have been discussed in relation to the coexistence of both the superconductivity and the Kondo regime. Finally, we have

page 215

March 24, 2021

216

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

derived the exact equation for the Kondo regime in a nanosystem and discuss the condensation energy from the viewpoint of energy levels.

5.5. Interaction of Nanoscale Ferromagnetic Granules in London Superconductors Recent experiments have fabricated structured arrays of ferromagnetic nanoparticles in proximity to a bulk superconductor. We consider the theory of interactions between two nanoscale ferromagnetic particles embedded in a superconductor. In the London limit approximation, we will show that the interactions between ferromagnetic particles can lead to either parallel or antiparallel spin alignment. The crossover between these is dependent on the ratio of the interparticle spacing and the London penetration depth. We show that a phase transition between spin orientations can occur, as the temperature is varied. Finally, we comment on the extension of these results to arrays of nanoparticles in diﬀerent geometries. We show that a phase transition between spin orientations can occur under variation of the temperature. Finally, we comment on the extension of these results to arrays of nanoparticles in diﬀerent geometries. Magnetism and superconductivity are two competing collective ordered states in metals. In the case of ferromagnetism, the exchange interactions lead to the parallel alignment of electronic spins, while electron–phonon interactions in the BCS superconductivity lead to the spin singlet pairing of electrons. Clearly, these two types of order are generally mutually incompatible. In bulk systems, the frustration between the electron singlet pairing and the spin ordering is resolved by the FFLO (Fulde–Ferrell [261], Larkin– Ovchinnikov [262]) state. However, this has proved elusively experimentally, and few examples are known. In particular the FFLO state appears to be highly sensitive to disorder. In recent years, however, there has been observed a great increase of the interest in the interactions between ferromagnetism and superconductivity in artiﬁcially structured systems. Advances in nanotechnology and microfabrication have made it possible to build hybrid structures containing both ferromagnetic and superconducting components which interact magnetically or via the proximity eﬀect [263,273]. Superconductor– ferromagnetic–superconductor planar structures have been found to show the π-junction Josephson behavior [265–267]. Ferromagnet–superconductor– ferromagnet spin valve structures have also been fabricated [268] with potential applications to spintronics. More complex types of structures have also been produced; for example, Moschalkov et al. fabricated arrays

page 216

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

217

Fig. 5.16. Schematic diagram of a nanocomposite superconductor containing ferromagnetic granules.

of ferromagnetic nanoscale dots on superconducting substrates [269, 270]. A description of such structures based upon the Ginzburg–Landau theory was developed by Peeters [271]. In this section, we consider the interaction between magnetic nanoparticles embedded in a superconductor, as shown in Fig. 5.16. Theoretical studies of such systems can be carried out exactly in two limiting cases depending on the relative magnitudes of the London penetration depth λ, and the coherence length, ξ. If we consider the nanoparticles to be essentially pointlike on the scale of both these characteristic lengths, then they correspond to eﬀective point-like magnetic-moments of the form mi δ (r − ri ), (5.94) M (r) = i

where the particle at ri has magnetic moment mi . Interactions between these isolated moments arise directly from magnetic dipole–dipole forces modiﬁed by the screening of the bulk supercurrents. A second source of the interaction between the moments is the RKKY interaction modiﬁed by the presence of the BCS energy gap Δ. It is clear that the range of the dipolar forces is determined by the penetration depth λ, while the usual oscillatory power-law RKKY interaction is truncated exponentially on a length scale of the order of ξw . Therefore, the dipolar forces dominate for superconductors in the London limit r0 λ, while the RKKY interactions −1 + l−1 , and are more important in the Pippard case r0 l, where r0−1 = ξw l is the mean free path [16]. Here, we consider the London limit and neglect RKKY interactions. Magnetic impurities interacting via RKKY interactions were considered by Larkin [272]. In the London limit, we ﬁrst derive general

page 217

March 24, 2021

218

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

expressions for the conﬁguration of magnetic ﬁelds and the interaction energy of an ensemble of ferromagnetic granules. Then we consider the case of two interacting nanoparticles. It is found that, as a function of the temperature, an orientational phase transition can take place. The conditions for such a phase transition to occur are derived for a chain of ferromagnetic granules. Finally, we comment on the application of these results to the determination of the equilibrium conﬁgurations of more general lattices of ferromagnetic particles.

5.5.1. Magnetic ﬁeld of ferromagnetic inclusions in a London superconductor We determine the magnetic conﬁgurations in superconducting nanocomposite systems by means of Maxwell’s equations. The total current, j, includes both normal and superconducting parts, j = js + jn .

(5.95)

The role of the normal currents in a superconductor is negligible, since the superconductor exhibits weak magnetic characteristics in the normal state. However, a normal current will be present within the ferromagnetic inclusions. This normal-state current can be written in the traditional form jn = ∇ × M,

(5.96)

where M is the magnetization of a material. The supercurrent obeys the usual London equation ∇ × js = −

ns e2 B m

(5.97)

in SI units [68, 264], where B is the magnetic ﬁeld, n s is the superﬂuid density, and m and e are the electron mass and charge, respectively. Combining relations (5.95)–(5.97) with the Maxwell equation ∇ × B = μ0 j, the magnetic ﬁeld can be found in the form ∇ × (∇ × B) + λ−2 B = μ0 ∇ × (∇ × M),

(5.98)

where λ is the London penetration depth of the ﬁeld in the superconductor. Since div B = 0, Eq. (5.98) can be rewritten as −∇2 B + λ−2 B = μ0 ∇ × (∇ × M).

(5.99)

page 218

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

219

For the boundary conditions, we assume that the magnetic ﬁeld in the superconductor vanishes far from the region of the ferromagnetic inclusions. According to these boundary conditions, the solution of Eq. (5.99) can be expressed as follows: " " μ0 d3 r G "r − r " ∇ × (∇ × M r ), (5.100) B (r) = 4π where the Green’s function is given by " exp (− |r − r | /λ) " . G " r − r " = |r − r |

(5.101)

After the double integration by parts and some algebraic manipulations, this expression can be rewritten in the general form $ 3R (R · M (r )) M (r ) μ0 3 d r exp (−R/λ) · − B (r) = 4π R5 R3 % 2R (R · M (r )) R R2 , (5.102) × 1+ + 2 − λ λ λ2 · R3 where R = r − r , R = |r − r |. Expression (5.102) determines the magnetic ﬁeld outside of the ferromagnetic inclusions. Since the magnetization of the system M(r) is deﬁned by (5.96), we have in (5.101) that M(r) = 0 outside of the volume of ferromagnetic granules.

5.5.2. Magnetic ﬁeld of ferromagnetic quantum dots in a superconducting nanocomposite material Assuming that the sizes of the ferromagnetic inclusions are on the nanometer length scale, they will appear essentially point-like on the scale of the penetration depth λ. In this case, we can approximate the magnetization as a sum of point magnetic moments, as shown in Eq. (5.94). Using this approximation in the general expression Eq. (5.102), we ﬁnd the result (see Appendix B): $ 3Ri (Ri · mi ) mi μ0 exp (−Ri /λ) · − 3 B (r) = 4π Ri5 Ri i % 2Ri (Ri · mi ) Ri Ri2 + 2 − , (5.103) × 1+ λ λ λ2 · Ri3 where Ri = r − ri and Ri = |r − ri |.

page 219

March 24, 2021

220

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

It is apparent from Eq. (5.103) that if the temperature of a superconductor approaches Tc , and the penetration depth λ → ∞, then expression (5.103) tends to the limit μ0 3Ri (Ri · mi ) mi − 3 , B (r) = 4π Ri5 Ri i

(5.104)

which describes the usual magnetic ﬁeld of isolated dipoles in the normalstate medium. In the other limiting case, if the distance between granules is much more than the depth penetration, we have Ri (Ri · mi ) μ0 exp(−Ri /λ) · − mi . (5.105) B (r) = 4π Ri · λ2 Ri2 i

5.5.3. Interaction energy of quantum dots in a superconducting nanocomposite material To determine the collective states of the magnetic moments in superconducting nanocomposite materials in the London limit, we make use the expression for the free energy F of the system [288] 1 (5.106) d3 r{B2 + λ2 (∇ × B)2 }. F = 2μ0 Integrating by parts and using the Gauss theorem, we transform Eq. (5.106) to the following form: 1 d3 r B B + λ2 ∇ × (∇ × B) = −2πλ2 d3 r B · ∇ × (∇ × M). F = 2μ0 (5.107) Integrating by parts and using the Gauss theorem again, we transform Eq. (5.107) to the form 2 (5.108) d3 r M · ∇ × (∇ × B). F = −2πλ Then, using the London equation (5.98) and omitting the magnetostatic self-energy from consideration, we ﬁnd the interaction energy of magnetic moments. The obtained expression can be used to determine the collective

page 220

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

221

state of magnetization of an ensemble of granules: 3 (Rij · mj ) (Rij · mi ) mi · mj μ0 exp (−Rij /λ) · − U= 5 3 8π Rij Rij i j & 2 2 (Rij · mj ) (Rij · mi ) Rji Rij + 2 − , (5.109) × 1+ 3 λ λ λ2 · Rij where Rij = rj − ri , Rij = |rj − ri |, i = j.

5.5.4. Spin orientation phase transitions in a nanocomposite material with arrays of ferromagnetic quantum dots We begin by studying the magnetic conﬁguration of an isolated pair of magnetic moments. The interaction energy of such a pair can be written as $ 3 (R12 · m1 ) (R12 · m2 ) m2 · m1 μ0 − U = − exp (−R12 /λ) · 5 3 4π R12 R12 % 2 2 (R12 · m1 ) (R12 · m2 ) R12 R12 + 2 − . (5.110) × 1+ 3 λ λ λ2 · R12 Let us introduce a coordinate system with the origin at the ﬁrst magnetic moment m1 and the polar axis along the line connecting magnetic moments. In this coordinate system, the magnetic moments have the components mi = mi (cos ϕi sin θi , sin ϕi sin θi , cos θi ), and their interaction energy (5.110) is written in the form U=

exp(−R12 /λ) μ0 m1 m2 · · f (θi , ϕi , R12 /λ) , 3 4π R12

(5.111)

where f (θi , ϕi , x) = −2 (1 + x) cos θ1 cos θ2 + (1 + x + x2 ) sin θ1 sin θ2 cos ϕ (5.112) and ϕ = ϕ2 − ϕ1 . Diﬀerentiating the function f (θi , ϕi , x) with respect to angular variables and equating the results to zero, we ﬁnd that there are four possible stable

page 221

March 24, 2021

222

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

energy conﬁgurations: θ1 = θ2 = 0, θ1 = θ2 = π,

(5.113)

0 ϕ < 2π, θ1 = θ2 = π/2, ϕ = π, θ1 = θ2 = π/2, ϕ = 0, θ1 = 0,

θ2 = π,

0 ϕ < 2π,

(5.114)

(5.115)

(5.116)

which are illustrated in Fig. 5.17. The further analysis shows that conﬁgurations Eqs. (5.115) and (5.116) are saddle points, not energy minima. Evaluating the second derivatives of (5.112), we obtain the stability condition of conﬁguration (5.113): 2 R R (5.117) − − 1 0. λ λ This implies that the ferromagnetic ordering of the pair of magnetic moments is possible if √ 1 R (1 + 5). (5.118) λ 2 It turns out that if condition (5.118) is violated, then the alternative conﬁguration (5.114) is a stable energy minimum. We can conclude that if the temperature changes, and the penetration depth parameter λ (T ) varies in such a way that condition (5.118) is not satisﬁed, then the ground-state orientation will change from (5.113) to (5.114). This result is readily generalized to ordered arrays of ferromagnetic granules, and so we conclude that orientational phase transitions are possible in systems of quantum dots in a superconducting matrix. For example, it is clear that condition (5.118) can be applied to linear chains of quantum dots. On the other hand, the results for square or cubic lattices remain to be determined. We have considered the interactions between nanoscale magnetic dots embedded in a bulk superconducting material. Our approach is valid for materials which are well described in the London limit r0 λ, since RKKY interactions are negligible. We have shown that, depending on the dimensionless parameter R/λ, diﬀerent stable ground states occur. So, as

page 222

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

223

Fig. 5.17. Four energy saddle points of a pair of ferromagnetic quantum dots, as deﬁned in Eq. (5.113). Of four, 1 and 2 correspond to the ground state, depending on condition Eq. (5.118). States 3 and 4 are never stable.

the temperature varies, orientational phase transitions will take place for periodic arrays of such quantum dots. Of course, our calculation does not include all types of interactions which deﬁne the orientation of magnetic moments in space. In particular, we neglect the energy of a magnetic anisotropy of granules which is determined by the shape of granules or the type of their crystal lattice. However, when the shape of granules is close to the spherical one and the lattice of a ferromagnet has the cubic symmetry, then Eq. (5.109) will be essentially exact. In the experimental systems studied by V.V. Moshchalkov [270], a square of Pt/Co magnetic nanodots was deposited on the surface on the Pb superconductor, which is of type I(k = 0.48). The dots where about 0.26 μm in diameter, and they were deposited on the grid with a spacing of 0.6 μm. For Pb, the penetration depth is 39 nm at low temperatures. So, this array was in the limit R > λ and the dot–dot interaction would be expected to correspond to the antiferromagnetic alignment shown in the

page 223

March 24, 2021

224

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

second state in Fig. 5.17. With increase in the temperature, the transition to the ferromagnetic alignment would occur according to Eq. (5.118) at λ = 0.36R, i.e., 219 nm. −1/2 with t = According to the Casimir formula λ(T ) = λ(0)(1 − t4 ) T /Tc , this would occur at T = 7.14 K, as compared with Tc = 7.2 K. Therefore, the experimental conditions for the transition to be observed are certainly feasible. Of course, for an exact comparison with theory in this case, our theory should be generalized to deal with magnetic particles near the surface rather than with those embedded in the bulk of a superconductor. Of course, it would be interesting in the future to generalize our results to superconductors in the Pippard limit, where the RKKY interactions between quantum dots will dominate over dipolar forces [272]. Expression (5.110) can be used to study, by means of numerical methods, the magnet conﬁgurations and the orientational phase transitions in an ensemble of nanogranules. It is possible to determine the conditions of orientational transformations in the analytic form for the ordered structures (a chain of granules, plane and volume lattices). Inasmuch as the state of the magnetic subsystem of a specimen at phase transitions is changed, this phenomenon can be experimentally observed under changing a magnetic susceptibility in the region of low ﬁelds.

5.6. Spin-orientation Phase Transitions in a Two-dimensional Lattice of Ferromagnetic Granules in a London-type Superconductor In order to determine the collective state of magnetic moments in nanocomposite materials with the matrix made of a London-type superconductor, we use formula Eq. (5.103) for the energy of magnetic interaction. First of all, we note that the realization of one or other magnetic conﬁguration is deﬁned by both the competition of diamagnetic eﬀects from the side of the superconducting matrix and the magnetostatic interaction in the system of ferromagnetic granules. At lower temperatures eliminating the thermal disordering of the system, the magnetostatic interaction leads to a correlation of magnetic moments. As main conditions for the formation of magnetic conﬁgurations, we take the equivalence of all sites and the zero value of the net magnetic moment of the lattice. The planar lattice of granules by itself sets a preferred direction in space. Therefore, we will separate two conﬁgurations from the whole manifold of spatial orientations of magnetic moments. The ﬁrst conﬁguration is presented in Fig. 5.18. It is characterized by the orientation of the magnetization of granules which is orthogonal to the base plane. The alternation of the magnetization of

page 224

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

225

Fig. 5.18. Two-dimensional lattice of magnetic points. Magnetic moments (black color) are directed up or down (white color); a is the lattice constant.

neighboring granules decreases, to a certain extent, the energy of magnetic interaction. In addition, such a distribution of magnetic moments favors a decrease of the amplitude of a magnetic ﬁeld in the superconducting matrix, which is also advantageous from the energy viewpoint. Thus, the given conﬁguration can be considered as a version of the magnetic order. A conﬁguration of the second type is shown in Fig. 5.19. It is characterized by the distribution of magnetic moments in the base plane of the lattice such that the magnetic moments are aligned as magnetic chains with alternating directions of the magnetization. Here, like the conﬁguration presented in Fig. 5.18, the main requirement, the equivalence of the states of magnetic points, is satisﬁed. A similar distribution also decreases the energy of magnetostatic interaction, on the one hand, and favors a decrease in the amplitude of a magnetic ﬁeld in a superconductor, on the other hand. At the same time, the planar orientation of magnetic moments has the basic distinction from the orthogonal one. For example, by means of a continuous deformation of the magnetization in the base plane, the conﬁguration in Fig. 5.18 can be transferred into the structure shown in Fig. 5.19. Such a system is characterized by a coherent rotation of magnetic moments by an angle ±ϕ relative to the principal direction of the lattice. In this case, there occurs both the modulation of the direction of moments at sites of the lattice and some increase in the energy of magnetic chains, but these processes are accompanied by the formation of magnetic vortices in cells, which promotes a decrease in the energy of magnetic interaction. The states of separate magnetic points in the lattice remain equivalent at the zero total magnetization. Thus, the questions arise how the energy of the array of magnetic moments in the base plane shown in Fig. 5.20 depends on the angle ±ϕ

page 225

March 24, 2021

20:13

226

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.19. Two-dimensional lattice of magnetic points. Magnetic moments are aligned in the plane in the form of chains; a is the lattice constant.

and to which value it is equal in the equilibrium state. To answer these questions, we consider relation Eq. (5.110) for the interaction energy and reduce it to a single sum by virtue of the fact that the states of magnetic points are equivalent. In this case, in order to calculate the energy of the lattice, it is suﬃcient to determine the energy of a single magnetic point, e.g., m0,0 , located at the origin of the coordinate system and then to multiply the result by the total number of magnetic points N . Relation Eq. (5.110) becomes signiﬁcantly simpler: U =−

μ0 N 4π 2

$ % N (ri · mi ) (ri · m0,0 ) ∂ ∂2 3 1− + exp (−α · ri /δ) ∂α ∂α2 ri5 i

$ % N ∂ ∂2 N mi · m0,0 1− + + exp (−α · ri /δ) . 2 2 ∂α ∂α ri3

(5.119)

i

By writing formula (5.119), we used the method of diﬀerentiation with respect to the parameter α which should be set equal to 1 after the calculations. The index “i” stands for the summation over all sites of the lattice. Performing the summation in relation Eq. (5.119), it is convenient to introduce the pair of indices (n, k) deﬁning the position of a site in the lattice (Fig. 5.20) instead of the running index of magnetic points “i”. It is easy to see that the system represented in Fig. 5.20 possesses the translational invariance with a period of 2a so that mn,k = mn+2l,k+2p , l, p = ±1, ±2, . . . .

(5.120)

page 226

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

227

Fig. 5.20. Part of the lattice with a modulated planar distribution of the magnetization; a is the lattice constant. Circles stand for magnetic points, and the arrows on them indicate the directions of magnetic moments mn k in the base plane (n, k — the spatial indices of magnetic points). The angle ϕ deﬁnes the deviation of the moments of magnetic points from the principal direction of the lattice. The states of all points in the given conﬁguration are equivalent. The net magnetic moment is zero. The separated circles denote schematically magnetic vortices. The dotted lines are tangents to the directions of magnetic moments at sites of the lattice.

The lattice has only four types of magnetic points diﬀering from one another by a spatial orientation of magnetic moments. Their vector components depend on the angle ϕ in the following manner: ⎛ ⎞ cos ϕ ⎜ ⎟ mn,k = mn+2l,k+2p , m2l,2p = m0,0 = m ⎝ sin ϕ ⎠ , ⎛

m2l+1,2p = m1,0

m2l,2p+1 = m0,1

⎞

0

cos ϕ ⎜ ⎟ = m ⎝ − sin ϕ ⎠ , 0 ⎛ ⎞ − cos ϕ ⎜ ⎟ = m ⎝ sin ϕ ⎠ , ⎛

0 − cos ϕ

⎞

⎜ ⎟ m2l+1,2p+1 = m1,1 = m ⎝ − sin ϕ ⎠ , 0 l, p = ±1, ±2, . . . , where m is the modulus of the magnetic moment of a site.

(5.121)

page 227

March 24, 2021

228

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

After the substitution of Eq. (5.121) in Eq. (5.119) and the summation over sites of the unbounded lattice, we get the following interesting result. It turned out that the interaction energy of the system of magnetic points (see Fig. 5.20) does not depend on the angle ϕ and is determined by the relation U μ 0 m2 · F (a/δ) , = N 4π a3

(5.122)

where N is the number of sites of the lattice, m is the magnetic moment of a granule, F (a/δ) is the energy characteristic of a magnetic state which is a universal function of a single parameter and determines the dependence of the energy on both the period and the ﬁeld penetration depth in the case where the magnetic moments are distributed in the base plane of the lattice. It can be represented in the form of a sum ∞ ∞ ∂ ∂2 μ0 1 exp(−2α(a/δ) l2 + p2 ) −1 + + F (a/δ) = · 4π ∂α ∂α2 8 (l2 + p2 )3/2 l=1 p=0

∞ ∞ ∂2 ∂ 1 + − −1 + · ∂α ∂α2 4 l=−∞ p=−∞ exp(−α(a/δ) (2l + 1)2 + (2p + 1)2 ) × ((2l + 1)2 + (2p + 1)2 )3/2 ∞ ∞ ∂2 1 ∂ + − 3−3 ∂α ∂α2 2 l=−∞ p=−∞ ((2l + 1)2 − (2p)2 ) · exp(−α(a/δ) (2l + 1)2 + (2p)2 ) × . ((2l + 1)2 + (2p)2 )5/2 (5.123) Thus, there occurs the degeneration of the state in the parameter ϕ in the presence of a tough correlation of the mutual orientations of moments of the ensemble of magnetic points. The energies of the conﬁguration shown in Fig. 5.19 and the ensemble with a modulated distribution of the magnetization (see Fig. 5.20) coincide. In turn, the determination of the energy of magnetic interaction for the conﬁguration possessing the orthogonal orientation of magnetic moments (Fig. 5.18) requires a smaller amount of calculations, because the ﬁrst sum in formula Eq. (5.119) vanishes. The result of calculations can be represented in the form μ 0 m2 U⊥ = · Φ(a/δ), N 4π a3

(5.124)

page 228

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

229

where Φ (a/δ) is the energy characteristic of the magnetic state which a universal function of the single parameter and determines the dependence of the energy on both the period and the ﬁeld penetration depth under the distribution of magnetic moments normally to the base plane of the lattice. This function can be represented in the form μ0 ∂ ∂2 Φ (a/δ) = 1− + 4π ∂α ∂α2 ∞ ∞ 4 · exp(−α · (a/δ) · 2 · l2 + 2 · p2 ) 1 × · 2 (2 · l2 + 2 · p2 )3/2 l=1 p=0 & ∞ ∞ exp(−α · (a/δ) · 2 · (l + 1/2)2 + 2 · (p + 1/2)2 ) − . 2 + 2 · (p + 1/2)2 )3/2 (2 · (l + 1/2) l=−∞ p=−∞ (5.125) The calculation of the functions F (a/δ), Φ (a/δ) on the basis of relations (5.123) and (5.125) is not a diﬃcult task and can be realized with any mathematical software. The results are presented in the graphical form in Fig. 5.21. In Fig. 5.21, we represent the plots of the energy characteristics of two diﬀerent states of a magnetic lattice versus the ratio of the parameter of a cell and the penetration depth of the magnetic ﬁeld, a/δ. The limit a/δ → 0 corresponds to the transition of the matrix into the normal state. It is obvious that a lattice with planar orientation of magnetic moments (Figs. 5.19 and 5.20) possesses the lower energy in the normal state at a/δ = 0. Therefore, the state with the perpendicular direction of moments (Fig. 5.18)

Fig. 5.21. Plots of the energy characteristics F (a/δ) and Φ (a/δ) of states of the lattice with normal and planar orientations of magnetic moments, respectively. Values of F (0) and Φ(0) correspond to the transition of the superconducting matrix into the normal state.

page 229

March 24, 2021

230

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

cannot be realized at all in the absence of a superconductor. As the temperature decreases and the penetration depth diminishes gradually, the parameter a/δ begins to grow. When this parameter attains the value a0 /δ ≈ 3.3, the conﬁguration with the orthogonal orientation of magnetic moments (Fig. 5.18) becomes more advantageous in energy, and the orientation phase transition occurs in the system. At a decrease in the temperature, a similar scenario of events completely corresponds to a reorientation of the magnetic moments of an isolated pair of magnetic points which was considered in the previous work [288]. In conclusion, we note that an analogous phase transition can be expected to occur in a planar lattice with rectangular cell. The only diﬀerence will consist in the elimination of the degeneration relative to the directions of magnetic moments in the base plane. Of course, the direct observation of a phase transition will be hampered, because the problem involves the magnetic lattice surrounded by a superconductor. However, a similar orientation transformation must happen also in a lattice applied on the surface of a massive superconductor, though values of the parameter a0 /δ will be diﬀerent in this case.

5.7. Energy Spectrum and Wave Function of Electrons in Hybrid Superconducting Nanowires Recent advances in nanoscience have demonstrated that the fundamentally new physical phenomena can be found, when systems are reduced in size to dimensions, which become comparable to the fundamental microscopic length scales of the investigated material. Superconductivity is a macroscopic quantum phenomena, and, therefore, it is especially interesting to see how this quantum state is inﬂuenced when the samples are reduced to nanometer sizes. In such systems, new states of matter can be engineered that do not occur in bulk materials. A good example is the case of nanostructures composed of both superconducting and ferromagnetic metals. Here, the proximity eﬀects couple the Cooper pair condensate to the spin polarized band structure of the ferromagnet, allowing the local coexistence of both pairing and magnetism. In the bulk, the possibility of such coexistence was examined by Larkin–Ovchinnikov [274] and Fulde–Ferrell [275], giving the so-called LOFF state. But it was proved diﬃcult to ﬁnd this state in bulk materials, possibly because its high sensitivity to a disorder. In this section, we consider composite nanowires made from both superconducting and ferromagnetic metals. We consider the cylindrical geometry shown in Fig. 5.22, in which one metal forms the core of the nanowire and

page 230

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

Fig. 5.22.

231

Nanowire.

the second forms an outer cylindrical sheath. Mesoscopic wires with a similar geometry have been examined by Mota and coworkers [276–280]. In the case of a ferromagnetic core, we can compare the spectrum with results for planar hybrid S/F nanostructures, as reviewed recently by Lyuksyutov and Pokrovsky [281] and by Buzdin [282]. Below, we will calculate the wave functions and the energy spectrum of electrons in hybrid superconducting nanowires. The spectrum of electrons spectrum of electrons reminds a fractal structure such as Hoftstadter’s butterﬂy introduced in 1976 for the description of a behavior of electrons in a magnetic ﬁeld [286].

5.7.1. Methodology We model the hybrid superconductor-ferromagnet nanowire system by extending the self-consistent theory of a type II vortex developed by Gygi and Schl¨ uter [283] to the case of a ferromagnetic vortex core. We start with the eﬀective Pauli Hamiltonian for the spin-polarized electronic states of a normal metal p + eA)2 ˆ 0 = (ˆ δσσ + Vσσ (r), H σσ 2me

(5.126)

where −e is the electron charge, A(r) is the magnetic vector potential, and Vσ (r) is a general spin-dependent single potential, where σ is ↑/↓. This potential can be assumed to be the sum of the ionic, Hartree, and exchangecorrelation potentials of a self-consistent spin-polarized DFT calculation.

page 231

March 24, 2021

232

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

In this case, it has the form Vσ (r) = Vion (r) + VH (r) + Vxc (r) + μB (B + Bxc )σσσ ,

(5.127)

where Vxc (r) is the spin-independent part of the exchange-correlation potential, μB is the Bohr magneton, B(r) is the physical local magnetic ﬁeld, and Bxc is an eﬀective magnetic ﬁeld representing the exchange ﬁeld of spin-polarization in the ferromagnet. Here, σσσ is the vector of Pauli matrices. To model the superconducting elements of the hybrid system, this singleparticle Hamiltonian is supplemented by an eﬀective attraction, which we take as the BCS contact term V (r, r ) = −g(r)δ(r − r ),

(5.128)

where g(r) is the local attractive potential strength at r. This will be zero in the normal or ferromagnetic part of the nanowire and a constant g in the superconducting parts. For simplicity, we neglect a retardation of the attraction in the rest of this paper. The full eﬀective Hamiltonian for our system is ' ( 3 + 0 + + ˆ ψˆσ (r) − g(r)ψˆ (r)ψˆ (r)ψˆ↓ (r)ψˆ↑ (r) . ˆ = d r ψˆ (r)H H σ

↑

σσ

σσ

↓

(5.129) Here, ψˆσ+ (r) and ψˆσ (r) are the usual ﬁeld operators for the electrons. In the Hartree–Fock–Gorkov approximation, this Hamiltonian is diagonalized by a spin-dependent Bogoliubov–Valatin transformation ∗ γn + vnσ (r)ˆ γn+ , unσ (r)ˆ (5.130) ψˆσ (r) = n

ψˆσ+ (r) =

γn+ + vnσ (r)ˆ γn . u∗nσ (r)ˆ

(5.131)

n

The requirement that the quasiparticle creation and annihilation operators retain the fermion anticommutation laws, {ˆ γn , γˆn+ } = δnn , implies that nσ

∗ u∗nσ (r)unσ (r ) + vnσ (r)vnσ (r ) = δ(r − r )δσσ .

(5.132)

(5.133)

page 232

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

233

The resulting set of Bogoliubov–de Gennes equations is ⎞⎛ ⎞ ⎛ ˆ 1 + V↑↑ V↑↓ 0 Δ(r) H un↑σ ⎟⎜ ⎟ ⎜ ˆ 1 + V↓↓ ⎟ ⎜ un↓σ ⎟ ⎜ V↓↑ −Δ(r) 0 H ⎟⎜ ⎟ ⎜ ⎟⎜v ⎟ ⎜ ∗ (r) ˆ − H − V −V 0 −Δ 1 ↑↑ ↑↓ ⎠ ⎝ n↑σ ⎠ ⎝ ˆ 1 − V↓↓ vn↓σ Δ∗ (r) 0 −V↓↑ −H ⎛ ⎞ un↑σ ⎜ ⎟ ⎜ un↓σ ⎟ ⎟, (5.134) = Enσ ⎜ ⎜v ⎟ ⎝ n↑σ ⎠ vn↓σ ˆ 1 = (ˆ where H p + eA)2 /2me − μ, and μ is the chemical potential. The self-consistent pairing potential corresponds to a pure spin-singlet pairing state and is given by Δ(r) = g ψˆ↑ (r)ψˆ↓ (r).

(5.135)

Consider the special case where the magnetization of the ferromagnet is in the same collinear direction, Bxc , as the external ﬁeld B. Choosing it as the spin-quantization axis zˆ, we have V↑↓ = V↓↓ = 0. In this case, the full system of four matrix Bogoliubov–de Gennes equations is separated into a pair of 2 × 2 matrix equations ˆ 1 + V↑↑ Δ(r) un↑σ un↑σ H = Enσ , (5.136) ˆ 1 − V↓↓ vn↓σ vn↓σ −H Δ∗ (r) ˆ 1 + V↓↓ −Δ(r) un↓σ un↓σ H = Enσ . (5.137) ˆ 1 − V↑↑ vn↑σ vn↑σ −Δ∗ (r) −H

5.7.2. Calculation of the spectrum We will study the Bogoliubov–de Gennes equations, by using a numerical method for their solution. The calculation algorithm is realized with the use of the most powerful FORTRAN language specially developed for mathematical calculations. In view of the cylindrical symmetry of the system under study, we write the system of Bogoliubov–de Gennes equations in the form suitable for calculations. We will also use the fact that the amplitudes of the functions u(r) and v(r) tend to zero at the boundary point. The solutions of the equations are determined with the use of the Runge–Kutta method (Figs. 5.23 and 5.24).

page 233

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

234

Fig. 5.23.

Billiard 1.

Fig. 5.24.

Billiard 2.

Taking the symmetry of our system (cylindrical) to account and choosing the gauge, in which the parameter Δ(r) is real, we can write the system of Bogoliubov–de Gennes equations in the form u(r, θ, z) = uμnkz (r)e−iμθ e−ikz z , v(r, θ, z) = vμnkz (r)eiμθ e−ikz z ,

(5.138)

−

1 ∂ ∂2 uμnkz (r) + U (r) · uμnkz (r) + Δ(r) · vμnkz (r) = 0, uμnkz (r) − 2 ∂r r ∂r

−

1 ∂ ∂2 vμnkz (r) + U (r) · vμnkz (r) − Δ(r) · uμnkz (r) = 0, vμnkz (r) − 2 ∂r r ∂r (5.139)

page 234

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

Fig. 5.25.

Fig. 5.26.

235

Quasiparticle amplitude of the Andreev state.

Andreev spectrum as a function of the angular momentum for billiard 1. 2

2

kz where U (r) = μr2 − (Ef − m − Eμnkz ). The plot of wave functions is given z in Fig. 5.25 (E0 = 0.986669921875 eV, Ef = 1 eV, Δ = 0.1 eV, kz = 0, R1 = 50 nm, R2 = 100 nm, μ = 1). In Figs. 5.26 and 5.27, we present the results of calculations for the spectrum of Andreev states of the system. The resulting spectrum as a function of the angular momentum is shown in Fig. 5.26 for billiard 1 and Fig. 5.27 for billiard 2. The spectra demonstrate the splitting caused by the boundary eﬀect. The Andreev billiard systems are the analog of a classical billiard. The Andreev billiard is interpreted as a ballistic motion with the Andreev reﬂection at the interface with a superconductor. The Andreev reﬂection is a

page 235

March 24, 2021

20:13

236

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.27.

Andreev spectrum as a function of the angular momentum for billiard 2.

fundamental process that converts an electron incident on a superconductor into a hole, while a Cooper pair is added to the superconductivity condensate. Figures 5.26 and 5.27 demonstrate the electron-hole symmetry of the Andreev spectrum. One-dimensional solutions of the Bogoliubov–de Gennes equations pass into in two-dimensional ones, as μ increases. It is worth noting that we work in the clean limit (mean free path l λ, ξ). Estimates of the penetration depth and the length scale of order were performed in [285]: ⎧ T λ0 ⎪ ⎪ ⎪ ⎨ λ(T ) = √1 − t4 where t = Tc , (5.140) ⎪ ξ0 (1 − 0.25t) ⎪ ⎪ √ , ⎩ ξ(T ) = 1−t where λ0 = 46 nm and ξ0 = 74 nm, i.e., almost the characteristic lengths of lead at zero temperature in the clean limit. We have carried out also the calculations for MgB2 nanowires with the parameters (R1 = 150 nm, R2 = 200 nm, Mz = 0, kz = 0, Δ = 0.003 eV, Ef = 1 eV). In Fig. 5.28 (NS, R1 = 150 nm, R2 = 200 nm, Mz = 0, kz = 0, Δ = 0.003 eV, Ef = 1 eV), we present the spectrum as a function of the angular momentum for MgB2 nanowires (billiard 1), whereas Fig. 5.29 shows the analogous dependence in the case of billiard 2. These spectra have visual similarity with the winds of a butterﬂy. They possess the property of self-similarity (fractality) and are one of the not numerous fractal structures discovered in quantum physics. Hoftstadter’s

page 236

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

Fig. 5.28.

Fig. 5.29.

Andreev spectrum for MgB2 nanowires.

Andreev spectrum for MgB2 nanowires. (SN).

237

page 237

March 24, 2021

238

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.30. This butterﬂy is a fractal describing the spectrum of electrons in a periodic structure with magnetic ﬁeld.

butterﬂy is a mathematical object with fractal structure describing the behavior of electrons in a magnetic ﬁeld. Under the action of a magnetic ﬁeld, free electrons move along circumferences. The theory says that if the electrons are “locked” in a crystal atomic lattice, the trajectories of their motion will be much more complicated. An analogous situation is presented by the Andreev billiard. The fractal structures by themselves are rare in the quantum world. Therefore, Hoftstadter’s butterﬂy was not discovered for a long time, which was partially related to the complexity of experiments. Then scientists from Manchester succeeded to observe an intricate pattern on graphene in a magnetic ﬁeld representing Hoftstadter’s butterﬂy [287] (Fig. 5.30). We have studied hybrid nanowires, in which normal and superconducting regions are in close proximity, by using the Bogoliubov–de Gennes equations for superconductivity in a cylindrical nanowire. We have developed a method for numerical solutions of these equations in FORTRAN programme and present some preliminary results. We have succeeded to obtain the quantum energy levels and wave functions of a superconducting nanowire. The spectrum of states we calculated shows the interesting “Andreev Billiard” characteristics. Preliminary results are also obtained in the cases of a magnetic nanowire and a superconducting nanowire containing a vortex. The calculations for a superconducting nanowire can be extended to the cases of a superconductor-ferromagnet hybrid nanowire and a nanowire containing one or more superconducting ﬂux quanta [284]. The obtained spectra of electrons remind Hoftstadter’s butterﬂy [286].

page 238

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

239

5.8. Quantum Computer on Superconducting Qubits 5.8.1. Principle of quantum computers Silicon microprocessors, being the main element of modern computers, have attained the limit of development. The miniaturization, i.e., the aspiration to place as much as possible components on a more and more smaller area of a chip, has approached the boundary of physical possibilities. Further, it will be impossible to conserve the stability of the operation of computers. Many researchers believe that silicon processors will begin to go into the past in at most ﬁve years, and the production of chips will be based on the other material — carbon nanotubes. It is worth noting that the computational processes are accompanied by the release of heat. R. Feynman said: “Any classical computation is a physical process running with the release of heat.” As known, the calculations lead to an increase in the entropy and, hence, to the release of heat. The idea of the creation of quantum computers arose several decades ago, when it was proposed to reject the application of electric circuits in the processing of information and to pass to the use of quantum mechanics. The classical computers are processing the information only on the basis of ideas of one bit of information (it corresponds to the transition from state 0 to state 1 or conversely). The quantum computers can process the information, by basing on the ideas of a quantum bit (qubit) which allows one to realize simultaneously four logical operations (0 + 0 = 0, 0 + 1 = 1, 1 + 0 = 1, 1 + 1 = 2). Qubit is the abridged notation for quantum bit and means the unity of information coded in a quantum system which can be in the states |0, |1, and in any superposition of these states. Let the state of a qubit be described by the state |f which can be represented as a superposition of states |0 and |1: |f = a|0 + b|1, where a2 + b2 = 1.

(5.141)

Since the devices can register only classical quantities, the measurement of a quantum bit will give states |0 or |1 with probabilities determined by the squares of the coeﬃcients a and b. Figure 5.31 shows √the diﬀerence between an ordinary and a quantum qubit, here a = b = 1/ 2. The use of the principle of superposition allows one to increase the informational space exponentially with linear growth of the size of a physical

page 239

March 24, 2021

240

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.31.

Ordinary qubit and quantum qubit.

system, because the register including n qubits can be in a superposition of at once 2n states. In addition, quantum mechanics admits the existence of the so-called entangled states possessing no analogs in classical physics. An ensemble of qubits is a collection of qubits in diﬀerent but given states. It is worth noting that, even on the level of mathematics, a quantum computer operates in a basically diﬀerent way than that of a classical computer. Input data are coded in “quantum cells of memory.” In this case, the collection of qubits becomes a single quantum system. This system undergoes the sequence of elementary quantum operations. Quantum computations are a realization of the most astonishing idea to apply the principles of quantum mechanics to the world of computers. Ordinary computers, despite their complexity, use classical laws of mechanics. In the recent years, the theory of classical computations was developed on the basis of works by A. Turing. With the appearance of quantum computations, the new possibilities have arisen, and the situation is radically changed. Quantum methods can be successfully used in the solution of mathematical problems, though the time consumed for the solution of mathematical problems increases exponentially with the complexity of a problem. For the theory of quantum calculations, the physical nature of qubits is not of crucial importance; the basically important point is that the system in the course of calculations obeys the laws of quantum mechanics.

5.8.2. Superconducting qubits The realization of a quantum computer requires the availability of systems with doubly degenerate ground state. For this reason, a great attention is paid to systems with two-level wells which can be fabricated by facilities of

page 240

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

241

solid-state electronics. The modern technology allows one to produce circuits containing millions of transistors and Josephson junctions. By observing the operation of electrical circuits at temperatures close to the absolute zero, the researchers found a new proof of the fact that the laws of quantum mechanics are suitable not only for the microscopic objects (atoms and electrons), but also for large electronic schemes which include superconducting bits (qubits). Many years ago, the attempts to construct a Josephson computer on the basis of the Josephson tunnel logic hopelessly failed. The principal reason for the failure was the huge technological dispersion of parameters of tunnel junctions, which did not allow one to produce large microcircuits. A Josephson computer can be created only on the way having nothing in common with that based on semiconductors, namely it can be just a quantum computer. The hope is related to two circumstances. First, the fabrication of superconducting qubits is quite possible in the framework of the up-to-date technology. Second, the presence of a gap in the spectrum of excitations of a superconductor allows one to expect the suppression of generation in a system. Let us consider the ﬁrst steps on the way of the construction of a superconducting quantum computer. First, we consider, in brief, the Josephson eﬀect.

5.8.3. The Josephson eﬀect The Josephson eﬀect is certainly one of the most interesting phenomena in superconductivity. The Josephson eﬀect consists in the passage of a superconducting current through a thin dielectric layer separating two superconductors (the so-called Josephson junction). It was predicted by an English physicist B. Josephson on the basis of superconductivity theory (1962, Nobel’s prize in 1973) and discovered experimentally in 1963. Conduction electrons pass through a dielectric (a ﬁlm of copper oxide ∼10 ˚ A in thickness) due to the tunneling eﬀect [292,293]. In Fig. 5.32, we present a scheme of the Josephson tunneling between two superconductors. The Josephson stationary eﬀect consists in that the superconducting current Jc = J0 sin ϕ, 2eV dϕ = , dt

(5.142) (5.143)

page 241

March 24, 2021

242

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.32.

Scheme of the Josephson tunneling between two superconductors.

where ϕ is the phase diﬀerence on the interface of superconductors, V is the applied voltage, and J0 is the critical current through the junction. The Josephson eﬀect indicates the existence of the electron ordering in superconductors, namely, the phase coherence: in the ground state, all electron pairs have the same phase ϕ characterizing their wave function √ Ψ1 = ns1 eiϕ1 . According to quantum mechanics, the presence of a phase diﬀerence must cause a current through the junction. The discovery of such a current in experiment proves the existence of macroscopic phenomena in the nature which are directly determined by the phase of a wave function √ (5.144) Ψ = n eiψ .

5.8.3.1. Current passing through two series-connected Josephson junctions The Josephson current in the scheme drawn in Fig. 5.33 can be easily determined with the help of the elementary Feynman approach to a Josephson junction as a two-level quantum-mechanical system [4]. By introducing an twointermediate object, some island, with the wave function Ψ 0 into the iϕ1 and = n /2e level system characterized by the wave functions Ψ 1 s1 odinger equation in the form Ψ2 = ns2 /2eiϕ2 , we write the Schr¨ eV dΨ1 = Ψ1 + KΨ0 , dt 2 dΨ0 = KΨ1 + KΨ2 + E0 Ψ0 , i dt eV dΨ2 = KΨ0 − Ψ2 . i dt 2 i

(5.145) (5.146) (5.147)

The formula for a constant current running through two series-connected Josephson junctions at the zero external potential diﬀerence takes the form: √ ∂ nS1 K2 √ =− nS2 sin(ϕ2 − ϕ1 ). (5.148) J = ∂t E0

page 242

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

Fig. 5.33.

243

Current passing through two series-connected Josephson junctions.

This relation can be rewritten as follows: Jc = J0 sin(ϕ),

(5.149)

where ϕ = ϕ2 − ϕ1 is the phase diﬀerence. The relation obtained is named the Josephson formula (the Josephson stationary eﬀect) and determines the current of superconductive electron pairs due to the tunneling transition. The Josephson coupling energy is an important parameter of the Josephson junction. From (5.142), we have hJ0 hJ0 π cos ϕ. (5.150) sin ϕdϕ = − E = JV dt = 2 0 2e The Josephson eﬀect is still one of the phenomena that make superconductors such a fascinating area of study. Despite the more than 40-year intense studies and numerous applications, the Josephson eﬀect remains an important ﬁeld of researches in connection with the use of small superconducting grains.

5.8.3.2. SQUIDS The Josephson eﬀect allowed one to construct superconducting interferometers, SQUIDs (superconducting quantum interference device), which contain parallel weak connections between superconductors [289]. In Fig. 5.34, we present a scheme with Josephson junctions. The total current running from 1 to 2 is equal to I = I0 d [sin(Δϕ1 ) + sin(Δϕ2 )] ,

(5.151)

where Δϕ1 = ϕ2A − ϕ1A , Δϕ2 = ϕ2B − ϕ1B are the phase diﬀerences on the ﬁrst and the second Josephson junctions. There occurs a distinctive interference of the superconducting currents running through these connections.

page 243

March 24, 2021

244

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.34.

Basic diagram of a “quantum interferometer”.

Inside the superconductor, the current is zero j ≡ 0. We will use the following formula for the current j: j ∼ h∇ϕ −

2e A. c

(5.152)

We can write ϕ1B − ϕ1A

2e = hc

ϕ2B − ϕ2A =

2e hc

A · dl,

(5.153)

A · dl.

(5.154)

C1

C2

Summing up these two equations, we get ϕ1B − ϕ2B + ϕ2A − ϕ1A

2e = hc

A · dl = 2π

Φ . Φ0

(5.155)

Thus, we have Δϕ1 − Δϕ2 = 2π

Φ , Φ0

(5.156)

where Φ is the total quantum ﬂux. The ﬂux quantum is deﬁned as Φ0 =

h . 2e

(5.157)

page 244

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

245

For a balance SQUD ring system, we can write Φ , Φ0 Φ Δϕ2 = ϕ0 − π . Φ0 Δϕ1 = ϕ0 + π

(5.158)

The total current in the SQUD is I = I0 sin(Δϕ1 ) + I0 sin(Δϕ2 ) Φ Φ + I0 sin ϕ0 − π = I0 sin ϕ0 + π Φ0 Φ0 " " " Φ Φ "" " = Imax "cos π = 2I0 sin(ϕ0 ) cos π Φ0 Φ0 "

(5.159)

with Imax = 2I0 sin(ϕ0 ). In this case, the critical current turns out to be periodically dependent on the ﬂow of an external magnetic ﬁeld, which allows one to use such a unit for the exact measurement of the magnetic ﬁeld.

5.8.3.3. Flux qubit Let us consider the ﬁrst steps on the way of the creation of a superconducting computer. The simplest superconducting system demonstrating the coherency is SQUID which is a superconducting ring including a Josephson junction at one point. The energy of this system contains two terms: Josephson transition energy (cos Φ) and the energy related to the ring L: Φ (Φ − Φx )2 . (5.160) + H = −EJ cos 2π Φ0 2L Here, Φ is the diﬀerence of superconductive phases at the junction. The superconductive phase in the ring is proportional to a magnetic ﬂow applied to the ring (quantization of the magnetic ﬂow). If Φx is equal exactly to a half of the magnetic ﬂow, the potential of a SQUID becomes doubly degenerate. Two minima of the well correspond to the currents in the ring passing in the clockwise and counterclockwise directions , respectively [291]. A superposition of these states in SQUID was observed experimentally in works [291, 294]. These experiments demonstrated clearly the possibility to create a superposition of states in a system with a macroscopic number of particles. In the given case, the circular current including 1013 electrons was registered in a loop. The states participating in a superposition were macroscopically distinguishable, by diﬀering from one another by the

page 245

March 24, 2021

246

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.35.

Scheme of the Josephson tunneling between two superconductors.

currents, whose diﬀerence was several microamperes. We indicate that, at the recent time, the important notion has been introduced in the course of studies of structures with Josephson junctions. It is the notion of macroscopic quantum coherence. In such systems, the Josephson energy can have two almost degenerate minima at values of the phase which are separated by a potential barrier (see Fig. 5.35). It is possible that the phase passes from one minimum to another one due to the quantum-mechanical tunneling, and the eigenstates of the system are superpositions of the states localized in the ﬁrst and second minima. The operation of a superconducting computer requires low temperatures which are needed, in particular, to suppress heat-induced excitations destroying the quantum mechanical state of a system. It is worth noting that the best condition for the observation of these current states is deﬁned by a size of the superconducting ring. If the ring size is taken to be 1 cm, there appear the eﬀects of decoherence which will destroy the current states. But if the ring is taken much smaller (say, 5 μm), then it is possible to observe these states. These states were discovered in experiments with Rabi oscillations [294].

5.8.3.4. Charge qubit The second type of a superconducting bit can be realized in the “Cooper pair box” system which is characterized by two charge states: without excess Cooper pair |0 and with a single Cooper pair |1. “Cooper pair box” is a nanotransistor with Coulomb blockage with controlling voltage Vg , as shown in Fig. 5.36. A “Cooper pair box” is represented by an aluminum superconducting ﬁlm of the order of 1 mm in size with the working temperature of about several milli-Kelvin, which is signiﬁcantly lower than the superconducting temperature Tc . Its quantum state can be characterized by the number of Cooper pairs. According to the BCS theory, the groundstate of a superconductor is a superposition of states with diﬀerent numbers

page 246

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

247

Fig. 5.36. Cooper-pair box [× denotes a Josephson junction (JJ)], Cg and Vg are the capacitor and the controlling voltage.

of Cooper pairs. The excited, i.e., unpaired states in an ordinary superconductor are separated from the ground state by the energy gap. Therefore, as the number of electrons varies by 1, i.e., N → N ± 1, the ground-state energy must be changed by ±δ. The sign (plus or minus) depends on that the initial number of electrons N is even or odd. The eﬀects of parity of the number of electrons which are considered in this chapter in connection with mesoscopic superconductivity were successfully measured on nanotransistors with Coulomb blockage. The Hamiltonian of such a system can be written as H = Ec (n − ng )2 + Ej cos ϕ,

(5.161)

where Ec and Ej are the charging and Josephson energies, and ϕ is the phase change. In the charging mode where Ec Ej , only two lower charged states are of importance. The controlling voltage Vg induces a charge in the box n g = Cg

Vg , 2e

(5.162)

where 2e is the charge of each Cooper pair, and Cg is the gate capacitance. At ng = 1/2, such a system operates as a two-level atomic system, in which the states |0 and |1 can be realized. The control is realized by a voltage Vg . On the basis of such a qubit, a system of two qubits was realized [291, 292], and the formation of entangled states was demonstrated. The eﬀects of parity of the number of electrons which are considered in this chapter in connection with mesoscopic superconductivity were successfully measured on nanotransistors with Coulomb blockage.

5.8.3.5. Phase qubit There exists one more possibility to realize SQUIDs with the use of hightemperature superconductors possessing the d-pairing (n-loop ones) [293].

page 247

March 24, 2021

248

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

The physics of d-pairing was considered in Chapter 2. Quantum processors on the base of these SQUIDs are developed at the Canadian company “D-wave”. We note also that, in addition to superconducting qubits, quantum computers use qubits possessing other physical properties. Scientists at the Yale University took a very ﬁne aluminum plate in the fabrication of a quantum chip. A single qubit consists of one billion of aluminum atoms which behave themselves, nevertheless, as a single unit that can be in two energy states denoted as 0 and 1. Such quantum-mechanical states of a qubit cannot be long-term — their lifetime is about one microsecond. But it is suﬃcient for a chip to solve the so-called algorithm. We have considered the technologies of superconducting computers which represent a new type of quantum computers. These computers are based on the other mechanism obeying the laws of quantum mechanics. We recall that, till the recent time, the principle of devices was invariable, and the archetype of such devices is mechanical clocks. In such devices, all stages of their relative motion can be observed; therefore, it is quite simple to understand their structure. On the contrary, the principle of operation of quantum computers involves the speciﬁc features of quantum mechanics which are diﬃcult to understand. Nevertheless, by possessing the quantum resources, we can solve the very diﬃcult complicated problems. In particular, the most important potential ﬁeld of application of quantum computers is the problem of the exact calculation of properties of quantum systems.

5.8.4. Quantum computer Quantum computer is a computing unit using the quantum mechanical eﬀects in its operation and realizing the execution of quantum algorithms. Quantum computers are working on the basis of quantum logic. The idea of quantum computations was advanced independently and almost simultaneously by R. Feynman [297] at the beginning of the 1980s. In those works, it was proposed to use the operations with the states of a quantum system in computations. As distinct from the classical systems, a quantum system can stays in the superposition state, being simultaneously in all possible physical states. In quantum computations, the elementary step is a separate operation over the n-qubit superposition corresponding to the principle of quantum parallelism. In a classical computer, the single ouput value for one input state is calculated, whereas a quantum computer calculates the output values for all input states.

page 248

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

249

In other words, the quantum computer can solve rapidly problems such that their solution with an ordinary classical computer would take hundreds of years. Quantum computations are the basic innovation, since the invention of a microprocessor and quantum computers gives vast advantages as compared with the digital electronic computers on the basis of transistors. Quantum computers operate much faster and are more powerful than the modern ordinary computers. The former are else on the stage of development. However, several military agencies and national governments are ﬁnancing the studies on quantum computations aimed at the development of quantum computers for business, civil population, and safety purposes. The fabrication of a quantum computer as a real physical device is a fundamental problem of the physics of the 21st century. As of the beginning of 2020, only limited versions of a quantum computer are produced (the largest developed quantum registers have several tens of coupled qubits). Of course, the huge number of very complex theoretical and practical problems should be solved on the way to the practical realization of quantum computers. Till now, some versions of a construction of quantum computers are proposed on the basis of quantum points and superconducting junctions. Moreover, several commercial companies have declared the creation of real processors on the basis of superconducting qubits used, for example, in a computer “Orion” (Fig. 5.37). It includes a microchip with 16 qubits. Each qubit is composed of niobium particles surrounded by solenoids. In essence, “Orion” is an analog computer that solves the problems by the method of physical modeling. Such computer is suitable for the calculations

Fig. 5.37.

Photo of a 16-qubit processor “Orion”.

page 249

March 24, 2021

250

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

within complicated models (ﬁnancial, chemical, pharmaceutical, etc. ones) consuming much computer time. Among the principal tasks in the creation of a quantum computer, it is worth to mention the use of as many as possible number of qubits and its design. However, we should make a reservation about the existence of the problems related to the ambiguity of the interpretation of information. Therefore, the scientiﬁc society considers the declarations about the creation of quantum computers with prejudice.

5.8.4.1. D-wave quantum computer In 2011, the Canadian ﬁrm D-wave created the ﬁrst commercial quantum computer D-Wave-1 (DW-1) with 128 qubits and sold it for 10 mln dollars. It was purchased by the largest corporation Lockheed Martin of the militaryindustrial complex of the USA. The purpose, principle of operation, and architecture of DW-1 are based on the above-mentioned superconducting qubits. Unusual are the macroscopically large qubits in the register of this quantum computer that use the Josephson superconducting junctions. We now consider the operation of superconducting qubits in a quantum analog computer applying the physical mechanism of the phenomenon of superconductivity and the principles of functioning of Josephson junctions. At super-low temperatures of one or several Kelvins, the electrons in a superconducting metal are coupled due to the electron–phonon interaction and form the so-called Cooper pairs that are bosons with the zero spin, zero momentum, and charge −2e. As a result of the interaction of bosons with one another, the correlations appear between them. Moreover, at a deﬁnite critical temperature, the phase transition into the state of superconductivity occurs. In this case, there appears a gap in the electron energy spectrum, namely, the forbidden zone E in width. Above the gap, the one-electron energy levels are placed. The bosons not obeying the Pauli principle transit into a single quantum state with the energy lying below the gap bottom. Such correlated state of the gas of bosons that are in one quantum state is called the Bose-condensate. The Bose-condensate as a whole in the superconductor √ is described by a single complex wavefunction Ψ = n eiψ with a phase ﬁxed for the entire condensate, i.e., it behaves itself as one quantum particle. The formation of such coherent state of the ensemble of many particles in a lengthy specimen with macroscopic sizes is one of the examples of phenomena of macroscopic quantum physics.

page 250

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

251

For niobium and aluminium that are most frequently used in superconductors, the critical temperatures of the superconducting phase transitions Tc are equal, respectively, to 9.3 and 1.2 K. A Josephson qubit in the quantum computer DW-1 is a ring with a characteristic size of about one micron. It is produced of a superconducting metal, niobium, with two thin dielectric spacers. The ring is cooled down to a temperature of several milli-Kelvin. The quantum register of a computer including n qubits is described by the Hamiltonian H=

n i=1

hi σzi +

n i=1

Δi σxi +

Jij σzi σzj ,

(5.163)

i,j

where hi ∼ (Φi −Φ0 /2) is a shift of the controlling magnetic ﬂow through the contour of the ith qubit from the central value, Δi is the tunneling energy determining the frequency ω0i of the transition between the ground and excited levels of the ith qubit: ω0i ∼ Δi . The constant of interaction of the ith and jth qubits Jij is proportional to the mutual inductance of these qubits. The parameters of Hamiltonian (5.163) modeling a quantum computer can be controlled and be changed selectively and directedly according to the algorithm of solution of the problem. As a result, we get a macroscopic magnetic qubit. As a computational basis for it, we can use the spin or energy representation with regard for the solved problem. The quantum analog computer DW-1 has already successfully applied to the solution of a number of problems of the optimization and pattern recognition. We may assume its wide use in the control over the databases, analysis and forecasting of ﬁnancial risks, and other problems. The very form of Hamiltonian (5.163) presents a possibility to solve a wide spectrum of problems in the physics of ferromagnetism (Jij 0), as well as in the description of other physical systems whose Hamiltonians can be eﬃciently reduced to the form (5.163). The Josephson qubit is an experimentally realized object of the macroscopic quantum physics: its size is more than the size of an atomic qubit by about 10,000 times! The description of the realization of phenomena of the macroscopic quantum physics by a quantum computer can be found, for example, in [298, 299].

page 251

March 24, 2021

252

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Quantum computers are so powerful, because we have qubits of the highest quality with the lowest level of errors. Such computers demonstrate the combination of the use of identical completely coupled qubits and the exact control. The scientists are close to the great breakthrough in the design of largescale quantum computers. However, the creation of highly eﬃcient useful quantum computers is hampered by the problem of noises in them. In brief, this is a result of errors introduced by a quantum computer itself at the manipulation by qubits. Noises become a heavier problem, as the number of qubits and the size of a computer system increase. This means that the mentioned problem sets a particular obstacle for the development of those types of large quantum computers which would be the basis for new revolutionary technologies in the future. Potentially, the quantum computers can change many technologies, by allowing one to solve the problems unsolvable with available classical computers. But the former should be made noiseless to be reliable.

5.8.4.2. Quantum advantage of Google Since the quantum computers will be able to make calculations that are too hard for ordinary computers, the humanity will attain the quantum advantage. This event promises us to enter the truly revolutionary period in all spheres of our life. For example, quantum computers will help us to produce fantastic composites for new transport means, to design a new generation of electronic devices, and to change the digital systems. Recently, the company Google informed that its quantum processor Sycamore executed calculations for 3 min and 20 sec, whereas the classical supercomputer would make such work for 10 thou years. The processor Sycamore was fabricated from aluminium, indium (very soft metal), and silicon with the use of the Josephson eﬀect, when the superconduction current ﬂows through the junctions of two superconductors. In order to reach the state with superconductivity, the processor with the qubits that are minimal units of information in a quantum computer was cooled down to a temperature close to the absolute zero (20 milli-Kelvin), which is equal approximately to minus 273 Celsius degrees. With the help of the so-called attenuators (units that decrease the intensity of electromagnetic oscillations) and the additional ﬁlters, the supercooled Sycamore was connected with an ordinary electronics operating at room temperature. To read-oﬀ the information from the quantum computer became possible due to analog–digital transducers. The whole

page 252

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

253

system supports the quantum state of qubits and was able to prove the “randomness of numbers that were created by a generator of random numbers” for about 3 min. But the declaration about the advantage of quantum computers was answered at once by the experts of the IBM company which is the main competitor of Google in the ﬁeld of quantum computers. They elucidated that the calculations executed with the quantum processor Google Sycamore bear only a technical character, and the IBM supercomputer Summit can make the same for only two-three days. Apparently, the single laboratory experiment with the realization of a very speciﬁc processing procedure for a random sample outside any practical application gives no basis for the assertion that the quantum computers “exceed” the classical ones. In fact, the quantum computers will not “dominate”, but should operate in a tandem with ordinary computers, since each type of computers has the own unique advantages. It is expected that the growth of investments to quantum technologies and the increase in the demand for highly eﬃcient computations for the analysis of data will ensure the fast development in this ﬁeld in the nearest years. In addition, the appearance of local quantum computers for commercial applications will create the advantageous perspectives for the market of corporate quantum computations. At the present time, a new quantum Internet is developed. The quantum Internet that will join quantum computers able to solve the problems with incredible complexity, by ensuring the rapid information ﬂow and opening the completely new trends for scientiﬁc studies and the economic growth.

5.8.5. Topological quantum computers We now discuss brieﬂy the idea of a topological quantum computer presented in Fig. 5.38. Topological quantum calculations tend to realize a more elastic qubit, by using the non-Abelian forms of the matter for the storage of a quantum information. The non-Abelian forms of the matter are quasiparticles such as Majorana fermions and anyons (non-Abelian quasiparticles that are neither bosons, nor fermions). The most promising topological developments in the ﬁeld of quantum calculations are related to the non-Abelian braiding of chiral Majorana fermions at quantum points. The type of anyons which is necessary to create a universal quantum computer was not yet conﬁrmed experimentally (only some preliminary signs are available). Till now, this model of quantum calculations bears a purely theoretical character.

page 253

March 24, 2021

254

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.38.

Photo of a topological quantum computer.

We recall that topology is a branch of mathematics concerning those properties of a body that are invariable at its deformations such as the tension or ﬂattening. The topological properties are most stable. In order to break them, the much higher energy must be applied to the body, than in other cases. By intuition, the idea is clear: at any deformations of the body, its topology is invariant. A torus can be transformed into a cup, but the topology remains the same. As distinct from the ordinary digital computers operating on the basis of transistors, where the data are coded in binary digits (bits), the quantum computers use quantum bits. Those qubits can exist in a lot of states simultaneously, which gives potential for the execution of a huge number of simultaneous calculations in parallel, which signiﬁcantly reduces the time of searching for the answer. Since we need a more profound comprehension of the nature of a qubit as the base of quantum computers, it is useful to separate three signiﬁcant aspects in the operation of this element: 1. Superposition of states. A qubit has the wave nature, i.e., the smooth changes in its state are described by a wave function. If the maximum and minimum of a wave are described as 1 and 0, respectively, then a qubit stays permanently in these extreme and all intermediate states of the wave described by a phase, but with diﬀerent probabilities. 2. Interference of qubits. The interaction in a set of waves from diﬀerent sources generates the interference pattern. By adjusting the phases of

page 254

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

255

the sources of waves, such patterns can be made stable. In the quantum computer, namely such pattern with a beforehand known required form signalizes that the answer to a computational problem is obtained. The essence of algorithms for quantum calculations consists in the following. By ﬁne non-destructive actions onto qubits, their jointly consistent oscillations should be directed to the generation of a required interference pattern. 3. Entanglement of qubits. In order that the superpositions of a set of qubits in a quantum computer behave themselves as a unique coordinated system called a coherent one, the qubits should stay in the state of quantum entanglement with one another. To attain a coherent state for even several individual qubits is a highly complicated technical problem, because the quantum entanglement of particles under laboratory conditions is extremely brittle with a short life. As a rule, the coherence of a system is at once broken by a lowest electromagnetic “noise” and any other random actions of the environment at least on one of the qubits. Since the number of qubits in a useful computer is hundreds and thousands, it is obvious that the expected time of the appearance of such computing units on the market moves further and further into the future, until some revolutionarily new device appears. The researchers at the Delft Technical University under the support of the company Intel managed to construct a qubit that is stable to a highest degree and can form the states that are stable against the noises and are tangled with other qubits. This qubit was produced on the basis of Majorana fermion quasiparticles, and, on its basis, Aleksei Kitaev invented a “topological quantum computer”, by advancing a completely new conception of a quantum computing unit stable to distortions and noises from the environment. A. Kitaev made conclusion that the quantum calculations of states can be executed on quantum braids that are intertwined from ﬁlaments-trajectories. We now describe brieﬂy a Majorana fermion and the ideas by Kitaev.

5.8.5.1. Majorana fermion A Majorana fermion is a particle that is identical to the own antiparticle. In other words, a Majorana fermion is produced from a superposition of an electron and a hole. Moreover, this superposition is formed at the boundaries of a semiconductor and a superconductor (Fig. 5.39).

page 255

March 24, 2021

256

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

Fig. 5.39. On the left, a InSb wire put on the NbTiN superconductor in a magnetic ﬁeld is shown. On the ends of the wire and the chain, Majorana fermions are localized. Taken from [303].

The key speciﬁc feature of a Majorana fermion is in that it obeys a non-Abelian statistics. As a result, it can be used in quantum calculations. We now give the basic positions of the Majorana theory. From the mathematical viewpoint, the operator of annihilation of Majorana fermions γi is deﬁned as [300] γi† = γi ,

{γi , γj } = 2δij .

(5.164)

Generally speaking, any Dirac fermion ck (for the Dirac fermion we take the standard deﬁnition of a fermion operator) can be represented in terms of the Majorana operators 1 c = √ (γi + iγj ) , 2 1 c† = √ (γi − iγj ) , 2

(5.165)

{ci , c†j } = δij , {ci , cj } = 0. The key thing consists in the following. If the Majorana fermions are spatially separated, then the obtained Dirac fermion is also spatially nonlocal. In this case, its energy determined by the overlapping of the wave functions of spatially separated Majorana fermions is exponentially low [301] Hn = n c†n cn ,

n ∝ e−L/ξ ,

(5.166)

where L is the distance between Majorana fermions, and ξ is a characteristic scale of the spatial coherence. We will consider that the Majorana fermions

page 256

March 24, 2021

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Nanoscale Superconductivity

257

are well deﬁned, if L ξ. In this case, any local perturbations aﬀect exponentially weakly the state determined by two Majorana fermions. A Majorana fermion is a topological state protected by the electron–hole conjugation symmetry. This symmetry is analogous to the C symmetry in the physics of elementary particles [300]: ΞH(k)Ξ = −H(−k),

Ξ2 = −1,

(5.167)

if Hψn = n ψn , Ξψn = ψ−n ,

(5.168)

n = − −n . The above presented relations mean that, for every state with energy > 0, there exists a state with energy − > 0. But if = 0, then the operator of electron–hole symmetry transforms the state into itself: ΞψMF = ψMF ,

HψMF = 0.

(5.169)

The given state is a Majorana fermion. In a realization of Majorana fermions crucial is the electron–hole conjugation symmetry. This symmetry arises in the Bogolyubov–de Gennes equations describing the supercondictivity [300]. In this case, the operator of electron–hole conjugation is set as Ξ = σy τy K, where the Pauli matrix σi acts in the space of spins, τi acts in the electron–hole basis and K is the operator of complex conjugation. However, the presence of only the superconductivity is not suﬃcient for a realization of spatially separated Majorana fermions. For this purpose, it is necessary to remove all types of generation. As was mentioned above, a Majorana fermion is a topological state. To realize it, we need a nontrivial topology of the zone structure. It is known that the strong spin–orbit interaction in many materials leads to a nontrivial topology. So, it is logical to consider such materials. For the realization of spatially separated fermions the following conditions should be satisﬁed: supercondictivity + magnetic ﬁeld + nontrivial topology. The simplest way to the joining of all three conditions is given by the triplet superconduction parameter of order. It corresponds to the pairing of electrons with identical spins. If we produce a one-dimensional chain of superconductors with the triplet pairing, Majorana fermions will be localized on its ends. In the real superconductors, the spin degree of freedom is always present. In addition, the triplet parameter of order is suﬃciently rare in the Nature. One of the candidates is strontium ruthenate Sr2 RuO4 .

page 257

March 24, 2021

258

20:13

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-ch05

Modern Aspects of Superconductivity: Theory of Superconductivity

5.8.5.2. Kitaev’s superconducting chain Consider brieﬂy the Kitaev one-dimensional model describing a spinless pwave superconductor. Its Hamiltonian was given in [302, 303]: H = −μ

L j=1

c†j cj

−

L−1

(tp c†j cj+1 + Δc†j c†j+1 + h.c.),

(5.170)

j=1

where h.c. means the Hermitian conjugation, μ is the chemical potential cj is the electron annihilation operator at node j, and L is the chain length. The tunneling tp and the superconductor gap Δ = |Δ| eiα are the same for all nodes. For the sake of simplicity without any loss of generality, we take Δ = |Δ|. The Kitaev system can be realized experimentally by means of the contact of a nanowire with strong spin–orbit coupling (e.g., InSb and InAs nanowires, Fig. 5.39) with an s-wave superconductor in the Zeeman ﬁeld [300]. For clarity, in this work we focus on the condition μ = 0, tp = Δ [301]. By concluding, we note that the quantum computers represent a technological trend that can change potentially the world of highly eﬃcient calculations. This causes a huge interest of the scientiﬁc community and the signiﬁcant volume of investments to their development. At the present time, about ten diﬀerent experimental models of quantum units are available. Each unit can include up to several tens of quantum objects. Such models are characterized by diﬀerent levels of their development, but none of the models allows one to solve practical problems. In the future, the quantum computers will be claimed in all ﬁelds of the human activity requiring great volumes of calculations, so that it will be impossible to operate without quantum technologies.

page 258

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-sum

Summary and Conclusions

In this book, we have concentrated our attention on the most urgent problems of superconductivity such as the nature of high-temperature superconductivity, mechanisms and symmetry of pairing, two-gap superconductivity in magnesium diborades, mesoscopic superconductivity and the problems of room-temperature superconductivity. We considered some questions concerning the application of quantum ﬁeld theory to the problems of superconductivity. Quantum ﬁeld theory supplies the original and powerful means for the solution of certain problems of superconductivity. In the ﬁeld of superconductivity we meet the problem-maximum — it consists in the creation of room-temperature superconductors. We consider this problem in our book, give some recommendations on the search for these superconductors and analyze the possibility of the fabrication of artiﬁcial materials possessing the property of superconductivity at room temperature. The problem of high-temperature superconductivity in hydrides at high pressures is considered. We also have touched the questions of the application of superconducting qubits to quantum computers. It is shown that the description of superconducting qubits is based on the laws of quantum mechanics. We give a short review of the modern state of the problem of physical realization of quantum computers. The ideas of a topological quantum computer using qubits on the basis of Majorana fermion quasiparticles are considered. It is worth noting that HTSC is investigated more than two decades with great eﬀorts, but the whole pattern of the phenomenon is not else available. We are sure that the comprehension of HTSC will be attained when our knowledge of HTSC reaches the critical level which will be suﬃcient to understand the huge number of experimental data from a single viewpoint. The study is in progress. In particular, we mention the recent discovery

259

page 259

March 24, 2021

260

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-sum

Modern Aspects of Superconductivity: Theory of Superconductivity

of Cu-less superconductors with a high critical temperature which contain layers of FeAs. The physical properties and electron models of the high-temperature Fe-based superconductors are analyzed. The theoretical and experimental investigations of superconductivity and their practical applications at the present time form the wide, interesting and uncommon branch of science.

page 260

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appa

Appendix A

A.1. Two-particle Green Function for Multiband Superconductors In this appendix, we will solve the problem on determination of two-particle Green function for multiband superconductors. In Chapter 4, we considered the multiband superconductivity using a two-particle Green function. We will calculate a two-particle Green function for many-band superconductors. The Hamiltonian describing the systems of interacting electrons and phonons of a crystal is written in the following form: 1 ν2 ν2 ν1 ν 1 ενk a+ν a + Vq a+ν H= k1 σ1 ak2 σ2 ak2 +q,σ2 ak1 −q,σ1 kσ kσ N k,a,ν

1 +√ N

q,k1 ,σ1 ,ν1 ,k2 ,σ2 ,ν2

ν s χsq a+ν k,σ ak−q,σ Qq +

s Ωqs b+s q bq ,

(A.1)

q,s

k,σ,ν,q,s

where a+v kσ is the creation operator for the electron with the momentum k in band ν, avkσ is the annihilation operator for the electron with the momentum s k in band ν, b+s q , bq are creation and annihilation operators for the phonons with the momentum q, respectively, εvk is the energy of the electron with the s impulse k, Ωqs is the energy of the phonons, Qsq =b+s q +bq , s is the number ∗s s of phonon branch, V q = Vq , Xq = Xq are the Fourier components of the Coulomb interactions of electron and their coupling constant with the lattice phonons, respectively. We can see that both constants are independent on spin index of an electron. Let us introduce new operators for electron and phonon systems by rules avk = eS Ak,v e−S ,

bsq = eS βs,q e−S

where S is the anti-Hermitian operator (S + = −S).

261

(A.2)

page 261

March 24, 2021

262

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appa

Modern Aspects of Superconductivity: Theory of Superconductivity

In our unitary transformation, it will be more convenient to rewrite the term He–ph in the following form:

He–ph =

+v μ s χv,μ s,q ak ak−q Qq

s (χv,μ s,q = χq δv,μ ),

(A.3)

k,q,s,v,μ

where we united two indices and so ν = (ν, σ) and μ = (μ, σ ) are the complex indices which characterize the number of crystals electron zone and the spin of electron. The Hamiltonian describing the system of interacting electrons and phonons of the crystal after transformation by a unitary operator is written in the following form [139–143]:

H=

k,v

1 + 2N +

χsq 2 1 εvk − A+ k,v Ak,v N s,q Ωs,q q,k,v,k ,v

Vq − 2

χsq 2 s

Ωs,q

+ A+ k,v Ak ,v Ak −q,v Ak−q,v

+ Ωs,q βs,q βs,q + (higher order term).

(A.4)

s,q

The unitary transformation gives rise to renormalization of the electron energy (ﬁrst term) and renormalization of the Fourier component of the Coulomb electron–electron interaction. To calculate the density of electron states, we have to study the Green function for the case with approximation t → t − 0. The two-particle Green function can be written as follows: G2

t − t k + q, v; k2 − q, v2 k2 , v2 ; k, v

+ = −iT Ak+q,v (t)Ak2 −q,v2 (t)A+ k2 ,v2 (t − 0)Ak,v (t )(t → t − 0).

(A.5)

The equation for the Green function can be found from the motion of equation: i

∂ −iT Ak,v (t) A+ t k,v ∂t

∂ + Ak,v (t) Ak,v t , = δ t − t + −iT ∂t

(A.6)

page 262

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appa

Appendix A

263

where i

∂Ak,v = [Ak,v .H] = −iT Ak,v (t) A+ t = −iT Ak,v (t) A+ t k,v k,v ∂t 1 ˜ + Vq Ak2 ,v2 Ak2 +q,v2 Ak−q,v = ε˜vk Ak,v + N q,k2 ,v2

= ε˜k,v Ak,v −

1 ˜ Vq Ak+q,v Ak2 −q,v2 A+ k2 ,v2 , N

(A.7)

q,k2 ,v2

where ε˜vk

ε˜k,v

2 1 χsq = − , N s,q Ωs,q 1 = ε˜vk + V˜q . V˜q=0 − n N v q εvk

(A.8)

(A.9)

2

Therefore, the equation for the Green function (A.6) is transformed after inserting in it (A.7) to the following form: i

∂ −iT Ak,v (t) A+ t k,v ∂t = δ t − t + ε˜k,v −iT Ak,v (t) A+ k,v t 1 ˜ (t − 0) A+ Vq −iT Ak+q,v (t) Ak2 −q,v2 (t) A+ t . − k k,v ,v 2 2 N q,k2 ,v2

(A.10) Such two-particle Green function satisﬁes the equation of the Bethe–Salpeter type (we not split this function into two one-particle Green functions of the Gorkov type). The solution of this equation according to the Bogoliubov– Tyablikov method gives rise to the following expression for the Fourier component of the two-particle Green function:

f (k1 , μ; k2 , ν; ω) σ,σ ϕ (μ, ν; σ, σ ) k2 , ν; k1 , μ ω ∼ , G2 k1 + q, μ; k2 − q, ν 1 − V K(k1 , μ; k2 , ν; ω) (A.11) where μ ν 1 1 − nk1 +q − nk2 +q , K(k1 , μ; k2 , ν; ω) = N q ω − εk1 +q,μ − εk2 +q,ν

(A.12)

page 263

March 24, 2021

20:14

264

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appa

Modern Aspects of Superconductivity: Theory of Superconductivity

where V is the Fourier of the Coulomb interactions of electron, ϕ (μ, ν; σ, σ ) are some functions depending on the frequency ω, and momenta k1 and k2 of interacting electrons, f (k1 , μ; k2 , ν; ω) are expressed in terms of functions, nμk +q , εk1 +q,μ are numbers of ﬁlling and energy of electron, respectively, 1

ϕ μ, ν; σ, σ = δσσ δσ σ − δμν δσσ δσσ ,

(A.13)

and σ, σ are the spins of the ﬁrst (σ) and second (σ ) electrons. The superconducting gap is given by the zeros of the denominator of (A.11) [140,143]. Let us study the particular case supposing k1 = k2 = k0 + k and εk0,μ = εμ corresponds to the extremum of the zone. Then, expanding the energy by momentum k ± q in series up to terms of second order, we can obtain: εk±q,μ = εμ +

(k ± q)2 (k ± q)2 = εf + Δμ + , 2mμ 2mμ

(μ = 1, 2, . . .),

(A.14)

where mμ is the eﬀective mass of electron in the μ-energy band of the crystal, Δμ is a parameter which indicates the position of the extremum of μ band relative to the Fermi level, εk±q,μ is the energy of electrons. The sum in the denominator (A.11) is reduced to the following expression (we consider only one zone): 1 1 − nk+q − nk−q K k, k , ω = N q ω − εk+q − εk−q

Δ

dε 0 ω − 2 (εf + Δ1 ) − 2E − 2ε

Δ = 2N (εf ) − ln 1 − , a = 2N (εf )

(A.15)

where such assignments were used: ε = q 2 /2m; E = k2 /2m; a = ω − 2(εf + Δ1 ) − 2E; m∗1 = m1 /m and m are the reduced eﬀective mass of electron in the crystal energy zone and mass of free electron, respectively, √ (A.16) N (εf ) = 2π m∗1 m∗1 ε (1 − nk+q − nk−q ) εf ,

−1 εk − εf +1 . (A.17) nk = exp T The equation for superconducting gap has the following form:

Δ 1 − V N (εf ) − ln 1 − = 0. a

(A.18)

page 264

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appa

Appendix A (a)

(b)

265

(c)

Fig. A.1. The eﬀect of temperature on the K(k, μ; k, ν; ω) function (E = k2 /2m = 0) for diﬀerent structures of the energy zones: (a) Δ1 = −1, m∗1 = 1; (b) Δ2 = 0.2, m∗2 = −2; (c) Δ1 = −1, m∗1 = 1, Δ2 = 0.2, m∗2 = −2; curves 4, T = 2 K; curves 3, T = 10 K; curves 2, T = 50 K; curves 1, T = 100 K; arrows 5–7 correspond to diﬀerent 1/V values (arrow 5, V = −0.07; arrow 6, V = −0.06; arrow 7, V = −0.05). All energy values are taken as arbitrary values, i.e., V = V /M , where M is a scale factor (M = 1 eV, for convenience; i , m is the free electron mass). m∗i = m m

Fig. A.2. The temperature dependence of the superconducting gap: · · · theory, — BCS; • a-axis, b-axis-experiment.

The results of some numerical calculations are illustrated in Fig. A.1. We will study theoretically the situation close to the Ba2 Sr2 CaCu2 O8 crystal because it has a high Tc . The results of some numerical calculations of the temperature dependence of superconductivity are illustrated in Fig. A.2. For illustration, the experimental dependences of the superconducting gap

page 265

March 24, 2021

266

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appa

Modern Aspects of Superconductivity: Theory of Superconductivity

obtained for Ba2 Sr2 CaCu2 O8 crystal are presented in Fig. A.2 together with theoretical curves of BCS type and our calculation. The obtained dependences are not similar to standard BCS ones. It clearly seen that our r calculation predicting the maximum in the T dependence of the superconducting gap gives the curve which is closer to the experimental results. In our approach, we take into account that all electron bands (the numerical calculations show that only bands located near the Fermi are important) contribute to the superconductivity.

page 266

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appb

Appendix B

B.1. A Solution Method for the Ferromagnetic Granules in the London Superconductors In this appendix, we will solve the problem on determination of magnetic conﬁgurations in superconducting nanocomposite systems by means of Maxwell equation, which in a static case has the following form: ∇ × B = μ0 j,

(B.1)

where B is a magnetic ﬁeld and j is a speciﬁc electric current. The value j includes normal and superconducting parts. The role of normal currents in superconductors in the process of formation of magnetic ﬁelds is negligible since a superconductor substance exhibits weak magnetic characteristics in the normal state. However, ferromagnetic inclusions enter into the superconducting nanocomposites and the consideration of a normal current for these inclusions is necessarily required. Therefore, it may be supposed that j = jsp + jn .

(B.2)

The current of superconductivity can be locally connected with the vector potential of system, which allows us to write: ns e2 B. (B.3) m A speciﬁc current of charge carriers in the normal state can be written in the traditional form: ∇ × js = −

jn = ∇ × M,

(B.4)

where M is a magnetization of material. As a result, the term in (B.2) for the normal current is characterized only for the region ﬁlled by ferromagnetic material. 267

page 267

March 24, 2021

268

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appb

Modern Aspects of Superconductivity: Theory of Superconductivity

Combining relations (B.2), (B.3), (B.4) with the Maxwell equation ∇ × B = μ0 j the magnetic ﬁeld can be found in the form: ∇ × (∇ × B) + λ−2 B = μ0 ∇ × (∇ × M),

(B.5)

where λ is the London penetration depth of ﬁeld in the superconductor. Since ∇B = 0, using relations (B.1), (B.3), (B.4), the equation for magnetic ﬁeld can be presented in the form: ∇ × (∇ × B) + λ−2 B = μ0 ∇ × (∇ × M),

(B.6)

where δ = c2 Λ/4π is a London depth of ﬁeld penetration in the superconductor. If the condition ∇B = 0 is satisﬁed without ferromagnetic inclusions, then Eq. (B.5) can be transformed to ∇ × (∇ × B) + λ−2 B = μ0 ∇ × (∇ × M).

(B.7)

For boundary conditions, we assume that the magnetic ﬁeld vanishes outside of the localization region of ferromagnetic inclusions. According to these boundary conditions, the solution of Eq. (B.7) can be presented as follows: μ0 B (r) = 4π

d3 r G r − r ∇ × (∇ × M r ),

(B.8)

where the Green’s function is given by exp (− |r − r | /λ) . G r − r = |r − r | Sizes of quantum dots, the ﬁeld of which to be studied, are much less than the penetration depth λ. Henceforward, we consider magnetic moments as dotty magnetic dipole ones, supposing that M (r) =

mi δ (r − ri ),

(B.9)

i

where δ (r − ri ) is delta-function of Dirac, mi and is a magnetic moment of the ith granule. In this case, the integrand in (B.7) holds the space derivatives from singular values. Let us transform (B.9) in such a way as to diﬀerentiate the kernel of integrand. For this

purpose, we present the expression for the magnetic ∂ ) + rot M (r ) ∂ rot M (r · G (|r − r |), and, ﬁeld as H (r) = dv ∂r ∂r

page 268

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appb

Appendix B

269

using the Gauss theorem, we rewrite the relation (B.9) as

∂ ∂ H (r) = dv rot M r + rot M r · G r − r . ∂r ∂r (B.10) The integration in the ﬁrst term over the inﬁnite surface vanishes. Then, integrating by parts in the second term of (B.10), we obtain

H (r) = dS · rot M r · G r − r +

dv

∂ G r − r , rot M r ∂r 2

2

(B.11)

2

∂ ∂ ∂ ∂ ∂ ∂ +ey ∂y +ez ∂z , Δ = ∂x where ∇ = ex ∂x 2 + ∂y 2 + ∂z 2 − is the Laplace operator. In Eq. (B.11), the diﬀerentiation operators act no longer upon generalized functions but on the kernel of the integral operator. Taking into account that the relation (B.12) ΔG − δ−2 G = −4πδ r − r ,

holds for the Green function G (|r − r |), Eq. (B.11) is transformed to

3R (R · M (r )) M (r ) R R2 − · 1+ + 2 H (r) = dv exp(−R/δ) · R5 R3 δ δ 2R (R · M (r )) , − δ 2 · R3 (B.13) R = r − r , R = r − r . The expression (B.13) determines the magnetic ﬁeld out of ferromagnetic inclusions. Since the magnetization of system M (r) is deﬁned by (B.8), in (B.13) that, out of the volume of granules, it is considered dv M (r ) δ (r − r ) = 0. After integrating (B.13), we get the expression for magnetic ﬁeld in the form of superposition of parts of quantum dots:

3Ri (Ri · mi ) mi Ri Ri2 + 2 exp(−Ri /δ) · − 3 · 1+ H(r) = δ δ Ri5 Ri i

2Ri (Ri · mi ) − δ2 · Ri3 Ri = r − ri ,

,

Ri = |r − ri | .

(B.14)

page 269

March 24, 2021

270

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-appb

Modern Aspects of Superconductivity: Theory of Superconductivity

It has been apparent, when the temperature of superconductor and the depth penetration of magnetic ﬁeld λ → ∞ increase in the region adjacent to the ensemble of granules, then expression (B.14) tends to the limit μ0 3Ri (Ri · mi ) mi − 3 , (B.15) B (r) = 5 4π R R i i i which describes the magnetic ﬁeld of the system of dotty dipoles in the normal state medium. In the another limiting case, if the distance between granules is much more than the depth penetration, we have Ri (Ri · mi ) μ0 exp(−Ri /λ) · − mi . (B.16) B (r) = 4π Ri · λ2 Ri2 i

page 270

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

[1] Parks, R.D. (ed.) (1969). Superconductivity (Marcel-Dekker, New York). [2] Bednorz, J.G. and M¨ uller, K.A. (1986). Possible high-Tc superconductivity in the Ba–La–Cu–O System, Zeit. Phys. B 64, 1, pp. 189–193. [3] Schrieﬀer, J.R. (1983). Theory of superconductivity (Benjamin, New York). [4] Feynman, R.P. (1982). Statistical mechanics (Addison-Wesley, Redwood City). [5] Anderson, P.W.(1987). The resonating valence bond state in LaCuO and superconductivity, Science 4, pp. 1196–1198. [6] Anderson, P.W. (1959). Theory of dirty superconductivity, J. Phys. Chem. Solids 11, pp. 26–30. [7] London, F. and London, H. (1935). The electromagnetic equations of the supraconductor, Proc. Roy. Soc. (London) A 147, p. 71. [8] Ryder, L.H. (1996). Quantum ﬁeld theory, 2nd edn. (Cambridge University Press, Cambridge). [9] Ginzburg, V.L. and Landau, L.D. (1950). On the theory of superconductivity, Zh. Eksp. Theor. Fiz. 20, p. 11064. [10] Clark, K. et al. (2010). Superconductivity in just four pairs of (BETS)2 GaCl4 molecules, Nat. Nanotechnol. 5, p.261. [11] Tinkam, M. (1975). Introduction to superconductivity (McGraw-Hill, New York). [12] Nambu, Y. (1960). Quasi-particles and gauge invariance in the theory of superconductivity, Phys. Rev. 117, p. 648. [13] Takahashi, Y. (1976). Field theory for the solid state physics (Baifuhkan, in Japanese). [14] Nagao, H., Nishino,H., Shigeta Y. and Yamaguchi, K. (2000). Theoretical studies on anomalous phases of photodoped systems in two-band model, J. Chem. Phys. 113, pp. 11237–1244. [15] Kondo, J. (2002). Theory of multiband superconductivity, J. Phys. Soc. Jpn. 71, p. 1353. [16] Fetter, L.A. and Walecka, J.D. (1987). Quantum theory of many-particle systems (McGraw-Hill). [17] Abrikosov, A.A., Gorkov, L.P. and Dzyaloshinski, I.E. (1975). Methods of quantum ﬁeld theory in statistical physics (Dover Books). [18] Aono, S. (2003). Molecular orbital theory: spinor representation, J. Phys. Soc, Jpn. 72, pp. 3097–3105. 271

page 271

March 25, 2021

10:14

272

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[19] Kimura, M., Kawabe, H., Nishikawa, K. and Aono, S. (1986). EPR observations of trivalent titanium in orthophosphate single crystals, J. Chem. Phys. 85, pp. 1–6. [20] Salem, L. and Longuet-Higgins, H.C. (1959). The alternation of bond lengths in long conjugated chain molecules, Proc. Roy. Soc. London A 255, p. 172. [21] Peierls, R.E. (1955). Quantum theory of solids (Oxford University Press, Oxford). [22] Kimura, M., Kawabe, H., Nakajima, A., Nishikawa, K. and Aono, S. (1988). Possibility of superconducting and other phases in organic high polymers of polyacene carbon skeletons, Bull. Chem. Soc. Jpn. 61, pp. 4239–4224. [23] Kubo R. and Tomita, J. (1954). A general theory of magnetic resonance absorption, Phys. Soc. Japan 9, pp. 888–919. [24] Doi, Y. and Aono, S. (1974). Theory of line shape in nuclear magnetic resonance, Prog. Theoret. Phys. 51, pp. 1019–1029. [25] Hebel, L.C. and Slichter, C.P. (1959). Nuclear spin relaxation in normal and superconducting aluminum, Phys. Rev. 113, pp. 1504–1519. [26] Fibich, M. (1965). Phonon eﬀects on nuclear spin relaxation in superconductors, Phys. Rev. Lett. 14, pp. 561–564. [27] Maki, K. (1967). Gapless superconductors in superconductivity (ed.) Parks, R.D. (Maxel Dekker). [28] Uchino, K., Maeda, A. and Terasaki, I. (1959). Nature of the high temperature superconductor (Baifuukann, in Japanese). [29] Aono, S. (1998). Superconductivity as symmetry breaking classical treatment, Bull. Chem. Soc. Jpn. 71, pp. 49–56. [30] Scalapino, D.J. (1995). The case for dx2 −y2 pairing in the cuprate superconductors, Phys. Rep. 250, pp. 329–360. [31] Gorkov, L.P. (1959). Microscopic derivation of the Ginzburg-Landau equations in the theory of superconductivity, Sov. Phys. JETP 9, pp. 1364–1375. [32] Negele, J.W. and Orland, H. (1987). Quamtum many-particle systems (Addison-Wesley, Reading, MA). [33] Kawabe, H., Nishikawa, K. and Aono, S. (1994). Path integral approach to correlation energy, Int. J. Quantum Chem. 51, pp. 265–283. [34] Kruchinin, S. (2016). The quantum-ﬁeld approach to superconductivity theory, Rev. Theoret. Sci. 4, 2, pp. 117–144. [35] Feynman, R.P. (1948). Space-time approach to non-relativistic quantum mechanics, Rev. Mod. Phys. 20, pp. 367–387. [36] Hubbard, J. (1959). Calculation of partition functions, Phys. Rev. Lett. 3, pp. 77–78. [37] Das, A. (2006). Field theory: a path integral approach (World Scientiﬁc, Singapore). [38] DeWitt, B. (1984) Supermanifolds (Cambridge University Press, Cambridge). [39] Ferraz, A. and Nguyen, A.V. (1995). Supersymmetry and electron-hole excitations in semiconductors, Phys. Rev. B 51, pp. 10548–10555. [40] Yang, C.N. (1962). Concept of oﬀ-diagonal long-range order and the quantum phases of liquid He and of superconductors, Rev. Mod. Phys. 34, pp. 694–704.

page 272

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

273

[41] Dunne, L.J., Murrell, J.N. and Br¨andas, E.J. (1997). Oﬀ-diagonal long-range order, eta- pairing, and Friedel oscillations in high Tc cuprate superconductors and the ground state of the extended Hubbard model, Int. J. Quant. Chem. 63, pp. 675–684. [42] Ginzburg, V.L., Kirzhnitz, D.A. (1982) (eds). High-temperature superconductivity (Consultants Bureau, New York). [43] Fr¨ohlich H.(1954). On the theory of superconductivity, Proc. Roy. Soc. (London) A 223, pp. 296–305. [44] Bogolyubov, N.N. (1958). A new method in the theory of superconductivity, Zh. Eksp.Teor. Fiz. 34, pp. 58–65. [45] Josephson, B.D. (1974). The discovery of tunneling superconductivity, Rev. Mod. Phys. 1074, 46, pp. 251-254. [46] Maroushkine, A. (2004). Room-temperature superconductivity (Cambridge Int. Sci. Publ., Cambridge). [47] Davydov, A.S. (1990). High-temperature superconductivity (Naukova Dumka, Kiev). [48] Kruchinin, S.P. (2014). Physics of high-Tc superconductors, Rev. Theoret. Sci. 2, pp. 124–145. [49] Davydov, A.S. and Kruchinin, S.P. (1991). Interlayer eﬀects in the newest high-T superconductors, Physics C 179, pp. 461–468. [50] Davydov, A.S. and Kruchinin, S.P. (1991). Dependence of the superconducting transition temperature on the number of cuprate layers in a unit cell of high-temperature superconductors, Sov. J. Low. Temp. Phys. 17, 10, pp. 634–635. [51] Timusk, T. and Statt, B. (1999). The pseudogap in high-temperature superconductors: an experimental survey, Rep. Prog. Phys. 62, pp. 61–122. [52] Plakida, N.M. (1995). High-Tc superconductivity: experiment and theory (Springer), p. 306. [53] Brusov, P. (1999). Mechanisms of high temperature superconductivity (Rostov State University Publishing), p. 685. [54] Abrikosov, A.A. (1998). Fundamentals of the theory of metals (North-Holland, Amsterdam), p. 380 [55] Akhiezer, A.I., Pomeranchuk, I.Ya. (1959). On the interaction between conductivity electrons in ferromagnetics, Zh. Eksp. Teor. Fiz. 36, p. 819. [56] Akhiezer, A.I., Bar’yakhtar, V.G. and Peletminskii, S.V. (1968). Spin waves (North-Holland, Amsterdam), p. 369. [57] Little, W.A. (1964). Possibility of synthesizing on organic superconductivity, Phys. Rev. 134, p. 1416. [58] Alexandrov, A.S., Ranninger, J. (1981). Bipolaronic superconductivity, Phys. Rev. 23, 4, pp. 1796–1801. [59] Pekar, S.I. (1951). Studies on the electron theory of crystals (Gostekhizdat, Moscow), p. 168. [60] Lakhno, V. (2020). Translational-invariant bipolarons and superconductivity, Condens. Matter 5, 2, p.30. [61] Brusov, P. (1999). Mechanisms of high temperature superconductivity (Rostov State University Publishing, Rostov), p. 685.

page 273

March 25, 2021

10:14

274

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[62] Ausloos, M. and Kruchinin, S. (eds). (1999). Symmetry and pairing in superconductors. Proceedings of the NATO ARW (Kluwer Academic Publishers, Dordrecht), p. 410. [63] Annett, J. and Kruchinin, S.(eds.) (2002). New trends in superconductivity. Proceedings of a NATO ARW (Kluwer Academic Publishers, Dordrecht), p. 435. [64] Kruchinin, S. (eds.) (2003). Modern problems of superconductivity, Proceedings of Yalta conference, Mod. Phys. Lett. B 17, 10–12, pp. 393–724. [65] Sigrist, M. and Rice, T.M. (1995). Unusual paramagnetic phenomena in granular high-temperature superconductors — a consequence of d-wave pairing, Rev. Mod Phys. 67, 2, pp. 503–513. [66] Laughlin, R.B. (1998). Magnetic induction of dx2 +y2 + idxy order in high-Tc superconductors, Phys. Rev. Lett. 80, p. 5188. [67] Scalapino, D.J. (1999). The case for d pairing in the cuprate superconductors, Phys. Rep. 250, pp. 331–370. [68] Annet, J.F. (2003). Superconductivity, superﬂuids and condensates (University of Bristol, Oxford University Press), p. 183. [69] Volovik, G.E., Gorkov, L.P. (1985). Superconducting classes in heavy-fermion systems, Sov. Phys. JETP 61, p. 843. [70] Mineev, V.P. and Samokhin, K.V. (1998). Introduction in the theory of unconventional superconductivity (Moscow Fiz.-Tekh. Inst. Press, Moscow), p. 141. [71] Van Harligen, D.J. (1995). Phase -sensitive test of the symmetry of pairing state in the high-temperature superconductors- evidence for D symmetry, Rev. Mod. Phys. 67, 2, pp. 515–535. [72] Tsuei, C.C. and Kirtley, J.R. (2000). Pairing symmetry in cuprate superconductors, Rev. Mod. Phys. 72, 4, pp. 969–1015. [73] Pines, D. (1991). Spin ﬂuctuations and high temperature superconductivity the antiferromagnetically correlated oxides:YBaCuO, LaSrCuO, Physica C 185–189, pp. 120–129. [74] Monthoux, P., Balatsky, A.V. Pines, D. (1991). Toward a theory of high-temperature superconductivity in the antiferromagnetically correlated cuprates oxides, Phys. Rev. Lett. 67, 24, p. 3448. [75] Balatsky, A.V., Vekhter, I.V. and Zhu, J.X. (2008). Impurity-induced state in convenventional and unconventional superconductors, Rev. Mod. Phys. 78, pp. 373–433. [76] Izyumov, Yu.A. (1999). Spin-ﬂuctuation mechanism in high-Tc superconductivity and symmetry of order parameter, Usp. Phys. 169, 3, p. 215. [77] Morya, T., Ueda, K. (2000). Spin ﬂuctuations and high-temperature superconductivity, Adv. Phys. 49, 5, pp. 556–605. [78] Levi, B.G. (1993). In high-Tc superconductors, is d-wave the new wave, Phys. Today 5, pp. 17–20. [79] Manske, D. (2004). Theory of unconventional superconductors (Springer, Heidelberg). [80] Maple, M.B. (1986). New type superconductivity in f-electron system, Physics Today 4, p. 72.

page 274

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

275

[81] Miyake, K. and Schmitt-Rink, S. (1986). Spin ﬂuctuation mediated even party pairing in heavy fermion superconductors, Phys. Rev. B 34, 9, pp. 6554–6556. [82] Kruchinin, S.P. (1995). Functional integral of antiferromagnetic spin ﬂuctuations in high-temperature superconductors, Mod. Phys. Let. B 9, pp. 205–215. [83] Kruchinin, S.P. and Patapis, S.K. (1996). Thermodynamics of d-wave pairing in cuprate superconductors, J. Low Temp. Phys. 105, pp. 717–721. [84] Kruchinin, S.P. and Patapis, S.K.(1997). Speciﬁc heat of antiferromagnetic spin ﬂuctuations in cuprate superconductors, Physica C 282–285, pp. 1397– 1398. [85] Kruchinin, S.P. (2000). The pseudogap of antiferromagnetic spin ﬂuctuations in cuprate superconductors, Physica C 341–348, pp. 901–902. [86] Kruchinin, S.P. (2005). Condensation energy for spin ﬂuctuation mechanism of pairing in high-Tc superconductors, Proceedings a NATO Advanced Research Workshop “New challenges in superconductivity: Experimental advances and emerging theories”, ed. Ashkenazi, J. (Kluwer Academic Publishers, Dordrecht), pp. 145–150. [87] Popov, Y.N. (1987). Functional integrals and collective excitations (Cambridge University Press, Cambridge), p. 216. [88] Conwall, J., Jackiw, R. and Tomhoulis, E. (1974). Eﬀective action for composite operators, Phys. Rev. D 10, 8, pp. 2428–2444. [89] Weinberg, St. (1993). Eﬀective action and renormalization group ﬂow of anisotropic superconductors, Preprint UTTG 18, p. 1–17 [90] Shen, Z.X., Dessan, D.S., Wells, B.O., King, D.M., Spicer, W.E., Arko, A.J., Marshall, D., Lombarolo, L.W., Kapitulnik, A., Dickinson, P., Doniach, S., Carko, J.Di., Loesser, A.G. and Park, C.H. (1993). Anomalously large gap anisotropy in the a–b plane of Bi2 Sr2 CaCu2 O8+γ , Phys. Rev. Lett. 70, p. 1553. [91] Moler, M.B., Barr, D.I., Urbach, J.S., Hardy, W.H. and Kapitulnik, A. (1994). Magnetic ﬁeld dependence of the density of states of YBaCuO as determined from the speciﬁc heat, Phys. Rev. Lett. 73, p. 2744. [92] Momono, N., Ido, M., Nakano,T. and Oda, M. (1994). Low-temperature electronic speciﬁc heat in LaSrCuZnO, Physica C 235–240, pp. 1739–1740. [93] Loram, J.W., Mirza, K.A., Cooper, J.R. and Tallon, J.L. (1998). Speciﬁc heat evidence on the normal state pseudogap, J. Phys. Chem. Solid 59, 10–12, pp. 2091–2094. [94] Revaz, B., Genond, J.Y., Junod, A., Naumdier, K., Erb, A. and Walker, E. (1998). d-wave scaling relations in the mixed-state speciﬁc heat Y Ba2 Cu3 O7 , Phys. Rev. Lett. 80, 15, pp. 3364–3367. [95] Hasselbach, K., Kirtley, J.R. and Flouquet, J. (1994). Symmetry of the gap in superconducting UReSi, Phys. Rev. B 47, pp. 509–512. [96] Muhrer, G. and Schachinger, E. (2000). Free energy of a d-wave superconductor in the nearly antiferromagnetic Fermi liquid model, J. Low. Temp. Phys. 88–120, 1–2, pp. 65–88. [97] Dorbolo, S., Ausloos, M. and Houssa, M. (1998). Electronic speciﬁc heat of superconductors with van Hove singularities: eﬀects of a magnetic ﬁeld and thermal ﬂuctuations, Phys. Rev. B 57, pp. 5401–5411.

page 275

March 25, 2021

276

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[98] Dobrosavljevic-Crujic, L. and Miranovic, P. (2003). Low temperature speciﬁc heat in anisotropic superconductors, Physica C 397, pp. 117–122. [99] Bogolyubov, Jr. N.N. and Kruchinin, S.P. (2003). Modern approach to the calculation of the correlation function for superconductivity model, Mod. Phys. Lett. B 17, 10–12, pp. 709–724. [100] Kamihara, Y., Watanabe, T., Hirano, M. and Hosono, H. (2008). Iron-based layered superconductor La[O1−xFx ]FeAs (x = 0.05-0.12) with Tc = 26 K, J. Am. Chem. Soc. 130, pp. 3296–3297. [101] Song, C.L., Wang, Y.-L., Cheng, P., Jiang, Y.-P., Li, W., Zhang, T., Li, Z., He, K., Wang, L., Jia, J.-F., Hung, H.-H., Wu, C., Ma, X., Chen, X. and Xue, Q.-K. (2011). Direct observation of nodes and twofold symmetry in FeSe superconductor, Science 332, 6036, p. 1410. [102] Lee, J.J., Schmitt, F.T., Moore, R.G., Johnston, S., Cui, Y.-T., Li, W., Yi, M., Liu, Z.K., Hashimoto, M., Zhang, Y., Lu, D.H., Devereaux, T.P., Lee, D.-H. and Shen, Z.-X. (2014). Interfacial mode coupling as the origin of the enhancement of Tc in FeSe ﬁlms on SrTiO3x , Nature 515, p. 245. [103] Sadovskii, M.V. (2008). High-temperature superconductivity in layered iron compounds, Phys. Usp. 51, 12, pp. 1201–1227. [104] Izyumov, Yu.A. and Kurmaev, E.Z. (2008). FeAs systems: a new class of high-temperature superconductors, Phys. Usp. 51, 12, pp. 1261–1286. [105] Graser, S., Maier, T.A., Hirschfeld, P.J. and Scalapino, D.J. (2009). Neardegeneracy of several pairing channels in multiorbital models for the Fe pnictides, New J. Phys. 11, p. 025016. [106] Shirage, P. et al. (2010). Synthesis of ErFeAsO-based superconductors by the hydrogen doping method, Europhys. Lett. 92, pp. 57011–57015. [107] Leb`egue, S. (2007). Electronic structure and properties of the Fermi surface of the superconductor LaOFeP, Phys. Rev. B 75, p. 035110. [108] Rotter, M., Tegel, M. and Johrendt, D. (2008). Superconductivity at 38 K in the Iron Arsenide Ba1−x Kx )Fe2 As2 , Phys. Rev. Lett. 101, p. 107006. [109] Chen, G.F., Li, Z., Li, G., Hu, W.Z., Dong, J., Zhou, J., Zhang, X.-D., Zheng, P., Wang, N.-L. and Luo, J.-L. (2008). Superconductivity in holedoped (Sr1−x Kx )Fe2 As2 , Chin. Phys. Lett. 25, p. 9. [110] Tapp, J.H., Tang, Z., Lv, B., Sasmal, K., Lorenz, B., Chu, P.C. W. and Guloy, A.M. (2008). LiFeAs: An intrinsic FeAs-based superconductor with Tc = 18 K, Phys. Rev. B 78, p.060505. [111] Gooch, M., Lv, B., Lorenz, B., Guloy, A.M. and Chu, C.W. (2009). Evidence of quantum criticality in the phase diagram of Kx Sr1−x Fe2 As2 from measurements of transport and thermoelectricity, Phys. Rev. B 79, p. 104504. [112] Mizuguchi, Y., Tomioka, F., Tsuda, S., Yamaguchi, T. and Takano, Y. (2008). Superconductivity at 27 K in tetragonal FeSe under high pressure, Appl. Phys. Lett. 93, p. 152505. [113] Garbarino, G., Sow, A., Lejay, P., Sulpice, A., Toulemonde, P., Mezouar, M. and N´ un ˜ ez-Regueiro, M. (2009). High-temperature superconductivity (Tc onset at 34 K) in the high-pressure orthorhombic phase of FeSe, Europhys. Lett. 86, p. 27001.

page 276

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

277

[114] Gor’kov, L.P. (2016). Superconducting transition temperature: Interacting Fermi gas and phonon mechanisms in the nonadiabatic regime, Phys. Rev. B 93, p. 054517. [115] Gor’kov, L.P. (2016). Peculiarities of superconductivity in the single-layer FeSe/SrTiO3 interface, Phys. Rev. B 93, p. 060507. [116] Mizuguchi, Y., Hara, Y., Deguchi, K., Tsuda, S., Yamaguchi, T. and Takeda, K., Kotegawa, H., Tou, H., and Takano, Y. (2010). Anion height dependence of Tc for the Fe-based superconductor, Supercond. Sci. Technol. 23, 5, p. 054013 [117] Kruchinin, S.P., Zolotovsky, A. and Kim, H.T. (2013). Band structure of new ReFe AsO superconductors, J. Mod. Phys. 4, pp. 608-611. [118] Lu, D. H., Yi, M., Mo, S.-K., Erickson, A.S., Analytis, J., Chu, J.-H., Singh, D.J., Hussain, Z., Geballe, T.H., Fisher, I.R. and Shen, Z.-X. (2008). Electronic structure of the iron-based superconductor LaOFeP, Nature 455, p. 81. [119] Liu, C., Kondo, T., Tillman, M.E., Gordon, R., Samolyuk, G.D., Lee, Y., Martin, C., McChesney, J.L., Bud’ko, S., Tanatar, M.A., Rotenberg, E., Canﬁeld, P.C., Prozorov, R., Harmon, B.N. and Kaminski, A. (2008). Fermi surface and strong coupling superconductivity in single crystal NdFeAsO1−x Fx , Preprint, arXiv:0806.2147. [120] Coldea, A.I., Fletcher, J.D., Carrington, A., Analytis, J.G., Bangura, A.F., Chu, J.H., Erickson, A.S., Fisher, I.R., Hussey, N.E. and McDonald, R.D. (2008). Fermi surface of superconducting LaFePO determined from quantum oscillations, Phys. Rev. Lett. 101, p. 216402. [121] Hanaguri, T.T., Niitaka, S., Kuroki, K. and Takagi, H. (2010). Unconventional s-wave superconductivity in Fe(Se, Te), Science, 328, pp. 474–476. [122] De la Cruz, C., Huang, Q., Lynn, J.W., Li, J., Ratcliﬀ, W., Zarestky, J.L., Mook, H.A., Chen, G.F., Luo, J.L. and Wang, N.L. (2008). Pengcheng dai magnetic order close to superconductivity in the iron-based layered LaO1−x Fx FeAs systems, Nature 453, p. 899. [123] Dong, J., Zhang, H.J., Xu, G., Li, Z., Li, G., Hu, W.Z., Wu, D., Chen, G.F., Dai, X., Luo, J.L., Fang, Z. and Wang, N.L. (2008). Competing orders and spin-density-wave instability in La(O1−x Fx )FeAs, Europhys. Lett. 83, 2, p. 27006. [124] Basov, D.N. and Chubukov, A.V. (2011). Manifesto for a higher Tc , Nature Phys. 7, 4, pp. 272–276. [125] Barzykin, V. and Gor’kov, L.P. (2008). On superconducting and magnetic properties of iron oxypnictides, JETP Lett. 88, p.131. [126] Mazin, I.I., Singh, D.J., Johannes, M.D. and Du, M.H. (2008). Unconventional superconductivity with a sign reversal in the order parameter of LaFeAsOx Fx , Phys. Rev. Lett. 101, p. 057003. [127] Choi, H.-Y., Yun, J.H., Bang, Y. and Lee, H.C. (2009). Model for the inverse isotope eﬀect of FeAs-based superconductors in the π-phase-shifted pairing state, Preprint, arXiv:0904.1864v3. [128] Ding, L., He, C., Dong, J.K., Wu, T., Liu, R.H., Chen, X.H. and Li, S.Y. (2008). Speciﬁc heat of the iron-based high-Tc superconductor SmO1−x Fx FeA, Phys. Rev. B 77, p. 180510.

page 277

March 25, 2021

278

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[129] Wang, F., Zhai, H., Ran, Y., Vishwanath, A. and Lee, D.-H. (2009). Funtional renormalization group study of the pairing symmetry and pairing mechanism of the FeAs based high temperature superconductors, Preprint, arXiv:0804.4332. [130] Mazin, I.I., Singh, D.J., Johannes, M.D., and Du, M.H. (2008). Unconventional superconductivity with a sign reversal in the order parameter of LaFeAsO1−x Fx , Phys. Rev. Lett. 101, p. 057003. [131] Kuroki, K., Onari, S., Arita, R., Usui, H., Tanaka, Y., Kontani, H. and Aoki, H. (2008). Unconventional pairing originating from the disconnected Fermi surfaces of superconducting LaFeAsO, Phys. Rev. Lett. 101, p. 087004. [132] Bulut, N., Scalapino, D.J. and Scalettar, R.T. (1992). Nodeless d-wave pairing in a two-layer Hubbard model, Phys. Rev. B 45, p. 5577. [133] Okazaki, K., Ito, Y., Ota, Y., Kotani, Y., Shimojima, T., Kiss, T., Watanabe, S., Chen, C.-T., Niitaka, S., Hanaguri, T., Takagi, H., Chainani, A. and Shin, S. (2012). Evidence for a cos(4ϕ) modulation of the superconducting energy gap of optimally doped FeTe0.6 Se0.4 single crystals using laser angleresolved photoemission spectroscopy, Phys. Rev. Lett. 109, p.237011. [134] Raghu, S., Qi, X.-L, Liu, C.-X., Scalapino, D. and Zhang, S.-C. (2008). Minimal two-band model of the superconducting iron oxypnictides, Phys. Rev. B 77, p. 220503. [135] Kuroki, K., Onari, S., Arita, R., Usui, H., Tanaka, Y., Kontani, H. and Aoki, H. (2009). Unconventional pairing originating from the disconnected Fermi surfaces of superconducting LaFeAsO1−x Fx , Phys. Rev. Lett. 102, p. 109902. [136] Seo, K., Bernevig, B.A. and Hu, J. (2008). Pairing symmetry in a two-orbital exchange coupling model of oxypnictides, Phys. Rev. Lett. 101, p. 206404. [137] Nagao, H., Kruchinin, S.P., Yaremko, A.M. and Yamaguchi, K. (2002). Multiband superconductivity, Int. J. Mod. Phys. B 16, pp. 3419–3428. [138] Kruchinin, S.P. and Nagao, H. (2005) Two-gap superconductivity in MgB, Phys. Particles Nucl. 36, Suppl. 1, pp. 127–130. [139] Kruchinin, S.P. and Yaremko, A.M. (1998). Many zone eﬀect in cuprate superconductors, Supercond. Sci. Technol. 11, pp. 4–8. [140] Nagao, H., Kawabe, H., Kruchinin, S.P., Manske, D. and Yamaguchi, K. (2003). Theoretical studies on many band eﬀects superconductivity by using renormalization group approach, Mod. Phys. Lett. B 17, 10–12, pp. 423–431. [141] Nagao, H., Kawabe, H., Kruchinin, S.P., Manske, D. and Yamaguchi, K. (2003). Superconductivity in two-band model by renormalization group approach, Int. J. Mod. Phys. B 17, p. 3373–3376. [142] Yaremko, A.M., Mozdor, E.V. and Kruchinin, S.P. (1996). Coupled states of electron-phonon system, superconductivity and HTSC of crystals, Int. J. Mod. Phys. B 10, pp. 2665–2674. [143] Kruchinin, S.P. and Nagao, H. (2006). Multi-gap superconductivity in MgB2 , Proceedings a NATO Advanced Research Workshop “Symmetry and heterogeneity in High-Tc superconductors”, Bianconi, A. (ed.) (Kluwer Academic Publishers, Dorderecht), pp. 43–53. [144] Nagao, H., Yaremko, A., Kruchinin, S.P., Yamaguchi, K. (2002). Many band eﬀects in superconductivity, Proceedings of a NATO Advanced Research

page 278

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

[145] [146]

[147]

[148] [149]

[150] [151] [152] [153] [154] [155] [156]

[157] [158]

[159]

[160]

[161]

[162]

279

Workshop “New trends in superconductivity”, Annett, J., and Kruchinin, S.P. (eds) (Kluwer Academic Publishers, Dordrecht), pp. 155–167. Kruchinin, S. (2016). Multiband superconductivity, Rev. Theoret. Phys. 4, 2, pp. 165–178. Nakazawa, Y. and Kruchinin, S. (2018). Experimental and theoretical aspects of thermodynamic properties of quasi-1D and quasi-2D organic conductors and superconductors, Inter. J. Mod. Phys. B 30, 13, p. 1042008. Kruchinin, S., Zolotovsky, A., Yamashita, S. and Nakazawa, Y. (2016). Thermodynamics of the d-wave pairing in organic superconductors, Int. J. Mod. Phys. B 30, 13, p. 1042020. Bardeen, J., Cooper, L.N. and Schrieﬀer, J. R. (1957). Microscopic theory of superconductivity, Phys. Rev. 108, pp. 1175. Anderson, P.W. and Zou, Z. (1988). “Normal” tunneling and “normal” transport: diagnostics for the resonating-valence-bond state, Phys. Rev. Lett. 60, p. 132. Kampf, A.P. (1994). Magnetic correlations in high temperature superconductivity, Phys. Rep. 249, p. 219. Emery, V.J. (1987). Theory of high-Tc superconductivity in oxides, Phys. Rev. Lett. 58, p. 2794. Hirsch, J.E. (1985). Attractive interaction and pairing in fermion systems with strong on-site repulsion, Phys. Rev. Lett. 25, 1317. Zhang, F.C. and Rice, T.M. (1988). Eﬀective Hamiltonian for the superconducting Cu oxides, Phys. Rev. B 37, p. 3759. Fradkin, E. (1991). Field theories of condensed matter systems (AddisonWesley). Nagaosa, N. and Lee, P.A. (1990). Normal-state properties of the uniform resonating-valence-bond state, Phys. Rev. Lett. 64, p. 2450. Baskaran, G., Zou, Z. and Anderson, P. W. (1987). The resonating valence bond state and high-Tc superconductivity-a mean ﬁeld theory, Solid State Commun. 63, p. 973. Fukuyama, H. and Yoshida, K. (1987). Critical temperature of superconductivity caused by strong correlation, Jpn. J. Appl. Phys. 26, pp. 371–373. Yamamoto, S., Yamaguchi, K. and Nasu, K. (1990). Ab initio molecularorbital study on electron correlation eﬀects in CuO6 clusters relating to highTc superconductivity, Phys. Rev. B 42, pp. 266–272. Nagao, H., Kitagawa, Y., Kawakami, T., Yoshimoto, T., Saito, H. and Yamaguchi, K. (2001). Theoretical studies on ﬁeld-induced superconductivity in molecular crystals, Int. J. Quantum Chem. 85, pp. 608–618. Kimura, M., Kawabe, H., Nakajima, A., Nishikawa, K. and Aono, S. (1988). Possibility of superconducting and other phases in organic high polymers polyacene carbon skeletons, Bull. Chem. Soc. Jpn. 61, p. 4239. Torrance, J.B., Bezinge, A., Nazzal, A.I. and Parkin, S.S. (1989). Disappearance of high temperature superconductivity induced by high carrier concentrations, Physica C 162–164, p. 291. Ord, T., Kristoﬀel, N. and Rago, K. (2003). MgB2 superconductivity properties in a two-gap model, Mod. Phys. Let. B 17, pp. 667–673.

page 279

March 25, 2021

280

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[163] Suhl, H., Matthias, B.T. Walker, R. (1959). Bardeen–Cooper–Schrieﬀer theory of superconductivity in the case of overlapping bands, Phys. Rev. Lett. 3, p. 552. [164] Moskalenko, V.A. (1959). Superconductivity metals with overlapping energetic bands, Fiz. Metalloved. 8, p. 503. [165] Antipov, E. and Abakumov, A. (2008). Structural design of superconductors based on complex copper oxides, Phys. Usp. 51, p. 180. [166] M¨ uller, K.A. (2006). The search for new high temperature superconductors, Supercond. Sci. Technol. 58, pp. 1–3. [167] Bennemann, K.H., Ketterson, J.B. (2008). Superconductivity (Springer, Heidelberg), 1. [168] Nagamatsu, J., Nakamura, N., Muranaka, T., Zentani, Y. and Akimitsu, J. (2001). Superconductivity at 39 K in magneszium dieboride, Nature 410, p. 63. [169] Canﬁeld, J.P.C., Bud’ko, S.L. and Finnemore, D.K.(2003). An overview of the basic physical properties of MgB2 , Physica C 385, 1–2, pp. 1–3. [170] Binnig, G., Baratoﬀ, A., Hoening, Bednorz, J.G. (1980). Two-band superconductivity in Nb-doped SrTiO3 , Phys. Rev. Lett. 45, p. 1352. [171] An, J.M. and Picket, W.E. (2001). Superconductivity of MgB2 : covalent bonds driven metallic, Phys. Rev. Lett. 86, p. 4366. [172] Kortus, J., Mazin, I.I., Belashenko, K.D., Antropov. V.P. and Boyer,I.L. (2001). Superconductivity of metallic boron in MgB2 , Phys. Rev. Lett. 86, p. 4656. [173] Kondo, J. (1963). Superconductivity in transition metals, Prog. Theor. Phys. 29, p. 1. [174] Kristoﬀel, N., Ord, T. and Rago, K. (2003). MgB2 two-gap superconductivity with intra- and interband couplings, Europhys. Lett., 61, pp. 109–115. [175] Szabo, P., Samuely, P., Klein, T., Marcus, J., Fruchart, D., Miraglia, S., Marcenat, C. and Jansen, A. (2001). Evidence for two superconducting energy gaps in MgB2 by point-contact spectroscopy, Phys. Rev. Lett. 87, p. 137005. [176] McMillan, W.L. (1968). Transition temperature of strong-coupled superconductors, Phys. Rev. 167, p. 331. ¨ [177] Konsin, P., Kristoﬀel, N. and Ord, T. (1988). The interband interaction as a possible cause of high-temperature superconductivity, Phys. Lett. A 129, pp. 339–342. [178] Combescot, R. and Leyronas, X. (1995). Coupling between planes and chains in YBa2 Cu3 O7 : a possible solution for the order parameter controversy, Phys. Rev. Lett. 75, pp. 3732–3735. [179] Konsin, P. and Sorkin, B. (1998). Electric ﬁeld eﬀects in high-Tc cuprates, Phys, Rev. B 58, pp. 5795–5802. [180] Nagao, H., Nishino, M., Shigeta, Y., Yoshioka, Y. and Yamaguchi, K. (2000). Theoretical studies on superconducting and other phases: Triplet superconductivity, ferromagnetism, and ferromagnetic metal, J. Chem. Phys. 113, pp. 721–732. [181] Kondo, J. (2001). Superconductivity of the two-dimensional Hubbard models with a small U, J. Phys. Soc. Jpn. 70, p. 808.

page 280

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

281

[182] Nagao, H., Mitani, M., Nishino, M., Shigeta, Y., Yoshioka, Y. and Yamaguchi, K. (1999). Theoretical studies on anomalous phases in molecular systems with external ﬁeld: Possibility of photo-induced superconductivity, Int. J. Quantum Chem. 75, pp. 549–561. [183] Nagao, H., Nishino, M., Mitani, M., Yoshioka, Y. and Yamaguchi, K. (1997). Possibilities of charge- and/or spin-mediated superconductors and photo-induced superconductors in the intermediate region of metal-insulator transitions, Int. J. Quantum Chem. 65, pp. 947–957. [184] Nagao, H., Mitani, M., Nishino, M., Shigeta, Y., Yoshioka, Y. and Yamaguchi, K. (1988). Possibility of charge-mediated superconductors in the intermediate region of metal-insulator transitions, Int. J. Quantum Chem. 70, pp. 1075– 1084. [185] Bogoluibov, N.N. and Bogoluibov, Jr., N.N. (1986). An introduction to quantum statistical mechanics (Nauka, Moscow) (translated in English 1994). [186] Bogoliubov, N.N. and Shirkov, D.V. (1959). Introduction to the theory of quantized ﬁeld (Interscience Publishers Inc., New York). [187] Mattuck, R.D. (1976). A guide to Feynman diagrams in the many-body problem 2nd edn. (McGraw-Hill, New York). [188] Kimura, M., Kawabe, H., Nishikawa, K. and Aono, S. (1988). Possibility of superconducting and other phases in organic high polymers of polyacene carbon skeletons II. Screened electron–electron interaction, Bull. Chem. Soc. Jpn. 61, pp. 4245–4252. [189] Kimura, M., Kawabe, H., Nishikawa, K. and Aono, S.(1986). Superconducting and other phases in organic high polymers of polyacenic carbon skeletons. I. The method of sum of divergent perturbation series, J. Chem. Phys. 85, pp. 3090–3096. [190] Kimura, M., Kawabe, H., Nishikawa, K. and Aono, S.(1985). Superconducting and other phases in organic high polymers of polyacenic carbon skeletons. II. The mean ﬁeld method, J. Chem. Phys. 85, pp. 3097–3100. [191] Kimura, M., Kawabe, H., Nakajima, A., Nishikawa, K. and Aono, S. (1988). Possibility of superconducting and other phases in organic high polymers of polyacene carbon skeletons. II. Screened electron–electron interaction. Bull. Chem. Soc. Jpn. 61, pp. 4239–4244. [192] Bogoluibov, N.N. and Tyablikov, S. (1959). Retarded and advanced Green functions in statistical physics, Dokl. Acad. Sci. USSR 126, p. 53, Sov. Phys. Dokl. 4, p. 589. [193] Highlights of the year, Physics 12, 145, https://physics.aps.org/articles/v12/ 145. [194] Somayazulu, M. et al. (2019). Evidence for superconductivity above 260 K in lanthanum superhydride at megabar pressures, Phys. Rev. Lett. 122, p. 027001. [195] Drozdov, A.P., Kong, P.P., Minkov, V.S., Besedin, S.P., Kuzovnikov, M.A., Mozaﬀari, S., Balicas, L., Balakirev, F., Graf, D., Prakapenka, V.B., Greenberg, E., Knyazev, D.A., Tkacz, M. and Eremets M.I. (2018). Superconductivity at 250 K in lanthanum hydride under high pressures, Preprint, arXiv:1812.01561.

page 281

March 25, 2021

282

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[196] Peng, F. et al. (2007). Hydrogen clathrate structures in rare earth hydrides at high pressures: possible route to room-temperature superconductivity, Phys. Rev. Lett. 119, p.107001. [197] Drozdov, A.P., Eremets, M.I., Troyan, I.A., Ksenofontov, V. and Shylin, S.I. (2015). Conventional superconductivity at 203 kelvin at high pressures in the sulfur hydride system, Nature, p. 525. [198] Flores-Livas, J.A., Boeri, L., Sanna, A., Profeta, G., Arita, R. and Eremets, M. (2020). A perspective on conventional high-temperature superconductors at high pressure: Methods and materials, Phys. Rep. 856, 4, pp. 1–78. [199] Ginzburg, V.L. (1999). What problems of physics and astrophysics seem now to be especially important and interesting (thirty years later, already on the verge of XXI century)? Phys. Usp. 42, 4, p. 353. [200] Snider, E., Dasenbrock-Gammon, N., McBride, R., Debessai, M., Vindana, H., Vencatasamy, K., Lawler, K., Salamat, A. and Dias, R.P. (2020). Roomtemperature superconductivity in a carbonaceous sulfur hydride, Nature 586, pp. 373–377. [201] Ashcroft, N. (1968). Metallic hydrogen: A high-temperature superconductor? Phys. Rev. Lett. 21, pp. 1748–1749. [202] Bardeen, J., Cooper, L.N. and Schrieﬀer, J.R. (1957). Theory of superconductivity, Phys. Rev. 108, pp. 1175–1204. [203] Gor’kov, L.P. (1958). On the energy spectrum of superconductors, Sov. Phys. JETP 7, 3, p. 505. [204] Abrikosov, A.A., Dzyaloshinskii, I. and Gor’kov, L.P. (1975). Methods of quantum ﬁeld theory in statistical physics (Dover, New York). [205] Fetter, A., Walecka, J.D. (1971). Quantum theory of many-particle systems (Dover, New York). [206] Eliashberg, G.M. (1960). Interactions between electrons and lattice vibrations in a superconductor, Sov. Phys. JETP 38, p. 696. [207] Dynes, R. (1972). McMillan’s equation and the Tc of superconductors, Solid State Commun. 10, 7, pp. 615–618. [208] McMillan, W.L. (1968). Transition temperature of strong-coupled superconductors, Phys. Rev. 167, pp. 331–344. [209] Wen, X.-D. et al. (2011). Graphane sheets and crystals under pressure, Proc. Natl. Acad. Sci. USA 108, p.6833. [210] Allen, P.B. and Dynes, R.C. (1975). Transition temperature of strong-coupled superconductors reanalyzed, Phys. Rev. B 12, p.905. [211] Richarson, R.W. (1963). A restricted class of exact eigenstates of the pairingforce hamiltonian, Phys. Lett 3, pp. 277–279. [212] Matveev, K.A. and Larkin, A.I. (1997). Parity eﬀect in ground state energies of ultrasmall superconducting grains, Phys. Rev. Lett. 78, pp. 3749–3752. [213] Ralph, D.C., Black, C.T. and Tinkham, M. (1997). Gate-voltage studies of discrete electronic staes in aluminum nanoparticles, Phys. Rev. Lett. 78, p. 4087. [214] Schechter, M., Imry, Y., Levinson, Y. and von Delft, J. (2001). Thermodynamic properties of a small superconducting grain, Phys. Rev. B 63, pp. 214518–214534.

page 282

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

283

[215] Sierra, G. (2000). Conformal ﬁeld theory and the exact solution of the BCS hamiltonian, Nucl. Phys. B 572, pp. 517–527. [216] Stenuit, G., Michotte, S., Govaerts, J. and Piraux, L.P. (2003). Vortex matter in lead nanowires, Eur. Phys. J. B 33, pp. 103–110. [217] Kasumov, A.Yu. et al. (1999). Supercurrents through single-walled carbon nanotubes, Science 284, pp. 1508–1511. [218] Nagao, H., Kawabe, H. and Kruchinin. S. (2006). Nanosize two-gap superconductivity. Proceedings of a NATO ARW “Electron correlation in new materials and nanosystems”, (Scharnberg, K. and Kruchinin S., eds.) (Springer), pp. 117–127. [219] Kawabe, H., Nagao, H., Kruchinin, S. (2006). Exact solution of two-band superconductivity, Proceedings of a NATO ARW “Electron correlation in new materials and nanosystem”, (Scharnberg, K. and Kruchinin, S. eds.) (Springer), pp. 129–139. [220] Nagao, H. and Kruchinin, S.P. (2008). Kondo eﬀect coupled to superconductivity ultrasmall grains. Proceedings NATO ARW “Electron transport in nanosystems”, (Bonca, J. and Kruchinin, S. eds.) (Springer), pp. 105–115. [221] Kruchinin, S. and Nagao, H. (2012). Nanoscale superconductivity, Int. J. Mod. Phys. B 26, p. 1230013. [222] Kruchinin, S.P., Kawabe, H., Nagao, H. and Nakazawa, Y. (2013). Condensation energy for two-gap superconducting state in nanoparticles, J. Nanoparticles 3, pp. 1–6. [223] Dzhezherya, Yu., Novak, I.Yu. and Kruchinin, S. (2010). Orientational phase transitions of lattice of magnetic dots embedded in a London type superconductors, Supercond. Sci. Technol. 23, p.1–5. [224] Kruchinin, S. (2015). Kondo eﬀect in superconducting nanoparticles, Quantum Matter 4, p. 373–377. [225] Kruchinin, S. (2015). Richardson solution for superconductivity in ultrasmall grains, Quantum Matter 4, p. 378–383. [226] Kruchinin, S. (2016). Energy spectrum and wave function of electron in hybrid superconducting nanowires, Int. J. Mod. Phys. B 30, 13, p. 1042008. [227] Kruchinin, S.P., Dzezherya, Yu. and Annett, J.(2009). Interactions of nanoscale ferromagnetic granules in a London superconductors, Supercond. Sci. Technol. 19, pp. 381–384. [228] Ralph, D.C., Black, C.T. and Tinkham, M. (1995). Spectroscopic mesurements of discrete electronic states in single metal particles, Phys. Rev. Lett. 74, p. 3241. [229] Smith, R.A. and Ambegaokar, V. (1996). Eﬀect of level statistics on superconductivity in ultrasmall metallic grains, Phys. Rev. Lett. 77, p. 4962. [230] von Delft, J., Zaikin, A.D., Golubev, D.S. and Tichy, W. (1996). Parityaﬀected superconductivity in ultrasmall metallic grains, Phys. Rev. Lett. 77, pp. 3189–3192. [231] Yamaji, K. and Shimoi, Y. (1994). Superconducting transition of the twochain Hubbard model indicated by diagonalization calculations, Physica C 222, pp. 349–360.

page 283

March 25, 2021

284

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[232] Black, C.T., Ralph, D.C. and Tinkham, M. (1996). Spectroscopy of the superconducting dap in individual nanometer-scale aluminum particles, Phys. Rev. Lett. 76, pp. 688–611. [233] Braun, F. and von Delft, J. (1998). Fixed-N superconductivity: The crossover from the bulk to the few-electron limit, Phys. Rev. Lett. 81, pp. 4712–4715. [234] von Delft, J. and Braun, F. (1999). Superconductivity in ultrasmall metallic grains, Phys. Rev. B 59, pp. 9527–9544. [235] Gladilin, V.N., Fomin, V.M. and Devreese, J.T. (2002). Shape of nanosize superconducting grains: does it inﬂuence pairing characteristics, Solid State Comm. 121, pp. 519–523. [236] Jank´o, B., Smith, A. and Ambegaokar, V. (1994). BCS superconductivity with ﬁxed number parity, Phys. Rev. B 50, pp. 1152–1161. [237] Matveev, K.A. and Larkin, A.L. (1997). Parity eﬀect in ground state energies of ultrasmall superconducting grains, Phys. Rev. Lett., 78, pp. 3749–3752. [238] Richardson, R.W. and Sherman, N. (1964). Pairing models of Pb206, Pb204 and Pb202, Nucl. Phys. 523, pp. 253–268. [239] Richardson, R.W. (1977). Pairing in the limit of a large number of particles, J. Math. Phys. 6, pp. 1802–1811. [240] Richardson, R.W. (1966). Numerical study of the 8-32-particle eigenstate of the pairing hamiltonian, Phys. Rev. 141, pp. 949–955. [241] Sierra, G., Dukelsky, J., Dussel, G.G., von Delft, J. and Braun, F. (2000). Exact study of the eﬀect of level statistics in ultrasmall superconducting grains, Phys. Rev. B 61, pp. 11890–11893. [242] Kouwenhoven, L. and Glazman, L. (2001). The revival of the Kondo eﬀect, Phys. World 14, 1, pp. 33–38. [243] van der Wiel, G., De Franceschi, S., Fujisawa, T., Elzerman, J.M., Tarucha, S. and Kouwenhoven, L.P. (2000). The Kondo eﬀect in the unitary limit, Science 289, pp. 2105–2108. [244] Inoshita, T. (1998). Kondo eﬀect in quantum dots, Science 281, pp. 526–527. [245] Sasaki, S., De Franceschi, S., Elzerman, J.M., van der Wiel, W.G., Eto, M., Tarucha, S. and Kouwenhoven, L.P. (2000). Kondo eﬀect in an integer-spin quantum dot, Nature (London) 405, pp. 764–767. [246] Inoshita, T., Shimizu, A., Kuramoto, Y. and Sakaki, H. (1993). Correlated electron transport through a quantum dot: The multiple-level eﬀect, Phys. Rev. B 48, pp. 114725–14728. [247] Izumida, W., Sakai, O. and Shimizu, Y. (1998). Kondo eﬀect in single quantum dot systems-study with numerical renormalization group method, J. Phys. Soc. Jpn. 67, p. 2444. [248] Yeyati, A.L., Flores, F. and Martin-Rodero, A.(1999). Transport in multilevel quantum dots: from the Kondo eﬀect to the Coulomb blockade regime, Phys. Rev. Lett. 83, pp. 600–603. [249] Pasupathy, A.N., Bialczak, R.C., Martinek, J., Grose, J.E., Donev, L.A.K., McEuen, P.L. and Ralph, D.C. (2004). The Kondo eﬀect in the presence of ferromagnetism, Science 306, pp. 86–90. [250] Matsubayashi, D. and Eto, M. (2007). Spin splitting and Kondo eﬀect in quantum dots coupled to noncollinear ferromagnetic leads, Phys. Rev. B 75, p. 165319.

page 284

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

285

[251] Buitelaar, M.R., Nussbaumer, T. and Sch¨onenberger, C. (2002). Quantum dot in the Kondo regime coupled to superconductors, Phys. Rev. Lett. 89, p. 256801. [252] Ueda, A. and Eto, M. (2006). Resonant tunneling and Fano resonance in quantum dots with electron–phonon interaction, Phys. Rev. B 73, pp. 235353– 235365. [253] Eto, M. and Nazarov, Y.V. (2000). Enhancement of Kondo eﬀect in quantum dots with an even number of electrons, Phys. Rev. Lett. 85, pp. 1306–1309. [254] Reich, S., Leitus, G., Popovitz-Biro, R. and Schechter, M. (2003). Magnetization of small lead particles, Phys. Rev. Lett. 91, p. 147001. [255] Yamaji, K. and Shimoi, Y.(1994). Superconducting transition of the twochain Hubbard model indicated by diagonalization calculations, Physica C 222, pp. 349–360. [256] Combescot, R. and Leyronas, X. (1995). Coupling between planes and chains in YBa2 Cu3 O7 : a possible solution for the order parameter controversy, Phys. Rev. Lett. 75, pp. 3732–3735. [257] Cox, D.L. and Maple, M.B. (1995). Electronic pairing in exotic superconductors, Phys. Today 48, 2, p. 32. [258] Hewson, A. C. (1993). The Kondo problem to heavy fermion (Cambridge University Press, Cambridge). [259] Yoshimori, A. and Sakurai, A. (1970). Functional integral approach to the bound state due to the s-d exchange Interaction, Suppl. Prog. Theor. Phys. 46, pp. 162–181. [260] Eto, M. and Nazarov, Y.V. (2001). Mean ﬁeld theory of the Kondo-eﬀect in quantum dots with a even numbers of electrons, Phys. Rev. B 64, p. 85322. [261] Fulde, P. and Ferrell, A. (1964). Superconductivity in a strong spin-exchange ﬁeld, Phys. Rev. 135, pp. A550–A563. [262] Larkin, A. and Ovchinnikov, Y. (1965). Inhomogeneous state of superconductors, Sov. Phys. JETP 20, p. 762. [263] Lyuksyutov, I.F. and Pokrovsky, V.L. (2005). Ferromagnet superconductor hybrids, Adv. Phys. 54 pp. 67–136. [264] Kruchinin, S. (2017). Problems and solutions in special relativity and electromagnetism (World Scientiﬁc), p. 140. [265] Ryazanov, V.V., Oboznov, V.A., Rusanov, A.V., Veretennikov, A.V., Golubov, A.A. and Aarts, J. (2001). Coupling of two superconductors through a ferromagnet: Evidence for a π-junction, Phys. Rev. Lett. 86, pp. 2427–2430. [266] Frolov, S.M., Van Harlingen, D.J., Oboznov, V.A., Bolginov, V.V. and Ryazanov, V.V. (2004). Measurement of the current-phase relation of superconductor/ferromagnet/superconductor Josephson junctions, Phys. Rev. B 70, p. 144505. [267] Bell, C., Loloee, R., Burnell, G. and Blamire, M.G. (2005). Characteristics of strong ferromagnetic Josephson junctions with epitaxial barriers, Phys. Rev. B 71, p. 180501. [268] Ruotolo, A., Pepe, G.P., Bell, C. Leung, C.W. and Blamire, M.G. (2005). Modulation of the dc Josephson current in pseudo-spin-valve Josephson multilayers, Supercond. Sci. Technol. 18, pp. 921–926.

page 285

March 25, 2021

286

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Modern Aspects of Superconductivity: Theory of Superconductivity

[269] Lange, M., Van Bael, M.J., Van Look, L., Raedts, S., Moschalkov, V.V. and Bruynseraede, Y. (2002). Nanostructured superconductor ferromagnet bilayers. in New Trends in Superconductivity, Annett, J.F. and Kruchinin, S. (eds.), NATO Science Series II Mathematics Physics and Chemistry Vol. 67, pp. 365–373 (Kluwer Academic Publishers, Dordrecht). [270] Aladyshkin, A., Yu., Silhanek, A.V., Gillijns, W. and Moshchalkov, V.V. (2009). Nucleation of superconductivity and vortex matter in superconductorferromagnet hybrids, Supercond. Sci.Technol. 22, pp. 1–48 [271] Milosovec, M.V. and Peeters, F.M. (2005). Field-enhanced critical parameters in magnetically nanostructured superconductors, Europhys. Lett. 70, pp. 670–676. [272] Fetter, V.M. and Larkin, A.I. (2002). Spin glass versus superconductivity, Phys. Rev. B 66, p. 64526. [273] Andreev, A.F. (1998). Superﬂuidity, superconductivity, and magnetism in mesoscopics, Usp. Phys., 168, 6, pp. 656–663. [274] Larkin, A. and Ovchinnikov, Y. (1965). Nonuniform state of superconductors, Sov. Phys. JETP 20, 3, p. 762–770. [275] Fulde, P. and Ferrell, A. (1964). Superconductivity in a strong spin-exchange ﬁeld, Phys. Rev. 135, p.A550. [276] Mota, A.C., Visani, P., Polloni, A. and Aupke, K. (1994). Coherent phenomena in mesoscopic cylinders of Cu and Ag in proximity with a superconductor, Physica B 197, pp. 95–100. [277] M¨ uller-Allinger, F.B. and Mota, A.C. (2000). Reentrance of the induced diamagnetism in gold-niobium proximity cylinders, Phys. Rev. B 62, pp. 6120. [278] M¨ uller-Allinger, F.B. and Mota, A.C. (2000). Paramagnetic reentrant eﬀect in high purity mesoscopic AgNb proximity structures, Phys. Rev. Lett. 84, pp. 3161–3164. [279] M¨ uller-Allinger, F.B. and Mota, A.C. (2000). Magnetic response of clean NS proximity cylinders, Physica B 284–288, p.683–684. [280] Caroli. C. and Matricon, J. (1965). Excitations ´electroniques dans les supraconducteurs de 2`eme esp`ece. II. Excitations de basse ´energie, Phys. Kondens. Mater. 3, pp. 380–401. [281] Lyuksyutov, I.F. and Pokrovsky, V.L. (2005). Ferromagnet-superconductor hybrids, Adv. Phys. 54, pp. 67–136. [282] Buzdin, A.I. (2005). Proximity eﬀects in superconductor-ferromagnet heterostructures, Rev. Mod. Phys. 77, pp. 935–976. [283] Gygi, F. and Schl¨ uter, M. (1991). Self-consistent electronic structure of a vortex line in a type-II superconductor, Phys. Rev. B 43, pp. 7609–7621. [284] Wang, J. et al. (2010). Interplay between superconductivity and ferromagnetism in crystalline nanowires, Nature Phys. 6, p.389. [285] Shanenko, A.A., Croitoru, D., Vagov, A. and Peeters, M. (2008). Proceedings of NATO ARW “physical properties of nanosystems”, Bonca, J. and Kruchinin, S. (eds.) (Springer, Berlin), pp. 340–348. [286] Hofstadter, D. (1976). Energy levels and wave functions of Bloch electrons in rational and irrational magnetic ﬁelds, Phys. Rev. B 14, pp. 2239–2249.

page 286

March 25, 2021

10:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-bib

Bibliography

287

[287] Kretinin, A.V., Cao, Y., Tu, J.S., Yu, G.L., Jalil, R., Novoselov, K.S., Haigh, S.J., Gholinia, A., Mishchenko, A., Lozada, M., Georgiou, T., Woods, C.R., Withers, F., Blake, P., Eda, G., Wirsig, A., Hucho, C., Watanabe, K., Taniguchi, T., Geim, A.K. and Gorbachev, R.V. (2014). Electronic properties of graphene encapsulated with diﬀerent two-dimensional atomic crystals, Nano Lett. 14, 6, pp. 3270–3276. [288] Milosevic, M.V., Yampolskii, S.V. and Peeters, F.M. (2002). Magnetic pinning of vortices in a superconducting ﬁlm: the (anti)vortex-magnetic dipole interaction energy in the London approximation, Phys. Rev. B 66, p. 174519. [289] de Gennes P.-G.(1966). Superconductivity of metals and alloys (AddisionWesley, Advanced Book Programme). [290] Van der Wal, C. (2000). Quantum superposition of macroscopic persistentcurrent states, Science 290, p. 773. [291] You, J.Q. and Nori, F. (2005). Superconducting circuits and quantum information, Phys. Today 12, pp. 42–45. [292] Nakamura, Y., Pashkin, Y.A. and Tsai, J.S. (1999). Quantum oscillations in two coupled charge qubits, Nature 398, pp. 786–788. [293] Makhlin, Y., Schon, G. and Shnirman, A. (2001). Quantum-state engineering with Josephson-junction devices, Rev. Mod. Phys. 73, pp. 357–400. [294] Chiorescu, I., Nakamura, Y., Harmans, C.J.P.M. and Mooij J.E. (2003). Coherent quantum dynamics of a superconducting ﬂux qubit, Science 299, pp. 1869–1871. [295] Manin, Yu.I. (1980). Computable and noncomputable (Sov. Radio, Moscow, in Russian), p. 15. [296] Wiesner, S. (1983). Conjugate coding, SIGACT News 15, 1, pp. 78–88. [297] Feynman, R.P. (1982). Simulating physics with computers, Int. J. Theoret. Phys. 21, 6, pp. 467—488. [298] Emelyanov, V.I. and Vladimirova, V.V. (2012). The quantum physics. Bits and qubits (Moscow State University), 176 p. [299] Greenstein, G., Zajonc, A.G. (2006). The quantum challenge: modern research on the foundations of quantum mechanics (physics and astronomy) (Jones and Bartlett Publishers), p. 400. [300] Qi, Xiao-Liang, Zhang, Shou-Cheng 2011. Topological insulators and superconductors, Rev. Mod. Phys. 83, 4, pp. 1057–1110. [301] Kitaev, A.Yu. (2001). Unpaired Majorana fermions in quantum wires, Phys.Uspekhi. 44, 10S, p. 131. [302] Zhang, Q. and Wu, B. (2018). Majorana modes in solid state systems and its dynamics, Front. Phys. 13, 2, p. 137101. [303] Mourik, V. et al. (2012). Signatures of Majorana Fermions in hybrid superconductor-semiconductor nanowire devices, Science 336, 6084, p. 1003.

page 287

This page intentionally left blank

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-index

Index

acoustic phonons, 78, 83 anharmonic model, 76, 80 antiferromagnetic, 66, 74–76, 93–97, 105, 111, 275 anyonic superconductivity, 82

eﬀective interaction, 147, 160, 166, 187, 193, 194 exact solution, 183, 194, 195, 202, 206, 213, 214, 283 exchange interactions, 216 exciton mechanism, 79

basis functions, 85, 86 BCS theory, 28, 34, 47, 54, 68, 69, 77, 82, 83, 93, 109, 151, 153, 183, 186, 190, 192, 194, 211, 213 bipolaronic mechanism, 76, 83 Bose-condensation, 84 Bose-particles, 83 boson ﬁeld, 47, 49–51, 56, 59, 63

ferromagnetic, 78, 146, 185, 216–219, 221–224 ferromagnetic granules, 222, 267 FFLO, 216 ﬂux qubit, 245 free energy, 99–102, 105–107, 112, 220 gap equation, 21, 22, 25, 26, 53, 162, 189, 191 Gauss theorem, 220, 269 Ginzburg–Landau equation, 62 Green functions, 98, 150, 281 Green’s functions, 188

carbon nanotubes, 184, 239 charge qubit, 246 chemical potential, 4, 12, 20, 22, 27, 31, 35, 94, 98, 103, 147, 160, 163, 169, 187, 192, 196, 202, 211 condensation energy, 110, 185, 190, 193, 195, 204–206, 208, 210, 213–215 continual model, 97 Coulomb blockage, 246, 247 critical temperature, 22, 25, 29, 30, 34, 54, 55, 65–70, 73, 75, 77, 78, 93, 103, 109, 112, 155, 159, 164, 260 CuO2 planes, 66, 75

heat capacity, 93, 108–110, 112 heavy fermions, 86, 87, 93, 110 high-temperature superconductors, 66–71, 73, 74, 76, 78, 84, 86, 94, 95, 110–112, 273–275 HOMO, 27 HTSC, 65, 66, 69, 70, 75, 77, 79, 82, 86, 154–156, 259 Hubbard, 81 Hubbard model, 94 Hubbard-Stratonovitch transformation, 47, 49, 63

d-symmetry, 85, 89, 90, 92, 95, 110 Debye energy, 77, 187, 210 deformation energy, 24, 25 dielectric properties, 82

289

page 289

March 24, 2021

290

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-index

Modern Aspects of Superconductivity: Theory of Superconductivity

instability, 58, 95 interacting, 16, 26, 39, 41, 45, 217, 218 interaction constant, 187, 192, 194 interferometer, 243, 244 iron superconductors, 113 Jahn–Teller eﬀect, 81 Josephson junctions, 3, 88–92, 110, 241–243, 245–247 jump of the heat, 93, 109, 112 Knight shift, 88 Kondo eﬀect, 207, 208, 210, 212, 215, 283 Lagrangian, 3, 8, 46, 47, 56, 58–60, 98 length scale, 217, 219 level spacing, 183, 190, 191, 211, 215 London equation, 218 London superconductors, 216, 218, 267 LUMO, 27 magnetic resonance, 30, 34, 35 magnons, 78, 94 mechanism of pairing, 66, 67, 76, 78, 81, 82, 84–86, 97, 111, 164 mechanisms of pairing, 76, 77, 111 M g1−x Alx B2 , 159 mixed state, 85, 86 multiband superconductivity, 145, 271 N´eel temperature, 75 Nambu spinor, 4, 7, 9, 31, 41 Nambu–Goldstone theorem, 8 nanoscale superconductivity, 183 nanosize two-gap superconductivity, 184, 186, 187, 190, 192–194 NMR, 34, 88, 95–97 Noether theorem, 8 order parameters, 2, 46, 47, 212, 215 organic superconductors, 79, 80 π-junction, 92, 216 parity gap, 185, 190, 192–195, 205

path integral, 47–49, 60, 185, 187–189, 194 Peierls instability, 23 penetration depth, 66, 88, 95, 184, 216–219, 222, 223, 228–230, 268 phase diagram, 74, 75, 145, 149, 158, 165, 168, 171, 172 phase diﬀerence, 92, 242, 243 Pippard case, 217 plasmon mechanism, 82 polyacene, 23–25, 27 polymer, 22, 27, 79 propagator, 11, 12, 17, 18, 20, 21, 35, 40, 41, 44, 45, 56 pseudogap, 74, 75 quantum computer, 239–241, 248, 259 qubit, 239–241, 247, 248 Rabi oscillation, 246 relaxation, 30, 34, 35, 39, 46, 88 renormalization equation, 165, 170–172 renormalization group, 145, 158, 165, 166, 168 Richardson solution, 183 RKKY, 217, 222, 224 room-temperature, 1, 65, 68, 145, 153, 154 RTSC, 154 RVB, 1, 79 self-energy, 35, 39–41, 45, 220 size eﬀect, 184, 185 spin dynamics, 44, 97 spin ﬂuctuations, 66, 84, 93–97, 105, 111, 145, 274, 275 spin waves, 78, 94 spin-orientation phase transitions, 224 spinor, 3, 4, 6–9, 11, 13, 29, 31, 41, 51 SQUIDS, 243, 247, 248 superconducting grains, 186, 193, 207, 208, 210, 243 supersymmetry, 47, 59, 61 susceptibility, 35, 37, 39, 76, 94, 96, 97, 224 symmetry breaking, 3, 8, 56

page 290

March 24, 2021

20:14

Modern Aspects of Superconductivity (2nd Edn.) - 9.61in x 6.69in

b4202-index

Index

symmetry group, 85, 86, 88 symmetry of pairing, 67, 111, 274 theory of superconductivity, 1, 35, 46, 66, 84, 93, 145 thermodynamics, 66, 67, 93, 97, 112, 275 Tl-based, 71, 73 two-dimensional, 63, 80–82, 85, 88, 94, 106–108, 155, 156, 224–226 two-gap superconductivity, 145, 156, 164, 184–187, 189, 190, 192–194, 207, 278, 280 two-level, 240, 242, 247

ultrasmall grains, 194, 208, 210, 213–215, 283 U P t3 , 87 vertex correction, 165, 168, 169 yttrium ceramics, 70, 71

291

page 291